343 57 66MB
English Pages 1728 Year 2003
DOT/FAA/ARMMPDS01 Office of Aviation Research Washington, D.C. 20591
Metallic Materials Properties Development and Standardization (MMPDS)
January 2003 Scientific Report
This document is available to the U.S. public through the National Technical Information Service, Springfield (NTIS), Virginia 22161.
U.S. Department of Transportation Federal Aviation Administration
Technical Report Documentation Page 1. Report No.
2. Government Accession No.
3. Recipient's Catalog No.
DOT/FAA/ARMMPDS01 4. Title and Subtitle
5. Report Date
METALLIC MATERIALS PROPERTIES DEVELOPMENT AND STANDARDIZATION (MMPDS)
January 2003 6. Performing Organization Code
7. Author(s)
8. Performing Organization Report No.
Richard C. Rice1, Jana L. Jackson1, John Bakuckas2, and Steven Thompson3 10. Work Unit No. (TRAIS)
9. Performing Organization Name and Address 1
Battelle Memorial Laboratories 505 King Avenue Columbus, OH 43201 2
FAA William J. Hughes Technical Center Materials and Structures Branch, AAR450 Atlantic City International Airport, NJ 08405 3
U. S. Air Force Research Laboratory Materials and Manufacturing Directorate Wright Patterson Air Force Base, OH 45433 11. Contract or Grant No.
F3361597C5647 12. Sponsoring Agency Name and Address
13. Type of Report and Period Covered
U.S. Department of Transportation Federal Aviation Administration Office of Aviation Research Washington, DC 20591
Scientific Report January 1, 2002 – December 31, 2002
14. Sponsoring Agency Code 15. Supplementary Notes
16. Abstract
The Metallic Material Properties Development and Standardization (MMPDS) Handbook is the replacement document for MILHDBK5. It is recognized internationally as a reliable source of aircraft materials data for aerospace materials selection and analysis. Consistent and reliable methods are used to collect, analyze, and present statistically based material and fastener allowable properties. The Handbook is the only publicly available source in the U.S. for material allowables that the Federal Avaiation Administration generally accepts for compliance with Federal Aviation Regulations (FAR) for material strength properties and design values for aircraft certification and continued airworthiness. Moreover, it is the only publicly available source worldwide for fastener joint allowables that comply with the FARs. This edition, MMPDS01, incorporates the additions and changes to aircraft metallic material design properties and analysis guidelines approved at the 1st and 2nd MMPDS government/industry coordination meetings. This year, 2003, marks the first year of publication of the MMPDS Handbook and the final year of publication of MILHDBK5. For this year only, MMPDS01 and MILHDBK5J will be technically equivalent. In the spring of 2004, when the 1st Change Notice of MMPDS01 is published, MILHDBK5 will be designated noncurrent and MMPDS will become the only governmentrecognized source in the U.S. of published design allowable properties for metallic commercial and military aircraft structures and mechanically fastened joints. In this way, the 65year legacy of MILHDBK5, and its predecessor ANC5, will be maintained. 17. Key Words
18. Distribution Statement
Metallic materials, Design allowables, Mechanical fasteners, Aircraft design, Government/industry coordination
This document is available to the public through the National Technical Information Service (NTIS), Springfield, Virginia 22161.
19. Security Classif. (of this report)
Unclassified Form DOT F1700.7
20. Security Classif. (of this page)
Unclassified (872)
Reproduction of completed page authorized
21. No. of Pages
1632
22. Price
MMPDS01 31 January 2003
FOREWORD This handbook is approved for use by the Federal Aviation Administration (FAA) and all Departments and Agencies of the Department of Defense. MMPDS01 is equivalent to MILHDBK5J, the last edition of the Metallic Materials and Elements for Aerospace Vehicle Structures Handbook that was maintained by the U.S. Air Force. The FAA plans to publish annual updates and revisions to the MMPDS. MILHDBK5J is scheduled to be reclassified as noncurrent in the Spring of 2004. Beneficial comments (recommendations, additions, deletions) and any pertinent data that may be of use in improving this document should be addressed to: Chairman, MMPDS Coordination Activity (6094854784 voice or 6094854004 fax), AAR450, Materials and Structures Branch, FAA William J. Hughes Technical Center, Atlantic City International Airport, Atlantic City, NJ 08405. This document contains design information on the strength properties of metallic materials and elements for aerospace vehicle structures. All information and data contained in this Handbook have been coordinated with the FAA, the Air Force, the Army, the Navy, and industry prior to publication and are being maintained as a joint effort of the FAA and the Department of Defense. The electronic copy of the Handbook is technically consistent with the paper copy Handbook; however, minor differences exist in format, i.e., table or figure position. Depending on monitor size and resolution setting, more data may be viewed without onscreen magnification. The figures were converted to electronic format using one of several methods. For example, digitization or recomputation methods were used on most of the engineering figures like typical stressstrain and effect of temperature, etc. Scanning was used to capture informational figures such as those found in Chapters 1 and 9. These electronic figures were also used to generate the paper copy figures to maintain equivalency between the paper copy and electronic copy. In all cases, the electronic figures have been compared to the paper copy figures to ensure the electronic figure was technically equivalent. Appendix E provides a detailed list of all the figures in the Handbook, along with a description of each figure’s format. Custodians: FAA Army—AV Navy—AS Air Force—11
Preparing activity: FAA William J. Hughes Technical Center
(Project No. 15600187)
Review activities: FAA William J. Hughes Technical Center Army—ME, MI Navy—CG Air Force—80, 82, 84, 99
ii
MMPDS01 31 January 2003
EXPLANATION OF NUMERICAL CODE
For chapters containing materials properties, a decinumeric system is used to identify sections of text, tables, and illustrations. This system is explained in the examples shown below. Variations of this decinumerical system are also used in Chapters 1, 8, and 9. 2.4.2.1.1
Example A
General material category (in this case, steel) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A logical breakdown of the base material by family characteristics (in this case, intermediate alloy steels); or for element properties . . . . . . . . . . . . . . . . . . . . . . . . . Particular alloy to which all data are pertinent. If zero, section contains comments on the family characteristics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . If zero, section contains comments specific to the alloy; if it is an integer, the number identifies a specific temper or condition (heat treatment) . . . . . . . . . . . . . . . . . . . . . . . . . . . . Type of graphical data presented on a given figure (see following description) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Example B
3.2.3.1.X
Aluminum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2000 Series Wrought Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2024 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . T3, T351, T3510, T3511, T4, and T42 Tempers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Specific Property as Follows . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Tensile properties (ultimate and yield strength) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
1
Compressive yield and shear ultimate strengths . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
2
Bearing properties (ultimate and yield strength) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
3
Modulus of elasticity, shear modulus . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
4
Elongation, total strain at failure, and reduction of area . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
5
Stressstrain curves, tangentmodulus curves . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
6
Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
7
Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
8
FatigueCrack Propagation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
9
Fracture Toughness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
10
iii
MMPDS01 31 January 2003
CONTENTS Section Chapter 1 1.0 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Purpose and Use of Document . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.2 Scope of Handbook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Symbols and Definitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.2 International Systems of Units (SI) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Commonly Used Formulas . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.2 Simple Unit Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.3 Combined Stresses (see Section 1.5.3.5) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.4 Deflections (Axial) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.5 Deflections (Bending) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.6 Deflections (Torsion) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.7 Biaxial Elastic Deformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.8 Basic Column Formula . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.9 Inelastic StressStrain Response . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4 Basic Principles . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.2 Stress . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.3 Strain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.4 Tensile Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.5 Compressive Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.6 Shear Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.7 Bearing Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.8 Temperature Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.9 Fatigue Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.10 Metallurgical Instability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.11 Biaxial Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.12 Fracture Toughness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.13 FatigueCrackPropagation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5 Types of Failures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.2 Material Failures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.3 Instability Failures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6 Columns . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.2 Primary Instability Failures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.3 Local Instability Failure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.4 Correction of Column Test Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.7 ThinWalled and Stiffened ThinWalled Sections . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
I
Page 11 11 11 11 13 13 13 14 14 14 14 14 14 15 15 15 16 17 17 18 18 19 111 111 112 113 114 117 117 119 124 128 128 128 129 130 130 130 130 131 140
MMPDS01 31 January 2003
CONTENTS (Continued) Section References
Page . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 141
Chapter 2 2.0 Steel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Alloy Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.2 Material Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.3 Environmental Considerations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Carbon Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.0 Comments on Carbon Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.1 AISI 1025 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 LowAlloy Steels (AISI Grades and Proprietary Grades) . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.0 Comments on LowAlloy Steels (AISI and Proprietary Grades) . . . . . . . . . . . . . . . . 2.3.1 Specific Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Intermediate Alloy Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.0 Comments on Intermediate Alloy Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.1 5CrMoV . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.2 9Ni4Co0.20C . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.3 9Ni4Co0.30C . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5 HighAlloy Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.0 Comments on HighAlloy Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.1 18 Ni Maraging Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.2 AF1410 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.3 AerMet 100 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6 Precipitation and TransformationHardening Steels (Stainless) . . . . . . . . . . . . . . . . . . . . . . . 2.6.0 Comments on Precipitation and TransformationHardening Steels (Stainless) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.1 AM350 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 AM355 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.3 Custom 450 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.4 Custom 455 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.5 Custom 465 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.6 PH138Mo . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.7 155PH . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.8 PH157Mo . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.9 174PH . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.10 177PH . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7 Austenitic Stainless Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.0 Comments on Austenitic Stainless Steel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.1 AISI 301 and Related 300 Series Stainless Steels . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8 Element Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8.1 Beams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8.2 Columns . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8.3 Torsion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References ................................................................... NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
II
21 21 21 22 25 26 26 27 210 210 215 266 266 266 274 279 291 291 293 2104 2107 2115 2115 2115 2122 2128 2140 2151 2157 2167 2183 2195 2213 2220 2220 2222 2237 2237 2237 2240 2246
MMPDS01 31 January 2003
CONTENTS (Continued) Section Chapter 3 3.0 Aluminum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1.1 Aluminum Alloy Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1.2 Material Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1.3 Manufacturing Considerations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 2000 Series Wrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.1 2014 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.2 2017 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.3 2024 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.4 2025 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.5 2026 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.6 2090 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.7 2124 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.8 2219 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.9 2297 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.10 2424 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.11 2519 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.12 2524 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.13 2618 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 3000 Series Wrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4 4000 Series Wrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5 5000 Series Wrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.1 5052 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.2 5083 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.3 5086 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.4 5454 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.5 5456 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6 6000 Series Wrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.1 6013 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.2 6061 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.3 6151 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7 7000 Series Wrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.1 7010 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.2 7040 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.3 7049/7149 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.4 7050 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.5 7055 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.6 7075 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.7 7150 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.8 7175 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.9 7249 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.10 7475 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8 200.0 Series Cast Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.1 A201.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
III
Page 31 31 32 32 318 326 326 365 368 3150 3152 3154 3157 3166 3195 3199 3202 3205 3209 3218 3218 3218 3218 3231 3237 3247 3252 3258 3258 3262 3290 3293 3293 3302 3305 3322 3363 3368 3427 3439 3454 3458 3486 3486
MMPDS01 31 January 2003
CONTENTS (Continued) Section 3.9 300.0 Series Cast Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.1 354.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.2 355.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.3 C355.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.4 356.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.5 A356.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.6 A357.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.7 D357.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.9.8 359.0 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.10 Element Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.10.1 Beams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.10.2 Columns . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.10.3 Torsion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References ...................................................................
Page 3496 3496 3498 3501 3503 3506 3510 3513 3516 3518 3518 3519 3521 3525
Chapter 4 4.0 Magnesium Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.1 Alloy Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.2 Material Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.3 Physical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.4 Environmental Considerations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.5 Alloy and Temper Designations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.6 Joining Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 MagnesiumWrought Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 AZ31B . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.2 AZ61A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.3 ZK60A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Magnesium Cast Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.1 AM100A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.2 AZ91C/AZ91E . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.3 AZ92A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.4 EZ33A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.5 QE22A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.6 ZE41A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Element Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.1 Beams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.2 Columns . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.3 Torsion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References ...................................................................
41 41 41 41 42 42 43 45 46 46 417 419 427 427 429 433 439 444 448 453 453 453 456 457
Chapter 5 5.0 Titanium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 51 5.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 51 5.1.1 Titanium Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 51 NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
IV
MMPDS01 31 January 2003
CONTENTS (Continued) Section 5.1.2 Material Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.3 Manufacturing Considerations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.4 Environmental Considerations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Unalloyed Titanium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Commercially Pure Titanium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3 Alpha and NearAlpha Titanium Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Ti5Al2.5Sn . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.2 Ti8Al1Mo1V . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.3 Ti6Al2Sn4Zr2Mo . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 AlphaBeta Titanium Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Ti6Al4V . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.2 Ti6Al6V2Sn . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.3 Ti4.5Al3V2Fe2Mo . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Beta, NearBeta, and MetastableBeta Titanium Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5.1 Ti13V11Cr3Al . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5.2 Ti15V3Cr3Sn3Al (Ti153) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5.3 Ti10V2Fe3Al (Ti1023) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.6 Element Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.6.1 Beams . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References ...................................................................
Page 51 52 52 55 55 515 515 527 543 551 551 592 5110 5118 5118 5135 5139 5144 5144 5145
Chapter 6 6.0 HeatResistant Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Material Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 IronChromiumNickelBase Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.0 General Comments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 A286 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.2 N155 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 NickelBase Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.0 General Comments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 Hastelloy X . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Inconel 600 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.3 Inconel 625 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.4 Inconel 706 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.5 Inconel 718 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.6 Inconel X750 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.7 Rene 41 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.8 Waspaloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.9 HAYNES® 230® . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 CobaltBase Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4.0 General Comments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4.1 L605 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4.2 HS 188 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References ...................................................................
61 61 63 64 64 64 615 619 619 621 627 634 645 651 677 683 690 696 6116 6116 6117 6124 6140
NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
V
MMPDS01 31 January 2003
CONTENTS (Continued) Section Chapter 7 7.0 Miscellaneous Alloys and Hybrid Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Beryllium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.1 Standard Grade Beryllium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3 Copper and Copper Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.0 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.1 Maganese Bronzes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.2 Copper Beryllium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4 Multiphase Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.0 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.1 MP35N Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.2 MP159 Alloy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Aluminum Alloy Sheet Laminates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.0 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.1 2024T3 Aramid Fiber Reinforced Sheet Laminate . . . . . . . . . . . . . . . . . . . . . . . . . . References ...................................................................
71 71 71 71 78 78 79 712 721 721 721 727 732 732 732 750
Chapter 8 8.0 Structural Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Mechanically Fastened Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.1 Introduction and Fastener Indexes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.2 Solid Rivets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.3 Blind Fasteners . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.4 Swaged Collar/UpsetPin Fasteners . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.5 Threaded Fasteners . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.6 Special Fasteners . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Metallurgical Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.1 Introduction and Definitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.2 Welded Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.3 Brazing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Bearings, Pulleys, and Wire Rope . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References ...................................................................
81 82 82 811 837 8110 8125 8147 8150 8150 8150 8172 8172 8173
Chapter 9 9.0 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.2 Applicability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.3 Approval Procedures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.4 Documentation Requirements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.6 Data Basis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.7 Rounding Procedures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Material, Specification, Testing, and Data Requirements . . . . . . . . . . . . . . . . . . . . . . . . . . .
91 95 95 95 95 95 96 98 910 911
NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
VI
Page
MMPDS01 31 January 2003
CONTENTS (Continued) Section 9.2.1 Material Requirements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.2 Specification Requirements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.3 Required Test Methods/Procedures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.4 Data Requirements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.5 Experimental Design . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Submission of Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3.1 Recommended Procedures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3.2 Computer Software . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3.3 General Data Formats . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4 Substantiation of SBasis Minimum Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5 Analysis Procedures for Statistically Computed Minimum Static Properties . . . . . . . . . . . . 9.5.1 Specifying the Population . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.2 Regression Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.3 Combinability of Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.4 Determining the Form of Distribution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.5 Direct Computation Without Regression . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.6 Direct Computation by Regression Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.7 Indirect Computation without Regression (Reduced Ratios/Derived Properties) . . . . 9.5.8 Indirect Computation using Regression . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.6 Analysis Procedures for Dynamic and Time Dependent Properties . . . . . . . . . . . . . . . . . . . . 9.6.1 Load and Strain Control Fatigue Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.6.2 Fatigue Crack Growth Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.6.3 Fracture Toughness Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.6.4 Creep and CreepRupture Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7 Analysis Procedures for Structural Joint Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.1 Mechanically Fastened Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.2 FusionWelded Joint Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.8 Examples of Data Analysis and Data Presentation for Static Properties . . . . . . . . . . . . . . . . 9.8.1 Direct Analyses of Mechanical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.8.2 Indirect Analyses of Mechanical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.8.3 Tabular Data Presentation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.8.4 Room Temperature Graphical Mechanical Properties . . . . . . . . . . . . . . . . . . . . . . . . 9.8.5 Elevated Temperature Graphical Mechanical Properties . . . . . . . . . . . . . . . . . . . . . . 9.9 Examples of Data for Dynamic and Time Dependent Properties . . . . . . . . . . . . . . . . . . . . . . 9.9.1 Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.9.2 Fatigue Crack Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.9.3 Fracture Toughness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.9.4 Creep and Creep Rupture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.9.5 Mechanically Fastened Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.9.6 FusionWelded Joints . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10 Statistical Tables . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10.1 OneSided Tolerance Limit Factors, K, for the Normal Distribution, 0.95 Confidence, and n1 Degrees of Freedom . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10.2 0.950 Fractiles of the F Distribution Associated with n1 and n2 Degrees of Freedom . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
VII
Page 911 911 911 924 940 950 950 950 950 959 960 960 964 977 982 994 9104 9106 9109 9110 9110 9130 9133 9135 9142 9142 9158 9162 9162 9175 9179 9184 9202 9212 9212 9228 9230 9234 9240 9244 9247 9248 9250
MMPDS01 31 January 2003
CONTENTS (Continued) Section 9.10.3 0.950 Fractiles of the F Distribution Associated with n1 and n2 Degrees of Freedom . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10.4 0.95 and 0.975 Fractiles of the t Distribution Associated with df Degrees of Freedom . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10.5 Area Under the Normal Curve from 4 to the Mean +Zp Standard Deviations . . . . . 9.10.6 OneSided ToleranceLimit Factors for the ThreeParameter Weibull Acceptability Test with 95 Percent Confidence . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10.7 OneSided Tolerance Factors for the ThreeParameter Weibull Distribution With 95 Percent Confidence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.10.8 γvalues for Computing Threshold of ThreeParameter Weibull Distribution . . . . . . 9.10.9 Ranks, r, of Observations, n, for an Unknown Distribution Having the Probability and Confidence of T99 and T90 Values . . . . . . . . . . . . . . . . . . . . . . . . Standards and References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Appendices A.0 Glossary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.1 Abbreviations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.2 Symbols . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.3 Definitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.4 Conversion of U.S. Units of Measure Used in MMPDS to SI Units . . . . . . . . . . . . . B.0 Alloy Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . C.0 Specification Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . D.0 Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . E.0 Figure Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
NOTE: Information and data for alloys deleted from MMPDS may be obtained through the Chairman, MMPDS Coordination Activity.
VIII
Page 9251 9252 9253 9254 9255 9261 9264 9266
A1 A1 A5 A6 A17 B1 C1 D1 E1
MMPDS01 31 January 2003
CHAPTER 1 GENERAL 1.1
PURPOSE AND USE OF DOCUMENT
1.1.1 INTRODUCTION — Since many aerospace companies manufacture both commercial and military products, the standardization of metallic materials design data, which are acceptable to Government procuring or certification agencies is very beneficial to those manufacturers as well as governmental agencies. Although the design requirements for military and commercial products may differ greatly, the required design values for the strength of materials and elements and other needed material characteristics are often identical. Therefore, this publication provides standardized design values and related design information for metallic materials and structural elements used in aerospace structures. The data contained herein, or from approved items in the minutes of MMPDS coordination meetings, are acceptable to the FAA, the Air Force, the Navy, and the Army. Approval by the procuring or certificating agency must be obtained for the use of design values for products not contained herein. This printed document is distributed by the National Technical Information Service (NTIS). It is the only official form of MMPDS. If computerized thirdparty MMPDS databases are used, caution should be exercised to ensure that the information in these databases is identical to that contained in this Handbook. Copies of the document can be obtained from the NTIS at the US Department of Commerce Technology Administration as follows: US Department of Commerce Technology Administration National Technical Information Service 5285 Port Royal Road Springfield, VA 22161 (703) 6056000 http://www.ntis.gov 1.1.2 SCOPE OF HANDBOOK — This Handbook is primarily intended to provide a source of design mechanical and physical properties, and joint allowables. Material property and joint data obtained from tests by material and fastener producers, government agencies, and members of the airframe industry are submitted to MMPDS for review and analysis. Results of these analyses are submitted to the membership during semiannual coordination meetings for approval and, when approved, published in this Handbook. This Handbook also contains some useful basic formulas for structural element analysis. However, structural design and analysis are beyond the scope of this Handbook. References for data and various test methods are listed at the end of each chapter. The reference number corresponds to the applicable paragraph of the chapter cited. Such references are intended to provide sources of additional information, but should not necessarily be considered as containing data suitable for design purposes. 11
MMPDS01 31 January 2003
The content of this Handbook is arranged as follows: Chapter(s) 1 27 8 9
Subjects Nomenclature, Systems of Units, Formulas, Material Property Definitions, Failure Analysis, Column Analysis, ThinWalled Sections Material Properties Joint Allowables Data Requirements, Statistical Analysis Procedures
12
MMPDS01 31 January 2003
1.2
NOMENCLATURE
1.2.1 SYMBOLS AND DEFINITIONS — The various symbols used throughout the Handbook to describe properties of materials, grain directions, test conditions, dimensions, and statistical analysis terminology are included in Appendix A. 1.2.2 INTERNATIONAL SYSTEM OF UNITS (SI) — Design properties and joint allowables contained in this Handbook are given in customary units of U.S. measure to ensure compatibility with government and industry material specifications and current aerospace design practice. Appendix A.4 may be used to assist in the conversion of these units to Standard International (SI) units when desired.
13
MMPDS01 31 January 2003
1.3
COMMONLY USED FORMULAS
1.3.1 GENERAL — Formulas provided in the following sections are listed for reference purposes. Sign conventions generally accepted in their use are that quantities associated with tension action (loads, stresses, strains, etc.), are usually considered as positive and quantities associated with compressive action are considered as negative. When compressive action is of primary interest, it is sometimes convenient to identify associated properties with a positive sign. Formulas for all statistical computations relating to allowables development are presented in Chapter 9. 1.3.2 SIMPLE UNIT STRESSES — ft fc fb fs fx fx fs fA
= = = = = = =
P / A (tension) P / A (compression) My / I = M / Z (bending) S / A (average direct shear stress) SQ / Ib (longitudinal or transverse shear stress) Ty / Ip (shear stress in round tubes due to torsion) (T/2At) (shear stress due to torsion in thinwalled structures of closed section. Note that A is the area enclosed by the median line of the section.) = BfH ; fT = BfL (axial and tangential stresses, where B = biaxial ratio)
[1.3.2(a)] [1.3.2(b)] [1.3.2(c)] [1.3.2(d)] [1.3.2(e)] [1.3.2(f)] [1.3.2(g)] [1.3.2(h)]
1.3.3 COMBINED STRESSES (SEE SECTION 1.5.3.4) —
[
fs max = fs2 + ( f n / 2)
]
fA = fc + fb (compression and bending)
fn max = fn/2 + fs
2 1/ 2
[1.3.3(a)]
(compression, bending, and torsion)
[1.3.3(b)] [1.3.3(c)]
max
1.3.4 DEFLECTIONS (AXIAL) — e = δ / L (unit deformation or strain) E = f/e (This equation applied when E is obtained from the same tests in which f and e are measured.) δ = eL = (f / E)L = PL / (AE) (This equation applies when the deflection is to be calculated using a known value of E.)
[1.3.4(a)] [1.3.4(b)] [1.3.4(c)] [1.3.4(d)]
1.3.5 DEFLECTIONS (BENDING) — di/dx = M / (EI) (Change of slope per unit length of a beam; radians per unit length)
14
[1.3.5(a)]
MMPDS01 31 January 2003
i 2 = i1 +
∫ [M /( EI)]dx — Slope at Point 2. (This integral denotes the area under the
x2
x1
y 2 = y1 + i( x 2 − x1 ) +
1.3.5(b)]
curve of M/EI plotted against x, between the limits of x1 and x2.)
∫ (M / EI)(x − x) dx — Deflection at Point 2.
x2
2
[1.3.5(c)]
x1
(This integral denotes the area under the curve having an ordinate equal to M/EI multiplied by the corresponding distances to Point 2, plotted against x, between the limits of x1 and x2.)
∫
y 2 = y1 + idx — Deflection at Point 2. (This integral denotes the area under the x2
x1
[1.3.5(d)]
curve of x1(i) plotted against x, between the limits of x1 and x2.)
1.3.6 DEFLECTIONS (TORSION) — dφ / dx = T / (GJ) (Change of angular deflection or twist per unit length of a member, radians per unit length.)
Φ = ∫ [T / (GJ )] dx
[1.3.6(a)]
x2
x1
— Total twist over a length from x1 to x2. (This integral denotes the area under the curve of T/GJ plotted against x, between the limits of x1 and x2.)
Φ = TL/(GJ) (Used when torque T/GJ is constant over length L.)
[1.3.6(b)]
[1.3.6(c)]
1.3.7 BIAXIAL ELASTIC DEFORMATION — µ = eT/eL (Unit lateral deformation/unit axial deformation.) This identifies Poisson’s ratio in uniaxial loading.
[1.3.7(a)]
Eex = fx  µfy
[1.3.7(b)]
Eey = fy  µfx
[1.3.7(c)]
Ebiaxial = E(1  µB) — B = biaxial elastic modulus.
[1.3.7(d)]
1.3.8 BASIC COLUMN FORMULAS — c — conservative using tangent modulus Fc = π2 Et (LN / ρ)2 where LN = L / %&
[1.3.8(a)]
Fc = π2 E (LN / ρ)2 — standard Euler formula
[1.3.8(b)]
15
MMPDS01 31 January 2003
1.3.9 INELASTIC STRESSSTRAIN RESPONSE — etotal = f / E + ep (elastic strain response plus inelastic or plastic strain response)
[1.3.9(a)]
where ep = 0.002 * (f/f0.2ys)n,
[1.3.9(b)]
f0.2ys = the 0.2 percent yield stress and n = RambergOsgood parameter Equation [1.3.9(b)] implies a loglinear relationship between inelastic strain and stress, which is observed with many metallic materials, at least for inelastic strains ranging from the material’s proportional limit to its yield stress.
16
MMPDS01 31 January 2003
1.4 BASIC PRINCIPLES 1.4.1 GENERAL — It is assumed that users of this Handbook are familiar with the principles of strength of materials. A brief summary of that subject is presented in the following paragraphs to emphasize principles of importance regarding the use of allowables for various metallic materials. Requirements for adequate test data have been established to ensure a high degree of reliability for allowables published in this Handbook. Statistical analysis methods, provided in Chapter 9, are standardized and approved by all government regulatory agencies as well as MMPDS members from industry. 1.4.1.1 Basis — Primary static design properties are provided for the following conditions: Tension . . . . . . . . . Compression . . . . . Shear . . . . . . . . . . . Bearing . . . . . . . . .
Ftu and Fty Fcy Fsu Fbru and Fbry
These design properties are presented as A and B or Sbasis room temperature values for each alloy. Design properties for other temperatures, when determined in accordance with Section 1.4.1.3, are regarded as having the same basis as the corresponding room temperature values. Elongation and reduction of area design properties listed in room temperature property tables represent procurement specification minimum requirements, and are designated as Svalues. Elongation and reduction of area at other temperatures, as well as moduli, physical properties, creep properties, fatigue properties and fracture toughness properties are all typical values unless another basis is specifically indicated. Use of BValues — The use of Bbasis design properties is permitted in design by the Air Force, the Army, the Navy, and the Federal Aviation Administration, subject to certain limitations specified by each agency. Reference should be made to specific requirements of the applicable agency before using Bvalues in design. 1.4.1.2 Statistically Calculated Values — Statistically calculated values are S (since 1975), T99 and T90. S, the minimum properties guaranteed in the material specification, are calculated using the same requirements and procedure as AMS and is explained in Chapter 9. T99 and T90 are the local tolerance bounds, and are defined and may be computed using the data requirements and statistical procedures explained in Chapter 9. 1.4.1.3 Ratioed Values — A ratioed design property is one that is determined through its relationship with an established design value. This may be a tensile stress in a different grain direction from the established design property grain direction, or it may be another stress property, e.g., compression, shear or bearing. It may also be the same stress property at a different temperature. Refer to Chapter 9 for specific data requirements and data analysis procedures. Derived properties are presented in two manners. Room temperature derived properties are presented in tabular form with their baseline design properties. Other than room temperature derived properties are presented in graphical form as percentages of the room temperature value. Percentage 17
MMPDS01 31 January 2003
values apply to all forms and thicknesses shown in the room temperature design property table for the heat treatment condition indicated therein unless restrictions are otherwise indicated. Percentage curves usually represent short time exposures to temperature (thirty minutes) followed by testing at the same strain rate as used for the room temperature tests. When data are adequate, percentage curves are shown for other exposure times and are appropriately labeled. 1.4.2 STRESS — The term “stress” as used in this Handbook implies a force per unit area and is a measure of the intensity of the force acting on a definite plane passing through a given point (see Equations 1.3.2(a) and 1.3.2(b)). The stress distribution may or may not be uniform, depending on the nature of the loading condition. For example, tensile stresses identified by Equation 1.3.2(a) are considered to be uniform. The bending stress determined from Equation 1.3.2(c) refers to the stress at a specified distance perpendicular to the normal axis. The shear stress acting over the cross section of a member subjected to bending is not uniform. (Equation 1.3.2(d) gives the average shear stress.) 1.4.3 STRAIN — Strain is the change in length per unit length in a member or portion of a member. As in the case of stress, the strain distribution may or may not be uniform in a complex structural element, depending on the nature of the loading condition. Strains usually are present also in directions other than the directions of applied loads. 1.4.3.1 Poisson’s Ratio Effect — A normal strain is that which is associated with a normal stress; a normal strain occurs in the direction in which its associated normal stress acts. Normal strains that result from an increase in length are designated as positive (+) and those that result in a decrease in length are designated as negative (). Under the condition of uniaxial loading, strain varies directly with stress. The ratio of stress to strain has a constant value (E) within the elastic range of the material, but decreases when the proportional limit is exceeded (plastic range). Axial strain is always accompanied by lateral strains of opposite sign in the two directions mutually perpendicular to the axial strain. Under these conditions, the absolute value of a ratio of lateral strain to axial strain is defined as Poisson’s ratio. For stresses within the elastic range, this ratio is approximately constant. For stresses exceeding the proportional limit, this ratio is a function of the axial strain and is then referred to as the lateral contraction ratio. Information on the variation of Poisson’s ratio with strain and with testing direction is available in Reference 1.4.3.1. Under multiaxial loading conditions, strains resulting from the application of each directional load are additive. Strains must be calculated for each of the principal directions taking into account each of the principal stresses and Poisson’s ratio (see Equation 1.3.7 for biaxial loading). 1.4.3.2 Shear Strain — When an element of uniform thickness is subjected to pure shear, each side of the element will be displaced in opposite directions. Shear strain is computed by dividing this total displacement by the right angle distance separating the two sides. 1.4.3.3 Strain Rate — Strain rate is a function of loading rate. Test results are dependent upon strain rate, and the ASTM testing procedures specify appropriate strain rates. Design properties in this Handbook were developed from test data obtained from coupons tested at the stated strain rate or up to a value of 0.01 in./in./min, the standard maximum static rate for tensile testing materials per specification ASTM E 8. 1.4.3.4 Elongation and Reduction of Area — Elongation and reduction of area are measured in accordance with specification ASTM E 8. 18
MMPDS01 31 January 2003
1.4.4 TENSILE PROPERTIES — When a metallic specimen is tested in tension using standard procedures of ASTM E 8, it is customary to plot results as a “stressstrain diagram.” Typical tensile stressstrain diagrams are characterized in Figure 1.4.4. Such diagrams, drawn to scale, are provided in appropriate chapters of this Handbook. The general format of such diagrams is to provide a strain scale nondimensionally (in./in.) and a stress scale in 1000 lb/in. (ksi). Properties required for design and structural analysis are discussed in Sections 1.4.4.1 to 1.4.4.6. 1.4.4.1 Modulus of Elasticity (E) — Referring to Figure 1.4.4, it is noted that the initial part of stressstrain curves are straight lines. This indicates a constant ratio between stress and strain. Numerical values of such ratios are defined as the modulus of elasticity, and denoted by the letter E. This value applies up to the proportional limit stress at which point the initial slope of the stressstrain curve then decreases. Modulus of elasticity has the same units as stress. See Equation 1.3.4 (b). Other moduli of design importance are tangent modulus, Et, and secant modulus, Es. Both of these moduli are functions of strain. Tangent modulus is the instantaneous slope of the stressstrain curve at any selected value of strain. Secant modulus is defined as the ratio of total stress to total strain at any selected value of strain. Both of these moduli are used in structural element designs. Except for materials such as those described with discontinuous behaviors, such as the upper stressstrain curve in Figure 1.4.4, tangent modulus is the lowest value of modulus at any state of strain beyond the proportional limit. Similarly, secant modulus is the highest value of modulus beyond the proportional limit. Clad aluminum alloys may have two separate modulus of elasticity values, as indicated in the typical stressstrain curve shown in Figure 1.4.4. The initial slope, or primary modulus, denotes a response of both the lowstrength cladding and higherstrength core elastic behaviors. This value applies only up to the proportional limit of the cladding. For example, the primary modulus of 2024T3 clad sheet applies only up to about 6 ksi. Similarly, the primary modulus of 7075T6 clad sheet applies only up to approximately 12 ksi. A typical use of primary moduli is for low amplitude, high frequency fatigue. Primary moduli are not applicable at higher stress levels. Above the proportional limits of cladding materials, a short transition range occurs while the cladding is developing plastic behavior. The material then exhibits a secondary elastic modulus up to the proportional limit of the core material. This secondary modulus is the slope of the second straight line portion of the stressstrain curve. In some cases, the cladding is so little different from the core material that a single elastic modulus value is used. 1.4.4.2 Tensile Proportional Limit Stress (Ftp ) — The tensile proportional limit is the maximum stress for which strain remains proportional to stress. Since it is practically impossible to determine precisely this point on a stressstrain curve, it is customary to assign a small value of plastic strain to identify the corresponding stress as the proportional limit. In this Handbook, the tension and compression proportional limit stress corresponds to a plastic strain of 0.0001 in./in. 1.4.4.3 Tensile Yield Stress (TYS or Fty ) — Stressstrain diagrams for some ferrous alloys exhibit a sharp break at a stress below the tensile ultimate strength. At this critical stress, the material elongates considerably with no apparent change in stress. See the upper stressstrain curve in Figure 1.4.4. The stress at which this occurs is referred to as the yield point. Most nonferrous metallic alloys and most high strength steels do not exhibit this sharp break, but yield in a monotonic manner. This condition is also illustrated in Figure 1.4.4. Permanent deformation may be detrimental, and the industry adopted 0.002 in./in. plastic strain as an arbitrary limit that is considered acceptable by all regulatory agencies. For tension and compression, the corresponding stress at this offset strain is defined as the yield stress (see Figure 1.4.4). This value of plastic axial strain is 0.002 in./in. and the corresponding stress is defined as the yield stress. For practical purposes, yield stress can be determined from a stressstrain diagram by 19
MMPDS01 31 January 2003
extending a line parallel to the elastic modulus line and offset from the origin by an amount of 0.002 in./in. strain. The yield stress is determined as the intersection of the offset line with the stressstrain curve.
Figure 1.4.4. Typical tensile stressstrain diagrams.
110
MMPDS01 31 January 2003
1.4.4.4 Tensile Ultimate Stress (TUS or Fty ) — Figure 1.4.4 shows how the tensile ultimate stress is determined from a stressstrain diagram. It is simply the maximum stress attained. It should be noted that all stresses are based on the original crosssectional dimensions of a test specimen, without regard to the lateral contraction due to Poisson’s ratio effects. That is, all strains used herein are termed engineering strains as opposed to true strains which take into account actual cross sectional dimensions. Ultimate tensile stress is commonly used as a criterion of the strength of the material for structural design, but it should be recognized that other strength properties may often be more important. 1.4.4.5 Elongation (e) — An additional property that is determined from tensile tests is elongation. This is a measure of ductility. Elongation, also stated as total elongation, is defined as the permanent increase in gage length, measured after fracture of a tensile specimen. It is commonly expressed as a percentage of the original gage length. Elongation is usually measured over a gage length of 2 inches for rectangular tensile test specimens and in 4D (inches) for round test specimens. Welded test specimens are exceptions. Refer to the applicable material specification for applicable specified gage lengths. Although elongation is widely used as an indicator of ductility, this property can be significantly affected by testing variables, such as thickness, strain rate, and gage length of test specimens. See Section 1.4.1.1 for data basis. 1.4.4.6 Reduction of Area (RA) — Another property determined from tensile tests is reduction of area, which is also a measure of ductility. Reduction of area is the difference, expressed as a percentage of the original cross sectional area, between the original cross section and the minimum cross sectional area adjacent to the fracture zone of a tested specimen. This property is less affected by testing variables than elongation, but is more difficult to compute on thin section test specimens. See Section 1.4.1.1 for data basis. 1.4.5 COMPRESSIVE PROPERTIES — Results of compression tests completed in accordance with ASTM E 9 are plotted as stressstrain curves similar to those shown for tension in Figure 1.4.4. Preceding remarks concerning tensile properties of materials, except for ultimate stress and elongation, also apply to compressive properties. Moduli are slightly greater in compression for most of the commonly used structural metallic alloys. Special considerations concerning the ultimate compressive stress are described in the following section. An evaluation of techniques for obtaining compressive strength properties of thin sheet materials is outlined in Reference 1.4.5. 1.4.5.1 Compressive Ultimate Stress (Fcu ) – Since the actual failure mode for the highest tension and compression stress is shear, the maximum compression stress is limited to Ftu. The driver for all the analysis of all structure loaded in compression is the slope of the compression stress strain curve, the tangent modulus. 1.4.5.2 Compressive Yield Stress (CYS or Fcy ) — Compressive yield stress is measured in a manner identical to that done for tensile yield strength. It is defined as the stress corresponding to 0.002 in./in. plastic strain. 1.4.6 SHEAR PROPERTIES — Results of torsion tests on round tubes or round solid sections are plotted as torsion stressstrain diagrams. The shear modulus of elasticity is considered a basic shear property. Other properties, such as the proportional limit stress and shear ultimate stress, cannot be treated as basic shear properties because of “form factor” effects. The theoretical ratio between shear and tensile stress for homogeneous, isotropic materials is 0.577. Reference 1.4.6 contains additional information on this subject.
111
MMPDS01 31 January 2003
1.4.6.1 Modulus of Rigidity (G) — This property is the initial slope of the shear stressstrain curve. It is also referred to as the modulus of elasticity in shear. The relation between this property and the modulus of elasticity in tension is expressed for homogeneous isotropic materials by the following equation: G=
E 2(1 + µ )
[1.4.6.1]
1.4.6.2 Proportional Limit Stress in Shear (Fsp ) — This property is of particular interest in connection with formulas which are based on considerations of linear elasticity, as it represents the limiting value of shear stress for which such formulas are applicable. This property cannot be determined directly from torsion tests. 1.4.6.3 Yield and Ultimate Stresses in Shear (SYS or Fsy ) and (SUS or Fsu ) — These properties, as usually obtained from ASTM test procedures tests, are not strictly basic properties, as they will depend on the shape of the test specimen. In such cases, they should be treated as moduli and should not be combined with the same properties obtained from other specimen configuration tests. Design values reported for shear ultimate stress (Fsu) in room temperature property tables for aluminum and magnesium thin sheet alloys are based on “punch” shear type tests except when noted. Heavy section test data are based on “pin” tests. Thin aluminum products may be tested to ASTM B 831, which is a slotted shear test. Thicker aluminums use ASTM B 769, otherwise known as the Amsler shear test. These two tests only provide ultimate strength. Shear data for other alloys are obtained from pin tests, except where product thicknesses are insufficient. These tests are used for other alloys; however, the standards don’t specifically cover materials other than aluminum 1.4.7 BEARING PROPERTIES — Bearing stress limits are of value in the design of mechanically fastened joints and lugs. Only yield and ultimate stresses are obtained from bearing tests. Bearing stress is computed from test data by dividing the load applied to the pin, which bears against the edge of the hole, by the bearing area. Bearing area is the product of the pin diameter and the sheet or plate thickness. A bearing test requires the use of special cleaning procedures as specified in ASTM E 238. Results are identified as “drypin” values. The same tests performed without application of ASTM E 238 cleaning procedures are referred to as “wet pin” tests. Results from such tests can show bearing stresses at least 10 percent lower than those obtained from “dry pin” tests. See Reference 1.4.7 for additional information. Additionally, ASTM E 238 requires the use of hardened pins that have diameters within 0.001 of the hole diameter. As the clearance increases to 0.001 and greater, the bearing yield and failure stress tends to decrease. In the definition of bearing values, t is sheet or plate thickness, D is the pin diameter, and e is the edge distance measured from the center of the hole to the adjacent edge of the material being tested in the direction of applied load. 1.4.7.1 Bearing Yield and Ultimate Stresses (BYS or Fbry ) and (BUS or Fbru ) — BUS is the maximum stress withstood by a bearing specimen. BYS is computed from a bearing stressdeformation curve by drawing a line parallel to the initial slope at an offset of 0.02 times the pin diameter. Tabulated design properties for bearing yield stress (Fbry) and bearing ultimate stress (Fbru) are provided throughout the Handbook for edge margins of e/D = 1.5 and 2.0. Bearing values for e/D of 1.5 are not intended for designs of e/D < 1.5. Bearing values for e/D < 1.5 must be substantiated by adequate 112
MMPDS01 31 January 2003
tests, subject to the approval of the procuring or certificating regulatory agency. For edge margins between 1.5 and 2.0, linear interpolation of properties may be used. Bearing design properties are applicable to t/D ratios from 0.25 to 0.50. Bearing design values for conditions of t/D < 0.25 or t/D > 0.50 must be substantiated by tests. The percentage curves showing temperature effects on bearing stress may be used with both e/D properties of 1.5 and 2.0. Due to differences in results obtained between drypin and wetpin tests, designers are encouraged to consider the use of a reduction factor with published bearing stresses for use in design. 1.4.8 TEMPERATURE EFFECTS — Temperature effects require additional considerations for static, fatigue and fracture toughness properties. In addition, this subject introduces concerns for timedependent creep properties. 1.4.8.1 Low Temperature — Temperatures below room temperature generally cause an increase in strength properties of metallic alloys. Ductility, fracture toughness, and elongation usually decrease. For specific information, see the applicable chapter and references noted therein. 1.4.8.2 Elevated Temperature — Temperatures above room temperature usually cause a decrease in the strength properties of metallic alloys. This decrease is dependent on many factors, such as temperature and the time of exposure which may degrade the heat treatment condition, or cause a metallurgical change. Ductility may increase or decrease with increasing temperature depending on the same variables. Because of this dependence of strength and ductility at elevated temperatures on many variables, it is emphasized that the elevated temperature properties obtained from this Handbook be applied for only those conditions of exposure stated herein. The effect of temperature on static mechanical properties is shown by a series of graphs of property (as percentages of the room temperature allowable property) versus temperature. Data used to construct these graphs were obtained from tests conducted over a limited range of strain rates. Caution should be exercised in using these static property curves at very high temperatures, particularly if the strain rate intended in design is much less than that stated with the graphs. The reason for this concern is that at very low strain rates or under sustained loads, plastic deformation or creep deformation may occur to the detriment of the intended structural use. 1.4.8.2.1 Creep and StressRupture Properties — Creep is defined as a timedependent deformation of a material while under an applied load. It is usually regarded as an elevated temperature phenomenon, although some materials creep at room temperature. If permitted to continue indefinitely, creep terminates in rupture. Since creep in service is usually typified by complex conditions of loading and temperature, the number of possible stresstemperaturetime profiles is infinite. For economic reasons, creep data for general design use are usually obtained under conditions of constant uniaxial loading and constant temperature in accordance with Reference 1.4.8.2.1(a). Creep data are sometimes obtained under conditions of cyclic uniaxial loading and constant temperature, or constant uniaxial loading and variable temperatures. Section 9.3.6 provides a limited amount of creep data analysis procedures. It is recognized that, when significant creep appears likely to occur, it may be necessary to test under simulated service conditions because of difficulties posed in attempting to extrapolate from simple to complex stresstemperaturetime conditions. Creep damage is cumulative similar to plastic strain resulting from multiple static loadings. This damage may involve significant effects on the temper of heat treated materials, including annealing, and
113
MMPDS01 31 January 2003
the initiation and growth of cracks or subsurface voids within a material. Such effects are often recognized as reductions in short time strength properties or ductility, or both. 1.4.8.2.2 CreepRupture Curve — Results of tests conducted under constant loading and constant temperature are usually plotted as strain versus time up to rupture. A typical plot of this nature is shown in Figure 1.4.8.2.2. Strain includes both the instantaneous deformation due to load application and the plastic strain due to creep. Other definitions and terminology are provided in Section 9.3.6.2.
Figure 1.4.8.2.2. Typical creeprupture curve.
1.4.8.2.3 Creep or StressRupture Presentations — Results of creep or stressrupture tests conducted over a range of stresses and temperatures are presented as curves of stress versus the logarithm of time to rupture. Each curve represents an average, bestfit description of measured behavior. Modification of such curves into design use are the responsibility of the design community since material applications and regulatory requirements may differ. Refer to Section 9.3.6 for data reduction and presentation methods and References 1.4.8.2.1(b) and (c). 1.4.9 FATIGUE PROPERTIES — Repeated loads are one of the major considerations for design of both commercial and military aircraft structures. Static loading, preceded by cyclic loads of lesser magnitudes, may result in mechanical behaviors (Ftu , Fty , etc.) lower than those published in room temperature allowables tables. Such reductions are functions of the material and cyclic loading conditions. A fatigue allowables development philosophy is not presented in this Handbook. However, basic laboratory test data are useful for materials selection. Such data are therefore provided in the appropriate materials sections. In the past, common methods of obtaining and reporting fatigue data included results obtained from axial loading tests, plate bending tests, rotating bending tests, and torsion tests. Rotating bending tests apply completely reversed (tensioncompression) stresses to round cross section specimens. Tests of this type are now seldom conducted for aerospace use and have therefore been dropped from importance in this Handbook. For similar reasons, flexural fatigue data also have been dropped. No 114
MMPDS01 31 January 2003
significant amount of torsional fatigue data have ever been made available. Axial loading tests, the only type retained in this Handbook, consist of completely reversed loading conditions (mean stress equals zero) and those in which the mean stress was varied to create different stress (or strain) ratios (R = minimum stress or strain divided by maximum stress or strain). Refer to Reference 1.4.9(a) for load control fatigue testing guidelines and Reference 1.4.9(b) for strain control fatigue testing guidelines. 1.4.9.1 Terminology — A number of symbols and definitions are commonly used to describe fatigue test conditions, test results and data analysis techniques. The most important of these are described in Section 9.3.4.2. 1.4.9.2 Graphical Display of Fatigue Data — Results of axial fatigue tests are reported on SN and ε  N diagrams. Figure 1.4.9.2(a) shows a family of axial load SN curves. Data for each curve represents a separate Rvalue.
SN and ε  N diagrams are shown in this Handbook with the raw test data plotted for each stress or strain ratio or, in some cases, for a single value of mean stress. A bestfit curve is drawn through the data at each condition. Rationale used to develop bestfit curves and the characterization of all such curves in a single diagram is explained in Section 9.3.4. For load control test data, individual curves are usually based on an equivalent stress that consolidates data for all stress ratios into a single curve. Refer to Figure 1.4.9.2(b). For strain control test data, an equivalent strain consolidation method is used.
Elevated temperature fatigue test data are treated in the same manner as room temperature data, as long as creep is not a significant factor and room temperature analysis methods can be applied. In the limited number of cases where creep strain data have been recorded as a part of an elevated temperature fatigue test series, SN (or ε  N) plots are constructed for specific creep strain levels. This is provided in addition to the customary plot of maximum stress (or strain) versus cycles to failure. The above information may not apply directly to the design of structures for several reasons. First, Handbook information may not take into account specific stress concentrations unique to any given structural design. Design considerations usually include stress concentrations caused by reentrant corners, notches, holes, joints, rough surfaces, structural damage, and other conditions. Localized high stresses induced during the fabrication of some parts have a much greater influence on fatigue properties than on static properties. These factors significantly reduce fatigue life below that which is predictable by estimating smooth specimen fatigue performance with estimated stresses due to fabrication. Fabricated parts have been found to fail at less than 50,000 cycles of loading when the nominal stress was far below that which could be repeated many millions of times using a smoothmachined test specimen. Notched fatigue specimen test data are shown in various Handbook figures to provide an understanding of deleterious effects relative to results for smooth specimens. All of the mean fatigue curves published in this Handbook, including both the notched fatigue and smooth specimen fatigue curves, require modification into allowables for design use. Such factors may impose a penalty on cyclic life or upon stress. This is a responsibility for the design community. Specific reductions vary between users of such information, and depending on the criticality of application, sources of uncertainty in the analysis, and requirements of the certificating activity. References 1.4.9.2(a) and (b) contain more specific information on fatigue testing procedures, organization of test results, influences of various factors, and design considerations.
115
MMPDS01 31 January 2003 . .
80 M a te ria l= A , K t= B , N o tch T yp e = C , M e an S tre ss o r S tre ss R a tio =
x
70
x
Maximum Stress, ksi
x
60
x
x + ++
++
x
x+
+ + + ++
50
+
+ +
x →
x x
40
x x
x
+ +
++ +
x→ x→ +→ +→ +→ +→ + → + →
x
+ +
+ +
+++
+
+
30
→ →
→ → → →
20 10
L e ve l 1 L e ve l 2 L e ve l 3 L e ve l 4 R unout
N o te :
S tre sses are ba se d o n n e t se ctio n .
0 10 3
10 4
10 5
10 6
10 7
10 8
F a tig u e L ife , C ycle s Figure 1.4.9.2(a). Best fit S/N curve diagram for a material at various stress ratios.
. .
100 Material=A, Kt=B, Notch Type=C, Mean Stress or Stress Ratio =
90 x
Equivalent Stress, Seq
80
+
70
+ ++
x ++
x
x+
Level Level Level Level
1 2 3 4
+
60
x
+ ++ + +
x
+
x
50
x x + x
40
+
+
x x++ x + +
x
+ +
+++
30
+
+
20 10 0 10 3
Note: Stresses are based on net section.
10 4
10 5
10 6
10 7
10 8
Fatigue Life, Cycles Figure 1.4.9.2(b). Consolidated fatigue data for a material using the equivalent stress parameter.
116
MMPDS01 31 January 2003
1.4.10 METALLURGICAL INSTABILITY — In addition to the retention of strength and ductility, a structural material must also retain surface and internal stability. Surface stability refers to the resistance of the material to oxidizing or corrosive environments. Lack of internal stability is generally manifested (in some ferrous and several other alloys) by carbide precipitation, spheroidization, sigmaphase formation, temper embrittlement, and internal or structural transformation, depending upon the specific conditions of exposure. Environmental conditions, that influence metallurgical stability include heat, level of stress, oxidizing or corrosive media, and nuclear radiation. The effect of environment on the material can be observed as either improvement or deterioration of properties, depending upon the specific imposed conditions. For example, prolonged heating may progressively raise the strength of a metallic alloy as measured on smooth tensile or fatigue specimens. However, at the same time, ductility may be reduced to such an extent that notched tensile or fatigue behavior becomes erratic or unpredictable. The metallurgy of each alloy should be considered in making material selections. Under normal temperatures, i.e., between 65EF and 160EF, the stability of most structural metallic alloys is relatively independent of exposure time. However, as temperature is increased, the metallurgical instability becomes increasingly time dependent. The factor of exposure time should be considered in design when applicable. 1.4.11 BIAXIAL PROPERTIES — Discussions up to this point pertained to uniaxial conditions of static, fatigue, and creep loading. Many structural applications involve both biaxial and triaxial loadings. Because of the difficulties of testing under triaxial loading conditions, few data exist. However, considerable biaxial testing has been conducted and the following paragraphs describe how these results are presented in this Handbook. This does not conflict with data analysis methods presented in Chapter 9. Therein, statistical analysis methodology is presented solely for use in analyzing test data to establish allowables. If stress axes are defined as being mutually perpendicular along x, y, and zdirections in a rectangular coordinate system, a biaxial stress is then defined as a condition in which loads are applied in both the x and ydirections. In some special cases, loading may be applied in the zdirection instead of the ydirection. Most of the following discussion will be limited to tensile loadings in the x and ydirections. Stresses and strains in these directions are referred to as principal stresses and principal strains. See Reference 1.4.11. When a specimen is tested under biaxial loading conditions, it is customary to plot the results as a biaxial stressstrain diagram. These diagrams are similar to uniaxial stressstrain diagrams shown in Figure 1.4.4. Usually, only the maximum (algebraically larger) principal stress and strain are shown for each test result. When tests of the same material are conducted at different biaxial stress ratios, the resulting curves may be plotted simultaneously, producing a family of biaxial stressstrain curves as shown in Figure 1.4.11 for an isotropic material. For anisotropic materials, biaxial stressstrain curves also require distinction by grain direction. The reference direction for a biaxial stress ratio, i.e., the direction corresponding to B=0, should be clearly indicated with each result. The reference direction is always considered as the longitudinal (rolling) direction for flat products and the hoop (circumferential) direction for shells of revolution, e.g., tubes, cones, etc. The letter B denotes the ratio of applied stresses in the two loading directions. For example, biaxility ratios of 2 and 0.5 shown in Figure 1.4.11 indicate results representing both biaxial stress ratios of 2 or 0.5, since this is a hypothetical example for an isotropic material, e.g., crossrolled sheet. In a similar manner, the curve labeled B=1 indicates a biaxial stressstrain result for equally applied 117
MMPDS01 31 January 2003
stresses in both directions. The curve labeled B = 4, 0 indicates the biaxial stressstrain behavior when loading is applied in only one direction, e.g., uniaxial behavior. Biaxial property data presented in the Handbook are to be considered as basic material properties obtained from carefully prepared specimens.
Figure 1.4.11. Typical biaxial stressstrain diagrams for isotropic materials.
1.4.11.1 Biaxial Modulus of Elasticity — Referring to Figure 1.4.11, it is noted that the original portion of each stressstrain curve is essentially a straight line. In uniaxial tension or compression, the slope of this line is defined as the modulus of elasticity. Under biaxial loading conditions, the initial slope of such curves is defined as the biaxial modulus. It is a function of biaxial stress ratio and Poisson’s ratio. See Equation 1.3.7.4. 1.4.11.2 Biaxial Yield Stress — Biaxial yield stress is defined as the maximum principal stress corresponding to 0.002 in./in. plastic strain in the same direction, as determined from a test curve. In the design of aerospace structures, biaxial stress ratios other than those normally used in biaxial testing are frequently encountered. Information can be combined into a single diagram to enable interpolations at intermediate biaxial stress ratios, as shown in Figure 1.4.11.2. An envelope is constructed through test results for each tested condition of biaxial stress ratios. In this case, a typical biaxial yield stress envelope is identified. In the preparation of such envelopes, data are first reduced to nondimensional form (percent of uniaxial tensile yield stress in the specified reference direction), then a bestfit curve is fitted through the nondimensionalized data. Biaxial yield strength allowables are then obtained by multiplying the uniaxial Fty (or Fcy) allowable by the applicable coordinate of the biaxial stress ratio curve. To avoid possible confusion, the reference direction used for the uniaxial yield strength is indicated on each figure.
118
MMPDS01 31 January 2003
Figure 1.4.11.2. Typical biaxial yield stress envelope.
1.4.11.3 Biaxial Ultimate Stress — Biaxial ultimate stress is defined as the highest nominal principal stress attained in specimens of a given configuration, tested at a given biaxial stress ratio. This property is highly dependent upon geometric configuration of the test parts. Therefore, such data should be limited in use to the same design configurations. The method of presenting biaxial ultimate strength data is similar to that described in the preceding section for biaxial yield strength. Both biaxial ultimate strength and corresponding uniform elongation data are reported, when available, as a function of biaxial stress ratio test conditions. 1.4.12 FRACTURE TOUGHNESS — The occurrence of flaws in a structural component is an unavoidable circumstance of material processing, fabrication, or service. Flaws may appear as cracks, voids, metallurgical inclusions, weld defects, design discontinuities, or some combination thereof. The fracture toughness of a part containing a flaw is dependent upon flaw size, component geometry, and a material property defined as fracture toughness. The fracture toughness of a material is literally a measure of its resistance to fracture. As with other mechanical properties, fracture toughness is dependent upon alloy type, processing variables, product form, geometry, temperature, loading rate, and other environmental factors. This discussion is limited to brittle fracture, which is characteristic of high strength materials under conditions of loading resulting in planestrain through the cross section. Very thin materials are described as being under the condition of planestress. The following descriptions of fracture toughness properties applies to the currently recognized practice of testing specimens under slowly increasing loads. Attendant and interacting conditions of cyclic loading, prolonged static loadings, environmental influences other than temperature, and high strain rate loading are not considered.
119
MMPDS01 31 January 2003
1.4.12.1 Brittle Fracture — For materials that have little capacity for plastic flow, or for flaw and structural configurations, which induce triaxial tension stress states adjacent to the flaw, component behavior is essentially elastic until the fracture stress is reached. Then, a crack propagates from the flaw suddenly and completely through the component. A convenient illustration of brittle fracture is a typical loadcompliance record of a brittle structural component containing a flaw, as illustrated in Figure 1.4.12.1. Since little or no plastic effects are noted, this mode is termed brittle fracture. This mode of fracture is characteristic of the very highstrength metallic materials under planestrain conditions.
Figure 1.4.12.1. Typical loaddeformation record of a structural component containing a flaw subject to brittle fracture.
1.4.12.2 Brittle Fracture Analysis — The application of linear elastic fracture mechanics has led to the stress intensity concept to relate flaw size, component geometry, and fracture toughness. In its very general form, the stress intensity factor, K, can be expressed as
K = f a Y, ksi ⋅ in.1/ 2
[1.4.12.2]
where f = stress applied to the gross section, ksi a = measure of flaw size, inches Y = factor relating component geometry and flaw size, nondimensional. See Reference 1.4.12.2(a) for values. For every structural material, which exhibits brittle fracture (by nature of low ductility or planestrain stress conditions), there is a lower limiting value of K termed the planestrain fracture toughness, KIc.
120
MMPDS01 31 January 2003
The specific application of this relationship is dependent on flaw type, structural configuration and type of loading, and a variety of these parameters can interact in a real structure. Flaws may occur through the thickness, may be imbedded as voids or metallurgical inclusions, or may be partialthrough (surface) cracks. Loadings of concern may be tension and/or flexure. Structural components may vary in section size and may be reinforced in some manner. The ASTM Committee E 8 on Fatigue and Fracture has developed testing and analytical techniques for many practical situations of flaw occurrence subject to brittle fracture. They are summarized in Reference 1.4.12.2(a). 1.4.12.3 Critical PlaneStrain Fracture Toughness — A tabulation of fracture toughness data is printed in the general discussion prefacing most alloy chapters in this Handbook. These critical planestrain fracture toughness values have been determined in accordance with recommended ASTM testing practices. This information is provided for information purposes only due to limitations in available data quantities and product form coverages. The statistical reliability of these properties is not known. Listed properties generally represent the average value of a series of test results. Fracture toughness of a material commonly varies with grain direction. When identifying either test results or a general critical plane strain fracture toughness average value, it is customary to specify specimen and crack orientations by an ordered pair of grain direction symbols per ASTM E399. [Reference 1.4.12.2(a).] The first digit denotes the grain direction normal to the crack plane. The second digit denotes the grain direction parallel to the fracture plane. For flat sections of various products, e.g., plate, extrusions, forgings, etc., in which the three grain directions are designated (L) longitudinal, (T) transverse, and (S) short transverse, the six principal fracture path directions are: LT, LS, TL, TS, SL and ST. Figure 1.4.12.3(a) identifies these orientations. For cylindrical sections where the direction of principle deformation is parallel to the longitudinal axis of the cylinder, the reference directions are identified as in Figure 1.4.12.3(b), which gives examples for a drawn bar. The same system would be useful for extrusions or forged parts having circular cross section.
Figure 1.4.12.3(a). Typical principal fracture path directions.
Figure 1.4.12.3(b). Typical principal fracture path directions for cylindrical shapes.
1.4.12.3.1 Environmental Effects — Cyclic loading, even well below the fracture threshold stress, may result in the propagation of flaws, leading to fracture. Strain rates in excess of standard static rates may cause variations in fracture toughness properties. There are significant influences of temperature 121
MMPDS01 31 January 2003
on fracture toughness properties. Temperature effects data are limited. These information are included in each alloy section, when available. Under the condition of sustained loading, it has been observed that certain materials exhibit increased flaw propagation tendencies when situated in either aqueous or corrosive environments. When such is known to be the case, appropriate precautionary notes have been included with the standard fracture toughness information. 1.4.12.4 Fracture in PlaneStress and TransitionalStress States — Planestrain conditions do not describe the condition of certain structural configurations which are either relatively thin or exhibit appreciable ductility. In these cases, the actual stress state may approach the opposite extreme, planestress, or, more generally, some intermediate or transitionalstress state. The behavior of flaws and cracks under these conditions is different from those of planestrain. Specifically, under these conditions, significant plastic zones can develop ahead of the crack or flaw tip, and stable extension of the discontinuity occurs as a slow tearing process. This behavior is illustrated in a compliance record by a significant nonlinearity prior to fracture as shown in Figure 1.4.12.4. This nonlinearity results from the alleviation of stress at the crack tip by causing plastic deformation.
Figure 1.4.12.4. Typical loaddeformation record for nonplane strain fracture.
1.4.12.4.1 Analysis of PlaneStress and TransitionalStress State Fracture — The basic concepts of linear elastic fracture mechanics as used in planestrain fracture analysis also applies to these conditions. The stress intensity factor concept, as expressed in general form by Equation 1.4.12.2, is used to relate load or stress, flaw size, component geometry, and fracture toughness. However, interpretation of the critical flaw dimension and corresponding stress has two possibilities. This is illustrated in Figure 1.4.12.4.1. One possibility is the onset of nonlinear displacement with increasing load. The other possibility identifies the fracture condition, usually very close to the
122
MMPDS01 31 January 2003
Figure 1.4.12.4.1. Crack growth curve.
maximum load. Generally, these two conditions are separated in applied stress and exhibit large differences in flaw dimensions due to stable tearing. When a compliance record is transformed into a crack growth curve, the difference between the two possible Kfactor designations becomes more apparent. In most practical cases, the definition of nonlinear crack length with increasing load is difficult to assess. As a result, an alternate characterization of this behavior is provided by defining an artificial or “apparent” stress intensity factor.
Kapp = f ao Y
[1.4.12.4.1]
The apparent fracture toughness is computed as a function of the maximum stress and initial flaw size. This datum coordinate corresponds to point A in Figure 1.4.12.4.1. This conservative stress intensity factor is a first approximation to the actual property associated with the point of fracture. 1.4.12.5 Apparent Fracture Toughness Values for PlaneStress and TransitionalStress States — When available, each alloy chapter contains graphical formats of stress versus flaw size. This is provided for each temper, product form, grain direction, thickness, and specimen configuration. Data points shown in these graphs represent the initial flaw size and maximum stress achieved. These data have been screened to assure that an elastic instability existed at fracture, consistent with specimen type. The average Kapp curve, as defined in the following subsections, is shown for each set of data. 1.4.12.5.1 MiddleTension Panels — The calculation of apparent fracture toughness for middletension panels is given by the following equation.
K app = fc ( π a o ⋅ sec π a o / W)
1/ 2
[1.4.12.5.1(a)]
Data used to compute Kapp values have been screened to ensure that the net section stress at failure did not exceed 80 percent of the tensile yield strength; that is, they satisfied the criterion:
fc ≤ 0.8(TYS) / (1 − 2a / W)
[1.4.12.5.1(b)]
This criterion assures that the fracture was an elastic instability and that plastic effects are negligible. 123
MMPDS01 31 January 2003
The average Kapp parametric curve is presented on each figure as a solid line with multiple extensions where width effects are displayed in the data. As added information, where data are available, the propensity for slow stable tearing prior to fracture is indicated by a crack extension ratio, ∆2a/2ao. The coefficient (2) indicates the total crack length; the halfcrack length is designated by the letter “a.” In some cases, where data exist covering a wide range of thicknesses, graphs of Kapp versus thickness are presented. 1.4.13 FATIGUE CRACK GROWTH — Crack growth deals with material behavior between crack initiation and crack instability. In small size specimens, crack initiation and specimen failure may be nearly synonymous. However, in larger structural components, the existence of a crack does not necessarily imply imminent failure. Significant structural life exists during cyclic loading and crack growth. 1.4.13.1 Fatigue Crack Growth — Fatigue crack growth is manifested as the growth or extension of a crack under cyclic loading. This process is primarily controlled by the maximum load or stress ratio. Additional factors include environment, loading frequency, temperature, and grain direction. Certain factors, such as environment and loading frequency, have interactive effects. Environment is important from a potential corrosion viewpoint. Time at stress is another important factor. Standard testing procedures are documented in Reference 1.4.13.1. Fatigue crack growth data presented herein are based on constant amplitude tests. Crack growth behaviors based on spectrum loading cycles are beyond the scope of this Handbook. Constant amplitude data consist of crack length measurements at corresponding loading cycles. Such data are presented as crack growth curves as shown in Figure 1.4.13.1(a). Since the crack growth curve is dependent on initial crack length and the loading conditions, the above format is not the most efficient form to present information. The instantaneous slope, ∆a/∆N, corresponding to a prescribed number of loading cycles, provides a more fundamental characterization of this behavior. In general, fatigue crack growth rate behavior is evaluated as a function of the applied stress intensity factor range, ∆K, as shown in Figure 1.4.13.1(b). 1.4.13.2 Fatigue Crack Growth Analysis — It is known that fatiguecrackgrowth behavior under constantamplitude cyclic conditions is influenced by maximum cyclic stress, Smax, and some measure of cyclic stress range, ∆S (such as stress ratio, R, or minimum cyclic stress, Smin), the instantaneous crack size, a, and other factors such as environment, frequency, and temperature. Thus, fatiguecrackgrowth rate behavior can be characterized, in general form, by the relation da/dN . ∆a/∆N = g(Smax, ∆S or R or Smin, a, ...).
[1.4.13.3(a)]
By applying concepts of linear elastic fracture mechanics, the stress and crack size parameters can be combined into the stressintensity factor parameter, K, such that Equation 1.4.13.3(a) may be simplified to [1.4.13.3(b)] da/dN . ∆a/∆N = g(Kmax, ∆K, ...) where Kmax ∆K ∆K
= = =
the maximum cyclic stressintensity factor (1R)Kmax, the range of the cyclic stressintensity factor, for R $ 0 Kmax, for R # 0.
124
MMPDS01 31 January 2003
Figure 1.4.13.1(a). Fatigue crackgrowth curve.
Figure 1.4.13.1(b). Fatigue crackgrowthrate curve.
125
MMPDS01 31 January 2003
At present, in the Handbook, the independent variable is considered to be simply ∆K and the data are considered to be parametric on the stress ratio, R, such that Equation 1.4.13.3(b) becomes da/dN . ∆a/∆N = g(∆K, R).
[1.4.13.3(c)]
1.4.13.3 Fatigue Crack Growth Data Presentation — Fatigue crack growth rate data for constant amplitude cyclic loading conditions are presented as logarithmic plots of da/dN versus ∆K. Such information, such as that illustrated in Figure 1.4.13.3, are arranged by material alloy and heat treatment condition. Each curve represents a specific stress ratio, R, environment, and cyclic loading frequency. Specific details regarding test procedures and data interpolations are presented in Chapter 9.
126
MMPDS01 31 January 2003
Figure 1.4.13.3. Sample display of fatigue crack growth rate data.
127
MMPDS01 31 January 2003
1.5
TYPES OF FAILURES
1.5.1 GENERAL — In the following discussion, failure will usually indicate fracture of a member or the condition of a member when it has attained maximum load. 1.5.2 MATERIAL FAILURES — Fracture can occur in either ductile or brittle fashions in the same material depending on the state of stress, rate of loading, and environment. The ductility of a material has a significant effect on the ability of a part to withstand loading and delay fracture. Although not a specific design property for ductile materials, some ductility data are provided in the Handbook to assist in material selections. The following paragraphs discuss the relationship between failure and the applied or induced stresses. 1.5.2.1 Direct Tension or Compression — This type of failure is associated with ultimate tensile or compressive stress of the material. For compression, it can only apply to members having large cross sectional dimensions relative to their lengths. See Section 1.4.5.1. 1.5.2.2 Shear — Pure shear failures are usually obtained when the shear load is transmitted over a very short length of a member. This condition is approached in the case of rivets and bolts. In cases where ultimate shear stress is relatively low, a pure shear failure can result. But, generally members subjected to shear loads fail under the action of the resulting normal stress, usually the compressive stress. See Equation 1.3.3.3. Failure of tubes in torsion are not caused by exceeding the shear ultimate stress, but by exceeding a normal compressive stress which causes the tube to buckle. It is customary to determine stresses for members subjected to shear in the form of shear stresses although they are actually indirect measures of the stresses actually causing failure. 1.5.2.3 Bearing — Failure of a material in bearing can consist of crushing, splitting, tearing, or progressive rapid yielding in the direction of load application. Failure of this type depends on the relative size and shape of the two connecting parts. The maximum bearing stress may not be applicable to cases in which one of the connecting members is relatively thin. 1.5.2.4 Bending — For sections not subject to geometric instability, a bending failure can be classed as either a tensile or compressive failure. Reference 1.5.2.4 provides methodology by which actual bending stresses above the material proportional limit can be used to establish maximum stress conditions. Actual bending stresses are related to the bending modulus of rupture. The bending modulus of rupture (fb) is determined by Equation 1.3.2.3. When the computed bending modulus of rupture is found to be lower than the proportional limit strength, it represents an actual stress. Otherwise, it represents an apparent stress, and is not considered as an actual material strength. This is important when considering complex stress states, such as combined bending and compression or tension. 1.5.2.5 Failure Due to Stress Concentrations — Static stress properties represent pristine materials without notches, holes, or other stress concentrations. Such simplistic structural design is not always possible. Consideration should be given to the effect of stress concentrations. When available, references are cited for specific data in various chapters of the Handbook. 1.5.2.6 Failure from Combined Stresses — Under combined stress conditions, where failure is not due to buckling or instability, it is necessary to refer to some theory of failure. The “maximum shear” theory is widely accepted as a working basis in the case of isotropic ductile materials. It should be noted that this theory defines failure as the first yielding of a material. Any extension of this theory to cover conditions of final rupture must be based on evidence supported by the user. The failure 128
MMPDS01 31 January 2003
of brittle materials under combined stresses is generally treated by the “maximum stress” theory. Section 1.4.11 contains a more complete discussion of biaxial behavior. References 1.5.2.6(a) through (c) offer additional information. 1.5.3 INSTABILITY FAILURES — Practically all structural members, such as beams and columns, particularly those made from thin material, are subject to failure due to instability. In general, instability can be classed as (1) primary or (2) local. For example, the failure of a tube loaded in compression can occur either through lateral deflection of the tube acting as a column (primary instability) or by collapse of the tube walls at stresses lower than those required to produce a general column failure. Similarly, an Ibeam or other formed shape can fail by a general sidewise deflection of the compression flange, by local wrinkling of thin outstanding flanges, or by torsional instability. It is necessary to consider all types of potential failures unless it is apparent that the critical load for one type is definitely the controlling condition. Instability failures can occur in either the elastic range below the proportional limit or in the plastic range. These two conditions are distinguished by referring to either “elastic instability” or “plastic instability” failures. Neither type of failure is associated with a material’s ultimate strength, but largely depends upon geometry. A method for determining the local stability of aluminum alloy column sections is provided in Reference 1.7.1(b). Documents cited therein are the same as those listed in References 3.20.2.2(a) through (e). 1.5.3.1 Instability Failures Under Compression — Failures of this type are discussed in Section 1.6 (Columns). 1.5.3.2 Instability Failures Under Bending — Round tubes when subjected to bending are subject to plastic instability failures. In such cases, the failure criterion is the modulus of rupture. Equation 1.3.2.3, which was derived from theory and confirmed empirically with test data, is applicable. Elastic instability failures of thin walled tubes having high D/t ratios are treated in later sections. 1.5.3.3 Instability Failures Under Torsion — The remarks given in the preceding section apply in a similar manner to round tubes under torsional loading. In such cases, the modulus of rupture in torsion is derived through the use of Equation 1.3.2.6. See Reference 1.5.3.3. 1.5.3.4 Failure Under Combined Loadings — For combined loading conditions in which failure is caused by buckling or instability, no theory exists for general application. Due to the various design philosophies and analytical techniques used throughout the aerospace industry, methods for computing margin of safety are not within the scope of this Handbook.
129
MMPDS01 31 January 2003
1.6
COLUMNS
1.6.1 GENERAL — A theoretical treatment of columns can be found in standard texts on the strength of materials. Some of the problems which are not well defined by theory are discussed in this section. Actual strengths of columns of various materials are provided in subsequent chapters. 1.6.2 PRIMARY INSTABILITY FAILURES — A column can fail through primary instability by bending laterally (stable sections) or by twisting about some axis parallel to its own axis. This latter type of primary failure is particularly common to columns having unsymmetrical open sections. The twisting failure of a closed section column is precluded by its inherently high torsional rigidity. Since the amount of available information is limited, it is advisable to conduct tests on all columns subject to this type of failure. 1.6.2.1 Columns with Stable Sections — The Euler formula for columns which fail by lateral bending is given by Equation 1.3.8.2. A conservative approach in using this equation is to replace the elastic modulus (E) by the tangent modulus (Et) given by Equation 1.3.8.1. Values for the restraint coefficient (c) depend on degrees of ends and lateral fixities. End fixities tend to modify the effective column length as indicated in Equation 1.3.8.1. For a pinended column having no end restraint, c = 1.0 and LN = L. A fixity coefficient of c = 2 corresponds to an effective column length of LN = 0.707 times the total length. The tangent modulus equation takes into account plasticity of a material and is valid when the following conditions are met: (a) (b) (c) (d)
The column adjusts itself to forcible shortening only by bending and not by twisting. No buckling of any portion of the cross section occurs. Loading is applied concentrically along the longitudinal axis of the column. The cross section of the column is constant along its entire length.
MMPDS provides typical stress versus tangent modulus diagrams for many materials, forms, and grain directions. These information are not intended for design purposes. Methodology is contained in Chapter 9 for the development of allowable tangent modulus curves. 1.6.2.2 Column Stress (fco ) — The upper limit of column stress for primary failure is designated as fco. By definition, this term should not exceed the compression ultimate strength, regardless of how the latter term is defined. 1.6.2.3 Other Considerations — Methods of analysis by which column failure stresses can be computed, accounting for fixities, torsional instability, load eccentricity, combined lateral loads, or varying column sections are contained in References 1.6.2.3(a) through (d). 1.6.3 LOCAL INSTABILITY FAILURES — Columns are subject to failure by local collapse of walls at stresses below the primary failure strength. The buckling analysis of a column subject to local instability requires consideration of the shape of the column cross section and can be quite complex. Local buckling, which can combine with primary buckling, leads to an instability failure commonly identified as crippling. 1.6.3.1 Crushing or Crippling Stress (f cc ) — The upper limit of column stress for local failure is defined by either its crushing or crippling stress. The strengths of round tubes have been 130
MMPDS01 31 January 2003
thoroughly investigated and considerable amounts of test results are available throughout literature. Fewer data are available for other cross sectional configurations and testing is suggested to establish specific information, e.g., the curve of transition from local to primary failure. 1.6.4 CORRECTION OF COLUMN TEST RESULTS — In the case of columns having unconventional cross sections which are subject to local instability, it is necessary to establish curves of transition from local to primary failure. In determining these column curves, sufficient tests should be made to cover the following points. 1.6.4.1 Nature of “Short Column Curve” — Test specimens should cover a range of LN/ρ values. When columns are to be attached eccentrically in structural application, tests should be designed to cover such conditions. This is important particularly in the case of open sections, as maximum load carrying capabilities are affected by locations of load and reaction points. 1.6.4.2 Local Failure — When local failure occurs, the crushing or crippling stress can be determined by extending the short column curve to a point corresponding to a zero value for LN/ρ. When a family of columns of the same general cross section is used, it is often possible to determine a relationship between crushing or crippling stress and some geometric factor. Examples are wall thickness, width, diameter, or some combination of these dimensions. Extrapolation of such data to conditions beyond test geometry extremes should be avoided. 1.6.4.3 Reduction of Column Test Results on Aluminum and Magnesium Alloys to Standard Material — The use of correction factors provided in Figures 1.6.4.3(a) through (i) is acceptable to the Air Force, the Navy, the Army, and the Federal Aviation Administration for use in reducing aluminum and magnesium alloys column test data into allowables. (Note that an alternate method is provided in Section 1.6.4.4). In using Figures 1.6.4.3(a) through (i), the correction of column test results to standard material is made by multiplying the stress obtained from testing a column specimen by the factor K. This factor may be considered applicable regardless of the type of failure involved, i.e., column crushing, crippling or twisting. Note that not all the information provided in these figures pertains to allowable stresses, as explained below. The following terms are used in reducing column test results into allowable column stress: Fcy
is the design compression yield stress of the material in question, applicable to the gage, temper and grain direction along the longitudinal axis of a test column.
FcN
is the maximum test column stress achieved in test. Note that a letter (F) is used rather the customary lower case (f). This value can be an individual test result.
FcyN
is the compressive yield strength of the column material. Note that a letter (F) is used rather than the customary lower case (f). This value can be an individual test result using a standard compression test specimen.
Using the ratio of (FcN / FcyN), enter the appropriate diagram along the abscissa and extend a line upwards to the intersection of a curve with a value of (FcyN / Fcy). Linear interpolation between curves is permissible. At this location, extend a horizontal line to the ordinate and read the corresponding Kfactor. This factor is then used as a multiplier on the measured column strength to obtain the allowable. The basis for this allowable is the same as that noted for the compression yield stress allowable obtained from the room temperature allowables table. 131
MMPDS01 31 January 2003
If the above method is not feasible, due to an inability of conducting a standard compression test of the column material, the compression yield stress of the column material may be estimated as follows: Conduct a standard tensile test of the column material and obtain its tensile yield stress. Multiply this value by the ratio of compressiontotensile yield allowables for the standard material. This provides the estimated compression yield stress of the column material. Continue with the analysis as described above using the compression stress of a test column in the same manner. If neither of the above methods are feasible, it may be assumed that the compressive yield stress allowable for the column is 15 percent greater than minimum established allowable longitudinal tensile yield stress for the material in question. 1.6.4.4 Reduction of Column Test Results to Standard MaterialAlternate Method — For materials that are not covered by Figures 1.6.4.4(a) through (i), the following method is acceptable for all materials to the Air Force, the Navy, the Army, and the Federal Aviation Administration. (1)
Obtain the column material compression properties: Fcy, Ec, nc.
(2)
Determine the test material column stress (fcN) from one or more column tests.
(3)
Determine the test material compression yield stress (fcyN) from one or more tests.
(4)
Assume Ec and nc from (1) apply directly to the column material. They should be the same material.
(5)
Assume that geometry of the test column is the same as that intended for design. This means that a critical slenderness ratio value of (LN/ρ) applies to both cases.
(6)
Using the conservative form of the basic column formula provided in Equation 1.3.8.1, this enables an equality to be written between column test properties and allowables. If
Then
(7)
(8)
( L'/ ρ ) for design = ( L'/ ρ ) of the column test
[1.6.4.4(a)]
( Fc / E t ) for design = ( fc '/ E t ') from test
[1.6.4.4(b)]
Tangent modulus is defined as:
E t = df / de
[1.6.4.4(c)]
Total strain (e) is defined as the sum of elastic and plastic strains, and throughout the Handbook is used as:
e = ee + e p
[1.6.4.4(d)]
or,
f f e = + 0.002 E fy
132
n
[1.6.4.4(e)]
MMPDS01 31 January 2003
.
1.2
F cy' F cy
F cy'
Column material compressive yield stress =
F cy
Compressive yield stress (std)
1.1
.90
K = Correction Factor
.95
1.00
1.0
1.05 1.10 0.9
1.15 1.20 1.25 1.30
0.8
1.35
0.7 0.3
0.4
0.5
0.6
F c'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
F cy'
Column material compressive yield stress
Figure 1.6.4.4(a). Nondimensional material correction chart for 2024T3 sheet.
.
1.2
F cy'
F cy'
Column m aterial compressive yield stress =
F cy
F cy
Compressive yield stress (std)
1.1 .90
K = Correction Factor
.95
1.00
1.0
1.05 1.10 1.15
0.9
1.20 1.25 1.30 1.35 0.8
0.7 0.3
0.4
0.5
0.6
F c'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
F cy '
Column m aterial compressive yield stress
Figure 1.6.4.4(b). Nondimensional material correction chart for 2024T3 clad sheet.
133
MMPDS01 31 January 2003
.
1.2
Fcy' Fcy
Fcy'
Column material compressive yield stress =
Fcy
Compressive yield stress (std)
.90
1.1
K = Correction Factor
.95
1.00
1.0
1.05
1.10
0.9
1.15 1.20 1.25
0.8
1.30 1.35
0.7 0.3
0.4
0.5
0.6
F c'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
Fcy'
Column material compressive yield stress
Figure 1.6.4.4(c). Nondimensional material correction chart for 2024T4 extrusion less than 1/4 inch thick.
.
1.2
F cy'
F cy'
Column material compressive yield stress
F cy
=
F cy
Compressive yield stress (std)
.90 1.1
K = Correction Factor
.95
1.00
1.0
1.05
1.10
0.9
1.15 1.20 0.8
1.25 1.30 1.35
0.7 0.3
0.4
0.5
0.6
F c'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
F cy'
Column material compressive yield stress
Figure 1.6.4.4(d). Nondimensional material correction chart for 2024T4 extrusion 1/4 to 11/2 inches thick.
134
MMPDS01 31 January 2003 .
1.2
Fcy' Fcy
Fcy'
Column material compressive yield stress =
Fcy
Compressive yield stress (std)
.90
1.1
K = Correction Factor
.95
1.00
1.0
1.05 1.10 0.9 1.15 1.20 1.25 0.8 1.30 1.35
0.7 0.3
0.4
0.5
0.6
F c'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
Fcy'
Column material compressive yield stress
Figure 1.6.4.4(e). Nondimensional material correction chart for 2024T3 tubing.
.
1.2
F cy'
F cy' F cy
Column material compressive yield stress =
Compressive yield stress (std)
F cy
K = Correction Factor
1.1
.90
.95 1.00
1.0
1.05
1.10
0.9
1.15 1.20 1.25
0.8
1.30 1.35 0.7 0.3
0.4
0.5
0.6
F c'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
F cy'
Column material compressive yield stress
Figure 1.6.4.4(f). Nondimensional material correction chart for clad 2024T3 sheet.
135
MMPDS01 31 January 2003
.
1.2
Fcy'
Fcy'
Column material compressive yield stress
Fcy
=
Fcy
Compressive yield stress (std)
1.1
.90
K = Correction Factor
.95
1.00
1.0
1.05 1.10 0.9 1.15 1.20 1.25
0.8
1.30 1.35
0.7 0.3
0.4
0.5
0.6
Fc'
0.7
0.8
0.9
1.0
1.1
1.2
1.3
Maximum test column Stress =
Fcy'
Column material compressive yield stress
Figure 1.6.4.4(g). Nondimensional material correction chart for 7075T6 sheet.
.
1.2
F cy'
F cy'
Column material compressive yield stress
F cy
=
F cy
Compressive yield stress (std)
K = Correction Factor
1.1
.90
1.0
1.00
0.9
1.10 0.8 1.20
1.30 0.7 0.2
0.3
0.4
0.5
F c'
0.6
0.7
0.8
0.9
1.0
1.1
1.2
Maximum test column Stress =
F cy'
Column material compressive yield stress
Figure 1.6.4.4(h). Nondimensional material correction chart for AZ31BF and AZ61AF extrusion.
136
MMPDS01 31 January 2003
.
1.2
Fcy'
F cy'
Column material compressive yield stress
Fcy
=
Fcy
Compressive yield stress (std)
K = Correction Factor
1.1
.90 1.0
1.00 0.9
1.10 0.8 1.20
1.30 0.7 0.2
0.3
0.4
0.5
F c'
0.6
0.7
0.8
0.9
1.0
1.1
1.2
Maximum test column Stress =
F cy'
Column material compressive yield stress
Figure 1.6.4.4(i). Nondimensional material correction chart for AZ31BH24 sheet.
Equation 1.6.4.4(c) can be rewritten as follows:
Et =
f
f f + 0.002 n E fy
[1.6.4.4(f)]
n
Tangent modulus, for the material in question, using its compression allowables is:
Et =
Fc
F Fc + 0.002 n c c Ec Fcy
nc
[1.6.4.4(g)]
In like manner, tangent modulus for the same material with the desired column configuration is:
Et ' =
fc '
f ' fc ' + 0.002 n c c Ec fcy ' 137
nc
[1.6.4.4(h)]
MMPDS01 31 January 2003
Substitution of Equations 1.6.4.4(g) and 1.6.4.4(h) for their respective terms in Equation 1.6.4.4(b) and simplifying provides the following relationship:
F Fc + 0.002 n c c Ec Fcy
nc
f ' f ' = c + 0.002 n c c Ec fcy '
nc
[1.6.4.4(i)]
The only unknown in the above equation is the term Fc , the allowable column compression stress. This property can be solved by an iterative process. This method is also applicable at other than room temperature, having made adjustments for the effect of temperature on each of the properties. It is critical that the test material be the same in all respects as that for which allowables are selected from the Handbook. Otherwise, the assumption made in Equation 1.6.4.4(c) above is not valid. Equation 1.6.4.4(i) must account for such differences in moduli and shape factors when applicable.
138
MMPDS01 31 January 2003
1.7 THINWALLED AND STIFFENED THINWALLED SECTIONS A bibliography of information on thinwalled and stiffened thinwalled sections is contained in References 1.7(a) and (b).
139
MMPDS01 31 January 2003
REFERENCES 1.4.3.1
Goodman, S. and Russell, S.B., U.S. Air Force, “Poisson’s Ratio of Aircraft Sheet Materials for Large Strain,” WADCTR537, 58 pp (June1953).
1.4.4
“Test Methods of Tension Testing of Metallic Materials,” ASTM E 8.
1.4.5(a)
Hyler, W.S., “An Evaluation of CompressionTesting Techniques for Determining Elevated Temperature Properties of Titanium Sheet,” Titanium Metallurgical Laboratory Report No. 43, Battelle Memorial Institute, 38 pp, Appendix 28 pp (June 8, 1956).
1.4.5(b)
“Compression Testing of Metallic Materials at Room Temperature,” ASTM E 9.
1.4.6
Stange, A.H., Ramberg, W. and Back, G., “Torsion Tests of Tubes,” National Advisory Committee for Aeronautics, Report No. 601, pp 515535 (Feb. 1937).
1.4.7(a)
Stickley, G.W. and Moore, A.A., “Effects of Lubrication and Pin Surface on Bearing Strengths of Aluminum and Magnesium Alloys,” Materials Research and Standards, 2, (9), pp 747751 (September 1962).
1.4.7(b)
“Method of PinType Bearing Test of Metallic Materials,” ASTM E 238.
1.4.8.2.1(a)
“Recommended Practice for Conducting Creep, CreepRupture, and StressRupture Tests of Metallic Materials,” ASTM E 139.
1.4.8.2.1(b)
Rice, Richard, “Reference Document for the Analysis of Creep and Stress Rupture Data in MILHDBK5,” AFWALTR814097 (September 1981).
1.4.8.2.1(c)
Aarnes, M.N. and Tuttle, M.M., “Presentation of Creep Data for Design Purposes,” ASD Technical Report 61216 (June 1961) (MCIC 45114).
1.4.9(a)
“Recommended Practice for Constant Amplitude Axial Fatigue Tests of Metallic Materials,” ASTM E 466.
1.4.9(b)
“Recommended Practice for ConstantAmplitude LowCycle Fatigue Testing,” ASTM E 606.
1.4.9.2(a)
Grover, H.J., “Fatigue of Aircraft Structures,” Prepared for Naval Air Systems Command, Department of the Navy, 335 pp (1966).
1.4.9.2(b)
Osgood, C.C., “Fatigue Design,” WileyInterscience, A Division of John Wiley and Sons, Inc., 523 pp (1970).
1.4.11
Bert, C.W., Mills, E.J. and Hyler, W.S., “Mechanical Properties of Aerospace Structural Alloys Under BiaxialStress Conditions,” AFMLTR66229, (August 1966).
1.4.12.2(a)
“Standard Method of Test for PlaneStrain Fracture Toughness of Metallic Materials,” ASTM E 399.
140
MMPDS01 31 January 2003
1.4.13.1
“Test Method for Measurements of Fatigue Crack Growth Rates,” ASTM E 647.
1.4.13.2
Paris, P.C., “The Fracture Mechanics Approach to Fatigue,” Proc. 10th Sagamore Conference, p. 107, Syracuse University Press (1965).
1.5.2.4
Cozzone, F.P., “Bending Strength in the Plastic Range,” Journal of the Aeronautical Sciences, 10, pp 137151, (1943).
1.5.2.6(a)
Dieter, G.E., Jr., “Mechanical Metallurgy,” McGrawHill Book Company, Inc., 615 pp (1961).
1.5.2.6(b)
Freudenthal, A.M., “The Inelastic Behavior of Engineering Materials and Structures,” John Wiley and Sons, Inc., New York, 587 pp (1950).
1.5.2.6(c)
Parker, E.R., “Brittle Behavior of Engineering Structures,” John Wiley and Sons, Inc., New York, 323 pp (1957).
1.5.3.3
Lundquist, E.E., “Strength Tests of ThinWalled Duralumin Cylinders in Pure Bending,” U.S. National Advisory Committee for Aeronautics, Technical Note No. 479, 17 pp (December 1933).
1.6.2.3(a)
Hill, H.N. and Clark, J.W., “StraightLine Column Formulas for Aluminum Alloys,” Aluminum Company of America, Aluminum Research Laboratories, Technical Paper No. 12, 8 pp (1955).
1.6.2.3(b)
AFFDLTR6942, “Stress Analysis Manual,” Air Force Flight Dynamics Laboratory, Air Force Systems Command, WrightPatterson Air Force Base (February 1970).
1.6.2.3(c)
“Astronautic Structure Manual,” George C. Marshall Space Flight Center (August 15, 1970).
1.6.2.3(d)
Niles, A.S., and Newell, J.S., “Airplane Structure,” 2, Third Edition, John Wiley and Sons (1943).
1.7(a)
“Index of Aircraft Structures Research Reports,” U.S. National Advisory Committee for Aeronautics, Index No. 7E29, 40 pp (June 1947).
1.7(b)
Gerard, and Becker, H., “Handbook of Structural Stability,” National Advisory Committee for Aeronautics Technical Note, Nos. 3781, 102 pp (July 1957); 3782, 72 pp (July 1957); 3783, 154 pp (August 1957); 3784, 93 pp (August 1957); and 3785, 89 pp (August 1957).
141
MMPDS01 31 January 2003
This page is intentionally blank.
142
MMPDS01 31 January 2003
CHAPTER 2 STEEL This chapter contains the engineering properties and related characteristics of steels used in aircraft and missile structural applications. General comments on engineering properties and other considerations related to alloy selection are presented in Section 2.1. Mechanical and physical property data and characteristics pertinent to specific steel groups or individual steels are reported in Sections 2.2 through 2.7. Element properties are presented in Section 2.8.
2.1
GENERAL
The selection of the proper grade of steel for a specific application is based on material properties and on manufacturing, environmental, and economic considerations. Some of these considerations are outlined in the sections that follow. 2.1.1 ALLOY INDEX — The steel alloys listed in this chapter are arranged in major sections that identify broad classifications of steel partly associated with major alloying elements, partly associated with processing, and consistent generally with steelmaking technology. Specific alloys are identified as shown in Table 2.1.1. Table 2.1.1. Steel Alloy Index
Section 2.2 2.2.1 2.3 2.3.1 2.4 2.4.1 2.4.2 2.4.3 2.5 2.5.1 2.5.2 2.5.3 2.6 2.6.1 2.6.2 2.6.3 2.6.4 2.6.5 2.6.6 2.6.7 2.6.8 2.6.9 2.6.10
Alloy Designation Carbon steels AISI 1025 Lowalloy steels (AISI and proprietary grades) Specific alloys Intermediate alloy steels 5CrMoV 9Ni4Co0.20C 9Ni4Co0.30C High alloy steels 18 Ni maraging steels AF1410 AerMet 100 Precipitation and transformation hardening steel (stainless) AM350 AM355 Custom 450 Custom 455 Custom 465 PH138Mo 155PH PH157Mo 174PH 177PH
21
MMPDS01 31 January 2003 Table 2.1.1(Continued). Steel Alloy Index
Section 2.7 2.7.1
Alloy Designation Austenitic stainless steels AISI 301 and Related 300 Series Stainless Steels
2.1.2 MATERIAL PROPERTIES — One of the major factors contributing to the general utility of steels is the wide range of mechanical properties which can be obtained by heat treatment. For example, softness and good ductility may be required during fabrication of a part and very high strength during its service life. Both sets of properties are obtainable in the same material. All steels can be softened to a greater or lesser degree by annealing, depending on the chemical composition of the specific steel. Annealing is achieved by heating the steel to an appropriate temperature, holding, then cooling it at the proper rate. Likewise, steels can be hardened or strengthened by means of cold working, heat treating, or a combination of these. Cold working is the method used to strengthen both the lowcarbon unalloyed steels and the highly alloyed austenitic stainless steels. Only moderately high strength levels can be attained in the former, but the latter can be cold rolled to quite high strength levels, or “tempers”. These are commonly supplied to specified minimum strength levels. Heat treating is the principal method for strengthening the remainder of the steels (the lowcarbon steels and the austenitic steels cannot be strengthened by heat treatment). The heat treatment of steel may be of three types: martensitic hardening, age hardening, and austempering. Carbon and alloy steels are martensitichardened by heating to a high temperature, or “austenitizing”, and cooling at a recommended rate, often by quenching in oil or water. This is followed by “tempering”, which consists of reheating to an intermediate temperature to relieve internal stresses and to improve toughness. The maximum hardness of carbon and alloy steels, quenched rapidly to avoid the nose of the isothermal transformation curve, is a function in general of the alloy content, particularly the carbon content. Both the maximum thickness for complete hardening or the depth to which an alloy will harden under specific cooling conditions, and the distribution of hardness can be used as a measure of a material’s hardenability. A relatively new class of steels is strengthened by age hardening. This heat treatment is designed to dissolve certain constituents in the steel, then precipitate them in some preferred particle size and distribution. Since both the martensitic hardening and the agehardening treatments are relatively complex, specific details are presented for individual steels elsewhere in this chapter. Recently, special combinations of working and heat treating have been employed to further enhance the mechanical properties of certain steels. At the present time, the use of these specialized treatments is not widespread. Another method of heat treatment for steels is austempering. In this process, ferrous steels are austenitized, quenched rapidly to avoid transformation of the austenite to a temperature below the pearlite
22
MMPDS01 31 January 2003 and above the martensite formation ranges, allowed to transform isothermally at that temperature to a completely bainitic structure, and finally cooled to room temperature. The purpose of austempering is to obtain increased ductility or notch toughness at high hardness levels, or to decrease the likelihood of cracking and distortion that might occur in conventional quenching and tempering. 2.1.2.1 Mechanical Properties — 2.1.2.1.1 Strength (Tension, Compression, Shear, Bearing) — The strength properties presented are those used in structural design. The roomtemperature properties are shown in tables following the comments for individual steels. The variations in strength properties with temperature are presented graphically as percentages of the corresponding roomtemperature strength property, also described in Section 9.3.1 and associated subsections. These strength properties may be reduced appreciably by prolonged exposure at elevated temperatures. The strength of steels is temperaturedependent, decreasing with increasing temperature. In addition, steels are strain ratesensitive above about 600 to 800EF, particularly at temperatures at which creep occurs. At lower strain rates, both yield and ultimate strengths decrease. The modulus of elasticity is also temperaturedependent and, when measured by the slope of the stressstrain curve, it appears to be strain ratesensitive at elevated temperatures because of creep during loading. However, on loading or unloading at high rates of strain, the modulus approaches the value measured by dynamic techniques. Steel bars, billets, forgings, and thick plates, especially when heat treated to high strength levels, exhibit variations in mechanical properties with location and direction. In particular, elongation, reduction of area, toughness, and notched strength are likely to be lower in either of the transverse directions than in the longitudinal direction. This lower ductility and/or toughness results both from the fibering caused by the metal flow and from nonmetallic inclusions which tend to be aligned with the direction of primary flow. Such anisotropy is independent of the depthofhardening considerations discussed elsewhere. It can be minimized by careful control of melting practices (including degassing and vacuumarc remelting) and of hotworking practices. In applications where transverse properties are critical, requirements should be discussed with the steel supplier and properties in critical locations should be substantiated by appropriate testing. 2.1.2.1.2 Elongation — The elongation values presented in this chapter apply in both the longitudinal and long transverse directions, unless otherwise noted. Elongation in the short transverse (thickness) direction may be lower than the values shown. 2.1.2.1.3 Fracture Toughness — Steels (as well as certain other metals), when processed to obtain high strength, or when tempered or aged within certain critical temperature ranges, may become more sensitive to the presence of small flaws. Thus, as discussed in Section 1.4.12, the usefulness of highstrength steels for certain applications is largely dependent on their toughness. It is generally noted that the fracture toughness of a given alloy product decreases relative to increase in the yield strength. The designer is cautioned that the propensity for brittle fracture must be considered in the application of highstrength alloys for the purpose of increased structural efficiency. Minimum, average, and maximum values, as well as coefficient of variation of planestrain fracture toughness for several steel alloys, are presented in Table 2.1.2.1.3. These values are presented as indicative information and do not have the statistical reliability of roomtemperature mechanical properties. Data showing the effect of temperature are presented in the respective alloy sections where the information is available.
23
24
1650EF, 12 Hr, AC, 1525EF, 12 Hr, OQ, 100EF, Temp
H1000
9Ni4Co.20C
PH138Mo
Forging
Forging
Hand Forging
Forging
Plate
Forging
Plate
Plate
Bar
Bar
Bar
Bar
Bar
Bar
Bar
Bar
Product Form
231246 212227 212225
RLc c
RLc
LT
LT
LT
LT
LT
LT
LT
LT
LR
205212
186192
185192
214
217
214
217
217
229249
LR
250268
c
251265
223273
236281
CR
LR
CR
LR
Orientationb
a These values are for information only. b Refer to Figures 1.4.12.3(a) and 1.4.12.3(b) for definition of symbols. c LR also includes some LT, RL also includes some TL.
Quench and Temper
9Ni4Co.20C
1650EF, AusBay Quench 975EF, SQ 375EF, 1000EF 2 + 2
D6AC
1700EF, AusBay Quench 975EF, OQ 140EF, 1000EF 2 + 2
H1000
Custom 465
D6AC
H1000
Custom 465
1700EF, AusBay Quench 975EF, OQ 140EF, 1000EF 2 + 2
H950
Custom 465
D6AC
H950
Custom 465
1650EF, AusBay Quench 975EF, SQ 400EF, 1000EF 2 + 2
Anneal, HT to 290ksi
AerMet 100
D6AC
Anneal, HT to 290ksi
AerMet 100
1650EF, AusBay Quench 975EF, SQ 400EF, 1000EF 2 + 2
Anneal, HT to 280ksi
AerMet 100
D6AC
Anneal, HT to 280ksi
AerMet 100
Alloy
Heat Treat Condition
Yield Strength Range, ksi
4.08.0
3.04.0
3.0
0.81.5
0.81.5
0.81.5
0.8
1.5
312
312
312
312
310
310
2.7510
2.7510
Product Thickness Range, inches
3
3
2
1
1
1
1
1
1
1
1
1
1
1
1
1
Number of Sources
12
17
27
34
30
53
103
19
40
40
40
40
24
29
156
183
Sample Size
0.72.0
1.52.0
1.02.0
0.7
0.60.8
0.60.8
0.60.8
0.6
11.5
11.5
11.5
11.5
1
1
1
1
Specimen Thickness Range, inches
104
147
147
109
101
96
92
88
118
131
94
104
101
110
137
146
Max.
Table 2.1.2.1.3. Values of Room Temperature PlaneStrain Fracture Toughness of Steel Alloysa
90
134
129
95
92
66
64
62
109
120
82
89
88
99
112
121
Avg.
49
120
107
81
64
39
44
40
100
108
73
76
73
88
90
100
Min.
KIC, ksi /in.
21.5
8.5
8.3
6.7
8.9
18.6
18.9
22.5
3.7
5.2
6.4
7.4
9.7
6.5
8.5
7.9
Coefficient of Variation
MMPDS01 31 January 2003
MMPDS01 31 January 2003 2.1.2.1.4 StressStrain Relationships — The stressstrain relationships presented in this chapter are prepared as described in Section 9.3.2. 2.1.2.1.5 Fatigue — Axialload fatigue data on unnotched and notched specimens of various steels at room temperature and at other temperatures are shown as S/N curves in the appropriate section. Surface finish, surface finishing procedures, metallurgical effects from heat treatment, environment and other factors influence fatigue behavior. Specific details on these conditions are presented as correlative information for the S/N curve. 2.1.2.2 Physical Properties — The physical properties (ω, C, K, and α) of steels may be considered to apply to all forms and heat treatments unless otherwise indicated. 2.1.3 ENVIRONMENTAL CONSIDERATIONS — The effects of exposure to environments such as stress, temperature, atmosphere, and corrosive media are reported for various steels. Fracture toughness of highstrength steels and the growth of cracks by fatigue may be detrimentally influenced by humid air and by the presence of water or saline solutions. Some alleviation may be achieved by heat treatment and all highstrength steels are not similarly affected. In general, these comments apply to steels in their usual finished surface condition, without surface protection. It should be noted that there are available a number of heatresistant paints, platings, and other surface coatings that are employed either to improve oxidation resistance at elevated temperature or to afford protection against corrosion by specific media. In employing electrolytic platings, special consideration should be given to the removal of hydrogen by suitable baking. Failure to do so may result in lowered fracture toughness or embrittlement.
25
MMPDS01 31 January 2003
2.2
CARBON STEELS 2.2.0 COMMENTS ON CARBON STEELS
2.2.0.1 Metallurgical Considerations — Carbon steels are those steels containing carbon up to about 1 percent and only residual quantities of other elements except those added for deoxidation. The strength that carbon steels are capable of achieving is determined by carbon content and, to a much lesser extent, by the content of the residual elements. Through cold working or proper choice of heat treatments, these steels can be made to exhibit a wide range of strength properties. The finish conditions most generally specified for carbon steels include hotrolled, coldrolled, colddrawn, normalized, annealed, spheroidized, stressrelieved, and quenchedandtempered. In addition, the lowcarbon grades (up to 0.25 percent C) may be carburized to obtain high surface hardness and wear resistance with a tough core. Likewise, the higher carbon grades are amenable to selective flame hardening to obtain desired combinations of properties. 2.2.0.2 Manufacturing Considerations — Forging — All of the carbon steels exhibit excellent forgeability in the austenitic state provided the proper forging temperatures are used. As the carbon content is increased, the maximum forging temperature is decreased. At high temperatures, these steels are soft and ductile and exhibit little or no tendency to work harden. The resulfurized grades (freemachining steels) exhibit a tendency to rupture when deformed in certain hightemperature ranges. Close control of forging temperatures is required. Cold Forming — The very lowcarbon grades have excellent coldforming characteristics when in the annealed or normalized conditions. Mediumcarbon grades show progressively poorer formability with higher carbon content, and more frequent annealing is required. The highcarbon grades require special softening treatments for cold forming. Many carbon steels are embrittled by warm working or prolonged exposure in the temperature range from 300 to 700EF. Machining — The lowcarbon grades (0.30 percent C and less) are soft and gummy in the annealed condition and are preferably machined in the coldworked or the normalized condition. Mediumcarbon (0.30 to 0.50 percent C) grades are best machined in the annealed condition, and highcarbon grades (0.50 to 0.90 percent C) in the spheroidized condition. Finish machining must often be done in the fully heattreated condition for dimensional accuracy. The resulfurized grades are well known for their good machinability. Nearly all carbon steels are now available with 0.15 to 0.35 percent lead, added to improve machinability. However, resulfurized and leaded steels are not generally recommended for highly stressed aircraft and missile parts because of a drastic reduction in transverse properties. Welding — The lowcarbon grades are readily welded or brazed by all techniques. The mediumcarbon grades are also readily weldable but may require preheating and postwelding heat treatment. The highcarbon grades are difficult to weld. Preheating and postwelding heat treatment are usually mandatory for the latter, and special care must be taken to avoid overheating. Furnace brazing has been used successfully with all grades. Heat Treatment — Due to the poor oxidation resistance of carbon steels, protective atmospheres must be employed during heat treatment if scaling of the surface cannot be tolerated. Also, these steels are subject to decarburization at elevated temperatures and, where surface carbon content is critical, should be heated in reducing atmospheres.
26
MMPDS01 31 January 2003 2.2.0.3 Environmental Considerations — Carbon steels have poor oxidation resistance above about 900 to 1000EF. Strength and oxidationresistance criteria generally preclude the use of carbon steels above 900EF. Carbon steels may undergo an abrupt transition from ductile to brittle behavior. This transition temperature varies widely for different carbon steels depending on many factors. Cautions should be exercised in the application of carbon steels to assure that the transition temperature of the selected alloy is below the service temperature. Additional information is contained in References 2.2.0.3(a) and (b). The corrosion resistance of carbon steels is relatively poor; clean surfaces rust rapidly in moist atmospheres. Simple oil film protection is adequate for normal handling. For aerospace applications, the carbon steels are usually plated to provide adequate corrosion protection. 2.2.1 AISI 1025 2.2.1.0 Comments and Properties — AISI 1025 is an excellent general purpose steel for the majority of shop requirements, including jigs, fixtures, prototype mockups, low torque shafting, and other applications. It is not generally classed as an airframe structural steel. However, it is available in aircraft quality as well as commercial quality. Manufacturing Considerations — Coldfinished flatrolled products are supplied principally where maximum strength, good surface finish, or close tolerance is desirable. Reasonably good forming properties are found in AISI 1025. The machinability of bar stock is rated next to these sulfurized types of freemachining steels, but the resulting surface finish is poorer. Specifications and Properties — Material specifications for AISI 1025 steel are presented in Table 2.2.1.0(a). The roomtemperature mechanical and physical properties are shown in Table 2.2.1.0(b). The effect of temperature on thermal expansion is shown in Figure 2.2.1.0. Table 2.2.1.0(a). Material Specifications for AISI 1025 Carbon Steel Specification Form ASTM A 108 Bar AMS 5075 Seamless tubing AMST5066a Tubing AMS 5077 Tubing AMS 5046 Sheet, strip, and plate AMSS7952 Sheet and strip a Noncurrent specification
27
MMPDS01 31 January 2003
Table 2.2.1.0(b). Design Mechanical and Physical Properties of AISI 1025 Carbon Steel AMS 5046 and AMS 5075, AMS 5077 ASTM A 108 Specification . . . . . . . . . . . AMSS7952 and AMST5066a Form . . . . . . . . . . . . . . . . . . Sheet, strip, and plate Tubing Bar Condition . . . . . . . . . . . . . . Annealed Normalized All Thickness, in. . . . . . . . . . . ... ... ... Basis . . . . . . . . . . . . . . . . . . S S Sb Mechanical Properties: Ftu, ksi: L .................. 55 55 55 LT . . . . . . . . . . . . . . . . . 55 55 55 ST . . . . . . . . . . . . . . . . . ... ... 55 Fty, ksi: L .................. 36 36 36 LT . . . . . . . . . . . . . . . . . 36 36 36 ST . . . . . . . . . . . . . . . . . ... ... 36 Fcy, ksi: L .................. 36 36 36 LT . . . . . . . . . . . . . . . . . 36 36 36 ST . . . . . . . . . . . . . . . . . ... ... 36 Fsu, ksi . . . . . . . . . . . . . . . 35 35 35 Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . ... ... ... (e/D = 2.0) . . . . . . . . . . . 90 90 90 Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . ... ... ... (e/D = 2.0) . . . . . . . . . . . ... ... ... e, percent: c c L .................. ... c LT . . . . . . . . . . . . . . . . . ... ... E, 103 ksi . . . . . . . . . . . . . 29.0 Ec, 103 ksi . . . . . . . . . . . . 29.0 3 G, 10 ksi . . . . . . . . . . . . . 11.0 µ ................... 0.32 Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . 0.284 C, Btu/(lb)(EF) . . . . . . . . 0.116 (122 to 212EF) K, Btu/[(hr)(ft2)(EF)/ft] . . 30.0 (at 32EF) 6 α, 10 in./in./EF . . . . . . . . See Figure 2.2.1.0 a Noncurrent specification. b Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. c See applicable specification for variation in minimum elongation with ultimate strength.
28
MMPDS01 31 January 2003
α,  Between 70 F and indicated temperature
α, 106 in./in./F
9
8
7
6
5 0
200
400
600
800
1000
1200
1400
1600
Temperature, F Figure 2.2.1.0. Effect of temperature on the thermal expansion of 1025 steel.
29
MMPDS01 31 January 2003
2.3
LOWALLOY STEELS (AISI GRADES AND PROPRIETARY GRADES) 2.3.0 COMMENTS ON LOWALLOY STEELS (AISI AND PROPRIETARY GRADES)
2.3.0.1 Metallurgical Considerations — The AISI or SAE alloy steels contain, in addition to carbon, up to about 1 percent (up to 0.5 percent for most airframe applications) additions of various alloying elements to improve their strength, depth of hardening, toughness, or other properties of interest. Generally, alloy steels have better strengthtoweight ratios than carbon steels and are somewhat higher in cost on a weight, but not necessarily strength, basis. Their applications in airframes include landinggear components, shafts, gears, and other parts requiring high strength, through hardening, or toughness. Some alloy steels are identified by the AISI fourdigit system of numbers. The first two digits indicate the alloy group and the last two the approximate carbon content in hundredths of a percent. The alloying elements used in these steels include manganese, silicon, nickel, chromium, molybdenum, vanadium, and boron. Other steels in this section are proprietary steels which may be modifications of the AISI grades. The alloying additions in these steels may provide deeper hardening, higher strength and toughness. These steels are available in a variety of finish conditions, ranging from hot or coldrolled to quenchedandtempered. They are generally heat treated before use to develop the desired properties. Some steels in this group are carburized, then heat treated to produce a combination of high surface hardness and good core toughness. 2.3.0.2 Manufacturing Conditions — Forging — The alloy steels are only slightly more difficult to forge than carbon steels. However, maximum recommended forging temperatures are generally about 50EF lower than for carbon steels of the same carbon content. Slower heating rates, shorter soaking period, and slower cooling rates are also required for alloy steels. Cold Forming — The alloy steels are usually formed in the annealed condition. Their formability depends mainly on the carbon content and is generally slightly poorer than for unalloyed steels of the same carbon content. Little cold forming is done on these steels in the heattreated condition because of their high strength and limited ductility. Machining — The alloy steels are generally harder than unalloyed steels of the same carbon content. As a consequence, the lowcarbon alloy steels are somewhat easier to finish machine than their counterparts in the carbon steels. It is usually desirable to finish machine the carburizing and throughhardening grades in the final heattreated condition for better dimensional accuracy. This often leads to two steps in machining: rough machining in the annealed or hotfinished condition, then finish machining after heat treating. The latter operation, because of the relatively high hardness of the material, necessitates the use of sharp, welldesigned, highspeed steel cutting tools, proper feeds, speeds, and a generous supply of coolant. Mediumand highcarbon grades are usually spheroidized for optimum machinability and, after heat treatment, may be finished by grinding. Many of the alloy steels are available with added sulfur or lead for improved machinability. However, resulfurized and leaded steels are not recommended for highly stressed aircraft and missile parts, because of drastic reductions in transverse properties. Welding — The lowcarbon grades are readily welded or brazed by all techniques. Alloy welding rods comparable in strength to the base metal are used, and moderate preheating (200 to 600EF) is usually necessary. At higher carbon levels, higher preheating temperatures, and often postwelding stress relieving, are required. Certain alloy steels can be welded without loss of strength in the heataffected zone provided that the welding heat input is carefully controlled. If the composition and strength level are such that the strength of the welded joint is reduced, the strength of the joint may be restored by heat treatment after welding. 210
MMPDS01 31 January 2003 Heat Treatment — For the low alloy steels, there are various heat treatment procedures that can be applied to a particular alloy to achieve any one of a number of specific mechanical (for example tensile) properties. Within this chapter, there are mechanical properties for three thermal processing conditions: annealed, normalized, and quenched and tempered. The specific details of these three thermal processing conditions are reviewed in Reference 2.3.0.2.5. In general, the annealed condition is achieved by heating to a suitable temperature and holding for a specified period of time. Annealing generally softens the material, producing the lowest mechanical properties. The normalized condition is achieved by holding to a slightly higher temperature than annealing, but for a shorter period of time. The purpose of normalizing varies depending on the desired properties; it can be used to increase or decrease mechanical properties. The quenched and tempered condition, discussed in more detail below, is used to produce the highest mechanical properties while providing relatively high toughness. The mechanical properties for these three processing conditions for specific steels are as shown in Tables 2.3.1.0(c), (f), and (g). Maximum hardness in these steels is obtained in the asquenched condition, but toughness and ductility in this condition are comparatively low. By means of tempering, their toughness is improved, usually accompanied by a decrease in strength and hardness. In general, tempering temperatures to achieve very high strength should be avoided when toughness is an important consideration. In addition, these steels may be embrittled by tempering or by prolonged exposure under stress within the “blue brittle” range (approximately 500 to 700EF). Strength levels that necessitate tempering within this range should be avoided. The mechanical properties presented in this chapter represent steels heat treated to produce a quenched structure containing 90 percent martensite at the center and tempered to the desired Ftu level. This degree of through hardening is necessary (regardless of strength level) to insure the attainment of reasonably uniform mechanical properties throughout the cross section of the heattreated part. The maximum diameter of round bars of various alloy steels capable of being through hardened consistently are given in Table 2.3.0.2. Limiting dimensions for common shapes other than round are determined by means of the “equivalent round” concept in Figure 2.3.0.2. This concept is essentially a correlation between the significant dimensions of a particular shape and the diameter of a round bar, assuming in each instance that the material, heat treatment, and the mechanical properties at the centers of both the respective shape and the equivalent round are substantially the same. For the quenched and tempered condition, a large range of mechanical property values can be achieved as indicated in Table 2.3.0.2. Various quench media (rates), tempering temperatures, and times can be employed allowing any number of processing routes to achieve these values. As a result of these processing routes, there are a large range of mechanical properties that can be obtained for a specific alloy. Therefore, the properties of a steel can be tailored to meet the needs for a specific component/application. Because of the potential for several different processing methods for these three conditions, the MIL, Federal, and AMS specifications do not always contain minimum mechanical property values (Sbasis). They may contain minimum mechanical property values for one specific quenched and tempered condition. Those specifications cited in this Handbook that do not contain mechanical properties are identified with a footnote in Tables 2.3.1.0(a) and (b). The possible mechanical properties for these alloys covered in the specifications for the normalized, and quenched and tempered conditions in Table 2.3.0.2 are presented in Tables 2.3.1.0 (g1) and (g2). Users must rely on their own inhouse specifications or appropriate industry specifications to validate that the required strength was achieved. Therefore, no statistical basis (A, B, S) for these values are indicated in Tables 2.3.1.0 (g1) and (g2).
211
MMPDS01 31 January 2003
Table 2.3.0.2. Maximum Round Diameters for LowAlloy Steel Bars (Through Hardening to at Least 90 Percent Martensite at Center) Maximum Diameter of Round or Equivalent Round, in.a Ftu, ksi
0.5
0.8
1.0
1.7
2.5
3.5
5.0
270 & 280
...
...
...
...
...
...
300Mc
260
...
...
...
AISI 4340b
AISI 4340c
AISI 4340d
220
...
...
...
200
...
AISI 8740
#180
AISI 4130 and 8630
AISI 8735 4135 and 8740
b,e
c,e
D6AC
b
... D6ACc
AMS Grades
AMS Grades
AISI 4140
AISI 4340b AMS Gradesb,e
AISI 4340d AISI 4340c c,e AMS Grades
D6ACc
AISI 4140
AISI 4340b AMS Gradesb,e
AISI 4340d AISI 4340c c,e D6ACb AMS Grades
D6ACc
a This table indicates the maximum diameters to which these steels may be through hardened consistently by quenching as indicated. Any steels in this table may be used at diameters less than those indicated. The use of steels at diameters greater than those indicated should be based on hardenability data for specific heats of steel. b Quenched in molten salt at desired tempering temperature (“martempering”). c Quenched in oil at a flow rate of 200 feet per minute. d Quenched in water at a flow rate of 200 feet per minute. e 4330V, 4335V, and HyTuf.
212
MMPDS01 31 January 2003
Figure 2.3.0.2. Correlation between significant dimensions of common shapes other than round, and the diameters of round bars.
213
MMPDS01 31 January 2003 2.3.0.3 Environmental Considerations — Alloy steels containing chromium or high percentages of silicon have somewhat better oxidation resistance than the carbon or other alloy steels. Elevatedtemperature strength for the alloy steels is also higher than that of corresponding carbon steels. The mechanical properties of all alloy steels in the heattreated condition are affected by extended exposure to temperatures near or above the temperature at which they were tempered. The limiting temperatures to which each alloy may be exposed for no longer than approximately 1 hour per inch of thickness or approximately onehalf hour for thicknesses under onehalf inch without a reduction in strength occurring are listed in Table 2.3.0.3. These values are approximately 100EF below typical tempering temperatures used to achieve the designated strength levels. Table 2.3.0.3. Temperature Exposure Limits for LowAlloy Steels
Exposure Limit, EF Ftu, ksi
125
150
180
200
220
260
270 & 280
...
...
...
...
Alloy: AISI 4130 and 8630
925
775
575
AISI 4140 and 8740
1025
875
725
625
...
...
...
AISI 4340
1100
950
800
700
...
350
...
AISI 4135 and 8735
975
825
675
...
...
...
D6AC
1150
1075
1000
950
900
500
...
HyTuf
875
750
650
550
450
...
...
4330V
925
850
775
700
500
...
...
4335V
975
875
775
700
500
...
...
...
475
300M
...
...
...
...
...
...
a Quenched and tempered to Ftu indicated. If the material is exposed to temperatures exceeding those listed, a reduction in strength is likely to occur.
Lowalloy steels may undergo a transition from ductile to brittle behavior at low temperatures. This transition temperature varies widely for different alloys. Caution should be exercised in the application of lowalloy steels at temperatures below 100EF. For use at a temperature below 100EF, an alloy with a transition temperature below the service temperature should be selected. For low temperatures, the steel should be heat treated to a tempered martensitic condition for maximum toughness. Heattreated alloy steels have better notch toughness than carbon steels at equivalent strength levels. The decrease in notch toughness is less pronounced and occurs at lower temperatures. Heattreated alloy steels may be useful for subzero applications, depending on their alloy content and heat treatment. Heat treating to strength levels higher than 150 ksi Fty may decrease notch toughness. The corrosion properties of the AISI alloy steels are comparable to the plain carbon steels.
214
MMPDS01 31 January 2003 2.3.1 SPECIFIC ALLOYS 2.3.1.0 Comments and Properties — AISI 4130 is a chromiummolybdenum steel that is in general use due to its wellestablished heattreating practices and processing techniques. It is available in all sizes of sheet, plate, and tubing. Bar stock of this material is also used for small forgings under onehalf inch in thickness. AISI 4135, a slightly higher carbon version of AISI 4130, is available in sheet, plate, and tubing. AISI 4140 is a chromiummolybdenum steel that can be heat treated in thicker sections and to higher strength levels than AISI 4130. This steel is generally used for structural machined and forged parts onehalf inch and over in thickness. It can be welded but it is more difficult to weld than the lower carbon grade AISI 4130. AISI 4340 is a nickelchromiummolybdenum steel that can be heat treated in thicker sections and to higher strength levels than AISI 4140. AISI 8630, 8735, and 8740 are nickelchromiummolybdenum steels that are considered alternates to AISI 4130, 4135, and 4140, respectively. There are a number of steels available with compositions that represent modifications to the AISI grades described above. Four of the steels that have been used rather extensively at Ftu = 220 ksi are D6AC, HyTuf, 4330V, and 4335V. It should be noted that this strength level is not used for AISI 4340 due to embrittlement encountered during tempering in the range of 500 to 700EF. In addition, AISI 4340 and 300M are utilized at strength levels of Ftu = 260 ksi or higher. The alloys, AISI 4340, D6AC, 4330V, 4335V, and 300M, are available in the consumable electrode melted grade. Material specifications for these steels are presented in Tables 2.3.1.0(a) and (b). The roomtemperature mechanical and physical properties for these steels are presented in Tables 2.3.1.0(c) through 2.3.1.0(g). Mechanical properties for heattreated materials are valid only for steel heat treated to produce a quenched structure containing 90 percent or more martensite at the center. Figure 2.3.1.0 contains elevated temperature curves for the physical properties of AISI 4130 and AISI 4340 steels. 2.3.1.1 AISI LowAlloy Steels — Elevated temperature curves for heattreated AISI lowalloy steels are presented in Figures 2.3.1.1.1 through 2.3.1.1.4. These curves are considered valid for each of these steels in each heattreated condition but only up to the maximum temperatures listed in Table 2.3.0.1(b). 2.3.1.2 AISI 4130 and 8630 Steels — Typical stressstrain and tangentmodulus curves for AISI 8630 are shown in Figures 2.3.1.2.6(a) through (c). Bestfit S/N curves for AISI 4130 steel are presented in Figures 2.3.1.2.8(a) through (h). 2.3.1.3 AISI 4340 Steel — Typical stressstrain and tangentmodulus curves for AISI 4340 are shown in Figures 2.3.1.3.6(a) through (c). Typical biaxial stressstrain curves and yieldstress envelopes for AISI 4340 alloy steel are presented in Figures 2.3.1.3.6(d) through (g). Bestfit S/N curves for AISI 4340 are presented in Figures 2.3.1.3.8(a) through (o). 2.3.1.4 300M Steel — Bestfit S/N curves for 300M steel are presented in Figures 2.3.1.4.8(a) through (d). Fatiguecrackpropagation data for 300M are shown in Figure 2.3.1.4.9. 2.3.1.5 Figure 2.3.1.5.9.
D6AC Steel — Fatiguecrackpropagation data for D6AC steel are presented in
215
MMPDS01 31 January 2003 Table 2.3.1.0(a). Material Specifications for Air Melted LowAlloy Steels Form Alloy
Sheet, strip, and plate
Bars and forgings
Tubing
4130
AMSS18729, AMS 6350a, AMS 6351a
AMSS6758a, AMS 6348a, AMS 6370a, AMS 6528a
AMST6736, AMS 6371a, AMS 6360, AMS 6361, AMS 6362, AMS 6373, AMS 6374
8630
AMSS18728b, AMS 6350a
AMSS6050, AMS 6280a
AMS 6281a
4135
AMS 6352a
...
AMS 6372a, AMS 6365, AMST6735b
8735
AMS 6357a
AMS 6320a
AMS 6282a
4140
AMS 6395a
AMSS5626a, AMS 6382a, AMS 6349a, AMS 6529a
AMS 6381a
4340
AMS 6359a
AMSS5000a, AMS 6415a
AMS 6415a
8740
AMS 6358a
AMSS6049b, AMS 6327, AMS 6322a
AMS 6323a
4330V
...
AMS 6427a AMS 6427
4335V
a
AMS 6430
AMS 6433 AMS 6430
a Specification does not contain minimum mechanical properties. b Noncurrent specification.
Table 2.3.1.0(b). Material Specifications for Consumable Electrode Melted LowAlloy Steels
Form Alloy
Sheet, strip, and plate
Bar and forgings
Tubing
4340
AMS 6454a
AMS 6414
AMS 6414
D6AC
AMS 6439
AMS 6431, AMS 6439
AMS 6431
4330V
...
AMS 6411
AMS 6411
HyTuf
...
AMS 6425
AMS 6425
4335V
AMS 6435
AMS 6429
AMS 6429
300M (0.40C)
...
AMS 6417
AMS 6417
300M (0.42C)
...
AMS 6419, AMS 6257
AMS 6419, AMS 6257
a Specification does not contain minimum mechanical properties.
216
MMPDS01 31 January 2003
Table 2.3.1.0(c1). Design Mechanical and Physical Properties of Air Melted LowAlloy Steels
Alloy . . . . . . . . . . . . . . . . . . .
AISI 4130
AISI 4135
AISI 8630
Specification [see Tables 2.3.1.0(a) and (b)] . . . . . . . . .
AMS 6360 AMS 6373 AMS 6374 AMST6736 AMSS18729
AMS 6365 AMST6735a
AMSS18728a
Form . . . . . . . . . . . . . . . . . . . .
Sheet, strip, plate, and tubing
Tubing
Sheet, strip, and plate
Normalized and tempered, stress relievedb
Condition . . . . . . . . . . . . . . . . Thickness or diameter, in. . . .
#0.188
>0.188
#0.188
#0.188
#0.188
#0.188
Basis . . . . . . . . . . . . . . . . . . . .
S
S
S
S
S
S
Ftu, ksi . . . . . . . . . . . . . . . . .
95
90
100
95
95
90
Fty, ksi . . . . . . . . . . . . . . . . .
75
70
85
80
75
70
Fcy, ksi . . . . . . . . . . . . . . . . .
75
70
89
84
75
70
Fsu, ksi . . . . . . . . . . . . . . . . .
57
54
60
57
57
54
(e/D = 1.5) . . . . . . . . . . . . .
...
...
...
...
...
...
(e/D = 2.0) . . . . . . . . . . . . .
200
190
190
180
200
190
(e/D = 1.5) . . . . . . . . . . . . .
...
...
...
...
...
...
(e/D = 2.0) . . . . . . . . . . . . .
129
120
146
137
129
120
Mechanical Properties:
Fbru, ksi:
Fbry, ksi:
e, percent . . . . . . . . . . . . . . .
See Table 2.3.1.0(d)
E, 103 ksi . . . . . . . . . . . . . . .
29.0
Ec, 103 ksi . . . . . . . . . . . . . .
29.0
G, 103 ksi . . . . . . . . . . . . . . .
11.0
µ .....................
0.32
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . . . . . .
See Figure 2.3.1.0
a Noncurrent specification. b Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing.
217
MMPDS01 31 January 2003
Table 2.3.1.0(c2). Design Mechanical and Physical Properties of Air Melted LowAlloy Steels
Alloy . . . . . . . . . . . . . . . . . . . Specification [see Tables 2.3.1.0(a) and (b)] . . . . . . . . .
AISI 4130 AMS 6361 AMST6736
AMS 6362 AMST6736
Form . . . . . . . . . . . . . . . . . . . .
Tubing
Condition . . . . . . . . . . . . . . . .
Quenched and tempereda
AMST6736
Thickness or diameter, in. . . .
#0.188
#0.188
All Walls
Basis . . . . . . . . . . . . . . . . . . . .
S
S
S
Ftu, ksi . . . . . . . . . . . . . . . . .
125
150
180
Fty, ksi . . . . . . . . . . . . . . . . .
100
135
165
Fcy, ksi . . . . . . . . . . . . . . . . .
109
141
173
Fsu, ksi . . . . . . . . . . . . . . . . .
75
90
108
(e/D = 1.5) . . . . . . . . . . . . .
194
231
277
(e/D = 2.0) . . . . . . . . . . . . .
251
285
342
(e/D = 1.5) . . . . . . . . . . . . .
146
210
257
(e/D = 2.0) . . . . . . . . . . . . .
175
232
284
Mechanical Properties:
Fbru, ksi:
Fbry, ksi:
e, percent . . . . . . . . . . . . . . .
See Table 2.3.1.0(e)
E, 103 ksi . . . . . . . . . . . . . . .
29.0
Ec, 103 ksi . . . . . . . . . . . . . .
29.0
G, 103 ksi . . . . . . . . . . . . . . .
11.0
µ .....................
0.32
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . . . . . .
See Figure 2.3.1.0
a Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing.
218
MMPDS01 31 January 2003
Table 2.3.1.0(c3). Design Mechanical and Physical Properties of Air Melted LowAlloy Steels
Alloy . . . . . . . . . . . . . . . . . . .
AISI 8630
Specification [see Tables 2.3.1.0(a) and (b)] . . . . . . . . .
AMSS6050
AISI 8740 AMSS6049a
AMS 6327
Form . . . . . . . . . . . . . . . . . . . .
Bars and forgings
Condition . . . . . . . . . . . . . . . .
Quenched and temperedb
Thickness or diameter, in. . . .
#1.500
#1.750
Basis . . . . . . . . . . . . . . . . . . . .
S
S
Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . . .
125
125
125
Fty, ksi . . . . . . . . . . . . . . . . .
100
103
100
Fcy, ksi . . . . . . . . . . . . . . . . .
109
108
109
Fsu, ksi . . . . . . . . . . . . . . . . .
75
75
75
(e/D = 1.5) . . . . . . . . . . . . .
194
192
194
(e/D = 2.0) . . . . . . . . . . . . .
251
237
251
(e/D = 1.5) . . . . . . . . . . . . .
146
160
146
(e/D = 2.0) . . . . . . . . . . . . .
175
177
175
Fbru, ksi:
Fbry, ksi:
e, percent . . . . . . . . . . . . . . .
See Table 2.3.1.0(e)
E, 103 ksi . . . . . . . . . . . . . . .
29.0
Ec, 103 ksi . . . . . . . . . . . . . .
29.0
G, 103 ksi . . . . . . . . . . . . . . .
11.0
µ .....................
0.32
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . . . . . .
See Figure 2.3.1.0
a Noncurrent specification b Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing.
219
MMPDS01 31 January 2003
Table 2.3.1.0(c4). Design Mechanical and Physical Properties of Air Melted LowAlloy Steels
Alloy . . . . . . . . . . . . . . . . . . .
AISI 4135
Specification [see Tables 2.3.1.0(a) and (b)] . . . . . . . . .
AMST6735
Form . . . . . . . . . . . . . . . . . . . .
Tubing
Condition . . . . . . . . . . . . . . . .
Quenched and tempereda #0.8
Wall thickness, in. . . . . . . . . . Basis . . . . . . . . . . . . . . . . . . . .
< 0.5b
S
S
S
S
Ftu, ksi . . . . . . . . . . . . . . . . .
125
150
180
200
Fty, ksi . . . . . . . . . . . . . . . . .
100
135
165
165
Fcy, ksi . . . . . . . . . . . . . . . . .
109
141
173
181
Fsu, ksi . . . . . . . . . . . . . . . . .
75
90
108
120
(e/D = 1.5) . . . . . . . . . . . . .
194
231
277
308
(e/D = 2.0) . . . . . . . . . . . . .
251
285
342
380
(e/D = 1.5) . . . . . . . . . . . . .
146
210
257
274
(e/D = 2.0) . . . . . . . . . . . . .
175
232
284
302
Mechanical Properties:
Fbru, ksi:
Fbry, ksi:
e, percent . . . . . . . . . . . . . . .
See Table 2.3.1.0(e)
E, 103 ksi . . . . . . . . . . . . . . .
29.0
Ec, 103 ksi . . . . . . . . . . . . . .
29.0
G, 103 ksi . . . . . . . . . . . . . . .
11.0
µ .....................
0.32
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . . . . . .
See Figure 2.3.1.0
a Design values are applicable only to parts for which the indicated Ftu and through hardening has been substantiated by adequate quality control testing. b Wall thickness at which through hardening is achieved and verified through quality control testing. b The Sbasis value in MILT6735 is 165 ksi.
220
MMPDS01 31 January 2003
Table 2.3.1.0(d). Minimum Elongation Values for LowAlloy Steels in Condition N
Elongation, percent Form
Thickness, in.
Full tube
Strip
Sheet, strip, and plate (T) . . . . . .
Less than 0.062 . . . . . . . . . . . . . . .

8
Over 0.062 to 0.125 incl. . . . . . . . .

10
Over 0.125 to 0.187 incl. . . . . . . . .

12
Over 0.187 to 0.249 incl. . . . . . . . .

15
Over 0.249 to 0.749 incl. . . . . . . . .

16
Over 0.749 to 1.500 incl. . . . . . . . .

18
Up to 0.035 incl. (wall) . . . . . . . . .
10
5
Over 0.035 to 0.188 incl. . . . . . . . .
12
7
Over 0.188 . . . . . . . . . . . . . . . . . . .
15
10
Tubing (L) . . . . . . . . . . . . . . . . .
Table 2.3.1.0(e). Minimum Elongation Values for HeatTreated LowAlloy Steels
Elongation in 2 in., percent Sheet specimens
Round specimens (L)
Tubing (L)
Ftu, ksi
Elongation in 4D, percent
Reduction of area, percent
Less than 0.032 in. thick
0.032 to 0.060 in. thick
Over 0.060 in. thick
Full tube
Strip
125
17
55
5
7
10
12
7
140
15
53
4
6
9
10
6
150
14
52
4
6
9
10
6
160
13
50
3
5
8
9
6
180
12
47
3
5
7
8
5
200
10
43
3
4
6
6
5
221
MMPDS01 31 January 2003 Table 2.3.1.0(f1). Design Mechanical and Physical Properties of LowAlloy Steels Alloy . . . . . . . . . . . . . . .
HyTuf
4330V
4335V
4335V
D6AC
AISI 4340a
0.40C 300M
0.42C 300M AMS 6257 AMS 6419
Specification . . . . . . . . . . AMS 6425 AMS 6411 AMS 6430 AMS 6429 AMS 6431 AMS 6414 AMS 6417 Form . . . . . . . . . . . . . . . .
Bar, forging, tubing
Condition . . . . . . . . . . . .
Quenched and temperedb
Thickness or diameter, in. Basis . . . . . . . . . . . . . . . .
c
d
e
f
S
S
S
S
S
S
S
S
Ftu, ksi . . . . . . . . . . . . .
220
220
205
240
220
260
270
280
Fty, ksi . . . . . . . . . . . . .
185
185
190
210
190
217
220
230
Fcy, ksi . . . . . . . . . . . . .
193
193
199
220
198
235
236
247
Fsu, ksi . . . . . . . . . . . . .
132
132
123
144
132
156
162
168
(e/D = 1.5) . . . . . . . . .
297
297
315
369
297
347
414g
430g
(e/D = 2.0) . . . . . . . . .
385
385
389
465
385
440
506g
525g
(e/D = 1.5) . . . . . . . . .
267
267
296
327
274
312
344c
360c
(e/D = 2.0) . . . . . . . . .
294
294
327
361
302
346
379c
396c
L ................
10
10
10
10
12
10
8
7
LT . . . . . . . . . . . . . . .
a
a
7
7
9
...
...
...
Mechanical Properties:
Fbru, ksi:
Fbry, ksi:
e, percent:
5
5
E, 103 ksi . . . . . . . . . . .
29.0
Ec, 103 ksi . . . . . . . . . .
29.0
3
G, 10 ksi . . . . . . . . . . .
11.0
µ .................
0.32
Physical Properties: ω, lb/in.3 . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . .
See Figure 2.3.1.0
a Applicable to consumableelectrode vacuummelted material only. b Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. c Thickness# 1.70 in. for quenching in molten salt at desired tempering temperature (martempering); #2.50 in. for quenching in oil at flow rate of 200 feet/min. d Thickness# 3.50 in. for quenching in molten salt at desired tempering temperature (martempering); #5.00 in. for quenching in oil at flow rate of 200 feet/min. e Thickness# 1.70 in. for quenching in molten salt at desired tempering temperature (martempering); #2.50 in. for quenching in oil at flow rate of 200 feet/min.; #3.50 in. for quenching in water at a flow rate of 200 feet/min. f Thickness #5.00 in. for quenching in oil at a flow rate of 200 feet/min. g Bearing values are “dry pin” values per Section 1.4.7.1.
222
MMPDS01 31 January 2003
Table 2.3.1.0(f2). Design Mechanical and Physical Properties of LowAlloy Steels Alloy . . . . . . . . . . . . . . . . . . . .
4335V
D6AC
Specification . . . . . . . . . . . . . .
AMS 6435
AMS 6439
Form . . . . . . . . . . . . . . . . . . . . .
Sheet, strip, and plate
Condition . . . . . . . . . . . . . . . . .
Quenched and tempereda
Thickness or diameter, in. . . . .
b
#0.250
$0.251
Basis . . . . . . . . . . . . . . . . . . . . .
S
S
S
Ftu, ksi . . . . . . . . . . . . . . . . . .
220
215
224
Fty, ksi . . . . . . . . . . . . . . . . . .
190
190
195
Fcy, ksi . . . . . . . . . . . . . . . . . .
198
198
203
Fsu, ksi . . . . . . . . . . . . . . . . . .
132
129
134
(e/D = 1.5) . . . . . . . . . . . . . .
297
290
302
(e/D = 2.0) . . . . . . . . . . . . . .
385
376
392
(e/D = 1.5) . . . . . . . . . . . . . .
274
274
281
(e/D = 2.0) . . . . . . . . . . . . . .
302
302
310
L .....................
10
...
...
LT . . . . . . . . . . . . . . . . . . . .
7
7
7
Mechanical Properties:
Fbru, ksi:c
Fbry, ksi:
c
e, percent:
E, 103 ksi . . . . . . . . . . . . . . . .
29.0
3
29.0
3
G, 10 ksi . . . . . . . . . . . . . . . .
11.0
µ ......................
0.32
Ec, 10 ksi . . . . . . . . . . . . . . .
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . . . . . . .
See Figure 2.3.1.0
a b c
Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. Thickness #1.70 in. for quenching in molten salt at desired tempering temperature (martempering); #2.50 in. for quenching in oil at a flow rate of 200 feet/min. Bearing values are “dry pin” values per Section 1.4.7.1.
223
MMPDS01 31 January 2003
Table 2.3.1.0(g1). Design Mechanical and Physical Properties of LowAlloy Steels Alloy . . . . . . . . . . . . . . . . . . .
AISI 4130
AISI 4135
AISI 8630
AISI 8735
Specification [see Tables 2.3.1.0(a) and (b)] . . . . . . . . .
AMS 6350 AMS 6528 AMSS6758
AMS 6352 AMS 6372
AMS 6281
AMS 6357
Form . . . . . . . . . . . . . . . . . . . .
Sheet, strip, plate, bars, and forgings
Sheet, strip, plate, and tubing
Tubing
Sheet, strip, and plate
Normalized and tempered, stress relieveda
Condition . . . . . . . . . . . . . . . . Thickness or diameter, in. . . .
#0.188
>0.188
#0.188
>0.188
#0.188 >0.188 #0.188
>0.188
b
Basis . . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . . .
95
90
95
90
95
90
95
90
Fty, ksi . . . . . . . . . . . . . . . . .
75
70
75
70
75
70
75
70
Fcy, ksi . . . . . . . . . . . . . . . . .
75
70
75
70
75
70
75
70
Fsu, ksi . . . . . . . . . . . . . . . . .
57
54
57
54
57
54
57
54
(e/D = 1.5) . . . . . . . . . . . . .
...
...
...
...
...
...
...
...
(e/D = 2.0) . . . . . . . . . . . . .
200
190
200
190
200
190
200
190
(e/D = 1.5) . . . . . . . . . . . . .
...
...
...
...
...
...
...
...
(e/D = 2.0) . . . . . . . . . . . . .
129
120
129
120
129
120
129
120
Fbru, ksi:
Fbry, ksi:
e, percent . . . . . . . . . . . . . . .
See Table 2.3.1.0(d)
E, 103 ksi . . . . . . . . . . . . . . .
29.0
Ec, 103 ksi . . . . . . . . . . . . . .
29.0
3
G, 10 ksi . . . . . . . . . . . . . . .
11.0
µ .....................
0.32
Physical Properties:
a b
ω, lb/in.3 . . . . . . . . . . . . . . .
0.283
C, K, and α . . . . . . . . . . . . .
See Figure 2.3.1.0
Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. There is no statistical basis (T99 or T90) or specification basis (S) to support the mechanical property values in this table. See Heat Treatment in Section 2.3.0.2.
224
MMPDS01 31 January 2003
Table 2.3.1.0(g2). Design Mechanical and Physical Properties of LowAlloy Steels
Alloy . . . . . . . . . . . . . .
See steels listed in Table 2.3.0.2 for the applicable strength levels
4330V
Specification . . . . . . . . AMS 6427
See Tables 2.3.1.0(a) and (b)
Form . . . . . . . . . . . . . . .
All wrought forms
Condition . . . . . . . . . . .
Quenched and tempereda
Thickness or diameter, in. . . . . . . . . . . . . . . . . .
b
# 2.5
c
d
Basis . . . . . . . . . . . . . . . Mechanical Properties:
Ftu, ksi . . . . . . . . . . . . Fty, ksi . . . . . . . . . . . . Fcy, ksi . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . (e/D = 2.0) . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . (e/D = 2.0) . . . . . . . .
220 185 193 132
125 100 109 75
140 120 131 84
150 132 145 90
160 142 154 96
180 163 173 108
200 176 181 120
297 385
209 251
209 273
219 287
230 300
250 326
272 355
267 294
146 175
173 203
189 218
202 231
230 256
255 280
e, percent: L ............... LT . . . . . . . . . . . . . .
10 5a
See Table 2.3.1.0(e)
E, 103 ksi . . . . . . . . . . Ec, 103 ksi . . . . . . . . . G, 103 ksi . . . . . . . . . . µ ................
29.0 29.0 11.0 0.32
Physical Properties: ω, lb/in.3 . . . . . . . . . . C, K, and α . . . . . . . . a b
c
d
0.283 See Figure 2.3.1.0
Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. For Ftu # 180 ksi, thickness # 0.50 in. for AISI 4130 and 8630; # 0.80 in. for AISI 8735, 4135, and 8740; # 1.00 in. for AISI 4140; # 1.70 in. for AISI 4340, 4330V, 4335V, and HyTuf [Quenched in molten salt at desired tempering temperature (martempering)]; # 2.50 in. for AISI 4340, 4330V, 4335V, and HyTuf (Quenched in oil at a flow rate of 200 feet/min.); # 3.50 in. for AISI 4340 (Quenched in water at a flow rate of 200 feet/min.); # 5.00 in. for D6AC (Quenched in oil at a flow rate of 200 feet/min.) For Ftu = 200 ksi AISI 4130, 8630, 4135, 8740 not available; thickness # 0.80 in. for AISI 8740; # 1.00 in. for AISI 4140; # 1.70 in. for AISI 4340, 4330V, 4335V, and HyTuf [Quenched in molten salt at desired tempering temperature (martempering)]; # 2.50 in. for AISI 4340, 4330V, 4335V, and HyTuf (Quenched in oil at a flow rate of 200 feet/min.); # 3.50 in. for AISI 4340 (Quenched in water at a flow rate of 200 feet/min.); # 5.00 in. for D6AC (Quenched in oil at a flow rate of 200 feet/min.) There is no statistical basis (T99 or T90) or specification basis (S) to support the mechanical property values in this table. See Heat Treatment in Section 2.3.0.2.
225
MMPDS01 31 January 2003
45
45
40
40
35
35
30
30
25
25
C, Btu/ (lb)(°F)
20 0.4 15 0.3 10
α  Between 70 °F and indicated temperature K  At indicated temperature C  At indicated temperature
9 α, 4130
8 7
α, 4340
6 K, 4130
α, 106 in./in./°F
50
K, Btu/ [ (hr)(ft2)(°F)/ft]
50
5 4
20 K, 4340
3
15 10
5 0.2
5
0.1 0
0 400
200
0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.3.1.0. Effect of temperature on the physical properties of 4130 and 4340 alloy steels.
226
MMPDS01 31 January 2003
200 Strength at temperature Exposure up to 1/2 hr
180
Percentage of room Temperature Strength
160 140 120 Fty
100 80 Ftu
60 Fty
40 20 0 400
200
0
200
400
600
800
1000
1200
Temperature, F Figure 2.3.1.1.1. Effect of temperature on the tensile ultimate strength (Ftu) and tensile yield strength (Fty) of AISI lowalloy steels (all products).
227
MMPDS01 31 January 2003 100 Strength at temperature Exposure up to ½ hr
Percentage of Room Temperature Strength
80
60
Fcy 40 Fsu
20
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.3.1.1.2. Effect of temperature on the compressive yield strength (Fcy) and the shear ultimate strength (Fsu) of heattreated AISI lowalloy steels (all products).
100 Fbry
Strength at temperature Exposure up to ½ hr
Percentage of Room Temperature Strength
80 Fbru Fbry 60
40
20
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.3.1.1.3. Effect of temperature on the bearing ultimate strength (Fbru) and the bearing yield strength (Fbry) of heattreated AISI lowalloy steels (all products).
228
MMPDS01 31 January 2003
120
110
Percentage of Room Temperature Modulus
E & Ec 100
90
80
Modulus at temperature Exposure up to 1/2 hr TYPICAL
70
60 200
0
200
400
600
800
1000
Temperature, °F
Figure 2.3.1.1.4. Effect of temperature on the tensile and compressive modulus (E and Ec) of AISI lowalloy steels.
Figure 2.3.1.2.6(a). Typical tensile stressstrain curves at room temperature for heattreated AISI 8630 alloy steel (all products).
229
MMPDS01 31 January 2003 200
150ksi level
150
Stress, ksi
125ksi level
100 Normalized
50 TYPICAL
0 0
5
10
15
20
25
30
3 Compressive Tangent Modulus, 10 ksi
Figure 2.3.1.2.6(b). Typical compressive tangentmodulus curves at room temperature for heattreated AISI 8630 alloy steel (all products).
120 500 °F 100 850 °F
Stress, ksi
80 1000 °F 60
RambergOsgood 40
n (500 °F) = 9.0 n (850 °F) = 19 n (1000 °F) = 4.4 TYPICAL
20
1/2hr exposure
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 2.3.1.2.6(c). Typical tensile stressstrain curves at elevated temperatures for heattreated AISI 8630 alloy steel, Ftu = 125 ksi (all products).
230
MMPDS01 31 January 2003
Figure 2.3.1.2.8(a). Bestfit S/N curves for unnotched 4130 alloy steel sheet, normalized, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(a) Test Parameters: Loading  Axial Frequency  11001800 cpm Temperature  RT Environment  Air
Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 117
Specimen Details:
TYS, ksi Temp., EF 99 RT
Unnotched 2.883.00 inches gross width 0.801.00 inch net width 12.0 inch net section radius
No. of Heats/Lots: Not specified Equivalent Stress Equations:
Surface Condition: Electropolished
For stress ratios of 0.60 to +0.02 Log Nf = 9.652.85 log (Seq  61.3) Seq = Smax (1R)0.41 Std. Error of Estimate, Log (Life) = 0.21 Standard Deviation, Log (Life) = 0.45 R2 = 78%
References: 3.2.3.1.8(a) and (f) [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Sample Size = 23 For a stress ratio of 1.0 Log Nf = 9.273.57 log (Smax43.3)
231
MMPDS01 31 January 2003
Figure 2.3.1.2.8(b). Bestfit S/N curves for notched, Kt = 1.5, 4130 alloy steel sheet, normalized, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(b) Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 117 123
Specimen Details:
Test Parameters: Loading  Axial Frequency  11001500 cpm Temperature  RT Environment  Air
TYS, ksi Temp., EF 99 RT (unnotched) RT (notched) Kt 1.5
No. of Heats/Lots: Not specified Equivalent Stress Equations: Log Nf = 7.942.01 log (Seq  61.3) Seq = Smax (1R)0.88 Std. Error of Estimate, Log (Life) = 0.27 Standard Deviation, Log (Life) = 0.67 R2 = 84%
Edge Notched, Kt = 1.5 3.00 inches gross width 1.50 inches net width 0.76 inch notch radius
Surface Condition: Electropolished Sample Size = 21 Reference:
3.2.3.1.8(d) [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
232
MMPDS01 31 January 2003
Figure 2.3.1.2.8(c). Bestfit S/N curves for notched, Kt = 2.0, 4130 alloy steel sheet, normalized, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(c) Test Parameters: Loading  Axial Frequency  11001800 cpm Temperature  RT Environment  Air
Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 117 120
TYS, ksi Temp., EF 99 RT (unnotched) RT (notched) Kt 2.0
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 17.16.49 log (Seq) Seq = Smax (1R)0.86 Std. Error of Estimate, Log (Life) = 0.19 Standard Deviation, Log (Life) = 0.78 R2 = 94%
Specimen Details: Notched, Kt = 2.0 Notch Gross Net Notch Type Width Width Radius Edge 2.25 1.500 0.3175 Center 4.50 1.500 1.500 Fillet 2.25 1.500 0.1736
Sample Size = 107 Surface Condition: Electropolished [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
References: 3.2.3.1.8(b) and (f)
233
MMPDS01 31 January 2003 . .
80 70
x
x
60
Maximum Stress, ksi
4130 Sheet Normalized, Kt=4.0, Edge and Fillet Notches, Mean Stress = 0.0 10.0 + 20.0 30.0 x Runout →
x
x + ++
++
x +
+
x
+ + + ++
50
x+
x x
40
x x
x
+
x
+ + ++ +
+ +++
30
+ + +
+
→ →
→ → → →
20 10
x→ x→ +→ + → +→ + + → → + →
Note: Stresses are based on net section.
0 103
10 4
10 5
10 6
10 7
10 8
Fatigue Life, Cycles Figure 2.3.1.2.8(d). Bestfit S/N curves diagram for notched, Kt = 4.0, 4130 alloy steel sheet, normalized, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(d) Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi TYS, ksi 117 99 120
—
Test Parameters: Loading  Axial Frequency  11001800 cpm Temperature  RT Environment  Air
Temp., EF RT (unnotched) RT (notched) Kt = 4.0
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 12.64.69 log (Seq) Seq = Smax (1R)0.63 Std. Error of Estimate, Log (Life) = 0.24 Standard Deviation, Log (Life) = 0.70 R2 = 88%
Specimen Details: Notched, Kt = 4.0 Notch Gross Net Notch Type Width Width Radius Edge 2.25 1.500 0.057 Edge 4.10 1.496 0.070 Fillet 2.25 1.500 0.0195
Sample Size = 87 Surface Condition: Electropolished References:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
3.2.3.1.8(b), (f), and (g)
234
MMPDS01 31 January 2003
Figure 2.3.1.2.8(e). Bestfit S/N curves diagram for notched, Kt = 5.0, 4130 alloy steel sheet, normalized, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(e) Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 117
TYS, ksi 99
120
Specimen Details:
—
Test Parameters: Loading  Axial Frequency  11001500 cpm Temperature  RT Environment  Air
Temp., EF RT (unnotched) RT (notched) Kt = 5.0
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 12.04.57 log (Seq) Seq = Smax (1R)0.56 Std. Error of Estimate, Log (Life) = 0.18 Standard Deviation, Log (Life) = 0.87 R2 = 96%
Edge Notched, Kt = 5.0 2.25 inches gross width 1.50 inches net width 0.075 inch notch radius
Surface Condition: Electropolished Sample Size = 38 Reference:
3.2.3.1.8(c) [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
235
MMPDS01 31 January 2003
Figure 2.3.1.2.8(f). Bestfit S/N curves for unnotched 4130 alloy steel sheet, Ftu = 180 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(f) Test Parameters: Loading  Axial Frequency  201800 cpm Temperature  RT Environment  Air
Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 180
Specimen Details:
TYS, ksi 174
Temp., EF RT
Unnotched 2.88 inches gross width 1.00 inch net width 12.0 inch net section radius
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 20.37.31 log (Seq) Seq = Smax (1R)0.49 Std. Error of Estimate, Log (Life) = 0.39 Standard Deviation, Log (Life) = 0.89 R2 = 81%
Surface Condition: Electropolished Reference:
3.2.3.1.8(f)
Sample Size = 27 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
236
MMPDS01 31 January 2003 . .
140 4130 Sht Hard, KT=2.0 EN Mean Stress 0.0 50.0
Maximum Stress, ksi
120
→
Runout
100
80 → →
60
40 →
20
→
→
Note: Stresses are based on net section.
0 10 3
10 4
10 5
10 6
10 7
10 8
Fatigue Life, Cycles Figure 2.3.1.2.8(g). Bestfit S/N curves for notched, Kt = 2.0, 4130 alloy steel sheet, Ftu = 180 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(g) Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 180
Specimen Details:
TYS, ksi 174
Test Parameters: Loading  Axial Frequency  211800 cpm Temperature  RT Environment  Air
Temp., EF RT
Edge Notched 2.25 inches gross width 1.50 inches net width 0.3175 inch notch radius
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 8.872.81 log (Seq  41.5) Seq = Smax (1R)0.46 Std. Error of Estimate, Log (Life) = 0.18 Standard Deviation, Log (Life) = 0.77 R2 = 94%
Surface Condition: Electropolished Reference:
3.2.3.1.8(f)
Sample Size = 19 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
237
MMPDS01 31 January 2003
Figure 2.3.1.2.8(h). Bestfit S/N curves for notched, Kt = 4.0, 4130 alloy steel sheet, Ftu = 180 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.2.8(h) Test Parameters: Loading  Axial Frequency  231800 cpm Temperature  RT Environment  Air
Product Form: Sheet, 0.075 inch thick Properties:
TUS, ksi 180
Specimen Details:
TYS, ksi 174
Temp., EF RT
Edge Notched 2.25 inches gross width 1.50 inches net width 0.057 inch notch radius
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 12.44.45 log (Seq) Seq = Smax (1R)0.60 Std. Error of Estimate, Log (Life) = 0.11 Standard Deviation, Log (Life) = 0.90 R2 = 98%
Surface Condition: Electropolished Reference:
3.2.3.1.8(f)
Sample Size = 20 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
238
MMPDS01 31 January 2003 200 200ksi level 180ksi level 150
Stress, ksi
140ksi level 100
50
TYPICAL 0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 2.3.1.3.6(a). Typical tensile stressstrain curves at room temperature for heattreated AISI 4340 alloy steel (all products).
300
312 °F
Longitudinal 1/2hr exposure
110 °F 250 RT
Stress, ksi
200
150
RambergOsgood 100
n (RT) = 7.0 n (110 °F) = 8.2 n (312 °F) = 8.9 TYPICAL
50
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 2.3.1.3.6(b). Typical tensile stressstrain curves at cryogenic and room temperature for AISI 4340 alloy steel bar, Ftu = 260 ksi.
239
MMPDS01 31 January 2003
250
Stress, ksi
200
150
100
RambergOsgood
50
n (RT) = 13 TYPICAL 0 0
2
4
6
8
10
12
20
25
30
Strain, 0.001 in./in.
0
5
10
15
Compressive Tangent Modulus, 103 ksi
Figure 2.3.1.3.6(c). Typical compressive stressstrain and compressive tangentmodulus curves at room temperature for AISI 4340 alloy steel bar, Ftu = 260 ksi.
240
MMPDS01 31 January 2003
Figure 2.3.1.3.6(d). Typical biaxial stressstrain curves at room temperature for AISI 4340 alloy steel (machined thinwall cylinders, axial direction = longitudinal direction of bar stock), Ftu = 180 ksi. A biaxial ratio, B, denotes the ratio of hoop stresses to axial stresses.
241
MMPDS01 31 January 2003
B= 4
OO 120
3
2
1.5
1
Axial Stress, FA, percent Fty
100
80
0.67
60
0.50
40
0.33 0.25
20
Cylindrical Specimens 0 0
20
40
60
80
100
0 120
Hoop Stress, FH, percent Fty
Figure 2.3.1.3.6(e). Biaxial yieldstress envelope at room temperature for AISI 4340 alloy steel (machined thinwall cylinders, axial direction = longitudinal direction of bar stock), Ftu = 180 ksi, Fty measured in the hoop direction.
242
MMPDS01 31 January 2003
300
B=
2 0.5
Maximum Principal Stress, ksi
250
1 0, ∞
200
150
100
50
0 0
4
8
12
16
20
24
Strain, 0.001 in./in.
Figure 2.3.1.3.6(f). Typical biaxial stressstrain curves at room temperature for AISI 4340 alloy steel (machined thinwall cylinders, axial direction = longitudinal direction of bar stock), Ftu = 260 ksi. A biaxial ratio B of zero corresponds to the hoop direction.
243
MMPDS01 31 January 2003
B= 4
OO 120
3
2
1.5
1
Axial Stress, FA, percent Fty
100
80
0.67
60
0.50
40
0.33 0.25
20
Cylindrical Specimens 0 0
20
40
60
80
100
0 120
Hoop Stress, FH, percent Fty
Figure 2.3.1.3.6(g). Biaxial yieldstress envelope at room temperature for AISI 4340 alloy steel (machined thinwall cylinders, axial direction = longitudinal direction of bar stock), Ftu = 260 ksi, Fty measured in the hoop direction.
244
MMPDS01 31 January 2003
Figure 2.3.1.3.8(a). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar, Ftu = 125 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(a) Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi TYS, ksi Temp., EF 125 — RT (unnotched) 150 — RT (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 14.966.46 log (Seq60) Seq = Smax (1R)0.70 Std. Error of Estimate, Log (Life) = 0.35 Standard Deviation, Log (Life) = 0.77 R2 = 75%
Specimen Details: Unnotched 0.400 inch diameter Surface Condition: Hand polished to RMS 10 Reference:
2.3.1.3.8(a) Sample Size = 9 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
245
MMPDS01 31 January 2003
Figure 2.3.1.3.8(b). Bestfit S/N curves for notched, Kt = 3.3, AISI 4340 alloy steel bar, Ftu = 125 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(b) Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
TUS, ksi TYS, ksi Temp., EF 125 — RT (unnotched) 150 — RT (notched)
No. of Heat/Lots: 1
Specimen Details: Notched, VGroove, Kt=3.3 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Equivalent Stress Equation: Log Nf = 9.753.08 log (Seq20.0) Seq = Smax (1R)0.84 Std. Error of Estimate, Log (Life) = 0.40 Standard Deviation, Log (Life) = 0.90 R2 = 80%
Surface Condition: Lathe turned to RMS 10
Sample Size = 11
Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(a)
246
MMPDS01 31 January 2003
Figure 2.3.1.3.8(c). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(c) Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi TYS, ksi Temp., EF 158 147 RT (unnotched) 190 — RT (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 10.763.91 log (Seq  101.0) Seq = Smax (1R)0.77 Std. Error of Estimate, Log (Life) = 0.17 Standard Deviation, Log (Life) = 0.33 Adjusted R2 Statistic = 73%
Specimen Details: Unnotched 0.400 inch diameter Surface Condition: Hand polished to RMS 10 Reference:
2.3.1.3.8(b) Sample Size = 9 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
247
MMPDS01 31 January 2003
Figure 2.3.1.3.8(d). Bestfit S/N curves for notched AISI 4340 alloy steel bar, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(d) Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
TUS, ksi TYS, ksi Temp.,EF 158 147 RT (unnotched) 190 — RT (notched)
No. of Heat/Lots: 1
Specimen Details: Notched, VGroove, Kt = 3.3 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Equivalent Stress Equation: Log Nf = 7.902.00 log (Seq40.0) Seq = Smax (1R)0.60 Std. Error of Estimate, Log (Life) = 0.27 Standard Deviation, Log (Life) = 0.74 R2 = 86%
Surface Condition: Lathe turned to RMS 10
Sample Size = 11
Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(a)
248
MMPDS01 31 January 2003
Figure 2.3.1.3.8(e). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar at 600EF, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(e) Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  600EF Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi TYS, ksi Temp., EF 158 147 RT (unnotched) 153 121 600 (unnotched) 190 — RT (notched) 176 — 600 (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 22.369.98 log (Seq60.0) Seq = Smax (1R)0.66 Std. Error of Estimate Log (Life) = 0.24 Standard Deviation, Log (Life) = 1.08 R2 = 95%
Specimen Details: Unnotched 0.400 inch diameter
Sample Size = 11 Surface Condition: Hand polished to RMS 10 Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(b)
249
MMPDS01 31 January 2003
Figure 2.3.1.3.8(f). Bestfit S/N curves for notched, Kt = 3.3, AISI 4340 alloy steel bar at 600EF, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(f) Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi 158 153 190 176
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
TYS, ksi Temp., EF 147 RT (unnotched) 121 600 (unnotched) — RT (notched) — 600 (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 10.393.76 log (Seq30.0) Seq = Smax (1R)0.62 Std. Error of Estimate, Log (Life) = 0.36 Standard Deviation, Log (Life) = 1.06 R2 = 89%
Specimen Details: Notched, VGroove, Kt = 3.3 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Sample Size = 11 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Surface Condition: Lathe turned to RMS 10 Reference:
2.3.1.3.8(b)
250
MMPDS01 31 January 2003
Figure 2.3.1.3.8(g). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar at 800EF, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(g) Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  800EF Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi 158 125 190 154
TYS, ksi Temp., EF 147 RT (unnotched) 101 800 (unnotched) — RT (notched) — 800 (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 17.537.35 log (Seq60.0) Seq = Smax (1R)0.66 Std. Error of Estimate, Log (Life) = 0.42 Standard Deviation, Log (Life) = 0.99 R2 = 82%
Specimen Details: Unnotched 0.400 inch diameter
Sample Size = 15 Surface Condition: Hand polished to RMS 10 Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(b)
251
MMPDS01 31 January 2003
Figure 2.3.1.3.8(h). Bestfit S/N curves for notched, Kt = 3.3, AISI 4340 alloy steel bar at 800EF, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(h) Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi 158 125 190 154
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  800EF Atmosphere  Air
TYS, ksi Temp., EF 147 RT (unnotched) 101 800 (unnotched) — RT (notched) — 800 (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 7.312.01 log (Seq48.6) Seq = Smax (1R)0.92 Std. Error of Estimate, Log (Life) = 0.60 Standard Deviation, Log (Life) = 1.14 R2 = 72%
Specimen Details: Notched, VGroove, Kt = 3.3 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Sample Size = 9 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Surface Condition: Lathe turned to RMS 10 Reference:
2.3.1.3.8(b)
252
MMPDS01 31 January 2003
Figure 2.3.1.3.8(i). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar at 1000EF, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(i) Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  1000EF Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi 158 81 190 98
TYS, ksi Temp., EF 147 RT (unnotched) 63 1000EF (unnotched) — RT (notched) — 1000EF (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 16.857.02 log (Seq40.0) Seq = Smax (1R)0.80 Std. Error of Estimate, Log (Life) = 0.42 Standard Deviation, Log (Life) = 1.20 R2 = 88%
Specimen Details: Unnotched 0.400 inch diameter
Sample Size = 13 Surface Condition: Hand polished to RMS 10 Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(b)
253
MMPDS01 31 January 2003
Figure 2.3.1.3.8(j). Bestfit S/N curves for notched, Kt = 3.3, AISI 4340 alloy steel bar at 1000EF, Ftu = 150 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(j) Product Form: Rolled bar, 1.125 inch diameter, air melted
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  1000EF Atmosphere  Air
Properties: TUS, ksi TYS, ksi Temp., EF 158 147 RT (unnotched) 81 63 1000EF (unnotched) 190 — RT (notched) 98 — 1000EF (notched)
No. of Heat/Lots: 1 Equivalent Stress Equation: Log Nf = 9.763.75 log (Seq30.0) Seq = Smax (1R)0.50 Std. Error of Estimate, Log (Life) = 0.40 Standard Deviation, Log (Life) = 1.22 R2 = 89%
Specimen Details: Notched, VGroove, Kt = 3.3 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Sample Size = 12 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Surface Condition: Lathe turned to RMS 10 Reference:
2.3.1.3.8(b)
254
MMPDS01 31 January 2003
Figure 2.3.1.3.8(k). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar and die forging, Ftu = 200 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(k) Product Form: Rolled bar, 1.125 inch diameter, air melted Die forging (landing gearB36 aircraft), air melted Properties:
TUS, ksi 208, 221 251
TYS, ksi 189, 217 —
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
Temp., EF RT (unnotched) RT (notched)
Specimen Details: Unnotched 0.300 and 0.400inch diameter Surface Condition:
No. of Heat/Lots: 2 Equivalent Stress Equation: Log Nf = 9.312.73 log (Seq93.4) Seq = Smax (1R)0.59 Std. Error of Estimate, Log (Life) = 0.49 Standard Deviation, Log (Life) = 0.93 R2 = 72%
Hand polished to RMS 510 Sample Size = 26
References:
2.3.1.3.8(a) and (c) [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
255
MMPDS01 31 January 2003
Figure 2.3.1.3.8(l). Bestfit S/N curves for notched, Kt = 3.3, AISI 4340 alloy steel bar, Ftu = 200 ksi, longitudinal direction. Correlative Information for Figure 2.3.1.3.8(l)
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi 208 251
TYS, ksi Temp., EF — RT (unnotched) — RT (notched)
No. of Heat/Lots: 1
Specimen Details: Notched, VGroove, Kt = 3.3 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Equivalent Stress Equation: Log Nf = 7.521.96 log (Seq31.2) Seq = Smax (1R)0.65 Std. Error of Estimate, Log (Life) = 0.16 Standard Deviation, Log (Life) = 0.62 R2 = 93%
Surface Condition: Lathe turned to RMS 10
Sample Size = 26
Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(a)
256
MMPDS01 31 January 2003
Figure 2.3.1.3.8(m). Bestfit S/N curves for unnotched AISI 4340 alloy steel bar and billet, Ftu = 260 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(m) Test Parameters: Loading  Axial Frequency  1800 to 2500 cpm Temperature  RT Atmosphere  Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Billet, 6 inches RCS air melted Properties:
TUS, ksi 266, 291 352
TYS, ksi 232 —
Temp., EF RT (unnotched) RT (notched)
No. of Heat/Lots: 2
Surface Condition: Hand polished to RMS 10
Equivalent Stress Equation: Log Nf = 11.623.75 log (Seq80.0) Seq = Smax (1R)0.44 Std. Error of Estimate, Log (Life) = 0.64 Standard Deviation, Log (Life) = 0.86 R2 = 45%
References:
Sample Size = 41
Specimen Details: Unnotched 0.200 and 0.400 inch diameter
2.3.1.3.8(a) and (b)
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
257
MMPDS01 31 January 2003
Figure 2.3.1.3.8(n). Bestfit S/N curves for notched, Kt = 2.0, AISI 4340 alloy steel bar, Ftu = 260 ksi, longitudinal direction. Correlative Information for Figure 2.3.1.3.8(n)
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi 266 390
Test Parameters: Loading  Axial Frequency  2000 to 2500 cpm Temperature  RT Atmosphere  Air
TYS, ksi Temp., EF 232 RT (unnotched) — RT (notched)
No. of Heat/Lots: 1
Specimen Details: Notched, VGroove, Kt = 2.0 0.300 inch gross diameter 0.220 inch net diameter 0.030 inch root radius, r 60E flank angle, ω
Equivalent Stress Equation: Log Nf = 9.462.65 log (Seq50.0) Seq = Smax (1R)0.64 Std. Error of Estimate, Log (Life) = 0.22 Standard Deviation, Log (Life) = 0.34 R2 = 58%
Surface Condition: Lathe turned to RMS 10
Sample Size = 30
Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.3.8(a)
258
MMPDS01 31 January 2003 . .
250 225
+ +
200
Maximum Stress, ksi
AISI 4340 RT Kt=3.0 Stress Ratio 1.00 0.00 + 0.54 Runout →
175
+
+ +
150
Note: Stresses are based on net section.
+ + + +
125
+ → + → + →
+ +
100 → →
75
→
→ → →→
50 25 0 103
104
105
106
107
108
Fatigue Life, Cycles Figure 2.3.1.3.8(o). Bestfit S/N curves for notched, Kt = 3.0, AISI 4340 alloy steel bar, Ftu = 260 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.3.8(o) Test Parameters: Loading—Axial Frequency—2000 to 2500 cpm Temperature—RT Atmosphere—Air
Product Form: Rolled bar, 1.125 inch diameter, air melted Properties:
TUS, ksi TYS, ksi 266 232 352
—
Temp., EF RT (unnotched) RT (notched)
No. of Heats/Lots: 1 Equivalent Stress Equation: Log Nf = 7.141.74 log (Seq  56.4) Seq = Smax (1R)0.51 Std. Error of Estimate, Log (Life) = 0.32 Standard Deviation, Log (Life) = 0.59 R2 = 71%
Specimen Details: Notched, VGroove, Kt = 3.0 0.270 inch gross diameter 0.220 inch net diameter 0.010 inch root radius, r 60E flank angle, ω
Sample Size = 29
Surface Condition: Lathe turned to RMS 10
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Reference: 2.3.1.3.8(a)
259
MMPDS01 31 January 2003
Figure 2.3.1.4.8(a). Bestfit S/N curves for unnotched 300M alloy forging, Ftu = 280 ksi, longitudinal and transverse directions.
Correlative Information for Figure 2.3.1.4.8(a) Test Parameters: Loading  Axial Frequency  1800 to 2000 cpm Temperature  RT Atmosphere  Air
Product Forms: Die forging, 10 x 20 inches CEVM Die forging, 6.5 x 20 inches CEVM RCS billet, 6 inches CEVM Forged Bar, 1.25 x 8 inches CEVM Properties:
TUS, ksi 274294
No. of Heat/Lots: 6
TYS, ksi Temp., EF 227247 RT
Equivalent Stress Equation: Log Nf = 14.85.38 log (Seq63.8) Seq = Sa + 0.48 Sm Std. Error of Estimate, Log (Life) = 55.7 (1/Seq) Standard Deviation, Log (Life) = 1.037 R2 = 82.0
Specimen Details: Unnotched 0.200  0.250 inch diameter Surface Condition: Heat treat and finish grind to a surface finish of RMS 63 or better with light grinding parallel to specimen length, stress relieve References:
Sample Size = 104 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.4.8(a), (c), (d), (e)
260
MMPDS01 31 January 2003
Figure 2.3.1.4.8(b). Bestfit S/N curves for unnotched, Kt = 2.0, 300M alloy forged billet, Ftu = 280 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.4.8(b) Test Parameters: Loading  Axial Frequency Temperature  RT Atmosphere  Air
Product Form: Forged billet, unspecified size, CEVM Properties:
TUS, ksi 290 456
TYS, ksi Temp., EF 242 RT (unnotched) — RT (notched)
No. of Heats/Lots: 3 Equivalent Stress Equation: Log Nf = 12.875.08 log (Seq55.0) Seq = Smax (1R)0.36 Std. Error of Estimate, Log (Life) = 0.79 Standard Deviation, Log (Life) = 1.72 R2 = 79%
Specimen Details: Notched, 60E VGroove, Kt=2.0 0.500 inch gross diameter 0.250 inch net diameter 0.040 inch root radius, r 60E flank angle, ω
Sample Size = 70
Surface Condition: Heat treat and finish grind notch to RMS 63 ± 5; stress relieve Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.4.8(b)
261
MMPDS01 31 January 2003
Figure 2.3.1.4.8(c). Bestfit S/N curves for notched, Kt = 3.0, 300M alloy forging, Ftu = 280 ksi, longitudinal and transverse directions.
Correlative Information for Figure 2.3.1.4.8(c) Test Parameters: Loading  Axial Frequency Temperature  RT Atmosphere  Air
Product Forms: Forged billet, unspecified size, CEVM Die forging, 10 x 20 inches, CEVM Die forging, 6.50 x 20 inches, CEVM Properties:
TUS, ksi 290292 435
TYS, ksi 242247 —
Temp., EF RT (unnotched) RT (notched)
Specimen Details: Notched 60E VGroove, Kt = 3.0 0.500 inch gross diameter 0.250 inch net diameter 0.0145 inch root radius, r 60E flank angle, ω Surface Condition: Heat treat and finish grind notch to RMS 63 or better; stress relieve References:
2.3.1.4.8(a), (b), (c)
262
No. of Heats/Lots: 5 Equivalent Stress Equation: Log Nf = 10.403.41 log (Seq20.0) Seq = Smax (1R)0.51 Std. Error of Estimate, Log (Life) = 18.3 (1/Seq) Standard Deviation, Log (Life) = 2.100 R2 = 97.4 Sample Size = 99 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
MMPDS01 31 January 2003
Figure 2.3.1.4.8(d). Bestfit S/N curves for notched, Kt = 5.0, 300M alloy forged billet, Ftu = 280 ksi, longitudinal direction.
Correlative Information for Figure 2.3.1.4.8(d) Test Parameters: Loading  Axial Frequency Temperature  RT Atmosphere  Air
Product Forms: Forged billet, unspecified size, CEVM Properties:
TUS, ksi 290 379
TYS, ksi Temp., EF 242 RT (unnotched) — RT (notched)
No. of Heat/Lots: 2 Equivalent Stress Equation: Log Nf = 9.613.04 log (Seq10.0) Seq = Smax (1R)0.52 Std. Error of Estimate, Log (Life) = 0.28 Standard Deviation, Log (Life) = 0.81 R2 = 88%
Specimen Details: Notched, 60E VGroove, Kt=5.0 0.500 inch gross diameter 0.250 inch net diameter 0.0042 inch root radius, r 60E flank angle, ω
Sample Size = 48
Surface Condition: Heat treat and finish grind notch to RMS 63 maximum; stress relieve Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
2.3.1.4.8(b)
263
MMPDS01 31 January 2003
Figure 2.3.1.4.9. Fatiguecrackpropagation data for 3.00inch hand forging and 1.80inch thick, 300M steel alloy plate (TUS: 280290 ksi). [References  2.3.1.4.9(a) and (b).] Specimen Thickness: Specimen Width: Specimen Type:
0.9001.000 inches 3.097.41 inches CT
264
Environment: Temperature: Orientation:
Lowhumidity air RT LT and TL
MMPDS01 31 January 2003
Figure 2.3.1.5.9. Fatiguecrackpropagation data for 0.80inch D6AC steel alloy plate. Data include material both oil quenched and salt quenched (TUS: 230240 ksi). [Reference  2.3.1.5.9.] Specimen Thickness: Specimen Width: Specimen Type:
0.700.75 inch 1.55.0 inches CT
Environment: Temperature: Orientation:
265
Dry air and lab air RT LT
MMPDS01 31 January 2003
2.4
INTERMEDIATE ALLOY STEELS
2.4.0 COMMENTS ON INTERMEDIATE ALLOY STEELS — The intermediate alloy steels in this section are those steels that are substantially higher in alloy content than the alloy steels described in Section 2.3, but lower in alloy content than the stainless steels. Typical of the intermediate alloy steels is the 5CrMoV aircraft steel and the 9Ni4Co series of steels. 2.4.0.1 Metallurgical Considerations — The alloying elements added to these steels are similar to those used in the lower alloy steels and, in general, have the same effects. The difference lies in the quantity of alloying additions and the extent of these effects. Thus, higher chromium contents provide improved oxidation resistance. Additions of molybdenum, vanadium, and tungsten, together with the chromium, provide deep airhardening properties and improve the elevatedtemperature strength by retarding the rate of tempering at high temperatures. Additions of nickel to nonsecondary hardening steels lower the transition temperature and improve lowtemperature toughness. 2.4.1 5CRMOV 2.4.1.0 Comments and Properties — Alloy 5CrMoV aircraft steel exhibits high strength in the temperature range up to 1000EF. Its characteristics also include air hardenability in thick sections; consequently, little distortion is encountered in heat treatment. This steel is available either as airmelted or consumable electrode vacuummelted quality although only consumable electrode vacuummelted quality is recommended for aerospace applications. The heat treatment recommended for this steel consists of heating to 1850EF ± 50, holding 15 to 25 minutes for sheet or 30 to 60 minutes for bars depending on section size, cooling in air to room temperature, tempering three times by heating to the temperature specified in Table 2.4.1.0(a) for the strength level desired, holding at temperature for 2 to 3 hours, and cooling in air. Table 2.4.1.0(a). Tempering Temperatures for 5CrMoV Aircraft Steel
Ftu, ksi
Temperature, EF
Hardness, Rc
280 260 240 220
1000 ± 10 1030 ± 10 1050 ± 10 1080 ± 10
5456 5254 4952 4649
Material specifications for 5CrMoV aircraft steel are presented in Table 2.4.1.0(b). The roomtemperature mechanical and physical properties are shown in Tables 2.4.1.0(c) and (d). The mechanical properties are for 5CrMoV steel heat treated to produce a structure containing 90 percent or more martensite at the center prior to tempering.
266
MMPDS01 31 January 2003
Table 2.4.1.0(b). Material Specifications for 5CrMoV Aircraft Steel Specification
Form
AMS 6437 AMS 6488 AMS 6487
Sheet, strip, and plate (air melted) Bar and forging (air melted, premium quality) Bar and forging (CEVM)
The roomtemperature properties of 5CrMoV aircraft steel are affected by extended exposure to temperatures near or above the tempering temperature. The limiting temperature to which the alloy may be exposed for extended periods without significantly affecting its roomtemperature properties may be estimated at 100EF below the tempering temperature for the desired strength level. The effect of temperature on the physical properties is shown in Figure 2.4.1.0.
19
8
6
6
17
α, 10 in./in./°F
7
2
K, Btu/[(hr)(ft )(°F)/ft]
α 18
K 16
5
α  Between 70 °F and indicated temperature K  At indicated temperature
15
4
14 0
200
400
600
800
1000
1200
1400
3 1600
Temperature, °F
Figure 2.4.1.0. Effect of temperature on the physical properties of 5CrMoV aircraft steel.
2.4.1.1 HeatTreated Condition — The effect of temperature on various mechanical properties for heattreated 5CrMoV aircraft steel is presented in Figures 2.4.1.1.1(a) through 2.4.1.1.4.
267
MMPDS01 31 January 2003 Table 2.4.1.0(c). Design Mechanical and Physical Properties of 5CrMoV Aircraft Steel Bar and Forging
Specification . . . . . . . . . . . . . . . . . . . . . . . . . Form . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . . . . . . . . . . . . . . . . . Crosssectional area, in.2. . . . . . . . . . . . . . . . . Basis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ................................ T ................................ Fty, ksi: L ................................ T ................................ Fcy, ksi: L ................................ T ................................ Fsu, ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . . . . . . e, percent: L ................................ T ................................ RA, percent: L ................................ T ................................ E, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . µ ................................. Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . . . . . . . . . . K and α . . . . . . . . . . . . . . . . . . . . . . . . . . . . a b c d
AMS 6487 and AMS 6488 Bars and forgings Quenched and tempered a,b
Sc
Sc
... 240
260a 260b
... 280
... 200
215a 215b
... 240
... 220 144
... 234 156
... 260 168
... 400
... 435
... 465
... 315
... 333
... 365
9 ...
8a ...
7 ...
... ...
30a 6b
... ...
S
c
30.0 30.0 11.0 0.36 0.281 0.11 (32EF)d See Figure 2.4.1.0
Longitudinal properties applicable to crosssectional area #25 sq. in. Transverse properties applicable only to product sufficiently large to yield tensile specimens not less than 4.50 inches in length. Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. Calculated value.
268
MMPDS01 31 January 2003
Table 2.4.1.0(d). Design Mechanical and Physical Properties of 5CrMoV Aircraft Steel Sheet, Strip, and Plate
Specification . . . . . . . . . . . . . . . . . . . .
AMS 6437
Form . . . . . . . . . . . . . . . . . . . . . . . . . . .
Sheet, strip, and plate
Condition . . . . . . . . . . . . . . . . . . . . . . .
Quenched and tempered
Thickness, in. . . . . . . . . . . . . . . . . . . . Basis . . . . . . . . . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ........................... LT . . . . . . . . . . . . . . . . . . . . . . . . . . Fty, ksi: L ........................... LT . . . . . . . . . . . . . . . . . . . . . . . . . . Fcy, ksi: L ........................... LT . . . . . . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . e, percent: L ........................... LT, in 2 inchesb . . . . . . . . . . . . . . . . LT, in 1 inch . . . . . . . . . . . . . . . . . .
... Sa
Sa
... 240
... 260
... 280
... 200
... 220
... 240
... 220 144
... 240 156
... 260 168
... 400
... 435
... 465
... 315
... 340
... 365
... 6 8
... 5 7
... 4 6
S
a
E, 103 ksi . . . . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . . . . . µ ............................
30.0 30.0 11.0 0.36
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . . . . . K and α . . . . . . . . . . . . . . . . . . . . . . . a b c
0.281 0.11c (32EF) See Figure 2.4.1.0
Design values are applicable only to parts for which the indicated Ftu has been substantiated by adequate quality control testing. For sheet thickness greater than 0.050 inch. Calculated value.
269
MMPDS01 31 January 2003
Percentage of Room Temperature Ftu
100
Strength at temperature Exposure up to 1000 hr
80
60 1/2 hr 10 hr 40 100 hr 1000 hr
20
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.4.1.1.1(a). Effect of temperature on the ultimate tensile strength (Ftu) of 5CrMoV aircraft steel.
Percentage of Room Temperature Fty
100
Strength at temperature Exposure up to 1000 hr
80
60
1/2 hr
10 hr
40
100 hr 20
1000 hr
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.4.1.1.1(b). Effect of temperature on the tensile yield strength (Fty) of 5CrMoV aircraft steel.
270
MMPDS01 31 January 2003 100
Percentage of Room Temperature Fcy
Strength at temperature Exposure up to 1000 hr 80
60
1/2 hr and 10 hr
100 hr
40
1000 hr
20
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.4.1.1.2(a). Effect of temperature on the compressive yield strength (Fcy) of 5CrMoV aircraft steel.
100
Percentage of Room Temperature Fsu
Strength at temperature Exposure up to 1000 hr 80 1/2 hr and 10 hr 60
100 hr
40
1000 hr 20
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.4.1.1.2(b). Effect of temperature on the ultimate shear strength (Fsu) of 5CrMoV aircraft steel.
271
MMPDS01 31 January 2003 100
Percentage of Room Temperature Fbru
Strength at temperature Exposure up to 1000 hr 80
1/2 hr and 10 hr 60
40
100 hr
1000 hr 20
0 0
200
400
600
800
1000
1200
1400
1600
Temperature, °F
Figure 2.4.1.1.3(a). Effect of temperature on the ultimate bearing strength (Fbru) of 5 CrMoV aircraft steel.
.
100
Strength at temperature Exposure up to 1000 hr
Percentage of Room Temperature Fbry
80
60
1/2 hr and 10 hr
40
100 hr 20
1000 hr
0
0
200
400
600
800
1000
1200
1400
1600
Temperature, F
Figure 2.4.1.1.3(b). Effect of temperature on the bearing yield strength (Fbry) of 5CrMoV aircraft steel.
272
MMPDS01 31 January 2003
.
100
Percentage of Room Temperature Modulus
80
E & Ec 60
40
Modulus at temperature Exposure up to 1000 hr 20
0
TYPICAL
0
200
400
600
800
1000
1200
1400
1600
Temperature, F
Figure 2.4.1.1.4. Effect of temperature on the tensile and compressive moduli (E and Ec) of 5CrMoV aircraft steel.
273
MMPDS01 31 January 2003 2.4.2 9NI4CO0.20C 2.4.2.0 Comments and Properties — The 9Ni4Co0.20C alloy was developed specifically to have excellent fracture toughness, excellent weldability, and high hardenability when heattreated to 190 to 210 ksi ultimate tensile strength. The alloy can be readily welded in the heattreated condition with preheat and postheat usually not required. The alloy is through hardening in section sizes up to at least 8 inches thick. The alloy may be exposed to temperatures up to 900EF (approximately 100EF below typical tempering temperature) without microstructural changes which degrade room temperature strength. The heat treatment for this alloy consists of normalizing at 1650 ± 25EF for 1 hour per inch of cross section, cooling in air to room temperature, heating to 1525 ± 25EF for 1 hour per inch of cross section, quenching in oil or water, hold at 100 ± 20EF for 2 hours within 2 hours after quenching, and double tempering at 1035 ± 10EF for 2 hours. A material specification for 9Ni4Co0.20C steel is presented in Table 2.4.2.0(a). Room temperature mechanical and physical properties are shown in Table 2.4.2.0(b). The effect of temperature on thermal expansion is shown in Figure 2.4.2.0. Table 2.4.2.0(a). Material Specification for 9Ni4Co0.20C Steel Specification Form AMS 6523 Sheet, strip, and plate
2.4.2.1 HeatTreated Condition — Effect of temperature on various mechanical properties is presented in Figures 2.4.2.1.1, 2.4.2.1.2, and 2.4.2.1.4. Typical tensile stressstrain curves at room and elevated temperatures are shown in Figure 2.4.2.1.6(a). Typical compression stressstrain and tangentmodulus curves are presented in Figure 2.4.2.1.6(b).
274
MMPDS01 31 January 2003 Table 2.4.2.0(b). Design Mechanical and Physical Properties of 9Ni4Co0.20C Steel Plate
Specification . . . . . . . . . . . . . . . . . . . . . .
AMS 6523
Form . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Plate
Condition . . . . . . . . . . . . . . . . . . . . . . . . .
Quenched and tempered
Thickness, in. . . . . . . . . . . . . . . . . . . . . .
$0.250
25#32 All $0.750 #0.749 S S
7 ...
... ...
... ...
... ... ...
53 ...
60 ...
T62a #25 $0.750 S
6 ...
... ...
... ...
... ... ...
53 ...
60 ...
>25#32 $0.750 S
AMSQQA200/2
a Design allowables were based upon data obtained from testing samples of material, supplied in O or F temper, which were heat treated to demonstrate response to heat treatment by suppliers. b The mechanical properties are to be based upon the thickness at the time of quench. c Sbasis. d Bearing values are “dry pin” values per Section 1.4.7.1. e For 0.3750.499 in.
Specification . . . . . . . . Form . . . . . . . . . . . . . . Temper . . . . . . . . . . . . CrossSectional Area, in.2 Thickness or Dia., in.b . Basis . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L .............. LT (Sbasis) . . . . . Fty, ksi: L .............. LT (Sbasis) . . . . . Fcy, ksi: L .............. LT . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . Fbrud, ksi: (e/D = 1.5) . . . . . . (e/D = 2.0) . . . . . . Fbryd, ksi: (e/D = 1.5) . . . . . . (e/D = 2.0) . . . . . . e, percent (Sbasis): L .............. LT . . . . . . . . . . . . E, 103 ksi . . . . . . . . . Ec, 103 ksi . . . . . . . . . G, 103 ksi . . . . . . . . . µ ................ Physical Properties: ω, lb/in.3 . . . . . . . . . . C, K, and α . . . . . . . .
Table 3.2.1.0(g). Design Mechanical and Physical Properties of 2014 Aluminum Alloy Extrusion
MMPDS01 31 January 2003
MMPDS01 31 January 2003 Table 3.2.1.0(h). Typical StressStrain Parameters for 2014 Aluminum Alloy Temper/Product Form
Condition
Temperature, EF
0.020.039 in. thickness RT 0.040.249 in. thickness ½ hr. exposure 100 hr. exposure ½ and 2 hr. exposure T6 Clad Sheet
1000 hr. exposure
Tension, ksi
Grain Direction
n
TYS
L
32
LT
TUS
nc
CYS
57
17
57
17
57
13
60
L
27
62
15
62
LT
20
60
17
65
9.5
60
8.0
62
4.0
54
6.4
46
8.2
47
10
20
6.0
16
7.0
22
4.3
9
6.0
8
13
7
200EF 300EF
½ hr. exposure
100 hr. exposure
400EF
LT
1000 hr. exposure ½ hr. exposure
500EF
½ hr. exposure 10 hr. exposure
600 EF
100 hr. exposure T62 Clad Plate
0.250  2.000 in. thickness
RT
T651 Plate
0.250  2.000 in. thickness
RT
T6 Bar, Rod and Shapes
> 3 in. thickness
RT
T6 Forging
T652 Hand Forging
T6 Extrusion
RT
2.001  3.000 in. thickness 0.125  0.499 in. thickness > 0.500 in. thickness
RT
RT
T62 Extrusion
< 0.499 in. thickness
RT
T651X Extrusion
0.500  0.749 in. thickness
RT
336
Compression, ksi
L
29
64
27
69
LT
29
64
27
70
L
30
66
15
68
LT
19
65
18
66
L
31
62
25
60
L
70
LT
68
L
18
62
67
17
63
LT
18
62
66
18
65
ST
13
60
22
67
23
62
15
64
26
68
14
72
L
29
64
17
68
LT
29
64
32
68
L
32
64
74
16
68
LT
18
64
70
18
68
L
71
0.60
0.55
160
0.50
140
0.45
120
0.40
α  Between 70 °F and indicated temperature K  At indicated temperature C  At indicated temperature
14 α 13 K (T6)
100
0.35
12
80
0.30
11
0.25
10
60
C 0.20
9
20
0.15
8
0
0.10
40
α, 106 in./in./°F
180
C, Btu/ (lb)(°F)
K, Btu/ [ (hr)(ft2)(°F)/ft]
200
400
200
0
200
400
600
800
1000
Temperature, °F Figure 3.2.1.0. Effect of temperature on the physical properties of 2014 aluminum alloy.
337
MMPDS01 31 January 2003
Figure 3.2.1.1.1(a). Effect of temperature on the tensile ultimate strength (Ftu) of 2014T6, T651, T6510 and T6511 aluminum alloy (bare and clad sheet and plate 0.0401.500 in. thick; extruded bar, rod and shapes $ 0.750 in. thick with crosssectional area # 32 sq. in.).
338
MMPDS01 31 January 2003
160
140
Percent F at Room Temperature tu
120 Strength at temperature Exposure up to 10,000 hr
100
80
60
1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
40
20
0 400
200
0
200
400
600
800
Temperature, F
Figure 3.2.1.1.1(b). Effect of temperature on the ultimate strength (Ftu) of 2014T6, T651, T6510 and T6511 aluminum alloy (bare and clad sheet 0.0200.039 in. thick; bare and clad plate 1.5014.000 in. thick; rolled bar, rod and shapes; hand and die forgings; extruded bar, rod and shapes 0.1250.749 in. thick with crosssectional area # 25 sq. in.).
339
MMPDS01 31 January 2003
160
140
Percent Fty at Room Temperature
120 Strength at temperature Exposure up to 10,000 hr
100
80
60
1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
40
20
0 400
200
0
200
400
600
800
Temperature, F
Figure 3.2.1.1.1(c). Effect of temperature on the tensile yield strength (Fty) of 2014T6, T651, T6510 and T6511 aluminum alloy (bare and clad plate 3.0014.000 in. thick; rolled bar, rod and shapes; hand and die forgings; extruded bar, rod and shapes 0.1250.499 in. thick with crosssectional area # 25 sq. in.).
340
MMPDS01 31 January 2003
160
140
Percent Fty at Room Temperature
120 Strength at temperature Exposure up to 10,000 hr 100
80
60
1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
40
20
0 400
200
0
200
400
600
800
Temperature, °F Figure 3.2.1.1.1(d). Effect of temperature on the tensile yield strength (Fty) of 2014T6, T651, T6510, and T6511 aluminum alloy (bare and clad sheet and plate 0.0203.000 in. thick; extruded bar, rod and shapes 0.5000.749 in. thick with crosssectional area # 25 sq. in. and $ 0.750 in. thick with crosssectional area # 32 sq. in.).
341
MMPDS01 31 January 2003
Percentage of Room Temperature Ftu
100
80 1/2 10 100 1000 10,000
60
hr hr hr hr hr
40
20 Strength at room tem perature Exposure up to 10,000 hr
N ot applicable to extrusions w ith t > 0.75 inch
0 0
100
200
300
400
500
600
700
800
Tem perature, °F
Figure 3.2.1.1.1(e). Effect of exposure at elevated temperatures on the roomtemperature tensile ultimate strength (Ftu) of 2014T6, T651, T6510, and T6511 aluminum alloy (all products except thick extrusions).
Percentage of Room Temperature Fty
100
80 1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
60
40 Not applicable to exrtrusions with t > 0.75 inch 20 Strength at room temperature Exposure up to 10,000 hr 0 0
100
200
300
400
500
600
700
Temperature, F
Figure 3.2.1.1.1(f). Effect of exposure at elevated temperature on the roomtemperature tensile yield strength (Fty) of 2014T6, T651, T6510, and T6511 aluminum alloy (all products except thick extrusions).
342
800
MMPDS01 31 January 2003
Percentage of Room Temperature Fcy
100
80
1/2 hr 2 hr 10 hr 100 hr 1000 hr
60
40
Strength at temperature Exposure up to 10,000 hr 20
Not applicable to extrusions with t > 0.75 inch 0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.1.1.2(a). Effect of temperature on the compressive yield strength (Fcy) of 2014T6, T651, T6510 and T6511 aluminum alloy (all products except thick extrusions).
Percentage of Room Temperature Fsu
100
80 1/2 hr 2 hr 10 hr 100 hr 1000 hr
60
40 Strength at temperature Exposure up to 1000 hr 20 Not applicable to extrusions with t > 0.75 inch 0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.1.1.2(b). Effect of temperature on the shear ultimate strength (Fsu) of 2014T6, T651, T6510 and T6511 aluminum alloy (all products except thick extrusions).
343
MMPDS01 31 January 2003
Percentage of Room Temperature Fbru
100
80
½ hr 2 hr 10 hr 100 hr 1000 hr
60
40
Strength at temperature Exposure up to 1000 hr 20
Not applicable to extrusions with t > 0.75 inch 0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.1.1.3(a). Effect of temperature on the bearing ultimate strength (Fbru) of 2014T6, T651, T6510 and T6511 aluminum alloy (all products except thick extrusions).
Percentage of Room Temperature Fbry
100
80
½ hr 2 hr 10 hr 100 hr 1000 hr
60
40 Strength at temperature Exposure up to 1000 hr 20 Not applicable to extrusions with t>0.75 inch 0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.1.1.3(b). Effect of temperature on the bearing yield strength (Fbry) of 2014T6, T651, T6510 and T6511 aluminum alloy (all products except thick extrusions).
344
MMPDS01 31 January 2003
Figure 3.2.1.1.4. Effect of temperature on the tensile and compressive moduli (E and Ec) of 2014 aluminum alloy.
345
MMPDS01 31 January 2003
100
Elongation at temperature Exposure up to 10,000 hr
Percent Elongation (e)
80
TYPICAL 60
10,000 hr 1000 hr 100 hr 10 hr 1/2 hr
40
20
0 0
100
200
300
400
500
600
700
800
Temperature, F
Figure 3.2.1.1.5(a). Effect of temperature on the elongation of 2014T6, T651, T6510 and T6511 aluminum alloy (all products except thick extrusions).
100
Elongation at room temperature Exposure up to 10,000 hr
Percent Elongation (e)
80
TYPICAL 1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
60
40
20
0 0
100
200
300
400
500
600
700
800
Temperature, F
Figure 3.2.1.1.5(b). Effect of exposure at elevated temperatures on the roomtemperature elongation of 2014T6, T651, T6510 and T6511 aluminum alloy (all products except thick extrusions).
346
MMPDS01 31 January 2003
100
80
Stress, ksi
Long Transverse 60
Longitudinal
40
RambergOsgood n (Ltension) = 32 n (LTtension) = 17
20
TYPICAL Thickness: 0.020  0.039 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.2.1.1.6(a). Typical tensile stressstrain curves for clad 2014T6 aluminum alloy sheet at room temperature.
100
80
Stress, ksi
Longitudinal 60
Long transverse
40
RambergOsgood n (Ltension) = 27 n (LTtension) = 20
20
TYPICAL Thickness: 0.040  0.249 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.2.1.1.6(b). Typical tensile stressstrain curves for clad 2014T6 aluminum alloy sheet at room temperature.
347
MMPDS01 31 January 2003
100
80
Long transverse
Stress, ksi
Long transverse 60
Longitudinal Longitudinal 40
RambergOsgood n (Lcomp.) = 17 n (LTcomp.) = 13
20
TYPICAL Thickness: 0.020  0.039 in. 0 0
2
4
6 Strain, 0.001 in./in.
8
10
12
3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(c). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at room temperature.
100
80
Stress, ksi
Long transverse
Long transverse
60
Longitudinal
Longitudinal
40
RambergOsgood n (Lcomp.) = 17 n (LTcomp.) = 13
20
TYPICAL Thickness: 0.040  0.249 in. 0 0
2
4
6 Strain, 0.001 in./in.
8
10
12
3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(d). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at room temperature.
348
MMPDS01 31 January 2003
100
Long Transverse
80
Stress, ksi
100hr exposure 1/2hr exposure 60
40
RambergOsgood n (1/2hr exp.) = 9.5 n (100hr exp.) = 8.0
20
TYPICAL 0 0
2
4
6 Strain, 0.001 in./in.
8
10
12
Compressive Tangent Modulus, 103 ksi
Figure 3.2.1.1.6(e). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at 200EF.
100
Long Transverse
Stress, ksi
80
60
1/2 & 2hr exposure 1000hr exposure
40
RambergOsgood 20
n (1/2 & 2hr exp.) = 4.0 n (1000hr exp.) = 6.4 TYPICAL
0 0
2
4
6 Strain, 0.001 in./in.
8
10
12
3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(f). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at 300EF.
349
MMPDS01 31 January 2003
60
Long Transverse 1/2hr exposure
50
RambergOsgood
Stress, ksi
40
n (1/2hr exp.) = 8.2 n (100hr exp.) = 10 n (1000hr exp.) = 6.0 1000hr exposure 100hr exposure
30
TYPICAL
20
10
0 0
2
4
6 Strain, 0.001 in./in.
8
10
12
Compressive Tangent Modulus, 103 ksi
Figure 3.2.1.1.6(g). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at 400EF.
50
Long Transverse
RambergOsgood n (1/2hr exp.) = 7.0
40
Stress, ksi
TYPICAL 1/2hr exposure
30
20
10
0 0
2
4
6 Strain, 0.001 in./in.
8
10
12
Compressive Tangent Modulus, 103 ksi
Figure 3.2.1.1.6(h). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at 500EF.
350
MMPDS01 31 January 2003 25 Long Transverse
20
Stress, ksi
15 100hr exposure 10hr exposure 1/2hr exposure 10
Ramberg  Osgood n (1/2hr exp.) = 4.3 n (10hr exp.) = 6.0 n (100hr exp.) = 13
5
TYPICAL 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(i). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2014T6 aluminum alloy sheet at 600EF.
100
LT  compression L  compression LT  tension L  tension
80 LT  compression L  compression
Stress, ksi
60
Ramberg  Osgood n(Ltension) = 29 n(LTtension) = 29 n (Lcomp.) = 27 n (LTcomp.) = 27
40
20
TYPICAL Thickness = 0.250  2.000 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(j). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for clad 2014T62 aluminum alloy plate at room temperature.
351
MMPDS01 31 January 2003 100
80
L  tension LT  tension
Stress, ksi
60
Ramberg  Osgood n ( L  tension) = 30 n (LT  tension) = 19
40
TYPICAL Thickness = 0.250  2.000 in. 20
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.2.1.1.6(k). Typical tensile stressstrain curves for 2014T651 aluminum alloy plate at room temperature.
100
LT  compression
80
L  compression LT  compression
60
Stress, ksi
L  compression
40 Ramberg  Osgood n (Lcomp.) = 15 n (LTcomp.) = 18 20 TYPICAL Thickness = 0.250  2.000 in.
0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 3.2.1.1.6(l). Typical compressive stressstrain and compressive tangentmodulus curves for 2014T651 aluminum alloy plate at room temperature.
352
MMPDS01 31 January 2003 100
80
L  tension L  compression 60
Stress, ksi
L  compression
40
Ramberg  Osgood n (tension) = 31 n (comp.) = 25 TYPICAL
20
Thickness ≤ 3.000 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(m). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2014T6 aluminum alloy rolled bar, rod, and shapes at room temperature.
100
80
ST  compression LT  compression L  compression L and LT  tension ST  tension
ST  compression LT  compression L  compression
Stress, ksi
60
Ramberg  Osgood n(Ltension) = 18 n(LTtension) = 18 n(STtension) = 13 n (Lcomp.) = 17 n (LTcomp.) = 18 n(STcomp.) = 22
40
20
TYPICAL Thickness = 2.001  3.000 in. 0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 3.2.1.1.6(n). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2014T652 aluminum alloy hand forging at room temperature.
353
MMPDS01 31 January 2003 100
80
L  compression
L  compression 60
Stress, ksi
L  tension
Ramberg  Osgood n (tension) = 23 n (comp.) = 15
40
TYPICAL Thickness = 0.125  0.499 in.
20
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(o). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2014T6 aluminum alloy extrusion at room temperature.
100
80
L  compression L  compression L  tension
Stress, ksi
60
Ramberg  Osgood n (tension) = 26 n (comp.) = 14
40
TYPICAL Thickness > 0.500 in. Area ≤ 25 in.2
20
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(p). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2014T6 aluminum alloy extrusion at room temperature.
354
MMPDS01 31 January 2003 100
LTCompression
80
LCompression LTCompression
60
Stress, ksi
LCompression LTension LTTension
40
Ramberg  Osgood n(Ltension) = 29 n(LTtension) = 17 n (Lcomp.) = 29 n (LTcomp.) = 32
20 TYPICAL Thickness ≤ 0.499 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(q). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2014T62 aluminum alloy extrusion at room temperature.
100
80 L and LT  compression
Stress, ksi
60 LT  tension L  tension Ramberg  Osgood n(Ltension) = 32 n(LTtension) = 16 n (Lcomp.) = 18 n (LTcomp.) = 18
40
20
TYPICAL Thickness = 0.500  0.749 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.1.1.6(r). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2014T651X aluminum alloy extrusion at room temperature.
355
MMPDS01 31 January 2003
Figure 3.2.1.1.6(s). Typical tensile stressstrain curves (full range) for 2014T6 aluminum alloy forging at room temperature.
356
MMPDS01 31 January 2003
[
[
Figure 3.2.1.1.6(t). Typical tensile stressstrain curves (full range) for 2014T652 aluminum alloy forging at room temperature.
357
MMPDS01 31 January 2003
!
;
≤
Figure 3.2.1.1.6(u). Typical tensile stressstrain curves (full range) for 2014T62 aluminum alloy extrusion at room temperature.
358
MMPDS01 31 January 2003
[
[
Figure 3.2.1.1.6(v). Typical tensile stressstrain curves (full range) for 2014T651X aluminum alloy extrusion at room temperature.
359
MMPDS01 31 January 2003
Figure 3.2.1.1.8(a). Bestfit S/N curves for unnotched 2014T6 aluminum alloy, various wrought products, longitudinal direction.
Correlative Information for Figure 3.2.1.1.8(a) Product Form: Drawn rod, 0.75 inch diameter Rolled bar, 1 x 7.5 inch and 1.125 inch diameter Rolled rod, 4.5 inch diameter Extruded rod, 1.25 inch diameter Extruded bar, 1.25 x 4 inch Hand forging, 3 x 6 inch Die forging, 4.5 inch diameter Forged slab, 0.875 inch Properties:
TUS, ksi 6778
Specimen Details:
TYS, ksi 6072
Temp.,EF RT
Unnotched
Gross Diameter, inches Net Diameter, inches 1.00 0.400 0.273 0.100 0.200 0.160 1.00 0.500
Test Parameters: Loading  Axial Frequency  1100 to 3600 cpm Temperature  RT Environment  Air No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 21.499.44 log (Seq) Seq = Smax (1R)0.67 Std. Error of Estimate, Log (Life) = 0.51 Standard Deviation, Log (Life) = 1.25 R2 = 83% Sample Size = 127 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Surface Condition: Mechanically polished and asmachined References:
3.2.1.1.8(a), (b), (d), and (e)
360
MMPDS01 31 January 2003
Figure 3.2.1.1.8(b). Bestfit S/N curves for notched, Kt = 1.6, 2014T6 aluminum alloy rolled bar, longitudinal direction.
Correlative Information for Figure 3.2.1.1.8(b) Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  RT Environment  Air
Product Form: Rolled bar, 1.125 inch diameter Properties:
TUS, ksi 72
Specimen Details:
TYS, ksi 64
Temp.,EF RT
Semicircular circumferential notch, Kt = 1.6 0.45 inch gross diameter 0.4 inch net diameter 0.01 inch root radius 60E flank angle, ω
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 10.654.02 log (Seq20.2) Seq = Smax (1R)0.55 Std. Error of Estimate, Log (Life) = 0.33 Standard Deviation, Log (Life) = 0.87 R2 = 86%
Surface Condition: Polished Reference:
3.2.1.1.8(b) Sample Size = 33 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
361
MMPDS01 31 January 2003
Figure 3.2.1.1.8(c). Bestfit S/N curves for notched, Kt = 2.4, 2014T6 aluminum alloy rolled bar, longitudinal direction.
Correlative Information for Figure 3.2.1.1.8(c) Product Form: Rolled bar, 1.125 inch diameter Properties:
TUS, ksi 72
Specimen Details:
TYS, ksi 64
Test Parameters: Loading  Axial Frequency  1800 cpm Temperature  RT Environment  Air
Temp.,EF RT
Circumferential Vnotch, Kt = 2.4 0.500 inch gross diameter 0.400 inch net diameter 0.032 inch notch radius 60E flank angle, ω
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 10.594.36 log (Seq11.7) Seq = Smax (1R)0.52 Std. Error of Estimate, Log (Life) = 0.38 Standard Deviation, Log (Life) = 1.18 R2 = 90%
Surface Condition: Polished Reference:
3.2.1.1.8(b) Sample Size = 39 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
362
MMPDS01 31 January 2003
Figure 3.2.1.1.8(d). Bestfit S/N curves for notched, Kt = 3.4, 2014T6 aluminum alloy rolled and extruded bar, longitudinal direction.
Correlative Information for Figure 3.2.1.1.8(d) Product Form: Extruded bar, 1.125 inch diameter Properties:
TUS, ksi 75
Specimen Details:
TYS, ksi 67
Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  RT Environment  Air
Temp.,EF RT
Circumferential Vnotch, Kt = 3.4 0.450 inch gross diameter 0.400 inch net diameter 0.010 inch notch radius 60E flank angle, ω
No. of Heats/Lots: Not specified Equivalent Stress Equation: Log Nf = 8.353.10 log (Seq10.6) Seq = Smax (1R)0.52 Std. Error of Estimate, Log (Life) = 0.34 Standard Deviation, Log (Life) = 1.10 R2 = 90%
Surface Condition: Smooth machine finish References:
3.2.1.1.8(b) and (c) Sample Size = 45 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
363
MMPDS01 31 January 2003 . .
60
Maximum Stress, ksi
Alum. 2014T6 Kt=2.4 Stress Ratio  1.000 Runout →
40
20 →→ Note: Stresses are based on net section.
0 103
104
105
106
107
108
Fatigue Life, Cycles Figure 3.2.1.1.8(e). Bestfit S/N curves for notched, Kt = 2.4, 2014T6 aluminum alloy hand forging, longitudinal and short transverse directions.
Correlative Information for Figure 3.2.1.1.8(e) Product Form: Hand forging, 3 x 6 inch Properties:
TUS, ksi TYS, ksi Not specified
Specimen Details:
Test Parameters: Loading  Axial Frequency  Not specified Temperature  RT Environment  Air
Temp.,EF RT
Circumferential Vnotch, Kt = 2.4 0.273 inch gross diameter 0.100 inch net diameter 0.010 inch notch radius 60E flank angle, ω
No. of Heats/Lots: Not specified
Surface Condition: Mechanically polished
Maximum Stress Equation: Log Nf = 12.45.95 log (Smax) Std. Error of Estimate, Log (Life) = 0.53 Standard Deviation, Log (Life) = 0.91 R2 = 66%
Reference:
Sample Size = 28
3.2.1.1.8(d)
364
MMPDS01 31 January 2003 3.2.2 2017 ALLOY 3.2.2.0 Comments and Properties — 2017 is a heattreatable AlCu alloy available in the form of rolled bar, rod, and wire, and is used principally for fasteners. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification for 2017 aluminum alloy is presented in Table 3.2.2.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.2.2.0(b). Figure 3.2.2.0 shows the effect of temperature on thermal expansion. Table 3.2.2.0(a). Material Specifications for 2017 Aluminum Alloy
Specification
Form
AMSQQA225/5 AMS 4118
Rolled bar and rod Bar and rod, rolled or coldfinished
15
13
α, 10
6
in./in./F
14
12
α − B e tw e e n 7 0 F a n d in d ic a te d te m p e r a tu r e 11 4 0 0
2 0 0
0
200
400
600
800
1000
T e m p e ra tu re , F
Figure 3.2.2.0. Effect of temperature on the thermal expansion of 2017 aluminum alloy.
The temper index for 2017 is as follows: Section 3.2.2.1
Temper T4, T451, and T42
3.2.2.1 T4, T451, and T42 Temper — The effect of temperature on modulus elasticity is presented in Figure 3.2.2.1.4. 365
MMPDS01 31 January 2003
Table 3.2.2.0(b). Design Mechanical and Physical Properties of 2017 Aluminum Alloy Bar and Rod; Rolled, Drawn, or ColdFinished Specification . . . . . . . . . . . . .
AMS 4118 and AMSQQA225/5
Form . . . . . . . . . . . . . . . . . . .
Bar and rod; rolled, drawn, or coldfinished
Temper . . . . . . . . . . . . . . . . .
T4, T451, T42a
CrossSectional Area, in.2 . . .
#50
Thickness or Diameter, in. . .
#8.000
Basis . . . . . . . . . . . . . . . . . . .
S
Mechanical Properties: Ftu, ksi: L .................. LT . . . . . . . . . . . . . . . . Fty, ksi: L .................. LT . . . . . . . . . . . . . . . . Fcy, ksi: L .................. LT . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . e, percent (Sbasis): L ..................
55 ... 32 ... 32b ... 33 83 105 45 51 12
E, 103 ksi . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . µ ...................
10.4 10.6 3.95 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . α, 106 in./in./EF . . . . . . . . a b
0.101 0.23 (at 212EF) 78 (at 77EF) See Figure 3.2.2.0
Design allowables were based upon data obtained from testing T4 material and from testing samples of bar and rod, supplied in the O or F temper, which were heat treated to T42 temper to demonstrate response to heat treatment by suppliers. For the stressrelieved temper T451, the Fcy value may be somewhat lower.
366
MMPDS01 31 January 2003
120
Percentage of Room Temperature E & Ec
Modulus at temperature 100
TYPICAL
80
60
40
20 600
400
200
0
200
400
600
800
1000
Temperature, °F Figure 3.2.2.1.4. Effect of temperature on the tensile and compression moduli (E and Ec) of 2017 aluminum alloy.
367
MMPDS01 31 January 2003 3.2.3 2024 ALLOY 3.2.3.0 Comments and Properties — 2024 is a heattreatable AlCu alloy which is available in a wide variety of product forms and tempers. The properties vary markedly with temper; those in T3 and T4 type tempers are noteworthy for their high toughness, while T6 and T8 type tempers have very high strength. This alloy has excellent properties and creep resistance at elevated temperatures. The T6 and T8 type tempers have very high resistance to corrosion. However, as shown in Table 3.1.2.3.1(a), 2024T3, T4, and T42 rolled plate, rod and bar, and extruded shapes and 2024T6 and T62 forgings have a ‘D’ SCC rating. This is the lowest rating and means that SCC failures have occurred in service or would be anticipated if there is any sustained stress. Inservice failures are caused by stresses produced by any combination of sources including solution heat treatment, straightening, forming, fitup, clamping, sustained service loads or high service compression stresses that produce residual tensile stresses. These stresses may be tension or compression as well as the stresses due to the Poisson effect, because the actual failures are caused by the resulting sustained shear stresses. Pinhole flaws in corrosion protection are sufficient for SCC. The weldability of the alloy is discussed in Section 3.1.3.4. The properties of extrusions should be based upon the thickness at the time of quenching prior to machining. Selection of the mechanical properties based upon its final machined thickness may be unconservative; therefore, the thickness at the time of quenching to achieve properties is an important factor in the selection of the proper thickness column. For extrusions having sections with various thicknesses, consideration should be given to the properties as a function of thickness. Material specifications for 2024 are presented in Table 3.2.3.0(a). Roomtemperature mechanical properties are shown in Tables 3.2.3.0(b) through (j2). The effect of temperature on the physical properties of this alloy is shown in Figure 3.2.3.0.
Table 3.2.3.0(a). Material Specifications for 2024 Aluminum Alloy
Specification
AMS 4037 AMS 4035 AMSQQA250/4 AMSQQA250/5 AMS 4120 AMSQQA225/6 AMS 4086 AMSWWT700/3 AMS 4152 AMS 4164 AMS 4165 AMSQQA200/3
Form
Bare sheet and plate Bare sheet and plate Bare sheet and plate Clad sheet and plate Bar and rod, rolled or coldfinished Rolled or drawn bar, rod, and wire Tubing, hydraulic, seamless, drawn Tubing Extrusion Extrusion Extrusion Extruded bar, rod, and shapes
368
MMPDS01 31 January 2003 .
 Between 70 F and indicated temperature K  At indicated temperature C  At indicated temperature 15
14
120
13
K (0)
12
0.30
11
60
0.25
10
6
80
C, Btu/(lb)(F)
2
K, Btu/[(hr)(ft )(F)/ft]
K (T3XX, T4X)
, 10 in./in./F
100
C 0.20
9
20
0.15
8
0
0.10
40
400
200
0
200
400
600
800
7 1000
Temperature, F
Figure 3.2.3.0. Effect of temperature on the physical properties of 2024 aluminum alloy.
The following temper designations are more specifically described than in Table 3.1.2.: T81—The applicable designation for 2024T3 sheet artificially aged to the required strength level. T361—Solution heat treated and naturally aged followed by cold rolling and natural aging treatment. T861—Solution heat treated and naturally aged followed by cold rolling and artificial aging treatment. T72—Solution heat treated and aged by user in accordance with AMS 2770 to provide high resistance to stresscorrosion cracking, applicable only to sheet.
369
MMPDS01 31 January 2003 The temper index for 2024 is as follows: Section 3.2.3.1 3.2.3.2 3.2.3.3 3.2.3.4 3.2.3.5
Temper T3, T351, T3510, T3511, T4, and T42 T361 (supersedes T36) T62 and T72 T81, T851, T8510, and T8511 T861 (supersedes T86)
3.2.3.1 T3, T351, T3510, T3511, T4, and T42 Temper — Figures 3.2.3.1.1(a) through 3.2.3.1.5(b) present elevated temperature curves for various properties. Figures 3.2.3.1.6(a) through (q) present tensile and compressive stressstrain curves and tangentmodulus curves for various product forms and tempers at various temperatures. Figures 3.2.3.1.6(r) through (w) are fullrange, stressstrain curves at room temperature for various product forms. Figures 3.2.3.1.8(a) through (i) provide S/N fatigue curves for unnotched and notched specimens for T3 and T4 tempers. 3.2.3.2 T361 (supersedes T36) Temper — 3.2.3.3 T62 and T72 Temper — Figures 3.2.3.3.1(a) through (d) and 3.2.3.3.5(a) and (b) show the effect of temperature on the tensile properties of the T62 temper. Figure 3.2.3.1.4 can be used for the elevated temperature curve for elastic moduli for this temper. Tensile and compressive stressstrain and tangentmodulus curves at room temperature are shown in Figure 3.2.3.3.6. 3.2.3.4 T81, T851, T852, T8510, and T8511 Temper — Figures 3.2.3.4.1(a) through (d), 3.2.3.4.2(a) and (b), 3.2.3.4.3(a) and (b), and 3.2.3.4.5(a) and (b) present elevated temperature curves for various mechanical properties for the T8XXX temper. Figures 3.2.3.4.1(e) and (f) contain graphs for determining tensile properties after complex thermal exposure. See Section 3.7.4.1 for a detailed discussion of their use. Figures 3.2.3.4.6(a) through (g) present tensile and compressive stressstrain and tangentmodulus curves for various products and tempers. Figures 3.2.3.4.6(h) through (j) are fullrange stressstrain curves at room temperature for various product forms. 3.2.3.5 T861 (T86) Temper — Figures 3.2.3.5.1(a) through (d), 3.2.3.5.2(a) and (b), 3.2.3.5.3(a) through (c), and 3.2.3.5.5(a) and (b) present effectoftemperature curves for various mechanical properties. Figures 3.2.3.5.6(a) through (d) present compressive stressstrain and tangentmodulus curves for sheet material at various temperatures. Graphical displays of the residual strength behavior of centercracked tension panels are presented in Figures 3.2.3.5.10(a) and (b).
370
371
48 42 ... 39 45 ... 38 97 119 72 86
48 43 ... 40 46 ... 41 107 133 75 90 ...
47 42 ... 39 45 ... 40 106 131 73 88 c
12
64 64 ...
66 65 ...
65 64 ...
0.1290.249 A B
...
76 90
100 122
41 47 ... 39
50 44 ...
66 66 ...
8
72 86
95 117
39 45 ... 37
48 42 ...
63 63 ...
...
76 90
98 120
41 47 ... 38
50 44 ...
65 65 ...
72 86
94 115
38 44 ... 37
47 42 ...
62 62 ...
... 6 10.7 10.9 4.0 0.33
76 90
97 119
40 46 ... 38
50 44 ...
64 64 ...
0.100 See Figure 3.2.3.0
7
72 86
94 115
39 44 ... 37
47 42 ...
62 62 ...
...
76 90
97 119
40 46 ... 38
49 44 ...
64 64 ...
4
72 86
91 111
37 43 46 35
46 42 38a
60 60 52a
...
76 90
94 115
39 45 48 37
48 44 40a
62 62 54a
2.0013.000 A B
4
70 84
86 106
35 41 44 34
43 41 38a
57 57 49a
...
74 88
89 109
37 43 47 35
46 43 39a
59 59 51a
3.0014.000 A B
8
82 97
111 137
47 53 ... 42
56 50 ...
68 67 ...
10.5 10.7 4.0 0.33
9
84 99
112 139
48 54 ... 42
56 51 ...
69 68 ...
9d 10.7 10.9 4.0 0.33
81 96
109 135
46 52 ... 41
54 49 ...
67 66 ...
AMSQQA250/4 Sheet Plate T361 0.020 0.063 0.2500.062 0.249 0.500 S S S
a Caution: This specific alloy, temper, and product form exhibits poor stresscorrosion cracking resistance in this grain direction. It corresponds to an SCC resistance rating of D, as indicated in Table 3.1.2.3.1(a). b Bearing values are “dry pin” values per Section 1.4.7.1. See Table 3.1.2.1.1. c See Table 3.2.3.0(c). d 10% for 0.500 inch.
Thickness, in. . . . . . . . . .
0.0080.009 Basis . . . . . . . . . . . . . . . . S Mechanical Properties: Ftu, ksi: L ................ 65 64 64 LT . . . . . . . . . . . . . . . 64 63 63 ST . . . . . . . . . . . . . . . ... ... ... Fty, ksi: L ................ 48 47 47 LT . . . . . . . . . . . . . . . 43 42 42 ST . . . . . . . . . . . . . . . ... ... ... Fcy, ksi: L ................ 39 40 39 LT . . . . . . . . . . . . . . . 45 46 45 ST . . . . . . . . . . . . . . . ... ... ... Fsu, ksi . . . . . . . . . . . . . . 39 40 39 Fbrub, ksi: (e/D = 1.5) . . . . . . . . . 104 104 106 (e/D = 2.0) . . . . . . . . . 129 129 131 Fbryb, ksi: (e/D = 1.5) . . . . . . . . . 73 75 73 (e/D = 2.0) . . . . . . . . . 88 90 88 e, percent (Sbasis): c LT . . . . . . . . . . . . . . . 10 ... 3 E, 10 ksi . . . . . . . . . . . 10.5 Ec, 103 ksi . . . . . . . . . . . 10.7 G, 103 ksi . . . . . . . . . . . 4.0 µ .................. 0.33 Physical Properties: ω, lb/in. . . . . . . . . . . . . . C, K, and α . . . . . . . . . .
Sheet T3 0.0100.128 A B
AMS 4037 and AMSQQA250/4 Plate T351 0.2500.5001.0011.5010.499 1.000 1.500 2.000 A B A B A B A B
Table 3.2.3.0(b1). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Sheet and Plate
Specification . . . . . . . . . . Form . . . . . . . . . . . . . . . . Temper . . . . . . . . . . . . . .
MMPDS01 31 January 2003
372 ... ... 4
67c 80c d
67 80
67 80 12
67 80 d
59 67 ...
56 64 d
52 48 37
52 52 38
5
80c 95c
5
... ...
... ...
... ... ...
... 50
... 63
S
2.0013.000
5
... ...
... ...
... ... ...
... 46
... 60
S
0.0100.249
T72a
a Design allowables in some cases were based upon data obtained from testing samples of material, supplied in the O or F temper, which were heat treated to demonstrate response to heat treatment by suppliers. Properties obtained by the user may be different than those listed if the material has been formed or otherwise cold or hot worked, particularly in the annealed temper, prior to solution heat treatment. b Bearing values are “dry pin” values per Section 1.4.7.1. c See Table 3.1.2.1.1. d See Table 3.2.3.0(c).
0.100 See Figure 3.2.3.0 71 (at 77EF) for T4X and 87 (at 77EF) for T6X, T7X, See Figure 3.2.3.0 See Figure 3.2.3.0
5
80 95
102c 132c
50 50
50 50
103 134
63 63
S
0.5002.000
63 64
S
0.2500.499
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . . . . α, 106 in./in./EF . . . . . . . . . . . .
5
80 95
103 134
52 53 38
50 50
63 64
S
0.0100.249
T62a
AMSQQA250/4
See Table 3.2.3.0(d) See Table 3.2.3.0(d) See Table 3.2.3.0(d) See Table 3.2.3.0(d)
8
... ...
85c 119c
94 121
98 123
99 123
... ... ...
37 41 36
40 41 36
42 41 37
42 41 37
42 42 38
40 40 37 96 122
... 38
38 38
38 38
38 38
38 38
42 42
40 40
93 118
... 58
S
60 60
S
61 61
S
2.0013.000
62 62
S
1.0012.000
62 62
S
0.5001.000
64 64
B
0.2500.499
Flat Sheet and Plate
62 62
A
0.0100.249
T42a
AMS 4035 and AMSQQA250/4
E, 103 ksi . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . µ ........................
Mechanical Properties: Ftu, ksi: L ...................... LT . . . . . . . . . . . . . . . . . . . . . Fty, ksi: L ...................... LT . . . . . . . . . . . . . . . . . . . . . Fcy, ksi: L ...................... LT . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . e, percent (Sbasis): LT . . . . . . . . . . . . . . . . . . . . .
Basis . . . . . . . . . . . . . . . . . . . . . .
0.0100.249
T4
Temper . . . . . . . . . . . . . . . . . . . .
Thickness, in. . . . . . . . . . . . . . . .
Coiled Sheet
Form . . . . . . . . . . . . . . . . . . . . . .
Specification . . . . . . . . . . . . . . . . AMSQQA250/4
Table 3.2.3.0(b2). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Sheet and Plate—Continued
MMPDS01 31 January 2003
MMPDS01 31 January 2003
Table 3.2.3.0(b3). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Sheet and Plate—Continued
Specification . . . . . . .
AMSQQA250/4
Form . . . . . . . . . . . . .
Sheet
Plate
Temper . . . . . . . . . . .
T81
T851
Thickness, in. . . . . . .
0.0100.249
Basis . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ............. LT . . . . . . . . . . . . Fty, ksi: L ............. LT . . . . . . . . . . . . Fcy, ksi: L ............. LT . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . Fbrua, ksi: (e/D = 1.5) . . . . . (e/D = 2.0) . . . . . Fbrya, ksi: (e/D = 1.5) . . . . . (e/D = 2.0) . . . . . e, percent (Sbasis): LT . . . . . . . . . . . .
0.2500.499
Sheet
Plate
T861
0.5001.000
1.0011.499
0.020 0.063 0.2500.062 0.249 0.500
A
B
A
B
S
S
S
S
S
67 67
68 68
67 67
68 68
66 66
66 66
71 70
72 71
70 70
59 58
61 60
58 58
60 60
58 58
57 57
63 62
67 66
64 64
59 58 40
61 60 41
58 59 38
60 61 39
58 58 37
56 57 37
63 65 40
67 69 40
64 67 40
100 127
102 129
102 131
103 133
100 129
100b 129b
108 140
110 142
108 140
83 94
86 97
86 101
89 105
86 101
85b 99b
90 105
96 112
93 109
5
...
5
...
5
5
3
4
4
3
E, 10 ksi . . . . . . . . Ec, 103 ksi . . . . . . . G, 103 ksi . . . . . . . . µ ..............
See Table 3.2.3.0(d) See Table 3.2.3.0(d) See Table 3.2.3.0(d) See Table 3.2.3.0(d)
Physical Properties: ω, lb/in.3 . . . . . . . . C, Btu/(lb)(EF) . . . . K, Btu/[(hr)(ft2)(EF)/ft] α, 106 in./in./EF . . .
0.100 See Figure 3.2.3.0 87 (at 77EF) See Figure 3.2.3.0
a Bearing values are “dry pin” values per Section 1.4.7.1. b See Table 3.1.2.1.1.
373
MMPDS01 31 January 2003
Table 3.2.3.0(c). Minimum Elongation Values for Bare 2024 Aluminum Alloy Sheet and Plate
Elongation (LT), percent Condition
.............................
Thickness, in.: 0.0100.020 0.0210.249 0.2500.499 0.5001.000 1.0011.500 1.5012.000
T3, T4, and T42
.......................... .......................... .......................... .......................... .......................... ..........................
12 15 12 8 7 6
Table 3.2.3.0(d). Modulus Values and Poisson's Ratio for Bare 2024 Aluminum Alloy Sheet and Plate, All Tempers
Property Thickness, in.: 0.0100.249 . . . . . . . . . . . . . . . . . . . . . . $0.250 . . . . . . . . . . . . . . . . . . . . . .
E
Ec
G
µ
10.5 10.7
10.7 10.9
4.0 4.0
0.33 0.33
374
0.0080.009 A B
0.0100.062 A B
0.0630.128 A B
0.1290.249 A B
0.2500.499 A B
0.5001.000a A B
375
62 62 ... 48 42 ... 39 44 ... 37 94 115 72 86 ...
60 60 ... 45 40 ... 37 42 ... 35 91 111 69 82 7
1.0011.500a A B
10.9 10.4
10.7 10.2
6
69 82
91 111
36 42 ... 35
45 40 ...
60 60 ...
...
72 86
94 115
38 44 ... 37
47 42 ...
62 62 ...
T351 1.5012.000a A B 60 60 54b 46 42 40b 37 43 48 35 91 111 72 86 ...
58 58 52b 44 40 38b 35 41 46 34 88 107 69 82 4
2.0013.000a A B
4
67 80
83 102
33 39 44 32
39 39 38b
55 55 49b
...
70 84
86 106
35 41 47 34
41 41 39b
57 57 51b
3.0014.000a A B
a These values, except in the ST direction, have been adjusted to represent the average properties across the whole section, including the 2½ percent nominal cladding thickness. b Caution: This specific alloy, temper, and product form exhibits poor stresscorrosion cracking resistance in this grain direction. It corresponds to an SCC resistance rating of D, as indicated in Table 3.1.2.3.1(a). c Bearing values are “dry pin” values per Section 1.4.7.1. See Table 3.1.2.1.1. d See Table 3.2.3.0(f).
Basis . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L . . . . . . . . . . . . . 59 60 60 61 62 63 63 64 62 64 61 63 LT . . . . . . . . . . . . 58 59 59 60 61 62 62 63 62 64 61 63 ST . . . . . . . . . . . . ... ... ... ... ... ... ... ... ... ... ... ... Fty, ksi: L . . . . . . . . . . . . . 44 45 44 45 45 47 45 47 46 48 45 48 LT . . . . . . . . . . . . 39 40 39 40 40 42 40 42 40 42 40 42 ST . . . . . . . . . . . . ... ... ... ... ... ... ... ... ... ... ... ... Fcy, ksi: L . . . . . . . . . . . . . 36 37 36 37 37 39 37 39 37 39 37 39 LT . . . . . . . . . . . . 42 43 42 43 43 45 43 45 43 45 42 45 ST . . . . . . . . . . . . ... ... ... ... ... ... ... ... ... ... ... ... Fsu, ksi . . . . . . . . . . . 37 37 37 38 38 39 39 40 37 38 36 37 Fbruc, ksi: (e/D = 1.5) . . . . . . 96 97 97 99 101 102 102 104 94 97 92 95 (e/D = 2.0) . . . . . . 119 121 121 123 125 127 127 129 115 119 113 117 Fbryc, ksi: (e/D = 1.5) . . . . . . 68 70 68 70 70 73 70 73 69 72 69 72 (e/D = 2.0) . . . . . . 82 84 82 84 84 88 84 88 82 86 82 86 e, percent (Sbasis): d LT . . . . . . . . . . . . 10 ... ... 15 ... 15 ... 12 ... 8 ... 3 E, 10 ksi: Primary . . . . . . . . 10.5 Secondary . . . . . . 9.5 10.0 Ec, 103 ksi: Primary . . . . . . . . 10.7 Secondary . . . . . . 9.7 10.2 G, 103 ksi . . . . . . . . . ... µ ............... 0.33 Physical Properties: ω, lb/in.3 . . . . . . . . . 0.100 C, K, and α . . . . . . . ...
Thickness, in. . . . . . .
T3
AMSQQA250/5 Flat sheet and plate
Table 3.2.3.0(e1). Design Mechanical and Physical Properties of Clad 2024 Aluminum Alloy Sheet and Plate
Specification . . . . . . . Form . . . . . . . . . . . . . Temper . . . . . . . . . . .
MMPDS01 31 January 2003
MMPDS01 31 January 2003 Table 3.2.3.0(e2). Design Mechanical and Physical Properties of Clad 2024 Aluminum Alloy Sheet and Plate—Continued
Specification . . . . . . .
AMSQQA250/5
Form . . . . . . . . . . . . .
Flat sheet and plate
Coiled sheet
Temper . . . . . . . . . . .
T361
T4 0.0100.062
0.0630.128
Thickness, in. . . . . . .
0.0200.062
0.0630.249
0.2500.499
0.500a
Basis . . . . . . . . . . . . .
S
S
S
S
A
B
A
B
62 61
65 64
65 64
64 63
58 58
59 59
61 61
62 62
53 47
53 48
53 48
52 47
36 36
38 38
38 38
39 39
44 50 38
45 51 40
45 51 40
44 50 39
36 36 37
38 38 37
38 38 38
39 39 39
101 125
105 131
105 131
104 129
96 119
97 121
101 125
102 127
78 92
79 94
79 94
78 92
63 76
66 80
66 80
68 82
8
9
9
10
...
15
...
10.5 9.5
10.5 10.0
10.7 10.2
10.5 9.5
10.5 10.0
10.7 9.7
10.7 10.2
10.9 10.4
10.7 9.7
10.7 10.2
Mechanical Properties: Ftu, ksi: L .............. LT . . . . . . . . . . . . Fty, ksi: L .............. LT . . . . . . . . . . . . Fcy, ksi: L .............. LT . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . (e/D = 2.0) . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . (e/D = 2.0) . . . . . . e, percent (Sbasis): LT . . . . . . . . . . . . E, 103 ksi: Primary . . . . . . . . Secondary . . . . . . Ec, 103 ksi: Primary . . . . . . . . Secondary . . . . . .
c
G, 103 ksi . . . . . . . . µ ...............
... 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . C, K, and α . . . . . . .
0.100 ...
a These values have been adjusted to represent the average properties across the whole section, including the 2½ percent nominal cladding thickness. b Bearing values are “dry pin” values per Section 1.4.7.1. c See Table 3.2.3.0(f).
376
377
b c d e
a
10.7 10.2
10.7 9.7
15 10.5 10.0
...
e
...
10
63 76
96 119
40 39 36
36 36
60 60
...
67 80
99 123
42 41 37
38 38
62 62
0.0630.249 Ac Bc
10.5 9.5
61 74
94 117
91 113
91 113
88 109 60 72
39 38 35
38 37 34
39 38 34
38 37 33
61 74
35 35
34 34
35 35
34 34
60 72
59 59
57 57
57 57
0.0100.062 A B
55 55
0.0080.009 A B
T42a
12
63 76
95 119
39 39 36
36 36
60 60
0.2500.499 Sc
0.100 ...
... 0.33
8
63 76
90 117
38 39 35
36 36
59 59
10.9 10.4
10.7 10.2
0.5001.000b Sc
AMSQQA250/5 Flat sheet and plate
... ...
83 115
e
4
... ...
... ... ...
35 39 35
63 76
... 36
... 56
58 58 36 36
2.0013.000b S
1.0012.000b Sc,d
5
75 89
97 126
49 49 35
47 47
60 60
0.0100.062 S
10.7 10.2
10.5 10.0
5
79 93
100 130
51 52 36
49 49
62 62
T62a 0.0630.249 Sc
10.9 10.4
10.7 10.2
5
79 93
100 130
51 51 36
49 49
62 62
10.7 9.7
10.5 9.5
5
... ...
... ...
... ... ...
... 43
... 56
10.7 10.2
10.5 10.0
5
... ...
... ...
... ... ...
... 45
... 58
T72a 0.250 0.0100.499 0.062 0.0630.249 Sc S S
Design allowables in some cases were based upon data obtained from testing samples of material, supplied in the O or F temper, which were heat treated to demonstrate response to heat treatment by suppliers. Properties obtained by the user may be different than those listed if the material has been formed or otherwise cold or hot worked, particularly in the annealed temper, prior to solution heat treatment. These values have been adjusted to represent the average properties across the whole section, including 2½ percent per side nominal cladding thickness. Bearing values are “dry pin” values per Section 1.4.7.1. See Table 3.1.2.1.1. See Table 3.2.3.0(f).
Basis . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ............... LT . . . . . . . . . . . . . . Fty, ksi: L ............... LT . . . . . . . . . . . . . . Fcy, ksi: L ............... LT . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . e, percent (Sbasis): LT . . . . . . . . . . . . . . E, 103 ksi: Primary . . . . . . . . . . Secondary . . . . . . . . Ec, 103 ksi: Primary . . . . . . . . . . Secondary . . . . . . . . G, 103 ksi . . . . . . . . . . µ ................ Physical Properties: ω, lb/in.3 . . . . . . . . . . C, K, and α . . . . . . . .
Thickness, in. . . . . . . . .
Specification . . . . . . . . . Form . . . . . . . . . . . . . . . Temper . . . . . . . . . . . . .
Table 3.2.3.0(e3). Design Mechanical and Physical Properties of Clad 2024 Aluminum Alloy Sheet and Plate—Continued
MMPDS01 31 January 2003
MMPDS01 31 January 2003
Table 3.2.3.0(e4). Design Mechanical and Physical Properties of Clad 2024 Aluminum Alloy Sheet and Plate—Continued
Specification . . . . .
AMSQQA250/5
Form . . . . . . . . . . .
Flat sheet and plate
Temper . . . . . . . . .
T851a
T81
0.5001.000b
0.0200.062
0.0630.249
0.2500.499
0.500b
B
S
S
S
S
S
65 65
66 66
63 63
65 64
70 69
68 68
67 67
59 56
56 56
58 58
56 56
59 58
65 64
62 62
61 61
55 55 38
57 57 39
56 57 37
58 59 37
56 56 36
59 61 36
65 67 39
62 65 39
61 64 38
96 122
100 127
99 127
100 129
96 123
99 128
107 138
105 136
104 134
78 90
83 94
83 98
86 101
83 98
84 99
93 109
90 105
88 104
5
5
5
...
5
3
4
4
4
10.5 9.5
10.5 10.0
10.7 10.2
10.5 9.5
10.5 10.0
10.5 10.2
10.7 9.7
10.7 10.2
10.9 10.4
10.7 9.7
10.7 10.2
10.9 10.4
Thickness, in. . . . .
0.0100.062
0.0630.249
Basis . . . . . . . . . . .
S
S
A
64 62
67 65
57 54
Mechanical Properties: Ftu, ksi: L ............ LT . . . . . . . . . . Fty, ksi: L ............ LT . . . . . . . . . . Fcy, ksi: L ............ LT . . . . . . . . . . Fsu, ksi . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . (e/D = 2.0) . . . . Fbry, ksi: (e/D = 1.5) . . . . (e/D = 2.0) . . . . e, percent (Sbasis): LT . . . . . . . . . . E, 103 ksi: Primary . . . . . . Secondary . . . . Ec, 103 ksi: Primary . . . . . . Secondary . . . .
T861a
0.2500.499
G, 103 ksi . . . . . . µ .............
... 0.33
Physical Properties: ω, lb/in.3 . . . . . . . C, K, and α . . . . .
0.100 ...
a Bearing values are “dry pin” values per Section 1.4.7.1. b These values have been adjusted to represent the average properties across the whole section, including the 2½ percent nominal cladding thickness.
378
MMPDS01 31 January 2003
Table 3.2.3.0(f). Minimum Elongation Values for Clad 2024 Aluminum Alloy Sheet and Plate
Elongation (LT), percent Temper . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Thickness, in.: 0.0100.020 0.0210.062 1.0011.500 1.5012.000
T3, T4, T42
........................ ........................ ........................ ........................
12 15 7 6
379
MMPDS01 31 January 2003
Table 3.2.3.0(g). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Drawn Tubing
Specification . . . . . . . . . . . . . . . . . . . .
AMS 4086 and WWT700/3
Form . . . . . . . . . . . . . . . . . . . . . . . . . .
WWT700/3
Drawn tubing
Temper . . . . . . . . . . . . . . . . . . . . . . . .
T3
T42a
T81
Wall Thickness, in. . . . . . . . . . . . . . . .
0.0180.500
0.0180.500
0.0100.249
Basis . . . . . . . . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ......................... LT . . . . . . . . . . . . . . . . . . . . . . . . Fty, ksi: L ......................... LT . . . . . . . . . . . . . . . . . . . . . . . . Fcy, ksi: L ......................... LT . . . . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . e, percent (Sbasis): L .........................
A
B
S
S
64 ...
66 ...
62 ...
66 ...
42 ...
45 ...
38 ...
58 ...
42 ... 39
45 ... 40
38 ... 38
... ... ...
96 122
99 126
93 118
... ...
59 67
63 72
53 61
... ...
b
b
b
E, 103 ksi . . . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . . . . µ ...........................
... 10.5 10.7 4.0 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . . . C, K, and α . . . . . . . . . . . . . . . . . . . .
0.100 See Figure 3.2.3.0
a Design allowables were based upon data obtained from testing samples of material supplied in the O or F temper, which were heat treated to demonstrate response to heat treatment by suppliers. Properties obtained by the user, however, may be lower than those listed if the material has been formed or otherwise cold or hot worked, particularly in the annealed temper, prior to solution heat treatment. b See Table 3.2.3.0(h).
380
MMPDS01 31 January 2003
Table 3.2.3.0(h). Minimum Elongation Values for 2024 Aluminum Alloy Drawn Tubing
Elongation (L), percenta Temper . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
T3, T42
Wall Thickness, in.: 0.0180.024 . . . . . . . . . . . . . . . . . . . . . . . . 0.0250.049 . . . . . . . . . . . . . . . . . . . . . . . . 0.0500.259 . . . . . . . . . . . . . . . . . . . . . . . . 0.2600.500 . . . . . . . . . . . . . . . . . . . . . . . .
10 12 14 16
Temper . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
T81
0.0100.024 . . . . . . . . . . . . . . . . . . . . . . . . 0.0250.049 . . . . . . . . . . . . . . . . . . . . . . . . 0.0500.249 . . . . . . . . . . . . . . . . . . . . . . . .
... 5 6
a Full section specimen.
381
MMPDS01 31 January 2003
Table 3.2.3.0(i1). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Bar and Rod; Rolled, Drawn, or ColdFinished Specification . . . . . . .
AMSQQA225/6
AMS 4120 and AMSQQA225/6
Form . . . . . . . . . . . . .
Bar and rod; rolled, drawn, or coldfinished
Temper . . . . . . . . . . .
T351
T361
Thickness, in. . . . . . .
0.5001.000
1.0012.000
2.0013.000
3.0014.000
4.0015.000a
5.0016.000a
6.0016.500a
#0.375
Basis . . . . . . . . . . . . .
S
S
S
S
S
S
S
S
62 61b
62 59b
62 57b
62 55b
62 54b
62 52b
62 ...
69 ...
45 36b
45 36b
45 36b
45 36b
45 36b
45 36b
45 ...
52 ...
34 41 37
34 41 37
34 41 37
34 41 37
34 41 37
34 41 37
... ... ...
... ... ...
90 115
90 115
90 115
90 115
90 115
90 115
... ...
... ...
63 74
63 74
63 74
63 74
63 74
63 74
... ...
... ...
10
10
10
10
10
10
10
10
Mechanical Properties: Ftu, ksi: L ............. LT . . . . . . . . . . . . Fty, ksi: L ............. LT . . . . . . . . . . . . Fcy, ksi: L ............. LT . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . (e/D = 2.0) . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . (e/D = 2.0) . . . . . . e, percent: L ............. 3
E, 10 ksi . . . . . . . . . Ec, 103 ksi . . . . . . . . G, 103 ksi . . . . . . . . µ ...............
10.5 10.7 4.0 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . C, K, and α . . . . . . .
0.100 See Figure 3.2.3.0
a For square, rectangular, hexagonal, or octagonal bar, minimum thickness is 4 inches, and maximum crosssectional area is 36 square inches. b Caution: This specific alloy, temper, and product form exhibits poor stresscorrosion cracking resistance in this grain direction. It corresponds to an SCC resistance rating of D, as indicated in Table 3.1.2.3.1(a).
382
383
... ... 10
56 64 10
56 64 10
59 67 10
59 67 10
59 67 10
59 67 10
59 67 10
63 72 10
... ... ... ... ... ... ... 10
... ... ... ... 10
40 ...
62 ...
S
#6.500c
... ... ...
38 ...
58 ...
S
6.5018.000d
T42b
AMSQQA225/6
a The T4 temper is obsolete and should not be specified for new designs. b These properties apply when samples of material supplied in the O or F temper are heat treated to demonstrate response to heat treatment. Properties obtained by the user, however, may be lower than those listed if the material has been formed or otherwise cold or hot worked, particularly in the annealed temper, prior to solution heat treatment. c For square, rectangular, hexagonal, or octagonal bar, maximum thickness is 4 inches, and maximum crosssectional area is 36 square inches. d Applies to rod only. e Caution: This specific alloy, temper, and product form exhibits poor stresscorrosion cracking resistance in this grain direction. It corresponds to an SCC resistance rating of D, as indicated in Table 3.1.2.3.1(a).
0.100 See Figure 3.2.3.0 71 (at 77EF) for T4X (See Figure 3.2.3.0)
... ...
93 118 93 118
93 118
93 118
93 118
93 118
93 118
93 118
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . C and α . . . . . . . . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . .
... ... 37
32 ... 37
32 ... 37
33 ... 37
33 ... 37
33 ... 37
33 ... 37
33 ... 37
36 ... 37
10.5 10.7 4.0 0.33
40 ...
40 36e
40 37e
42 39e
42 39e
42 40e
42 41e
42 42e
45 45e
E, 103 ksi . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . µ ......................
62 ...
62 52e
S
6.0016.500d
62 54e
S
5.0016.000c
62 54e
S
4.5015.000d
62 55e
S
4.0014.500c
62 57e
S
3.0014.000
62 59e
S
2.0013.000
62 61e
S
1.0012.000
T4a
Bar and rod; rolled, drawn, or coldfinished
AMS 4120 and AMSQQA225/6
62 61e
S
S
Basis . . . . . . . . . . . . . . . . . . . . .
Mechanical Properties: Ftu, ksi: L .................... LT . . . . . . . . . . . . . . . . . . . Fty, ksi: L .................... LT . . . . . . . . . . . . . . . . . . . Fcy, ksi: L .................... LT . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . e, percent: L ....................
0.5001.000
0.1250.499
Thickness, in. . . . . . . . . . . . . . .
Temper . . . . . . . . . . . . . . . . . . .
Form . . . . . . . . . . . . . . . . . . . . .
Specification . . . . . . . . . . . . . . .
Table 3.2.3.0(i2). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Bar and Rod; Rolled, Drawn, or ColdFinished—Continued
MMPDS01 31 January 2003
MMPDS01 31 January 2003
Table 3.2.3.0(i3). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Bar and Rod; Rolled, Drawn, or ColdFinished—Continued
Specification . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
AMSQQA225/6
Form . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Bar and rod; rolled, drawn, or cold finished
Temper . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
T6a
T62b
T851
Thickness,c in. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
#6.500
#6.500
0.5006.500
Basis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
S
S
S
62 ...
60 ...
66 ...
50 ...
46 ...
58 ...
... ... ...
... ... ...
... ... ...
... ...
... ...
... ...
... ...
... ...
... ...
5
5
5
Mechanical Properties: Ftu, ksi: L ........................................ LT . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Fty, ksi: L ........................................ LT . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Fcy, ksi: L ........................................ LT . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . e, percent: L ........................................ E, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . µ ......................................... Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . C and α . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . . . . . . . . . . . . . . . . . . . . .
10.5 10.7 4.0 0.33 0.100 See Figure 3.2.3.0 87 (at 77EF) for T6X and T8XX
a The T6 temper is obsolete and should not be specified for new designs. b These properties apply when samples of material supplied in the O or F temper are heat treated to demonstrate response to heat treatment. Properties obtained by the user, however, may be lower than those listed if the material has been formed or otherwise cold or hot worked, particularly in the annealed temper, prior to solution heat treatment. c For square, rectangular, hexagonal, or octagonal bar, maximum thickness is 4 inches, and maximum crosssectional area is 36 square inches.
384
385
5 5 4 8 8 ... 10 ... 10 ...
10
...
12
...
12
...
12
a The mechanical properties are to be based upon the thickness at the time of quench. b Bearing values are “dry pin” values per Section 1.4.7.1.
0.100 See Figure 3.2.3.0
82 96 82 96 79 93 57 69 59 71 65 78 62 75 66 80 63 77
67 81
57 69
59 71
55 67
59 71
55 67
68 79
61 71
Physical Properties: ω, lb/in.3 . . . . . . . C, K, and α . . . . .
92 117 96 123 94 123 84 106 86 108 91 115 86 109 93 118
88 111
90 113
84 105
80 101
78 97
81 101
78 98
90 114
84 108
10.8 11.0 4.1 0.33
59 59 36 59 59 36 57 57 35 45 38 32 45 39 33 51 43 35 49 41 33
50 44 36
49 42 34
48 47 35
41 40 33
40 43 31
38 40 30
39 44 32
37 41 31
38 45 31
58 57 58 57 56 55 48 36 48 36 54 41
52 39
54 41
52 39
54 43
46 37
47 39
44 37
47 40
44 38
47 41
42 37
34 41 29
66 61
S
66 64
S
64 64
S
68 52
S
68 53
S
74 57
B
70 54
A
74 58
B
70 55
A
#32
1.5004.500
70 60
B
0.2501.499 #20
0.0500.249
65 56
A
3.0004.499
>25  #32
1.5002.999
62 56
B
#25
3.0004.499
60 54
A
1.5002.999
62 57
B
0.7501.499
60 56
A
#20
0.5000.749
61 58
B
0.2500.499
T81, T8510, and T8511
AMSQQA200/3
57 54
A
#0.249
E, 10 ksi . . . . . . . Ec, 103 ksi . . . . . . G, 103 ksi . . . . . . . µ .............
3
Mechanical Properties: Ftu, ksi: L ........... LT . . . . . . . . . . Fty, ksi: L ........... LT . . . . . . . . . . Fcy, ksi: L ........... LT . . . . . . . . . . Fsu, ksi . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . (e/D = 2.0) . . . . Fbryb, ksi: (e/D = 1.5) . . . . (e/D = 2.0) . . . . e, percent (Sbasis): L ............
Basis . . . . . . . . . . . .
CrossSection Area, in.2
Thickness,a in. . . . . .
T3, T3510, and T3511
Extruded bar, rod, and shapes
Form . . . . . . . . . . . .
Temper . . . . . . . . . .
AMS 4152, AMS 4164, AMS 4165, and AMSQQA200/3
Specification . . . . . .
Table 3.2.3.0(j1). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Extrusion
MMPDS01 31 January 2003
386
10
36 47
64 81
38 29 24
38 27
57 39
2.2502.499 S
a Design allowables were based upon data obtained from testing samples of material supplied in the O or F temper, which were heat treated to demonstrate response to heat treatment by suppliers. Properties obtained by the user, however, may be lower than those listed if the material has been formed or otherwise cold or hot worked, particularly in the annealed temper, prior to solution heat treatment. b The mechanical properties are to be based upon the thickness at the time of quench. c Bearing values are “dry pin” values per Section 1.4.7.1.
Table 3.2.3.0(j2). Design Mechanical and Physical Properties of 2024 Aluminum Alloy Extrusion—Concluded Specification . . . . . . AMSQQA200/3 Form . . . . . . . . . . . . Extruded bar, rod, and shapes Temper . . . . . . . . . . T42a CrossSectional Area, in.2 # 25 0.2500.5000.7501.0001.2501.5001.7502.000Thickness or Diameter,b 0.499 0.749 0.999 1.249 1.499 1.749 1.999 2.249 in. # 0.249 Basis . . . . . . . . . . . . S S S S S S S S S Mechanical Properties: Ftu, ksi: L ............. 57 57 57 57 57 57 57 57 57 LT . . . . . . . . . . . 54 52 55 51 49 47 45 43 41 Fty, ksi: L ............. 38 38 38 38 38 38 38 38 38 LT . . . . . . . . . . . 35 34 36 33 32 31 30 29 28 Fcy, ksi: L ............. 38 38 38 38 38 38 38 38 38 LT . . . . . . . . . . . 38 39 37 36 35 34 33 31 30 Fsu, ksi . . . . . . . . . . 29 29 29 29 29 29 28 27 26 Fbruc, ksi: (e/D = 1.5) . . . . . 81 80 79 77 75 74 71 69 67 (e/D = 2.0) . . . . . 99 98 97 95 93 91 89 86 83 Fbryc, ksi: 56 55 (e/D = 1.5) . . . . . 53 51 49 47 44 41 39 69 67 (e/D = 2.0) . . . . . 65 63 61 59 56 53 50 e, percent: 12 12 L ............. 12 10 10 10 10 10 10 3 10.8 E, 10 ksi . . . . . . . . Ec, 103 ksi . . . . . . . 11.0 G, 103 ksi . . . . . . . . 4.1 µ .............. 0.33 Physical Properties: 0.100 ω, lb/in.3 . . . . . . . . C, K, and α . . . . . . See Figure 3.2.3.0
MMPDS01 31 January 2003
MMPDS01 31 January 2003
200 Strength at temperature Exposure up to 10,000 hr
180
Percent Ftu at Room Temperature
160
140
120
100 1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
80
60
40
20
0 400
200
0
200
400
600
800
Temperature, F
Figure 3.2.3.1.1(a). Effect of temperature on the tensile ultimate strength (Ftu) of 2024T3, T351, and 2024T4 aluminum alloy (all products except extrusions).
387
1000
MMPDS01 31 January 2003
200 Strength at temperature Exposure up to 10,000 hr
180
Percent Fty at Room Temperature
160
140
120
100 1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
80
60
40
20
0 400
200
0
200
400
600
800
1000
Temperature, F
Figure 3.2.3.1.1(b). Effect of temperature on the tensile yield strength (Fty) of 2024T3, T351, and 2024T4 aluminum alloy (all products except extrusions).
388
MMPDS01 31 January 2003
100
Percentage of Room Temperature Ftu
Strength at temperature Exposure up to 10,000 hr 80
60 1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
40
20
0 0
100
200
300
400
500
600
700
800
Temperature, F
Figure 3.2.3.1.1(c). Effect of temperature on the tensile ultimate strength (Ftu) of 2024T3, T3510, T3511, and T42 aluminum alloy extrusion. 100
Percentage of Room Temperature Fty
Strength at temperature Exposure up to 10,000 hr 80
1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
60
40
20
0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.3.1.1.(d). Effect of temperature on the tensile yield strength (Fty) of 2024T3, T3510, T3511, and T42 aluminum alloy extrusion.
389
MMPDS01 31 January 2003
Percentage of Room Temperature Ftu
100
80 1/2 hr 10 hr 100 hr 1000 hr 10,000 hr
60
40
20 Strength at room temperature Exposure up to 10,000 hr 0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.3.1.1(e). Effect of exposure at elevated temperatures on the roomtemperature tensile ultimate strength (Ftu) of 2024T3, T351, T3510, T3511, and T42 aluminum alloy (all products except thick extrusions).
Percentage of Room Temperature Fty
100
80
60
1/2 10 100 1000 10,000
40
hr hr hr hr hr
20 Strength at room temperature Exposure up to 10,000 hr 0 0
100
200
300
400
500
600
700
800
Temperature, F
Figure 3.2.3.1.1(f). Effect of exposure at elevated temperatures on the roomtemperature tensile yield strength (Fty) of 2024T3, T351, T3510, T3511, T4, and T42 aluminum alloy (all products except thick extrusions).
390
MMPDS01 31 January 2003 100
Percentage of Room Temperature Fcy
Strength at temperature Exposure up to 1000 hr 80
60
40 1/2 hr 2 hr 10 hr 20
100 hr 1000 hr
0 0
100
200
300
400
500
600
700
800
Temperature, °F
Figure 3.2.3.1.2(a). Effect of temperature on the compressive yield strength (Fcy) of flat clad 2024T3, coiled clad 2024T4 aluminum alloy sheet, and clad 2024T351 aluminum alloy plate.
Figure 3.2.3.1.2(b). Effect of temperature on the shear ultimate strength (Fsu) of flat clad 2024T3, coiled clad 2024T4 aluminum alloy sheet, and clad 2024T351 aluminum alloy plate.
391
MMPDS01 31 January 2003
Figure 3.2.3.1.3(a). Effect of temperature on the bearing ultimate strength (Fbru) of flat clad 2024T3, coiled clad 2024T4 aluminum alloy sheet, and clad 2024T351 aluminum alloy plate.
Figure 3.2.3.1.3(b). Effect of temperature on the bearing yield strength (Fbry) of flat clad 2024T3, coiled clad 2024T4 aluminum alloy sheet, and clad 2024T351 aluminum alloy plate.
392
MMPDS01 31 January 2003
Figure 3.2.3.1.4. Effect of temperature on the tensile and compressive moduli (E and Ec) of 2024 aluminum alloy.
Figure 3.2.3.1.5(a). Effect of temperature on the elongation of 2024T3, T351, T3510, T3511, T4, and T42 aluminum alloy (all products except thick extrusions).
393
MMPDS01 31 January 2003
!"#$
Figure 3.2.3.1.5(b). Effect of exposure at elevated temperature on the elongation (e) of 2024T3, T351, T3510, T3511, T4, and T42 aluminum alloy (all products except thick extrusions).
394
MMPDS01 31 January 2003 100
80 L  tension LT  compression LT  tension 60
L  compression
Stress, ksi
LT  compression
40
L  compression Ramberg  Osgood n(Ltension) = 50 n(LTtension) = 12 n (Lcomp.) = 15 n (LTcomp.) = 11
20
TYPICAL Thickness ≤ 0.249 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(a). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2024T3 aluminum alloy sheet at room temperature.
100
80
L  Tension LT  Compression LT  Tension
Stress, ksi
60
L  Compression
LT  Compression
40 L  Compression Ramberg  Osgood n (Ltension) = 50 n (LTtension) = 15 n (Lcomp.) = 13 n (LTcomp.) = 19
20
TYPICAL Thickness = 0.063  0.249 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(b). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at room temperature.
395
MMPDS01 31 January 2003 100 Long Transverse
80
Stress, ksi
60 2hr exposure
40
20 Ramberg  Osgood n (2hr exp.) = 8.0 TYPICAL 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(c). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at 212EF.
100 Long Transverse
80
1000hr exposure 100hr exposure 10hr exposure 1/2hr exposure
Stress, ksi
60
40
Ramberg  Osgood n (1/2hr exp.) = 9.6 n (10hr exp.) = 9.3 n (100hr exp.) = 8.0 n (1000hr exp.) = 10
20
TYPICAL
0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 3.2.3.1.6(d). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at 300EF.
396
MMPDS01 31 January 2003 100
Ramberg  Osgood n (1/2hr exp.) = 13 n (2hr exp.) = 16 n (100hr exp.) = 6.7
Long Transverse
80
TYPICAL
60
Stress, ksi
2hr exposure 1/2hr exposure
2hr exposure
1/2hr exposure 40 100hr exposure 100hr exposure 20
0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 3.2.3.1.6(e). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at 400EF.
50 Long Transverse
1/2hr exposure
40 1/2hr exposure 2hr exposure
2hr exposure
Stress, ksi
30 10hr exposure
10hr exposure
20
Ramberg  Osgood n (1/2hr exp.) = 8.6 n (2hr exp.) = 10 n (10hr exp.) = 8.4
10
TYPICAL 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(f). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at 500EF.
397
MMPDS01 31 January 2003 25 Long Transverse
1/2hr exposure 2hr exposure
20
Stress, ksi
15 10hr exposure 100hr exposure 10 Ramberg  Osgood n (1/2hr exp.) = 13 n (2hr exp.) = 13 n (10hr exp.) = 19 n (100hr exp.) = 8.5 n (1000hr exp.) = 16
5 1000hr exposure
TYPICAL 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(g). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at 600EF.
25 Long Transverse
Ramberg  Osgood n (1/2hr exp.) = 14 n (10hr exp.) = 15 n (100hr exp.) = 11
20
TYPICAL
Stress, ksi
15
1/2hr exposure 10
5
10hr exposure 100hr exposure 0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 3.2.3.1.6(h). Typical compressive stressstrain and compressive tangentmodulus curves for clad 2024T3 aluminum alloy sheet at 700EF.
398
MMPDS01 31 January 2003 60
Ltension
LTcompression 50
LTtension Lcompression
Stress, ksi
40
Lcompression
30
RambergOsgood TYS (ksi) n (Lcomp.) = 9.0 45 n (LTcomp.) = 12 50 n (Ltension) = 42 53 n (LTtension) = 9.0 47
20
10
TYPICAL Thickness: 0.5002.000 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. Compressive Tangent Modulus, 10 3 ksi. Figure 3.2.3.1.6(i). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2024T351 aluminum alloy plate at room temperature.
60
L and LT  compression
50
Ltension
Stress, ksi
40
LTtension
30
RambergOsgood TYS (ksi) n (Ltension) = 17 43.0 n (LTtension) = 16 42.0 n (Lcomp.) = 19 44.5 n (LTcomp.) = 19 44.5
20
10
TYPICAL Thickness: 0.5002.000 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. Compressive Tangent Modulus, 103 ksi. Figure 3.2.3.1.6(j). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2024T42 aluminum alloy plate at room temperature.
399
MMPDS01 31 January 2003 60
LT  compression L  compression L  tension 50
LT  tension
Stress, ksi
40
LT  compression L  compression 30
20
Ramberg  Osgood n (L  tension) = 18 n (LT  tension) = 16 n (L  comp.) = 12 n (LT  comp.) = 14
10
TYS CYS 45 46 48 48
TYPICAL Thickness = 1.000  1.750 in. 0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 3.2.3.1.6(k) Typical tension and compression stressstrain and compression tangent modulus curves for 2024T42 aluminum alloy plate at room temperature. Note, the data to generate these curves may have been from clad product, however, they are shown here without secondary modulus since it could not be positively confirmed the product was cladded. 100
Ramberg  Osgood n (tension) = 50 n (comp.) = 10
80
TYPICAL Thickness ≤ 5.500 in.
Stress, ksi
60
L  compression L  tension L  compression
40
20
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(l). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for 2024T4 aluminum alloy rolled bar, rod, and shapes at room temperature.
3100
MMPDS01 31 January 2003 60 L  tension LT  tension
50
Stress, ksi
40
30
20
Ramberg  Osgood n(Ltension) = 50 n(LTtension) = 14
10
TYPICAL Thickness = 0.250  0.749 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.2.3.1.6(m). Typical tensile stressstrain curves for 2024T351X aluminum alloy extrusion at room temperature.
60
LT  compression LT  compression 50
L  compression L  compression
Stress, ksi
40
30
Ramberg  Osgood n (Lcomp.) = 16 n (LTcomp.) = 17
20
TYPICAL Thickness = 0.250  0.749 in. 10
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.2.3.1.6(n). Typical compressive stressstrain and compressive tangentmodulus curves for 2024T351X aluminum alloy extrusion at room temperature.
3101
MMPDS01 31 January 2003 .
100
Stress, ksi
80
60
L  tension
L  compression
L  compression 40
RambergOsgood n (tension) = 50 n (comp.) = 15
20
TYPICAL Thickness: 0.125 inch, longitudinal and long transverse directions.
Correlative Information for Figure 3.7.10.1.8(b) Product Form: Sheet, > 0.125 inch through 0.249 inch thick Properties: T61 T761
TUS, ksi 8081 75
TYS, ksi 7376 6667
Loading  Axial Frequency  798, 1500, or 1728 cpm Temperature  RT Environment  Air
Temp.,EF RT RT
No. of Heats/Lots: 2 Maximum Stress Equation: Log Nf = 22.710.1 log (Smax) Std. Error of Estimate, Log (Life) = 0.657 Standard Deviation, Log (Life) = 1.380 R2=77%
Specimen Details: Unnotched, hourglass, 0.500 inch diameter 4.000 inch test section radius, R Surface Condition: As machined
Sample Size = 24 Reference: 3.2.6.1.9(d)
Test Parameters: 3468
MMPDS01 31 January 2003
Figure 3.7.10.1.8(c). Bestfit S/N curve for notched, Kt = 3.0, 7475T61 and T761 sheet, longitudinal and long transverse directions.
Correlative Information for Figure 3.7.10.1.8(c) Product Form: Sheet, 0.032 to 0.249 inch thick Properties: TUS, ksi T61 8182 T761 7577
TYS, ksi 7376 6770
Test Parameters: Loading  Axial Frequency  798, 1500, or 1728 cpm Temperature  RT Environment  Air
Temp.,EF RT RT
Specimen Details: Notched, edge notched Kt = 3.0 1.000 inch gross width 0.700 inch net width 0.050 inch root radius, r 60E flank angle, ω
No. of Heats/Lots: 2 Maximum Stress Equation: Log Nf = 13.46.29 log (Smax) Std. Error of Estimate, Log (Life) = 0.441 Standard Deviation, Log (Life) = 0.931 R2=78%
Surface Condition: As machined Sample Size = 99 Reference: 3.2.6.1.9(d)
3469
MMPDS01 31 January 2003
Figure 3.7.10.1.10(a). Residual strength behavior of 0.063inchthick 7475T61 aluminum alloy sheet at room temperature. Crack orientation is LT. [References 3.1.2.1.6(d) and 3.2.5.1.9(d).]
Figure 3.7.10.1.10(b). Residual strength behavior of 0.063inchthick 7475T61 aluminum alloy sheet at room temperature. Crack orientation is TL. [References 3.1.2.1.6(d) and 3.2.5.1.9(d).]
3470
MMPDS01 31 January 2003
Figure 3.7.10.1.10(c). Residual strength behavior of 0.063inchthick 7475T61 clad aluminum alloy sheet at room temperature. Crack orientation is LT. [Reference 3.2.5.1.9(d).]
Figure 3.7.10.1.10(d). Residual strength behavior of 0.063inchthick 7475T61 clad aluminum alloy sheet at room temperature. Crack orientation is TL. [Reference 3.2.5.1.9(d).]
3471
MMPDS01 31 January 2003 100
80
Longitudinal and Long Transverse
Stress, ksi
60 Short Transverse
40 Ramberg  Osgood n (Longitudinal) = 15 n (Long Transverse) = 13 n (Short Transverse) = 13
20
TYPICAL Thickness = 0.500  4.000 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.7.10.2.6(a). Typical tensile stressstrain curves for 7475T7351 aluminum alloy plate at room temperature.
100
80 Long Transverse Short Transverse Longitudinal
Stress, ksi
60
40 Ramberg  Osgood n (Lcomp.) = 20 n (LTcomp.) = 20 n (STcomp.) = 19
20
TYPICAL Thickness = 0.500  4.000 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.7.10.2.6(b). Typical compressive stressstrain and compressive tangentmodulus curves for 7475T7351 aluminum alloy plate at room temperature.
3472
MMPDS01 31 January 2003
Figure 3.7.10.2.8(a). Bestfit S/N curves for unnotched 7475T7351 plate, longitudinal and long transverse orientation.
Correlative Information for Figure 3.7.10.2.8(a)
Product Form: Plate, 0.5, 1.0, 2.0, 3.0, and 4.0inches thick Properties: L LT
TUS, ksi 70 71
Test Parameters: Loading — Axial Frequency — Not specified Temperature — RT Environment — Air
TYS, ksi Temp..,EF 60 RT 60 RT
No. of Heats/Lots: 5 Specimen Details: Unnotched Hourglass, 0.300 inch net diameter 9.875 inch test section radius Surface Condition: As machined
Equivalent Stress Equation: Log Nf = 17.427.56 log (Seq) Seq = Smax(1R)0.40 Std. Error of Estimate, Log (Life) = 0.433 Standard Deviation, Log (Life) = 0.857 R2 = 74%
References: 3.7.10.2.8(a) and (b)
Sample Size = 52 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
3473
MMPDS01 31 January 2003
Figure 3.7.10.2.8(b). Bestfit S/N curves for notched, Kt = 3.0, 7475T7351 and T7651 plate, longitudinal and long transverse direction.
(See following page for correlative information.)
3474
MMPDS01 31 January 2003 Correlative Information for Figure 3.7.10.2.8(b) Product Form: Plate, 0.5, 1.0, 1.5, 2.0, 3.0, and 4.0 inches thick Properties: L (T7351) LT (T7351) L (T7351) (T7651) L (T7351) LT (T7351)
TUS, ksi TYS, ksi 70 60 71 61 72 62 Not specified 72 63 73 62
Surface Condition: Not specified [Ref. (a) and (b)] As machined and deburred [Ref. (c)] 32 RMS [Ref. (d)] 10 RMS [Ref. (e)]
Temp.,EF RT RT RT
Test Parameters: Loading — Axial Frequency — Not specified [Ref. (a) and (b)] — 1800 cpm [Ref. (c) and (d)] — 1500 cpm [Ref. (e)] Temperature — RT Environment — Air
RT RT
Specimen Details: Notched, Kt = 3.0 Circumferentially notched 0.253 inch gross width 0.147 inch net width 0.013 inch root radius, r 60E flank angle, ω Edge notched 1.00 inch gross width 0.70 inch net width root radius not specified 60E flank angle, ω Edge notched 2.25 inch gross width 1.50 inch net width 0.113 inch root radius, r 60E flank angle, ω Circumferentially notched 1.375 inch gross width 0.25 inch net width 0.13 inch root radius, r 60E flank angle, ω
No. of Heats/Lots: 8 Equivalent Strain Equation: Log Nf = 8.463.21 log (Seq7.5) Seq = Smax(1R)0.72 Std. Error of Estimate, Log (Life) = 0.422 Standard Deviation, Log (Life) = 0.923 R2 = 79% Sample Size = 97 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
References: 3.7.10.2.8 (a) through (e)
3475
MMPDS01 31 January 2003
Figure 3.7.10.2.9(a). Fatiguecrackpropagation data for 1.5inchthick, 7475T7351 aluminum alloy plate [References 3.7.10.2.9(a) and (b)]. Specimen Thickness: Specimen Width: Specimen Type:
0.650inch 1.500inches C(T)
3476
Environment: Temperature: Orientation:
Lab air RT LT
MMPDS01 31 January 2003
Figure 3.7.10.2.9(b). Fatiguecrackpropagation data for 0.500inchthick, 7475T7351 aluminum alloy plate [Reference 3.7.10.2.9(c)]. Specimen Thickness: Specimen Width: Specimen Type:
0.528 to 0.530inch 4.6inches M(T)
3477
Environment: Temperature: Orientation:
95% R.H. RT LT
MMPDS01 31 January 2003 100
80 Longitudinal
Long Transverse
Stress, ksi
60
40
Ramberg  Osgood n (Ltension) = 26 n (LTtension) = 16 TYPICAL
20 Thickness = 0.040  0.249 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.7.10.3.6(a). Typical tensile stressstrain curves for 7475T761 aluminum alloy sheet at room temperature.
100
80
Long Transverse Longitudinal
Stress, ksi
60
40 Ramberg  Osgood n (Lcomp.) = 15 n (LTcomp.) = 19 20
TYPICAL Thickness = 0.040  0.249 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.7.10.3.6(b). Typical compressive stressstrain and compressive tangentmodulus curves for 7475T761 aluminum alloy sheet at room temperature.
3478
MMPDS01 31 January 2003 100
80
Stress, ksi
Longitudinal
60
Long transverse
40
RambergOsgood TYS (ksi) n (Ltension) = 9.0 63 n (LTtension) = 9.1 62
20
TYPICAL Thickness: 0.0400.062 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. Figure 3.7.10.3.6(c). Typical tensile stressstrain curves for clad 7475T761 aluminum alloy sheet at room temperature. 100
80
Stress, ksi
Longitudinal
60
Long transverse
40
RambergOsgood TYS (ksi) n (Ltension) = 9.0 64 n (LTtension) = 9.1 63
20
TYPICAL Thickness: 0.0630.187 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. Figure 3.7.10.3.6(d). Typical tensile stressstrain curves for clad 7475T761 aluminum alloy sheet at room temperature.
3479
MMPDS01 31 January 2003 100
80 Longitudinal
60
Stress, ksi
Long Transverse
40
Ramberg  Osgood n (Ltension) = 9.0 n (LTtension) = 9.1
20
TYPICAL Thickness = 0.188  0.249 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.7.10.3.6(e). Typical tensile stressstrain curves for clad 7475T761 aluminum alloy sheet at room temperature.
100
80 Long Transverse Longitudinal
Stress, ksi
60
40
Ramberg  Osgood n (Lcomp.) = 12 n (LTcomp.) = 16
20
TYPICAL Thickness = 0.040  0.062 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.7.10.3.6(f). Typical compressive stressstrain and compressive tangentmodulus curves for clad 7475T761 aluminum alloy sheet at room temperature.
3480
MMPDS01 31 January 2003 100
80 Long Transverse Longitudinal
Stress, ksi
60
40
Ramberg  Osgood n (Lcomp.) = 12 n (LTcomp.) = 16
20
TYPICAL Thickness = 0.063  0.187 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.7.10.3.6(g). Typical compressive stressstrain and compressive tangentmodulus curves for clad 7475T761 aluminum alloy sheet at room temperature.
100
80 Long Transverse Longitudinal
Stress, ksi
60
40
Ramberg  Osgood n (Lcomp.) = 12 n (LTcomp.) = 16
20
TYPICAL Thickness = 0.188  0.249 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.7.10.3.6(h). Typical compressive stressstrain and compressive tangentmodulus curves for clad 7475T761 aluminum alloy sheet at room temperature.
3481
MMPDS01 31 January 2003 100
80
Longitudinal 60
Stress, ksi
Long Transverse Ramberg  Osgood n (Ltension) = 33 n (LTtension) = 19
40
TYPICAL Thickness = 0.250  1.500 in.
20
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.7.10.3.6(i). Typical tensile stressstrain curves for 7475T7651 aluminum alloy plate at room temperature.
100
80
Long Transverse Longitudinal
Stress, ksi
60
Ramberg  Osgood n(Lcomp.) = 20 n(LTcomp.) = 20
40
TYPICAL Thickness = 0.250  1.500 in. 20
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.7.10.3.6(j). Typical compressive stressstrain and compressive tangentmodulus curves for 7475T7651 aluminum alloy plate at room temperature.
3482
MMPDS01 31 January 2003
!"
; ;
#$%&'
Figure 3.7.10.3.6(k). Typical tensile stressstrain (full range) curves for 7475T761 aluminum alloy sheet at room temperature.
3483
MMPDS01 31 January 2003
;
!
Figure 3.7.10.3.6(l). Typical tensile stressstrain (full range) curves for clad 7475T761 aluminum alloy sheet at room temperature.
3484
MMPDS01 31 January 2003
Figure 3.7.10.3.10(a). Residual strength behavior of 0.063inchthick 7475T761 aluminum alloy sheet at room temperature. Crack orientation is LT. [References 3.1.2.1.6(d) and 3.2.5.1.9(d).]
Figure 3.7.10.3.10(b). Residual strength behavior of 0.063inchthick 7475T761 aluminum alloy sheet at room temperature. Crack orientation is TL. [References 3.1.2.1.6(d) and 3.2.5.1.9(d).]
3485
MMPDS01 31 January 2003
3.8
200.0 SERIES CAST ALLOYS
Alloys of the 200 series contain copper as the principal alloying element, and are particularly useful for elevated temperature applications. 3.8.1 A201.0 ALLOY 3.8.1.0 Comments and Properties — A201.0 is a highstrength, heattreatable AlCuAg casting alloy. In the T7 (overaged) temper, it possesses high strength, moderate ductility and optimum resistance to stresscorrosion cracking. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification covering this alloy is presented in Table 3.8.1.0(a). Roomtemperature mechanical and physical properties are presented in Table 3.8.1.0(b). The effect of temperature on thermal expansion is shown in Figure 3.8.1.0. Table 3.8.1.0(a). Material Specification for A201.0 Aluminum Alloy
Specification
Form
AMSA21180
Casting (T7 temper)
The temper index for A201.0 is as follows: Temper T7
Section 3.8.1.1
3.8.1.1 T7 Temper — Figure 3.8.1.1.6 presents a typical tensile stressstrain curve. Strain control fatigue data are shown in Figures 3.8.1.1.8(a) through (c).
3486
MMPDS01 31 January 2003
Table 3.8.1.0(b). Design Mechanical and Physical Properties of A201.0 Aluminum Alloy Casting
Specification . . . . . . . . . . . . .
AMSA21180
Form . . . . . . . . . . . . . . . . . . .
Casting
Temper . . . . . . . . . . . . . . . . .
T7
Location Within Casting . . . . a
Designated area
Nondesignated area
....
1
2
10
11
Basis . . . . . . . . . . . . . . . . . . .
S
S
S
S
Mechanical Properties : Ftu, ksi: . . . . . . . . . . . . . . . .
60
60
60
56
Fty, ksi: . . . . . . . . . . . . . . . .
50
50
50
48
Fcy, ksi: . . . . . . . . . . . . . . . .
51
51
51
49
Fsu, ksi . . . . . . . . . . . . . . . . .
36
36
36
34
95 122
95 122
95 122
88 114
Strength Class Number
b,c
d
Fbru , ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . Fbryd, ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . .
74 87
74 87
74 87
71 83
e, percent . . . . . . . . . . . . . .
3
5
3
1.5
3
E, 10 ksi . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . µ .....................
10.3 10.7 4.0 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . α, 106 in./in./EF . . . . . . . . .
0.101 0.22 (at 212EF) 70 (at 77EF) See Figure 3.8.1.0
a The attainable strength class number is dependent on the casting configuration, complexity, and size (both weight and wall thickness). Favorable experience with a particular configuration may allow some foundries to produce a higher strength class number than others. In case of doubt regarding the strength class number, the designer should consult or negotiate with the foundry to determine the proper strength class number to assign for a specific casting. b For any casting process; i.e., special mold, permanent mold, or sand mold (including chilling). c The mechanical properties shown are reliably obtainable in castings of this alloy and heattreat condition when produced under the quality assurance provisions of AMSA21180. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. d Bearing values are “dry pin” values per Section 1.4.7.1.
3487
MMPDS01 31 January 2003
α
LQLQ)
Figure 3.8.1.0. Effect of temperature on the thermal expansion of A201.0 aluminum alloy casting.
3488
MMPDS01 31 January 2003
100
80
Stress, ksi
60
40
Ramberg  Osgood n (tension) = 14
20
TYPICAL
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.8.1.1.6. Typical tensile stressstrain curve for A201.0T7 aluminum alloy casting, designated area, at room temperature.
3489
MMPDS01 31 January 2003
Figure 3.8.1.1.8(a). Bestfit ε/N curves, cyclic stressstrain curve, and mean stress relaxation curve for A201.0T7 casting at 75EF.
3490
MMPDS01 31 January 2003 Correlative Information for Figure 3.8.1.1.8(a)
Test Parameters: Strain Rate/Frequency  20 cpm Wave Form  Triangular Temperature  75EF Atmosphere  Air
Product Form/Thickness: Casting Thermal Mechanical Processing History: T7, HIP Properties: TUS, ksi 5766
TYS, ksi 4557
E, ksi Temp.,EF 10,800 75
No. of Heats/Lots: 3
StressStrain Equations: Cyclic (Companion Specimen) Proportional Limit = 42 ksi (∆σ/2) = 72(∆εp/2)0.058 Mean Stress Relaxation, ksi σm = 33.3  4755(∆ε/2)
Equivalent Strain Equation: Log Nf = 6.544.60 log (εeq) εeq = (∆ε)0.37 (Smax/E)0.63 Std. Error of Estimate, Log (Life) = 0.242 Standard Deviation, Log (Life) = 0.587 Adjusted R2 Statistic: 83%
Specimen Details: Uniform gage test section 0.250 inch diameter
Sample Size: 26 [Caution: The equivalent strain model may provide unrealistic life predictions for strain ratios and ranges beyond those represented above.]
References: 3.8.1.1.8(a) and (b)
3491
MMPDS01 31 January 2003
Figure 3.8.1.1.8(b). Bestfit ε/N curves, cyclic stressstrain curve, and mean stress reduction curve for A201.0T7 casting at 200EF.
3492
MMPDS01 31 January 2003 Correlative Information for Figure 3.8.1.1.8(b)
Test Parameters: Strain Rate/Frequency  20 cpm Wave Form  Triangular Temperature  200EF Atmosphere  Air
Product Form/Thickness: Casting Thermal Mechanical Processing History: T7, HIP Properties: TUS, ksi 5359
TYS, ksi 4755
E, ksi Temp.,EF 10,339 200
No. of Heats/Lots: 3
StressStrain Equations: Cyclic (Companion Specimen) Proportional Limit = 39 ksi (∆σ/2) = 58(∆εp/2)0.041 Mean Stress Relaxation, ksi σm = 39.7  7049(∆ε/2)
Equivalent Strain Equation: Log Nf = 6.684.66 log (εeq) εeq = (∆ε)0.50 (Smax/E)0.50 Std. Error of Estimate, Log (Life) = 0.359 Standard Deviation in Log (Life) = 0.561 Adjusted R2 Statistic: 59%
Specimen Details: Uniform gage test section 0.250 inch diameter
Sample Size: 18 [Caution: The equivalent strain model may provide unrealistic life predictions for strain ratios and ranges beyond those represented above.]
Reference: 3.8.1.1.8(a)
3493
MMPDS01 31 January 2003
Figure 3.8.1.1.8(c). Bestfit 0/N curves, cyclic stressstrain curve, and mean stress relaxation curve for A201.0T7 casting at 350EF.
3494
MMPDS01 31 January 2003 Correlative Information for Figure 3.8.1.1.8(c)
Test Parameters: Strain Rate/Frequency  20 cpm Wave Form  Triangular Temperature  350EF Atmosphere  Air
Product Form/Thickness: Casting Thermal Mechanical Processing History: T7, HIP Properties: TUS, ksi 4853
TYS, ksi 4048
E, ksi 9,783
Temp.,EF 350
No. of Heats/Lots: 3
StressStrain Equations: Cyclic (Companion Specimen) Proportional Limit = 36 ksi (∆σ/2) = 50(∆εp/2)0.036 Mean Stress Relaxation, ksi σm = 30.0  5664(∆ε/2)
Equivalent Strain Equation: Log Nf = 12.447.07 log (εeq) εeq = (∆ε)0.52 (Smax/E)0.48 Std. Error of Estimate, Log (Life) = 0.000817 (1/εeq) Standard Deviation, Log (Life) = 0.545
Specimen Details: Uniform gage test section 0.250 inch diameter
Adjusted R2 Statistic: 93% Sample Size: 18
Reference: 3.8.1.1.8(a) [Caution: The equivalent strain model may provide unrealistic life predictions for strain ratios and ranges beyond those represented above.]
3495
MMPDS01 31 January 2003
3.9
300.0 SERIES CAST ALLOYS
Casting alloys of the 300.0 series contain silicon with added copper and/or magnesium as the principal alloying elements. They are heat treatable. Because of the high silicon content, they are among the easiest to cast by a variety of techniques. They have high resistance to corrosion. 3.9.1 354.0 ALLOY 3.9.1.0 Comments and Properties — 354.0 is a heattreatable AlSiMg alloy being among the highest strength of commercial casting alloys. It has good casting characteristics; however, its use is generally restricted to permanent mold castings. Refer to Section 3.1.3.4 for comments regarding the weldability. A material specification for 354.0 aluminum alloy is presented in Table 3.9.1.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.9.1.0(b). Table 3.9.1.0(a). Material Specifications for 354.0 Aluminum Alloy
Specification AMSA21180
Form Casting
3496
MMPDS01 31 January 2003
Table 3.9.1.0(b). Design Mechanical and Physical Properties of 354.0 Aluminum Alloy Casting
Specification . . . . . . . . . . . . .
AMSA21180
Form . . . . . . . . . . . . . . . . . . .
Casting
Temper . . . . . . . . . . . . . . . . .
T6
Location Within Casting . . . . a
Designated area
Nondesignated area
....
1
2
10
11
Basis . . . . . . . . . . . . . . . . . . .
S
S
S
S
Mechanical Properties : Ftu, ksi . . . . . . . . . . . . . . . . .
47
50
47
43
Fty, ksi . . . . . . . . . . . . . . . . .
36
42
36
33
Fcy, ksi . . . . . . . . . . . . . . . . .
36
42
36
33
Fsu, ksi . . . . . . . . . . . . . . . . .
29
31
29
27
Fbru , ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . .
81 101
86 107
81 101
74 92
Fbryd, ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . .
57 67
66 78
57 67
52 62
e, percent . . . . . . . . . . . . . .
3
2
3
2
Strength Class Number
b,c
d
3
E, 10 ksi . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . µ .....................
10.6 10.8 4.0 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . α, 106 in./in./EF . . . . . . . . .
0.098 0.23 (at 212EF) ... 1.6 (68 to 212EF)
a The attainable strength class number is dependent on the casting configuration, complexity, and size (both weight and wall thickness). Favorable experience with a particular configuration may allow some foundries to produce a higher strength class number than others. In case of doubt regarding the strength class number, the designer should consult or negotiate with the foundry to determine the proper strength class number to assign for a specific casting. b For any casting process; i.e., special mold, permanent mold, or sand mold (including chilling). c The mechanical properties shown are reliably obtainable in castings of this alloy and heattreat condition when produced under the quality assurance provisions of AMSA21180. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. d Bearing values are “dry pin” values per Section 1.4.7.1.
3497
MMPDS01 31 January 2003 3.9.2 355.0 ALLOY 3.9.2.0 Comments and Properties — 355.0 is a heattreatable AlSiMg alloy that is readily cast and has good pressure tightness. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification for 355.0 aluminum alloy is presented in Table 3.9.2.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.9.2.0(b). The effect of temperature on thermal expansion is shown in Figure 3.9.2.0.
Table 3.9.2.0(a). Material Specification for 355.0 Aluminum Alloy
Specification AMS 4281
Form Permanent mold casting
3498
MMPDS01 31 January 2003
Table 3.9.2.0(b). Design Mechanical and Physical Properties of 355.0 Aluminum Alloy Specification . . . . . . . . . . . . . . . . . . . .
AMS 4281
Form . . . . . . . . . . . . . . . . . . . . . . . . . . .
Permanent mold casting
Temper . . . . . . . . . . . . . . . . . . . . . . . . .
T6
Location Within Casting . . . . . . . . . . .
As specified
Basis . . . . . . . . . . . . . . . . . . . . . . . . . . .
S
Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . . . . . . . . . . . Fty, ksi . . . . . . . . . . . . . . . . . . . . . . . . . Fcy, ksi . . . . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . . . . . e, percent . . . . . . . . . . . . . . . . . . . . . . E, 103 ksi . . . . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . . . . . µ .............................
27 32 0.4a 10.3 10.3 3.8 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . . . . . . . . . α, 106 in./in./EF . . . . . . . . . . . . . . . . .
0.098 0.23 (at 212EF) 88 (at 77EF) See Figure 3.9.2.0
27a 17a 17 17 46 58
a Conformance to tensile property requirements is determined by testing specimens cut from casting only when specified on drawing. b Bearing values are “dry pin” values per Section 1.4.7.1.
3499
MMPDS01 31 January 2003
14
α, 106 in./in./F
13
12
11
α  Between 70F and indicated temperature
400
200
0
200
400
600
800
1000
Temperature, F Figure 3.9.2.0. Effect of temperature on the thermal expansion of 355.0 aluminum alloy casting.
3500
MMPDS01 31 January 2003 3.9.3 C355.0 ALLOY 3.9.3.0 Comments and Properties — C355.0 is an AlSiMg alloy similar to 355.0 but has impurities controlled to lower limits resulting in higher strengths. It has good casting characteristics. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification for C355.0 aluminum alloy is presented in Table 3.9.3.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.9.3.0(b).
Table 3.9.3.0(a). Material Specification for C355.0 Aluminum Alloy
Specification AMSA21180
Form Casting
3501
MMPDS01 31 January 2003
Table 3.9.3.0(b). Design Mechanical and Physical Properties of C355.0 Alloy Casting Specification . . . . . . . . . . . . . AMSA21180 Form . . . . . . . . . . . . . . . . . . . Casting Location Within Casting . . . . T6 a 1 2 3 10 Strength Class Number . . . . Basis . . . . . . . . . . . . . . . . . . . S S S S b,c Mechanical Properties : 41 Ftu, ksi . . . . . . . . . . . . . . . . . 44 50 41 31 Fty, ksi . . . . . . . . . . . . . . . . . 33 40 31 Fcy, ksi . . . . . . . . . . . . . . . . . 31 33 40 31 Fsu, ksi . . . . . . . . . . . . . . . . . 26 28 31 26 Fbrud, ksi: (e/D = 1.5) . . . . . . . . . . . . 70 75 86 70 (e/D = 2.0) . . . . . . . . . . . . 88 94 107 88 Fbryd, ksi: (e/D = 1.5) . . . . . . . . . . . . 49 52 63 49 (e/D = 2.0) . . . . . . . . . . . . 58 62 75 58 e, percent . . . . . . . . . . . . . . 3 3 2 3 3 10.1 E, 10 ksi . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . 10.3 3 G, 10 ksi . . . . . . . . . . . . . . 3.85 µ ..................... 0.33 Physical Properties: 0.098 ω, lb/in.3 . . . . . . . . . . . . . . . 0.23 (at 212EF) C, Btu/(lb)(EF) . . . . . . . . . . 88 (at 77EF) K, Btu/[(hr)(ft2)(EF)/ft] . . . . α, 106 in./in./EF . . . . . . . . . 12.4 (68 to 212EF)
Aluminum
11 S
12 S
37 30 30 23
35 28 28 22
63 79
60 75
47 59 1
44 52 1
a The attainable strength class number is dependent on the casting configuration, complexity, and size (both weight and wall thickness). Favorable experience with a particular configuration may allow some foundries to produce a higher strength class number than others. In case of doubt regarding the strength class number, the designer should consult or negotiate with the foundry to determine the proper strength class number to assign for a specific casting. b For any casting process; i.e., special mold, permanent mold, or sand mold (including chilling). c The mechanical properties shown are reliably obtainable in castings of this alloy and heattreat condition when produced under the quality assurance provisions of AMSA21180. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. d Bearing values are “dry pin” values per Section 1.4.7.1.
3502
MMPDS01 31 January 2003 3.9.4 356.0 ALLOY 3.9.4.0 Comments and Properties — 356.0 is among the easiest of alloys to cast by a variety of techniques. It is heat treatable, has intermediate strengths, and has high resistance to corrosion. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. Material specifications for 356.0 aluminum alloy are presented in Table 3.9.4.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.9.4.0(b). The effect of temperature on thermal expansion is given in Figure 3.9.4.0.
Table 3.9.4.0(a). Material Specifications for 356.0 Aluminum Alloy
Specification AMS 4284 AMS 4217 AMS 4260
Form Permanent mold casting Sand casting Investment casting
3503
MMPDS01 31 January 2003
Table 3.9.4.0(b). Design Mechanical and Physical Properties of 356.0 Aluminum Alloy Specification . . . . . . . . . . . AMS 4217 AMS 4260 AMS 4284 Form . . . . . . . . . . . . . . . . . . Sand casting Investment casting Permanent mold casting Temper . . . . . . . . . . . . . . . . T6 T6 T6 Location Within Casting . . Thick and thin areas As specified As specified Basis . . . . . . . . . . . . . . . . . . S S S Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . 25a 25a 22a,b 15a,b Fty, ksi . . . . . . . . . . . . . . . 16a 16a 15 Fcy, ksi . . . . . . . . . . . . . . . 16 16 Fsu, ksi . . . . . . . . . . . . . . . 14 16 16 Fbruc, ksi: (e/D = 1.5) . . . . . . . . . . . 43 43 38 (e/D = 2.0) . . . . . . . . . . . 53 53 47 Fbryc, ksi: (e/D = 1.5) . . . . . . . . . . . 25 25 24 (e/D = 2.0) . . . . . . . . . . . 30 30 28 e, percent . . . . . . . . . . . . . 1a 0.7a 0.7a,b E, 103 ksi . . . . . . . . . . . . . 10.3 Ec, 103 ksi . . . . . . . . . . . . 10.3 3 G, 10 ksi . . . . . . . . . . . . . 3.85 µ ................... 0.33 Physical Properties: 0.097 ω, lb/in.3 . . . . . . . . . . . . . 0.23 (at 212EF) C, Btu/(lb)(EF) . . . . . . . . 88 (at 77EF) K, Btu/[(hr)(ft2)(EF)/ft] . . α, 106 in./in./EF . . . . . . . . See Figure 3.9.4.0 a Conformance to tensile property requirements is determined by testing specimens cut from casting only when specified on drawing. b Not minimum values, but based upon average of not less than four specimens. c Bearing values are “dry pin” values per Section 1.4.7.1.
3504
MMPDS01 31 January 2003
α Between 70F and indicated temperature
α, 106 in./in./F
13
12
11
10
9
8
7 400
200
0
200
400
600
800
1000
Temperature, F Figure 3.9.4.0. Effect of temperature on the thermal expansion of 356.0 aluminum alloy casting.
3505
MMPDS01 31 January 2003 3.9.5 A356.0 ALLOY 3.9.5.0 Comments and Properties — A356.0 is an AlSiMg alloy similar to 356.0, but with impurities controlled to lower limits resulting in higher strengths and ductility. It has good casting characteristics and high resistance to corrosion. Refer to 3.1.3.4 for comments regarding the weldability of the alloy. Material specifications for A356.0 aluminum alloy are presented in Table 3.9.5.0(a). Roomtemperature mechanical and physical properties are shown in Tables 3.9.5.0(b) and (c). Table 3.9.5.0(a). Material Specifications for A356.0 Aluminum Alloy
Specification
Form
AMSA21180 AMS 4218
Casting Casting
The temper index for A356.0 is as follows: Temper T6P T6
Section 3.9.5.1 3.9.5.2
3.9.5.1 T6P Temper — Tensile stressstrain and fullrange stressstrain curves at room temperature are presented in Figures 3.9.5.1.6(a) and (b), respectively.
3506
MMPDS01 31 January 2003
Table 3.9.5.0(b). Design Mechanical and Physical Properties of A356.0 Aluminum Alloy Casting
Specification . . . . . . . . . . .
AMSA21180
Form . . . . . . . . . . . . . . . . .
Casting
Temper . . . . . . . . . . . . . . .
T6
Location Within Casting . . Strength Class Number
a
Designated area
Nondesignated area
..
1
2
3
10
11
12
Basis . . . . . . . . . . . . . . . . .
S
S
S
S
S
S
38 28 28 24
40 30 30 25
45 34 34 28
38 28 28 24
33 27 27 21
32 22 22 20
65 81
69 86
77 96
65 81
57 71
55 68
44 52 5
47 56 3
54 63 3
44 52 5
43 50 3
35 41 2
b,c
Mechanical Properties : Ftu, ksi . . . . . . . . . . . . . . . Fty, ksi . . . . . . . . . . . . . . . Fcy, ksi . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . Fbrud, ksi: (e/D = 1.5) . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . Fbryd, ksi: (e/D = 1.5) . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . e, percent . . . . . . . . . . . . . E, 103 ksi . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . µ ...................
10.4 10.5 3.9 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . α, 106 in./in./EF . . . . . . . .
0.097 0.23 (at 212EF) 88 (at 77EF) See Figure 3.9.4.0
a The attainable strength class number is dependent on the casting configuration, complexity, and size (both weight and wall thickness). Favorable experience with a particular configuration may allow some foundries to produce a higher strength class number than others. In case of doubt regarding the strength class number, the designer should consult or negotiate with the foundry to determine the proper strength class number to assign for a specific casting. b For any casting process; i.e., special mold, permanent mold, or sand mold (including chilling). c The mechanical properties shown are reliably obtainable in castings of this alloy and heattreat condition when produced under the quality assurance provisions of AMSA21180. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. d Bearing values are “dry pin” values per Section 1.4.7.1.
3507
MMPDS01 31 January 2003
Table 3.9.5.0(c). Design and Physical Properties of A356.0 Aluminum Alloy Casting
Specification . . . . . . . . . . . . . . . . .
AMS 4218
Form . . . . . . . . . . . . . . . . . . . . . . .
Sand, investment, permanent mold, and composite castings
Temper . . . . . . . . . . . . . . . . . . . . .
T6Pa
Location Within Casting . . . . . . . .
Any
Basis . . . . . . . . . . . . . . . . . . . . . . .
S
b
Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . . . . . . Fty, ksi . . . . . . . . . . . . . . . . . . . . . Fcy, ksi . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . e, percent . . . . . . . . . . . . . . . . . . E, 103 ksi . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . µ .........................
35 41 2 10.4 10.5 3.9 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . . K Btu/[(hr)(ft2)(EF)/ft] . . . . . . . . α, 106 in./in./EF . . . . . . . . . . . . .
0.097 0.23 (at 212EF) 88 (at 77EF) See Figure 3.9.4.0
32 22 22 20 55 68
a The letter, P, indicates a variation compared to the standard heat treatment procedure of this temper and/or a difference in the minimum tensile property requirements compared to the Aluminum Association’s registered limits. b The mechanical properties shown are reliably obtainable when produced under the quality assurance provisions of AMS 4218. These procedures require radiographic control and specific destructive testing for acceptance of each production lot. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting.
3508
MMPDS01 31 January 2003 50
40
Compression Tension
Stress, ksi
30
20
RambergOsgood n (tension) = 10 n (comp.) = 9.2
10
TYPICAL 0
0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 3.9.5.1.6(a). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for A356.0T6P aluminum alloy casting at room temperature.
50
Stress, ksi
40
30
20
10
TYPICAL 0 0.00
0.02
0.04
0.06
0.08
0.10
0.12
Strain, in./in.
Figure 3.9.5.1.6(b). Typical tensile stressstrain (fullrange) curve for A356.0T6P aluminum alloy casting at room temperature.
3509
MMPDS01 31 January 2003 3.9.6 A357.0 ALLOY 3.9.6.0 Comments and Properties — A357.0 is a heattreatable AlSiMg alloy generally used for permanent mold and premium quality castings in which special properties are developed by careful control of casting and chilling techniques. It has excellent casting characteristics, is heat treatable, and provides high strength, together with good toughness. The alloy also has excellent corrosion resistance. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification for A357.0 aluminum alloy is presented in Table 3.9.6.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.9.6.0(b). Table 3.9.6.0(a). Material Specification for A357.0 Aluminum Alloy
Specification
Form
AMSA21180
Casting
The temper index for A357.0 is as follows: Temper T6
Section 3.9.6.1
3.9.6.1 T6 Temper — Figure 3.9.6.1.6 presents a typical tensile stressstrain curve.
3510
MMPDS01 31 January 2003
Table 3.9.6.0(b). Design Mechanical and Physical Properties of A357.0 Aluminum Alloy Casting
Specification . . . . . . . . . . . . . . . . .
AMSA21180
Form . . . . . . . . . . . . . . . . . . . . . . .
Castinga
Temper . . . . . . . . . . . . . . . . . . . . .
T6
Location Within Casting . . . . . . . .
Designated area
Nondesignated area
Strength Class Numberb . . . . . . . . .
1
2
10
11
12
Basis . . . . . . . . . . . . . . . . . . . . . . .
S
S
S
S
S
Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . . . . . . .
45
50
38
41
45
Fty, ksi . . . . . . . . . . . . . . . . . . . . .
35
40
28
31
35
Fcy, ksi . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . .
35 28
40 31
28 24
31 26
35 28
Fbrud, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . .
77 96
86 107
65 81
70 88
77 96
Fbryd, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . .
55 65
63 75
44 52
49 58
55 65
e, percent . . . . . . . . . . . . . . . . . .
3
5
5
3
3
c
3
E, 10 ksi . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . µ .........................
10.4 10.5 3.9 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . . . . . α, 106 in./in./EF . . . . . . . . . . . . .
0.097 0.23 (at 212EF) 88 (at 77EF) 12.0 (68 to 212EF)
a For any casting process; i.e., special mold, permanent mold, or sand mold (including chilling). b The attainable strength class number is dependent on the casting configuration, complexity, and size (both weight and wall thickness). Favorable experience with a particular configuration may allow some foundries to produce a higher strength class number than others. In case of doubt regarding the strength class number, the designer should consult or negotiate with the foundry to determine the proper strength class number to assign for a specific casting. c The mechanical properties shown are reliably obtainable in castings of this alloy and heattreat condition when produced under the quality assurance provisions of AMSA21180. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. d Bearing values are “dry pin” values per Section 1.4.7.1.
3511
MMPDS01 31 January 2003
50
40
Stress, ksi
30
20
Ramberg  Osgood n (tension) = 16 10 TYPICAL
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.9.6.1.6. Typical tensile stressstrain curve for A357.0T6 aluminum alloy casting, Class 2, designated area, at room temperature.
3512
MMPDS01 31 January 2003 3.9.7 D357.0 ALLOY 3.9.7.0 Comments and Properties — D357.0 is a modification of A357.0 with narrower compositional limits and more stringent inspection requirements. These modifications were necessary to reduce variability in mechanical properties to a degree compatible with the determination of A and Bbasis values. D357.0 is a heattreatable AlSiMg alloy generally used for premium quality castings in which special properties are developed by careful control of casting and chilling techniques. It has excellent casting characteristics and provides high strength together with good toughness. The alloy also has excellent corrosion resistance. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification for D357.0 aluminum is presented in Table 3.9.7.0(a). Room temperature mechanical and physical properties are shown in Table 3.9.7.0(b). Table 3.9.7.0(a). Material Specification for D357.0 Aluminum Alloy
Specification
Form
AMS 4241
Casting
The temper index for D357.0 is as follows: Temper T6
Section 3.9.7.1
3.9.7.1 T6 Temper — Figure 3.9.7.1.6 presents a typical tensile stressstrain curve.
3513
MMPDS01 31 January 2003
Table 3.9.7.0(b). Design Mechanical and Physical Properties of D357.0 Aluminum Alloy Casting
Specification . . . . . . . . . . . . . . . . . .
AMS 4241
Form . . . . . . . . . . . . . . . . . . . . . . . .
Casting
Temper . . . . . . . . . . . . . . . . . . . . . .
T6
Thickness, in. . . . . . . . . . . . . . . . . .
#2.500
...
Location Within Casting . . . . . . . . .
Designated area
Nondesignated area
Basis . . . . . . . . . . . . . . . . . . . . . . . .
A
B
S
Mechanical Propertiesa: Ftu, ksi . . . . . . . . . . . . . . . . . . . . . .
46
49
45
Fty, ksi . . . . . . . . . . . . . . . . . . . . . .
39
41
36
Fcy, ksi . . . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . . . . .
39 29
41 31
36 28
Fbrub, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . .
79 99
84 105
77 96
Fbryb, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . . . .
62 73
65 77
57 67
e, percent (Sbasis) . . . . . . . . . . . .
3
...
2
3
E, 10 ksi . . . . . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . . . . µ ..........................
10.4 10.5 3.9 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . . . . . . α, 106 in./in./EF . . . . . . . . . . . . . .
0.097 0.23 (at 212EF) 88 (at 77EF) 12.0 (68 to 212EF)
a The mechanical properties shown are reliably obtainable when castings are produced under the quality assurance provisions of AMS 4241. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. b Bearing values are “dry pin” values per Section 1.4.7.1.
3514
MMPDS01 31 January 2003
50
40
Stress, ksi
30
20
Ramberg  Osgood n (tension) = 16
10
TYPICAL
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 3.9.7.1.6. Typical tensile stressstrain curve for D357.0T6 aluminum alloy casting, designated area, at room temperature.
3515
MMPDS01 31 January 2003 3.9.8 359.0 ALLOY 3.9.8.0 Comments and Properties — 359.0 is a relatively highstrength permanentmold casting alloy. It is heat treatable, and has good corrosion resistance. Refer to Section 3.1.3.4 for comments regarding the weldability of the alloy. A material specification for 359.0 aluminum alloy is presented in Table 3.9.8.0(a). Roomtemperature mechanical and physical properties are shown in Table 3.9.8.0(b). Table 3.9.8.0(a). Material Specification for 359.0 Aluminum Alloy
Specification
Form
AMSA21180
Casting
3516
MMPDS01 31 January 2003
Table 3.9.8.0(b). Design Mechanical and Physical Properties of 359.0 Aluminum Alloy Casting
Specification . . . . . . . . . . . . .
AMSA21180
Form . . . . . . . . . . . . . . . . . . .
Casting
Temper . . . . . . . . . . . . . . . . .
T6
Location Within Casting . . . .
Designated area
Nondesignated area
Strength Class Numbera . . . .
1
2
10
11
Basis . . . . . . . . . . . . . . . . . . .
S
S
S
S
Mechanical Properties : Ftu, ksi: . . . . . . . . . . . . . . . .
45
47
45
40
Fty, ksi: . . . . . . . . . . . . . . . .
35
38
34
30
Fcy, ksi: . . . . . . . . . . . . . . . .
35
38
34
30
Fsu, ksi . . . . . . . . . . . . . . . . .
28
29
28
25
77 96
81 101
77 96
69 86
b,c
d
Fbru , ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . Fbryd, ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . .
55 65
60 71
54 63
47 56
e, percent . . . . . . . . . . . . . .
4
3
4
3
3
E, 10 ksi . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . µ .....................
10.5 10.7 4.0 0.33
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] . . . . α, 106 in./in./EF . . . . . . . . .
0.097 0.23 (at 212EF) 88 (at 77EF) 11.0 (68 to 212EF)
a The attainable strength class number is dependent on the casting configuration, complexity, and size (both weight and wall thickness). Favorable experience with a particular configuration may allow some foundries to produce a higher strength class number than others. In case of doubt regarding the strength class number, the designer should consult or negotiate with the foundry to determine the proper strength class number to assign for a specific casting. b For any casting process; i.e., special mold, permanent mold, or sand mold (including chilling). c The mechanical properties shown are reliably obtainable in castings of this alloy and heattreat condition when produced under the quality assurance provisions of AMSA21180. These provisions require preproduction approval, documentation of foundry procedures, and specific destructive and nondestructive testing procedures for the acceptance of each production lot of castings. Strict adherence to these requirements is mandatory if these properties are to be reliably assured in each casting. d Bearing values are “dry pin” values per Section 1.4.7.1.
3517
MMPDS01 31 January 2003
3.10 ELEMENT PROPERTIES 3.10.1 BEAMS — See Chapter 1 and Reference 1.7.1 for general information on stress analysis of beams. 3.10.1.1 Simple Beams — Beams of solid, tubular, or similar cross sections can be assumed to fail through exceeding an allowable modulus of rupture in bending (Fb). In the absence of specific data, the ratio Fb/Ftu can be assumed to be 1.25 for solid sections. 3.10.1.1.1 Round Tubes — For round tubes, the value of Fb will depend on the D/t ratio as well as the ultimate tensile stress. The bending moduli of rupture of round tubes of various aluminum alloys are given in Figure 3.10.1.1.1. It should be noted that these values apply only when the tubes are restrained against local buckling at the loading points. 3.10.1.1.2 Unconventional Cross Section — Sections other than solid or tubular should be tested to determine the allowable bending stress.
 9:
Figure 3.10.1.1.1. Bending modulus of rupture for aluminum alloy round tubing.
3.10.1.2 BuiltUp Beams — Builtup beams will usually fail because of local failures of the component parts. In aluminumalloy construction, the strength of fittings and joints is an important feature (see Reference 3.10.1.2). 3.10.1.3 ThinWeb Beams — The allowable stress for thinweb beams will depend on the nature of the failure and is determined from the allowable stresses of the web in tension and of the flanges or stiffeners in compression.
3518
MMPDS01 31 January 2003 3.10.2 COLUMNS 3.10.2.1 Section 1.3.8.
Primary Failure — The general formula for primary instability is given in
3.10.2.2 Local Failure — The local stability of aluminum alloy column sections may be determined using the methods outlined in References 3.10.2.2(a) through (e). 3.10.2.3 Column Properties — Curves of the allowable column stresses for round and streamline tubing are given in Figure 3.10.2.3. The allowable stress is plotted against the effective slenderness ratio, defined by the formula: LN L ' ρ ρ c
3519
(3.10.2.3)
MMPDS01 31 January 2003
Figure 3.10.2.3. Allowable column and crushing stresses for 2024 and 6061 aluminum alloy tubing.
3520
MMPDS01 31 January 2003 3.10.3 TORSION 3.10.3.1 General — The torsional failure of aluminumalloy tubes may be due to plastic failure of metal, elastic instability of the walls, or an intermediate condition. Pure shear failure will not usually occur within the range of wall thicknesses commonly used for aircraft tubing. 3.10.3.2 Torsion Properties — The curves of Figures 3.10.3.2(a) through (g) are derived from the method outlined in Reference 2.8.1.1 and take into account the parameter L/D. The theoretical results set forth in Reference 2.8.3.2 have been found to be in good agreement with the experimental results.
Figure 3.10.3.2(a). Torsional modulus of rupture—2014T6 aluminum alloy rolled rod.
3521
MMPDS01 31 January 2003
!"
)89 NVL
! !
!"# $ 8: %&'' $ $ ( ) * $$ +
'W
Figure 3.10.3.2(b). Torsional modulus of rupture—2014T6 aluminum alloy forging.
Figure 3.10.3.2(c). Torsional modulus of rupture—2024T3 aluminum alloy tubing.
3522
MMPDS01 31 January 2003
Figure 3.10.3.2(d). Torsional modulus of rupture—2024T4 aluminum alloy tubing.
)VW NVL
Figure 3.10.3.2(e). Torsional modulus of rupture—6061T6 aluminum alloy tubing.
3523
MMPDS01 31 January 2003
60
7075  T6 rolled rod Ftu = 77 ksi 50
L/D
40
0 1/4 1/2
Fst, ksi
1
2 30
5 20
10 20
10
0 0
10
20
30
40
50
60
70
80
D/t
Figure 3.10.3.2(f). Torsional modulus of rupture—7075T6 aluminum alloy rolled rod.
## $ % # &' ) )(
89
(
)
! "
(
Figure 3.10.3.2(g). Torsional modulus of rupture—7075T6 aluminum alloy forging.
3524
MMPDS01 31 January 2003
REFERENCES 3.1(a)
Aluminum, Vol. I, “Properties, Physical Metallurgy and Phase Diagrams,” Vol. II, “Design and Application,” Vol. III, “Fabrication and Finishing,” American Society for Metals (1967).
3.1(b)
Aluminum Standards and Data, The Aluminum Association.
3.1.2
ANSI/ASC H35.1—1988, “American National Standard Alloy and Temper Designation Systems for Aluminum.”
3.1.2.1.1
Stickley, G. W., and Moore, A. A., “Effects of Lubrication and Pin Surface on Bearing Strengths of Aluminum and Magnesium Alloys,” Material Research & Standards, Vol. 2, No. 9, pp. 747 (September 1962).
3.1.2.1.4
Van Echo, J. A., Page, L. C., Simmons, W. F., and Cross, H. C., Part I, “Short Time Creep Properties of Structural Sheet Materials for Aircraft and Missiles,” WADC TR 6731, 65 pp. (August 1952).
3.1.2.1.5(a) Gideon, D. N., Favor, R. J., Grover, H. J., and McClure, G. M., “The Fatigue Behavior of Certain Alloys in the Temperature Range from Room Temperature to 423EF,” Advances in Cryogenic Engineering, Vol. 7, Plenum Press, New York, pp. 503508 (1962). 3.1.2.1.5(b) Keys, R. D., Keifer, T. F., and Schwartzberg, F. R., “Fatigue Behavior of Aluminum and Titanium Sheet Materials Down to 423EF,” Advances in Cryogenic Engineering, Vol. 10, Plenum Press, New York, pp. 113 (1965). 3.1.2.1.5(c) DeMoney, F. W., and Wolfer, G. C., “The Fatigue Properties of Aluminum Alloy 5083H113 and Butt Weldments at 70 and 300EF,” Advances in Cryogenic Engineering, Vol. 6, Plenum Press, New York, pp. 590603 (1961). 3.1.2.1.5(d) “Fatigue Design Handbook,” Vol. 4, Society of Automotive Engineers (1968). 3.1.2.1.5(e) Heywood, R. B., “Designing Against Fatigue of Metals,” Reinhold Publishing Corp. (1962). 3.1.2.1.5(f)
Grover, H. J., “Fatigue of Aircraft Structures,” Naval Air Systems Command, NAVAIR 011A13 (1966).
3.1.2.1.5(g) Harris, W. J., “Metallic Fatigue,” International Series of Monographs in Aeronautics and Astronautics, Vol. I (1961). 3.1.2.1.5(h) “Effect of Environment and Complex Load History of Fatigue Life,” ASTM STP 463 (1970). 3.1.2.1.5(i)
“Fatigue Crack Propagation,” ASTM STP 415 (1967).
3.1.2.1.5(j)
Pope, J. A., “Metal Fatigue,” London, Chapman and Hall (1959).
3.1.2.1.5(k) Rassweiler, G. M., and Grube, W. L., “Internal Stress and Fatigue in Metals,” Elsevier Publishing Company (1959). 3.1.2.1.5(l)
“Symposium on Fatigue of Aircraft Structures,” WADC TR 59507 (1959).
3525
MMPDS01 31 January 2003 3.1.2.1.5(m) “Symposium on Fatigue of Aircraft Structures: LowCycle, FullScale, and Helicopter,” ASTM STP 338 (1962). 3.1.2.1.5(n) Sines, G., and Waisman, J. L., “Metal Fatigue,” McGrawHill (1959). 3.1.2.1.5(o) “Symposium on the Basic Mechanisms of Fatigue,” ASTM STP 237 (1959). 3.1.2.1.5(p) Manson, S. S., “Fatigue: A Complex Subject—Some Simple Approximations,” Experimental Mechanics, Vol. 5, No. 7, pp. 193226 (July 1965). 3.1.2.1.5(q) Morrow, J. D., “Cyclic Plastic Strain Energy and the Fatigue of Metals,” Symposium on Internal Friction, Damping and Cyclic Plasticity, ASTM STP 378 (1964). 3.1.2.1.5(r)
Hartman, E. C., Holt, M., and Eaton, I. D., “Static and Fatigue Strength of HighStrength AluminumAlloy Bolted Joints,” National Advisory Committee for Aeronautics, Technical Note 2276, p. 61 (February 1952).
3.1.2.1.5(s)
Holt, M., “Results of Shear Fatigue Tests of Joints with 3/16InchDiameter 24S T31 Rivets in 0.064InchThick Al Clad Sheet,” U.S. National Advisory Committee for Aeronautics, Technical Note No. 2012, p. 51 (February 1950).
3.1.2.1.6(a) “Standard Method of Test for PlaneStrain Fracture Toughness of Metallic Materials,” ASTM Designation E399 (Annual). 3.1.2.1.6(b) Kaufman, J. G., Shilling, P. E., and Nelson, F. G., “Fracture Toughness of Aluminum Alloys,” Metals Engineering Quarterly, pp. 3947 (August 1969). 3.1.2.1.6(c) Kaufman, J. G., Moore, R. L., and Schilling, P. E., “Fracture Toughness of Structural Aluminum Alloys,” presented at 1969 ASM Materials Engineering Congress, Philadelphia, Pennsylvania (October 14, 1969). 3.1.2.1.6(d) Anon., “Fracture Mechanics Data on Aluminum,” from Aluminum Company of America (June 12, 1973) (MCIC 86213). 3.1.2.1.6(e) Eichenberger, T. W., “Fracture Resistance Data Summary,” Report D220947, The Boeing Company (June 1962) (MCIC 62306). 3.1.2.1.6(f)
Smith, S. H., and Liu, A. F., “Fracture Mechanics Application to Materials Evaluation and Selection for Aircraft Structure and Fracture Analysis,” D617756.
3.1.2.1.6(g) Allen, F. C., “Effects of Thickness on the Fracture Toughness of 7075 Aluminum in the T6 and T73 Conditions,” Damage Tolerance in Aircraft Structures, ASTM STP 486, pp. 1638 (1971). 3.1.2.1.6(h) Broek, D., “The Residual Strength of Aluminum Alloy Sheet Specimens Containing Fatigue Cracks or Saw Cuts,” NLRTR M. 2143, National Aerospace Laboratory, Amsterdam (1966). 3.1.2.1.6(i)
Broek, D., “The Effect of Finite Specimen Width on the Residual Strength of Light Alloy Sheet,” TR M. 2152, National Aero and Astronautical Research Institute, Amsterdam (1965) (MCIC 70485).
3526
MMPDS01 31 January 2003 3.1.2.1.6(j)
Feddersen, C. E., and Hyler, W. S., “Fracture and FatigueCrackPropagation Characteristics of 7075T7351 Aluminum Alloy Sheet and Plate,” Report No. G8902, Battelle Memorial Institute, Columbus, Ohio (March 1970) (MCIC 79089).
3.1.2.1.7(a) Campbell, J. E., “Aluminum Alloys for Cryogenic Service,” Materials Research & Standards, Vol. 4, No. 10, pp. 540548 (October 1964). 3.1.2.1.7(b) Bogardus, K. O., Stickley, G. W., and Howell, F. M., “A Review of Information on the Mechanical Properties of Aluminum Alloys at Low Temperatures,” National Advisory Committee on Aeronautics, Technical Note 2082, 64 pp. (May 1950). 3.1.2.1.7(c) Kaufman, J. G., Bogardus, K. O., and Wanderer, E. T., “Tensile Properties and Notch Toughness of Aluminum Alloys at 452EF in Liquid Helium,” Advances in Cryogenic Engineering, Vol. 13, Plenum Press, New York, pp. 294308 (1968). 3.1.2.1.7(d) Kaufman, J. G., and Wanderer, E. T., “Tensile Properties and Notch Toughness of 7000 Series Aluminum Alloys, Notably 7005, at 452EF,” Advances in Cryogenic Engineering, Vol. 15, Plenum Press, New York (to be published). 3.1.2.1.7(e) Kaufman, J. G., and Holt, M., “Evaluation of Fracture Characteristics of Aluminum Alloys at Cryogenic Temperatures,” Advances in Cryogenic Engineering, Vol. 10, Plenum Press, New York, pp. 7785 (1965). 3.1.2.1.7(f)
Kaufman, J. G., and Johnson, E. W., “New Data from Alcoa Research Laboratories on Aluminum in Cryogenic Applications,” Advances in Cryogenic Engineering, Vol. 6, Plenum Press, New York, pp. 637649 (1960).
3.1.2.1.8
Holt, M., and Bogardus, K. O., “The ‘Hot’ Aluminum Alloys,” Product Engineering (August 16, 1965).
3.1.2.3.1(a) Sprowls, D. O., and Brown, R. H., “Resistance of Wrought HighStrength Aluminum Alloys to Stress Corrosion,” Metal Progress, Part I (April 1962), and Part II (May 1962). 3.1.2.3.1(b) Rutemiller, H. C., and Sprowls, D. O., “Susceptibility of Aluminum Alloys to Stress Corrosion,” Materials Protection (June 1963). 3.1.2.3.1(c) Spuhler, E. H., and Burton, C. L., “Avoiding StressCorrosion Cracking in High Strength Aluminum Alloy Structures,” Alcoa Green Letter Booklet No. 188 (April 1970). 3.1.2.3.1(d) Jackson, J. D., and Boyd, W. K., “Preventing StressCorrosion Cracking of High Strength Alloy Parts,” Materials in Design Engineering (May 1966). 3.1.2.3.2
Lifka, B. W., Sprowls, D. O., and Kaufman, J. G., “Exfoliation and StressCorrosion Characteristics of High Strength, Heat Treatable Aluminum Alloy Plate,” Corrosion, Vol. 23, No. 11, pp. 335342 (November 1967).
3.2.1.1.8(a) Howell, F. M., and Miller, J. L., “Axial Stress, Fatigue Strength of Structural Aluminum Alloys,” American Society for Testing Materials, Vol. 55 (1955) (MMPDS Item 6217). 3.2.1.1.8(b) Lazan, B. J., and Blatherwick, A. A., “Fatigue Properties of Aluminum Alloys at Various Direct Stress Ratios, Part 1—Rolled Alloys,” WADC Technical Report 52307 (December 1952) (MCIC 107775). 3527
MMPDS01 31 January 2003 3.2.1.1.8(c) Lazan, B. J., and Blatherwick, A. A., “Fatigue Properties of Aluminum Alloys at Various Direct Stress Ratios, Part 2—Extruded Alloys,” WADC Technical Report 52307 (December 1952) (MCIC 107776) (Battelle Source M535). 3.2.1.1.8(d) Wang, D. Y., “Axial Loading Fatigue Properties of 7079T6, 7075T6, and 2014T6 Aluminum Alloy Hand Forgings,” WADC Technical Report 5859 (July 1958) (MCIC 108811). 3.2.1.1.8(e) Nordmark, G. E., Lifka, B. W., et al., “StressCorrosion and CorrosionFatigue Susceptibility of HighStrength Aluminum Alloys,” Alcoa Technical Report 70259 (November 1970) (MCIC 79945). 3.2.3.1.8(a) Grover, H. J., Bishop, S. M., and Jackson, L. R., “Fatigue Strengths of Aircraft Materials: AxialLoad Fatigue Tests on Unnotched Sheet Specimens of 24ST3 and 75ST6 Aluminum Alloys and of SAE 4130 Steel,” National Advisory Committee for Aeronautics, Technical Note 2324 (March 1951) (Battelle Source M506). 3.2.3.1.8(b) Grover, H. J., Bishop, S. M., and Jackson, L. R., “Fatigue Strengths of Aircraft Materials: AxialLoad Fatigue Tests on Notched Sheet Specimens of 24ST3 and 75ST6 Aluminum Alloys and of SAE 4130 Steel with StressConcentration Factors of 2.0 and 4.0,” National Advisory Committee for Aeronautics, Technical Note 2389 (June 1951) (Battelle Source M507). 3.2.3.1.8(c) Grover, H. J., Bishop, S. M., and Jackson, L. R., “Fatigue Strengths of Aircraft Materials; AxialLoad Fatigue Tests on Notched Specimens of 24ST3 and 75ST6 Aluminum Alloys and of SAE 4130 Steel with StressConcentration Factor of 5.0,” National Advisory Committee for Aeronautics, Technical Note 2390 (June 1951) (Battelle Source M508). 3.2.3.1.8(d) Grover, H. J., Hyler, W. S., and Jackson, L. R., “Fatigue Strengths of Aircraft Materials; AxialLoad Fatigue Tests on Notched Sheet Specimens of 24ST3 and 75ST6 Aluminum Alloys and of SAE 4130 Steel with StressConcentration Factor of 1.5,” National Advisory Committee for Aeronautics, Technical Note 2639 (February 1952) (Battelle Source M509). 3.2.3.1.8(e) Hardrath, H. F., and Ilig, W., “Fatigue Tests at Stresses Producing Failure in 2 to 10,000 Cycles 24ST3 and 75ST6 Aluminum Alloy Sheet Specimens with a Theoretical StressConcentration Factor of 4.0 Subjected to Completely Reversed Axial Load,” National Advisory Committee of Aeronautics, Technical Note 3132 (January 1954) (Battelle Source M510). 3.2.3.1.8(f)
Ilig, W., “Fatigue Tests on Notched and Unnotched Sheet Specimens of 2024T3 and 7075T6 Aluminum Alloys and of SAE 4130 Steel with Special Consideration of the Life Range from 2 to 10,000 Cycles,” National Advisory Committee for Aeronautics, Technical Note 3866 (December 1956) (Battelle Source M512).
3.2.3.1.8(g) Grover, H. J., Hyler, W. S., and Jackson, L. R., “Fatigue Strengths of Aircraft Materials; AxialLoad Fatigue Tests on EdgeNotched Sheet Specimens of 2024T3 and 7075T6 Aluminum Alloys and of SAE 4130 Steel with Notch Radii of 0.004 and 0.070 Inch,” National Aeronautics and Space Administration, Technical Note D111 (September 1959) (Battelle Source M513). 3.2.3.1.8(h) Naumann, E. C., Hardrath, H. F., and Guthrie, D. E., “AxialLoad Fatigue Tests of 2024T3 and 7075T6 AluminumAlloy Sheet Specimens Under Constant and Variable Amplitude Loads,” National Aeronautics and Space Administration, Technical Note D212 (December 1959) (Battelle Source M514). 3528
MMPDS01 31 January 2003 3.2.3.1.8(i)
Topper, T. H., and Morrow, J., “Simulation of the Fatigue Behavior at the Notch Root in Spectrum Loaded Notch Member (u),” Naval Air Development Center, Final Report (January 1970).
3.2.7.1.9(a) Pionke, L. J., and Linback, R. K., “Fracture Mechanics Data for 2024T861 and Aluminum,” NASA CR, MDDC E1153, McDonnell Douglas Astronautics Company (October 25, 1974). 3.2.7.1.9(b) Cervay, R. R., “Temperature Effect on the Mechanical Properties of Aluminum Alloy 2124T851,” AFMLTR75208 (December 1975). 3.2.7.1.9(c) Thompson, D. S., and Zinkham, R. E., “Program to Improve the Fracture Toughness and Fatigue Resistance of Aluminum Sheet and Plate for Airframe Applications,” AFMLTR73247, Vol. II (September 1974). 3.2.7.1.9(d) Babilion, C. F., Wygonik, R. H., Nordmark, G. E., and Lifka, B. W., “Mechanical Properties, Fracture Toughness, Fatigue, Environmental Fatigue Crack Growth Rates, and Corrosion Characteristics of HighToughness Aluminum Alloy Forgings, Sheet, and Plate,” AFMLTR7383 (April 1973) (MCIC 86842) (Battelle Source M118). 3.2.8.2.8
Ferguson, R. F., “Axial Stress Fatigue Strength of 2219T851 Aluminum Alloy Plate,” Report No. TFD71960, North American Rockwell, Los Angeles Division (July 29, 1971) (Battelle Source M216).
3.7.3.1.8(a) Rothweiler, C. E., and Maynard, P. S., “Evaluation of 7049T73 Aluminum Alloy for RA5C Wing Inner Panel Fold Rib,” CMES Contract N0025671C0064, Task No. NAR18 (P04610), Report No. NR72H278, North American Rockwell, Columbus, Ohio (July 14, 1972) (Battelle Source M170). 3.7.3.1.8(b) Anon., “Boeing Test Data on X7049T73,” Submitted to Battelle to provide input data for Item 6824 (1969) (MCIC 78639). 3.7.3.1.8(c) Mixon, W., and Turley, R. V., “Evaluation of Aluminum Alloys 7049T73 and 7175T736 Die Forging,” Engineering Technical Report No. ETRMDCJ0692, McDonnell Douglas (April 7, 1970) (MCIC 110111). 3.7.3.1.8(d) VanOrden, J. M., “Evaluation of 7049T73 Aluminum Alloy HandForged Billet,” Lockheed California Company, Report No. LR 23447 (February 1970) (Battelle Source M43). 3.7.3.1.8(e) “Effect of Manufacturing Processes on Structural Allowables—Phase I,” Battelle, Columbus, Ohio, AFWALTR854128 (January 1986). 3.7.4.2.8(a) Guthorn, P. S., “Design Properties and Processing Limits for Improved Aluminum Alloys,” McDonnell Douglas Corporation, MDCJ1912 (December 1983) (Battelle Source M629). 3.7.4.2.8(b) Garland, K., “Evaluation of X7050T736 Die Forgings,” McDonnell Aircraft Company, McDonnell Douglas Corporation, Report No. 514131.10 (February 1973) (MCIC 85880). 3.7.4.2.8(c) Deel, O. L., Ruff, P. E., and Mindlin, H., “Engineering Data on New Aerospace Structural Materials,” AFMLTR114 (June 1973) (Battelle Source M467). 3.7.4.2.8(d) Gallo, K. L., “Load Control Fatigue Data Reports,” Westmoreland Mechanical Testing and Research, Inc., March 1997. 3529
MMPDS01 31 January 2003 3.7.4.2.8(e) Deschapelles, J. B., “Improved Fatigue Resistance of 7050 Thick Plate Aluminum Through Minimization of Microporosity,” Effects of Product Quality and Design Criteria on Structural Integrity, ASTM STP 1337, R. C. Rice and D. E. Tritsch, Eds., American Society for Testing and Materials, 1998. 3.7.4.2.9(a) Northrop, attachments to letter from V. C. Frost to D. J. Jones (March 4, 1981) (Battelle Source M482). 3.7.4.2.9(b) Davis, R. E., Nordmark, G. E., and Walsh, J. D., “Design Mechanical Properties, Fracture Toughness, Fatigue Properties, Exfoliation, and StressCorrosion Resistance of 7050 Sheet, Plate, Hand Forgings, Die Forgings, and Extrusions,” Report N0001972C0512, Aluminum Company of America (July 1975) (Battelle Source M322). 3.7.4.3.8(a) Staley, J. T., Jacoby, J. E., Davies, R. E., Nordmark, G. E., Walsh, J. D., and Rudolph, F. R., “Aluminum Alloy 7050 Extrusions,” AFMLTR76129 (March 1977) (MCIC 99225) (Battelle Source M374). 3.7.6.1
Brownfield, C. D., and Badger, D. M., “Effects of TemperatureTimeStress Histories on the Mechanical Properties of Aircraft Structural Metallic Materials,” WADC TR 56585, Part II (September 1960).
3.7.6.1.8
Howell, F. M., and Miller, J. L., “Axial Fatigue Strengths of Several Structural Aluminum Alloys,” Proceedings of the American Society for Testing Materials, Philadelphia, PA (1956).
3.7.6.1.9(a) Hudson, C. M., and Hardrath, H. F., “Effects of Changing Stress Amplitude on the Rate of FatigueCrackPropagation in Two Aluminum Alloys,” National Aeronautics and Space Administration, Technical Note D960 (1961). 3.7.6.1.9(b) McEvily, A. J., and Ilig, W., “The Rate of FatigueCrack Propagation in Two Aluminum Alloys,” National Aeronautics and Space Administration, Technical Note 4394 (1958). 3.7.6.1.9(c) Broek, D., and Schijve, J., “The Influence of Mean Stress on the Propagation of Fatigue Cracks in Aluminum Alloy Sheet,” NLRTR, M. 2111, Reports and Transactions, National Aero and Astronautical Research Institute, pp. 4161 (1965). 3.7.6.1.9(d) Dubensky, R. G., “FatigueCrack Propagation in 2024T3 and 7075T6 Aluminum Alloys at High Stresses,” NASA CR1732 (1971). 3.7.6.1.9(e) Hudson, C. M., “Effect of Stress Ratios on FatigueCrack Growth in 7075T6 and 2024T3 Aluminum Alloy Specimens,” National Advisory Committee for Aeronautics, Technical Note D5390 (August 1969) (MCIC 75599). 3.7.6.1.9(f)
Gurin, P. J., “Crack Propagation Tests for Some Aluminum Alloy Materials,” LR 10498, Lockheed Aircraft Corporation (1955).
3.7.6.2.9(a) Unpublished Battelle, Columbus, Ohio data by C. F. Fedderson. 3.7.6.2.9(b) “B1 Program Data for Aluminum Alloys,” Rockwell International Corporation, Memorandum to H. D. Moran from E. W. Cawthorne, Battelle, Columbus, Ohio (April 3, 1974) (MCIC 88579).
3530
MMPDS01 31 January 2003 3.7.6.2.9(c) Ruff, P. E., and Smith, S. H., “Development of MILHDBK5 Design Allowable Properties and FatigueCrackPropagation Data for Several Aerospace Materials,” AFMLTR77162 (October 1977). 3.7.7.2.8
Unpublished Letter to D. Lahrman, Battelle, from Alcoa, “Fatigue Properties of 7150T77511 Extruded Shapes.” (December 9, 1993) (Battelle Source M798).
3.7.8.1.8(a) Unpublished Letter to P. Ruff, Battelle Memorial Institute, from LockheedGeorgia, “Fatigue Data on 7175T7351 Extrusions,” January 1982. 3.7.8.1.8(b) Carter, F. J., Bateh, E. J., and White, D. L., “C5A Wing Modification Program, Material Characterization Program, 7175T7511 Extrusions,” LockheedGeorgia Company, Report No. LG75ER01862, September 1977 (MCIC 122032). 3.7.8.1.8(c) Unpublished Letter to P. Ruff, Battelle Memorial Institute, from Aluminum Company of America, “Fatigue Data on 7175T73511 Extrusions and 7175T74 Forgings,” January 24, 1990 (Battelle Source M748). 3.7.8.2.8(a) Schimmelbusch, H. W., “Metallurgical Evaluation of 7175T736 and 7175T66 Die Forgings,” Boeing Company Document No. D624480, May 1970 (MCIC 78656). 3.7.8.2.8(b) Newcomer, R., “Evaluation of Aluminum Forging Alloy 7175T736,” McDonnell Aircraft Company Report No. MDC 70024, 1970 (MCIC 85881). 3.7.8.2.8(c) Deel, O. L., and Mindlin, H., “Engineering Data on New and Emerging Structural Materials,” AFML Report No. AFMLTR70252, October 1970 (Battelle Source M464). 3.7.10.2.8(d) Doepker, P., “Effect of Manufacturing Process on Structural Allowables,” AFWAL Report No. AFWALTR854049 (Battelle Source M626). 3.7.10.2.8(a) Brownhill, D. J., Davies, R. E., Nordmark, G. E., and Ponchel, B. M., “Exploratory Development for Design Data on Structural Aluminum Alloys in Representative Aircraft Environments,” AFMLTR77102 (July 1977) (MCIC 103463) (Battelle Source M397). 3.7.10.2.8(b) Unpublished letter to P. Vieth, Battelle, Columbus, Ohio from ALCOA, “Fatigue Data for 7050 and 7475 Products” (July 17, 1985) (Battelle Source M630). 3.7.10.2.8(c) Jones, R. L., and Coyle, T. E., “The Mechanical Stress Corrosion, Fracture Mechanics, and Fatigue Properties of 7050, 7475, and Ti8Mo8V2Fe3Al Plate and Sheet Alloys,” General Dynamics, Report No. FGT5791 (July 24, 1973) (MCIC 100670). 3.7.10.2.8(d) Figge, F. A., “Advanced Metallic Structure: Air Superiority Fighter Wind Design for Improved Cost, Weight, and Integrity,” AFFDLTR7352, Vol. III (June 1973) (MCIC 86574) (Battelle Source M278). 3.7.10.2.8(e) Deel, O. L., Ruff, P. E., and Mindlin, H., “Engineering Data on New Aerospace Structural Materials,” AFMLTR7597 (June 1975) (MCIC 95044) (Battelle Source M468). 3.7.10.2.9(a) Cervay, R. R., “Engineering Design Data for Aluminum Alloy 7475 in the T761 and T61 Conditions,” AFMLTR72173 (September 1972) (MCIC 85363).
3531
MMPDS01 31 January 2003 3.7.10.2.9(b) Cervay, R. R., “Static and Dynamic Fracture Properties for Aluminum Alloy 7475T651 and T7351,” AFMLTR7520 (April 1975). 3.8.1.1.8(a) Unpublished data from Garrett Turbine Engine Company, 1986 (Battelle Source M690). 3.8.1.1.8(b) Unpublished data from Northrop Corporation, 1988 (Battelle Source M701). 3.10.1.2
Eato, I. D., and Holt, M., “Flexural Fatigue Strengths of Riveted Box Beams—Alclad 14ST6, Alclad 75ST6, and Various Tempers of Alcald 24S,” National Advisory Committee for Aeronautics, Technical Note 2452, 25 pp. (November 1951).
3.10.2.2(a)
Gerard, G., and Becker, H., Handbook of Structural Stability, “Part I—Buckling of Flat Plates,” National Advisory Committee for Aeronautics, Technical Note 3781 (July 1957).
3.10.2.2(b)
Becker, H., Handbook of Structural Stability, “Part II—Buckling of Composite Elements,” National Advisory Committee for Aeronautics, Technical Note 3782 (July 1957).
3.10.2.2(c)
Gerard, G., and Becker, H., Handbook of Structural Stability, “Part III—Buckling of Curved Plates and Shells,” National Advisory Committee for Aeronautics, Technical Note 3783 (1957).
3.10.2.2(d)
Gerard, G., Handbook of Structural Stability, “Part IV—Failure of Plates and Composite Elements,” National Advisory Committee for Aeronautics, Technical Note 3784 (1957).
3.10.2.2(e)
Gerard, G., Handbook of Structural Stability, “Part V—Compressive Strengths of Flat Stiffened Panels,” National Advisory Committee for Aeronautics, Technical Note 3785 (August 1957).
3532
MMPDS01 31 January 2003
CHAPTER 4 MAGNESIUM ALLOYS 4.1
GENERAL
This chapter contains the engineering properties and characteristics of wrought and cast magnesium alloys used in aircraft and missile applications. Magnesium is a lightweight structural metal that can be strengthened greatly by alloying, and in some cases by heat treatment or cold work or by both. 4.1.1 ALLOY INDEX — The magnesium alloys in this chapter are listed in alphanumeric sequence in each of two parts, the first one being wrought forms of magnesium and the second cast forms. These sections and the alloys covered under each are shown in Table 4.1.
Table 4.1. Magnesium Alloys Index
Section 4.2 4.2.1 4.2.2 4.2.3 4.3 4.3.1 4.3.2 4.3.3 4.3.4 4.3.5 4.3.6
Designation MagnesiumWrought Alloys AZ31B AZ61A ZK60A MagnesiumCast Alloys AM100A AZ91C/AZ91E AZ92A EZ33A QE22A ZE41A
4.1.2 MATERIAL PROPERTIES 4.1.2.1 Mechanical Properties — The mechanical properties are given either as design values or for information purposes. The tensile strength (Ftu), tensile yield strength (Fty), elongation (e), and sometimes the compressive yield strength (Fcy) are guaranteed by procurement specifications. The properties obtained reflect the location of sample, type of test specimen and method of testing required by the product specification. The remaining design values are “derived” values; that is, sufficient tests have been made to ascertain that if a given material meets the requirements of the product specification, the material will have the compression (Fcy), shear (Fsu) and bearing (Fbru and Fbry) strengths listed. 4.1.2.1.1 Tension Testing — Roomtemperature tension tests are made according to ASTM E 8. The yield strength (Fty) is obtained by the “offset method” using an offset of 0.2 percent. The speed of testing for roomtemperature tests has a small effect on the strength and elongation values obtained on most magnesium alloys. The rate of stressing generally specified to the yield strength is less than 100,000 psi per minute and the rate of straining from the yield strength to fracture is less than 0.5 in./in./min. It can be
41
MMPDS01 31 January 2003 expected that the speed of testing used for roomtemperature tension tests will approach the maximum permitted. Elevatedtemperature tension tests are made according to ASTM E 21. The speed of testing has a considerable effect on the results obtained and no one standard rate of straining is given in ASTM E 21. The strain rates most commonly used on magnesium are 0.005 in./in./min. to the yield and 0.10 in./in./min. from yield to fracture [see References 4.1.2.1.1(a) to (d)]. 4.1.2.1.2 Compression Testing — Compression test methods used for magnesium are specified in ASTM E 9. The values given for the compressive yield strength (Fcy), are taken at an offset of 0.2 percent. References 4.1.2.1.2(a) and (b) provide information on test techniques. 4.1.2.1.3 Bearing Testing — Bearing tests of magnesium alloys are made according to ASTM E 238. The size of pin used has a significant effect on the values obtained, especially the bearing ultimate strength (Fbru). On tests made to obtain the data on magnesium alloys shown in this document, pin diameters of 0.187 and 0.250 inch were used. For pin diameters significantly larger than 0.250 inch lower values may be obtained. Additional information on bearing testing is given in References 4.1.2.1.3(a) and (b). Bearing values in the property tables are considered to be “dry pin” values in accordance with the discussion in Section 1.4.7.1. 4.1.2.1.4 Shear Testing — The shear strength values used in this document were obtained by the “double shear” method using a pintype specimen, the “punch shear” method and the “tension shear” method as applicable. Just as tensile ultimate strength (Ftu) values vary with location and direction of sample in relation to the method of fabrication, the shear strength (Fsu) may be expected to reflect the effect of orientation, either as a function of the sampling or the maximum stresses imposed by the method of test. Information on shear testing is given in Reference 4.1.2.1.4. 4.1.2.1.5 Stress Raisers — The effect of notches, holes, and stress raisers on the static properties of magnesium alloys is described in References 4.1.2.1.5(a) through (c). Additional data on the strength properties of magnesium alloys are presented in References 4.1.2.1.5(d) through (h). 4.1.2.1.6 Creep — Some creep data on magnesium alloys are summarized in Reference 4.1.2.1.6. 4.1.2.1.7 Fatigue — Roomtemperature axial load fatigue data for several magnesium alloys are presented in appropriate alloy sections. References 4.1.2.1.7(a) and (b) provide additional data on fatigue of magnesium alloys. 4.1.3 PHYSICAL PROPERTIES — Selected experimental data from the literature were used in determining values for physical properties. In other cases, enough information was available to calculate the constants. Estimated values of some of the remaining constants were also included. Estimated values are noted. 4.1.4 ENVIRONMENTAL CONSIDERATIONS — Corrosion protection must be considered for all magnesium applications. Protection can be provided by anodic films, chemical conversion coatings, paint systems, platings, or a combination of these methods. Proper drainage must be provided to prevent entrapment of water or other fluids. Dissimilar metal joints must be properly and completely insulated, including barrier strips and sealants. Strainhardened or agehardened alloys may be annealed or overaged by prolonged exposure to elevated temperatures, with a resulting decrease in strength. Maximum recommended temperatures for prolonged service are reported, where available, for specific alloys.
42
MMPDS01 31 January 2003 4.1.5 ALLOY AND TEMPER DESIGNATIONS — Standard ASTM nomenclature is used for the alloys listed. Temper designations are given in ASTM B 296. A summary of the temper designations is given in Table 4.1.5. Table 4.1.5. Temper Designation System for Magnesium Alloysa Basis of Codification The designations for temper are used for all forms of magnesium and magnesium alloy products except ingots and are based on the sequence of basic treatments used to produce the various tempers. The temper designation follows the alloy designation, the two being separated by a dash. Basic temper designations consist of letters. Subdivisions of the basic tempers, where required, are indicated by a digit or digits following the letter. These designate specific sequences of basic treatments, but only operations recognized as significantly influencing the characteristics of the product are indicated. Should some other variation of the same sequence of basic operations be applied to the same alloy, resulting in different characteristics, then additional digits are added to the designation.
NOTE—In material specifications containing reference to two or more tempers of the same alloy which result in identical mechanical properties, the distinction between the tempers should be covered in suitable explanatory notes. Basic Temper Designations F As Fabricated. Applies to the products that acquire some temper from shaping processes not having special control over the amount of strainhardening or thermal treatment. O
Annealed Recrystallized (wrought products only). Applies to the softest temper of wrought products.
H
StrainHardened (wrought products only). Applies to products that have their strength increased by strainhardening with or without supplementary thermal treatments to produce partial softening. The H is always followed by two or more digits. H1
StrainHardened Only. Applies to products that are strainhardened to obtain the desired mechanical properties without supplementary thermal treatment. The number following this designation indicates the degree of strainhardening.
H2
StrainHardened and Then Partially Annealed. Applies to products which are strainhardened more than the desired final amount and then reduced in strength to the desired final amount by partial annealing. The number following this designation indicates the degree of strainhardening remaining after the product has been partially annealed.
H3
StrainHardened and Stabilized. Applies to products that are strainhardened and then stabilized by a low temperature heating to slightly lower their strength and increase ductility. This designation applies only to alloys which, unless stabilized, gradually age soften at room temperature. The number following this designation indicates the degree of strainhardening remaining after the product has been strainhardened a specific amount and then stabilized.
Subdivisions of the “H1", “H2" and “H3" Tempers: The digit following the designations “H1", “H2", and “H3" indicates the final degree of strain hardening. Tempers between 0 (annealed) and 8 (full hard) are designated by numerals 1 through 7. Material having a strength about midway between that of the 0 temper and that of the 8 temper is designated by the numeral 4 (half hard); between 0 and 4 by the numeral 2 (quarter hard); between 4 and 8 by the numeral 6 (threequarter
a From ASTM B 29696.
43
MMPDS01 31 January 2003 Table 4.1.5. Temper Designation System for Magnesium Alloys (Continued)a
hard), etc. The third digit, when used, indicates a variation of a twodigit H temper. It is used when the degree of control of temper or the mechanical properties are different from but close to those for the twodigit H temper to which it is added. Numerals 1 through 9 may be arbitrarily assigned as the third digit for an alloy and product to indicate a specific degree of control of temper or special mechanical property limits. W
Solution HeatTreated. An unstable temper applicable only to alloys which spontaneously age at room temperature after solution heattreatment. This designation is specific only when the period of natural aging is indicated: for example, W ½ hr.
T
Thermally Treated to Product Stable Tempers Other Than F, O, or H. Applies to products which are thermally treated, with or without supplementary strainhardening, to product stable tempers. The T is always followed by one or more digits. Numerals 1 through 10 have been assigned to indicate specific sequences of basic treatments, as follows. T1
Cooled from an Elevated Temperature Shaping Process and Naturally Aged to a Substantially Stable Condition. Applies to products for which the rate of cooling from an elevated temperature shaping process, such as casting or extrusion, is such that their strength is increased by room temperature aging.
T3
Solution Heattreated and Then Cold Worked. Applies to products that are cold worked to improve strength, or in which the effect of cold work in flattening and straightening is recognized in applicable mechanical properties.
T4
Solution Heattreated and Naturally Aged to a Substantially Stable Condition. Applies to products that are not cold worked after solution heattreatment, or in which the effect of cold work in flattening or straightening may not be recognized in applicable mechanical properties.
T5
Cooled from an ElevatedTemperature Shaping Process and Then Artificially Aged. Applies to products which are cooled from an elevatedtemperature shaping process, such as casting or extrusion, and then artificially aged to improve mechanical properties or dimensional stability or both.
T6
Solution Heattreated and Then Artificially Aged. Applies to products that are not cold worked after solution heattreatment, or in which the effect of cold work is flattening or straightening may not be recognized in applicable mechanical properties.
T7
Solution Heattreated and Then Stabilized. Applies to products that are stabilized to carry them beyond the point of maximum strength to provide control of some special characteristics.
T8
Solution Heattreated, Cold Worked, and Then Artificially Aged. Applies to products which are cold worked to improve strength, or in which the effect of cold work in flattening or straightening is recognized in applicable mechanical properties.
T9
Solution Heattreated, Artificially Aged, and Then Cold Worked. Applies to products that are cold worked to improve strength.
a From ASTM B 29696.
44
MMPDS01 31 January 2003 Table 4.1.5. Temper Designation System for Magnesium Alloys (Continued)a
T10
Cooled from an Elevated Temperature Shaping Process, Artificially Aged, and Then Cold Worked. Applies to products which are artificially aged after cooling from an elevated temperature shaping process, such as extrusion, and then cold worked to further improve strength.
A period of natural aging at room temperature may occur between or after the operations listed for tempers T3 through T10. Control of this period is exercised when it is metallurgically important. Additional digits, may be added to designations T1 through T10 to indicate a variation in treatment that significantly alters the characteristics of the product. a From ASTM B 29696.
4.1.6 JOINING METHODS — Most magnesium alloys may be welded; refer to “Comments and Properties” in individual alloy sections. Adhesive bonding and brazing may be used to join magnesium to itself or other alloys. All types of mechanical fasteners may be used to join magnesium. Refer to Section 4.1.4 when using mechanical fasteners or joining of dissimilar materials with magnesium alloys.
45
MMPDS01 31 January 2003
4.2
MAGNESIUMWROUGHT ALLOYS 4.2.1 AZ31B
4.2.1.0 Comments and Properties — AZ31B is a wrought magnesiumbase alloy containing aluminum and zinc. It is available in the form of sheet, plate, extruded sections, forgings, and tubes. AZ31B has good roomtemperature strength and ductility and is used primarily for applications where the temperature does not exceed 300EF. Increased strength is obtained in the sheet and plate form by strain hardening with a subsequent partial anneal (H24 and H26 temper). No treatments are available for increasing the strength of this alloy after fabrication. Forming of AZ31B must be done at elevated temperatures if small radii or deep draws are required. If the temperatures used are too high or the times too great, H24 and H26 temper material will be softened. This alloy is readily welded but must be stress relieved after welding to prevent stress corrosion cracking. Material specifications covering AZ31B wrought products are given in Table 4.2.1.0(a). Roomtemperature mechanical and physical properties are shown in Tables 4.2.1.0(b) through (d). The effect of temperature on physical properties is shown in Figure 4.2.1.0. Table 4.2.1.0(a). Material Specifications for AZ31B Magnesium Alloy
Specification AMS 4375 AMS 4376 AMS 4377 ASTM B 107 ASTM B 91
Form Sheet and plate Plate Sheet and plate Extrusion Forging
The temper index for AZ31B is as follows: Temper O H24 H26 F
Section 4.2.1.1 4.2.1.2 4.2.1.3 4.2.1.4
4.2.1.1 AZ31BO Temper — Effect of temperature on the tensile modulus of sheet and plate is presented in Figure 4.2.1.1.4. Typical roomtemperature stressstrain and tangentmodulus curves are presented in Figure 4.2.1.1.6. 4.2.1.2 AZ31BH24 Temper — Effect of temperature on the mechanical properties of sheet and plate is shown in Figures 4.2.1.2.1 through 4.2.1.2.4, and 4.2.1.2.6. Typical roomtemperature tension and compression stressstrain and tangentmodulus curves for sheet are shown in Figure 4.2.1.2.6. 4.2.1.3 AZ31BH26 Temper 4.2.1.4 AZ31BF Temper — Figures 4.2.1.4.8 (a) and (b) contain fatigue data for forged disk at room temperature.
46
MMPDS01 31 January 2003
Table 4.2.1.0(b). Design Mechanical and Physical Properties of AZ31B Magnesium Alloy Sheet and Plate
Specification . . . . . . . Form . . . . . . . . . . . . . . Temper . . . . . . . . . . . . Thickness, in. . . . . . . . Basis . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L .............. LT . . . . . . . . . . . . . Fty, ksi: L .............. LT . . . . . . . . . . . . . Fcy, ksi: L .............. LTa . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . e, percent . . . . . . . . . L ..............
AMS 4375 Sheet Plate 0
AMS 4377 Plate H24
Sheet
0.016 0.061 0.250 0.501 2.001 0.016 0.063 0.250 0.375 0.501 1.0010.060 0.249 0.500 2.000 3.000 0.062 0.249 0.374 0.500 1.000 2.000
2.0013.000
S
S
S
S
S
S
S
S
S
S
S
S
32 ...
32 ...
32 ...
32 ...
32 ...
39 40
39 40
38 39
37 38
36 37
34 35
34 ...
18 ...
15 ...
15 ...
15 ...
15 ...
29 32
29 32
26 29
24 27
22 25
20 23
18 ...
... ... 17
12 ... 17
10 ... 17
10 ... ...
8 ... ...
... ... 18
24 ... 18
20 ... 18
16 ... 18
13 ... ...
10 ... ...
9 ... ...
50 60
50 60
50 60
... ...
... ...
58 68
58 68
56 65
54 63
... ...
... ...
... ...
29 29
29 29
27 27
... ...
... ...
43 43
43 43
38 38
34 34
... ...
... ...
... ...
12
12
12
10
9
6
6
8
8
8
8
8
3
E, 10 ksi . . . . . . . . . Ec, 103 ksi . . . . . . . . G, 103 ksi . . . . . . . . . µ ............... Physical Properties: ω, lb/in.3 . . . . . . . . . C, K, and α . . . . . . .
6.5 6.5 2.4 0.35 0.0639 See Figure 4.2.1.0
a Fcy(LT) allowables are equal to or greater than Fcy(L) allowables. b Bearing values are “dry pin” values per Section 1.4.7.1.
47
MMPDS01 31 January 2003
Table 4.2.1.0(c). Design Mechanical and Physical Properties of AZ31B Magnesium Alloy Plate
Specification . . . . . . . Form . . . . . . . . . . . . . . Temper . . . . . . . . . . . . Thickness, in. . . . . . . . Basis . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L .............. LT . . . . . . . . . . . . . Fty, ksi: L .............. LT . . . . . . . . . . . . . Fcy, ksi: L .............. LTa . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . e, percent: L .............. E, 103 ksi . . . . . . . . . Ec, 103 ksi . . . . . . . . G, 103 ksi . . . . . . . . . µ ............... Physical Properties: ω, lb/in.3 . . . . . . . . . C, K, and α . . . . . . .
0.2500.375 S
0.3760.438 S
0.4390.500 S
AMS 4376 Plate H26 0.5010.750 S
39 40
38 39
38 39
37 38
37 38
35 36
35 36
27 30
26 29
26 29
25 28
23 26
22 25
21 24
22 ... 18
21 ... 18
18 .... 18
17 ... ...
16 ... ...
15 ... ...
14 ... ...
58 68
56 65
56 65
... ...
... ...
... ...
... ...
40 40
39 39
36 36
... ...
... ...
... ...
... ...
6
6
6
6 6.5 6.5 2.4 0.35
6
6
6
0.7511.000 S
1.0011.500 S
1.5012.000 S
0.0639 See Figure 4.2.1.0
a Fcy(LT) allowables are equal to or greater than Fcy(L) values. b Bearing values are "dry pin" values per Section 1.4.7.1.
48
MMPDS01 31 January 2003
Table 4.2.1.0(d). Design Mechanical and Physical Properties of AZ31B Magnesium Alloy Extrusion and Forging
Specification . . . . . . . Form . . . . . . . . . . . . . . Temper . . . . . . . . . . . . Thickness, in. . . . . . . . Basis . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L .............. LT . . . . . . . . . . . . . Fty, ksi: L .............. LT . . . . . . . . . . . . . Fcy, ksi: L .............. LT . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . e, percent: L .............. E, 103 ksi . . . . . . . . . Ec, 103 ksi . . . . . . . . G, 103 ksi . . . . . . . . . µ ............... Physical Properties: ω, lb/in.3 . . . . . . . . . C, K, and α . . . . . . .
ASTM B 107 ASTM B 91 Extruded bar, rod, and Extruded Extruded tube Forging solid shapes hollow shapes F 0.250 1.500 2.5000.028 0.251#0.249 ... All 1.499 2.499 4.999 0.250b 0.750b S S S S S S S S
35 ...
35 ...
34 ...
32 ...
32 ...
32 ...
32 ...
34 ...
21 ...
22 ...
22 ...
20 ...
16 ...
16 ...
16 ...
19 ...
... ... 17
12 ... 17
12 ... 17
10 ... ...
10 ... ...
10 ... ...
10 ... ...
... ... ...
36 45
36 45
36 45
... ...
... ...
... ...
... ...
... ...
23 23
23 23
23 23
... ...
... ...
... ...
... ...
... ...
7
7
7
7
8
8
4
6
6.5 6.5 2.4 0.35 0.0639 See Figure 4.2.1.0
a Wall thickness for tube; for outside diameter # 6.000 inches. b Bearing values are “dry pin” values per Section 1.4.7.1.
49
MMPDS01 31 January 2003
200
0.45
180
0.40
160
0.35
140
K, Btu/ [ (hr)(ft2)(°F)/ft]
120
α  Between 70 °F and indicated temperature K  At indicated temperature C  At indicated temperature
18
α, 106 in./in./°F
0.50
C, Btu/ (lb)(°F)
220
16 α
14
12
0.30 C 0.25
100
0.20
80
0.15 K, O & H24
60
0.10
40
0.05
20
0.00 400
200
0
200
400
600
800
1000
Temperature, °F Figure 4.2.1.0. Effect of temperature on the physical properties of AZ31B.
410
MMPDS01 31 January 2003
Figure 4.2.1.1.4. Effect of temperature on the tensile modulus (E) of AZ31BO sheet and plate.
25 Tension
20
Compression
Stress, ksi
15
10
Ramberg  Osgood n (Ltension) = 12 n (Lcomp.) = 30
5
TYPICAL
0 0
2
4
6 8 Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
10
12
Figure 4.2.1.1.6. Typical tensile and compressive stressstrain and compressive tangentmodulus curves for AZ31BO sheet and plate at room temperature.
411
MMPDS01 31 January 2003
Figure 4.2.1.2.1. Effect of temperature on the tensile ultimate strength (Ftu) and the tensile yield strength (Fty) of AZ31BH24 sheet and plate.
412
MMPDS01 31 January 2003
Figure 4.2.1.2.2. Effect of temperature on the compressive yield strength (Fcy) and the shear ultimate strength (Fsu) of AZ31BH24 sheet and plate.
Figure 4.2.1.2.3. Effect of temperature on the bearing ultimate strength (Fbru) and the bearing yield strength (Fbry) of AZ31BH24 sheet and plate.
413
MMPDS01 31 January 2003
Figure 4.2.1.2.4. Effect of temperature on the tensile modulus (E) of AZ31BH24 sheet and plate.
50
40
Tension
Stress, ksi
30 Compression
20
Ramberg  Osgood n (tension) = 4.3 n (comp.) = 15
10
TYPICAL
0 0
2
4
6
8
10
12
Strain, 0.001 in./in. 3 Compressive Tangent Modulus, 10 ksi
Figure 4.2.1.2.6. Typical tensile and compressive stressstrain and compressive tangentmodulus curves for AZ31BH24 sheet at room temperature.
414
MMPDS01 31 January 2003
Figure 4.2.1.4.8(a). Bestfit S/N curves for unnotched AZ31BF magnesium alloy forged disk, transverse direction.
Correlative Information for Figure 4.2.1.4.8(a) Product Form: Forged disk, 1 inch thick
No. of Heats/Lots: 1
Properties:
Equivalent Stress Equation:
TUS, ksi 38
TYS, ksi 26
Temp.,EF RT
Specimen Details: Unnotched 0.75 inch gross diameter 0.30 inch net diameter Surface Condition: Polished sequentially with No. 320 aluminum oxide cloth, No. 0, 00, and 000 emery paper and finally No. 600 aluminum oxide powder in water References:
For R values between 1.0 and 0.50 Log Nf = 7.132.20 log (Seq12.9) Seq = Smax(1R)0.56 Std. Error of Estimate, Log (Life) = 0.613 Standard Deviation, Log (Life) = 0.916 R2 = 55.2% For R values between 0.0 and 0.50 Log Nf = 8.873.26 log (Seq15.0) Seq = Smax(1R)0.33 Std. Error of Estimate, Log (Life) = 0.829 Standard Deviation, Log (Life )= 1.014 R2 = 33.2%
4.2.1.1.8 Sample Size = 194
Test Parameters: Loading  Axial Frequency  1500 cpm Temperature  RT Environment  Air
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
415
MMPDS01 31 January 2003
Figure 4.2.1.4.8(b). Bestfit S/N curves for notched, Kt = 3.3, AZ31BF magnesium alloy forged disk, transverse direction.
Correlative Information for Figure 4.2.1.4.8(b) Product Form: Forged disk, 1 inch thick Properties:
TUS, ksi 38
TYS, ksi 26
Test Parameters: Loading  Axial Frequency  1500 cpm Temperature  RT Environment  Air
Temp.,EF RT
Specimen Details: Notched, Kt = 3.3 0.350 inch gross diameter 0.280 inch net diameter 0.010 inch root radius, r 60E flank angle, ω Reference:
No. of Heats/Lots: 1 Maximum Stress Equation: Log Nf = 8.284.34 log (Smax) Std. Error of Estimate, Log (Life) = 0.534 Standard Deviation, Log (Life) = 0.707 R2 = 43%
4.2.1.1.8
Sample Size = 34
416
MMPDS01 31 January 2003 4.2.2 AZ61A 4.2.2.0 Comments and Properties — AZ61A is a wrought magnesiumbase alloy containing aluminum and zinc. It is available in the form of extruded sections, tubes, and forgings in the asfabricated (F) temper. AZ61A is much like AZ31B in general characteristics. The increased aluminum content increases the strength and decreases the ductility slightly. Severe forming must be done at elevated temperatures. This alloy is readily welded but must be stress relieved after welding to prevent stress corrosion cracking. Material specifications covering AZ61A are given in Table 4.2.2.0(a). Roomtemperature mechanical and physical properties are shown in Table 4.2.2.0(b).
Table 4.2.2.0(a). Material Specifications for AZ61A Magnesium Alloy
Specification
Form
AMS 4350 ASTM B 91
Extrusion Forging
417
MMPDS01 31 January 2003
Table 4.2.2.0(b). Design Mechanical and Physical Properties of AZ61A Magnesium Alloy Extrusion and Forging
Specification . . . . . . . . Form . . . . . . . . . . . . . . .
AMS 4350 Extruded bar, rod, and solid shapes
Temper . . . . . . . . . . . . .
Extruded hollow shapes F
Extruded tube
Forging
S
0.0280.750b S
40 ...
36 ...
36 ...
38 ...
24 ...
22 ...
16 ...
16 ...
22 ...
14 ... 19
14 ... 19
14 ... ...
11 ... ...
11 ... ...
14 ... 19
45 55
45 55
... ...
... ...
... ...
50 60
28 32
28 32
... ...
... ...
... ...
28 32
8
9
7
7
7
6
S
0.2502.499 S
2.5004.499a S
38 ...
40 ...
21 ...
Thickness, in. . . . . . . . .
#0.249
Basis . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ............... LT . . . . . . . . . . . . . . Fty, ksi: L ............... LT . . . . . . . . . . . . . . Fcy, ksi: L ............... LT . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . Fbruc, ksi: (e/D = 1.5) . . . . . . . . (e/D = 2.0) . . . . . . . . Fbryc, ksi: (e/D = 1.5) . . . . . . . . (e/D = 2.0) . . . . . . . . e, percent: L ............... E, 103 ksi . . . . . . . . . . Ec, 103 ksi . . . . . . . . . G, 103 ksi . . . . . . . . . . µ ................ Physical Properties: ω, lb/in.3 . . . . . . . . . . C, Btu/(lb)(EF) . . . . . K, Btu/[(hr)(ft2)(EF)/ft] α, 106 in./in./EF . . . . . a b c d
ASTM B 91
All
6.3 6.3 2.4 0.31 0.0647 0.25 (at 78EF)d 46 (212 to 572EF) 14 (65 to 212EF)
For crosssectional area #25 square inches. Wall thickness for outside diameters #6.000 inches. Bearing values are “dry pin” values per Section 1.4.7.1. Estimated.
418
... S
MMPDS01 31 January 2003 4.2.3 ZK60A 4.2.3.0 Comments and Properties — ZK60A is a wrought magnesiumbase alloy containing zinc and zirconium. It is available as extruded sections, tubes, and forgings. Increased strength is obtained by artificial aging (T5) from the asfabricated (F) temper. ZK60A has the best combination of high roomtemperature strength and ductility of the wrought magnesiumbase alloys. It is used primarily at temperatures below 300EF. ZK60A has good ductility as compared with other highstrength magnesium alloys and can be formed or bent cold into shapes not possible with those alloys having less ductility. It is not considered a weldable alloy. Material specifications for ZK60A are given in Table 4.2.3.0(a). Roomtemperature mechanical and physical properties are shown in Tables 4.2.3.0(b) and (c). Elevated temperature curves for physical properties are shown in Figures 4.2.3.0. Table 4.2.3.0(a). Material Specifications for ZK60A Magnesium Alloy
Specification ASTM B 107 AMS 4352 AMS 4362
Form Extrusion Extrusion Die and hand forgings
The temper index for ZK60A is as follows: Temper F T5
Section 4.2.3.1 4.2.3.2 4.2.3.1 ZK60AF Temper
4.2.3.2 ZK60AT5 Temper — Typical roomtemperature tension and compression stressstrain curves for extrusions are shown in Figures 4.2.3.2.6(a) and (b). Fatigue curves are presented in Figure 4.2.3.2.8(a) through (c).
419
MMPDS01 31 January 2003
Table 4.2.3.0(b). Design Mechanical and Physical Properties of ZK60A Magnesium Alloy Extrusion
Specification . . . . . . . . . . .
ASTM B 107
Form . . . . . . . . . . . . . . . . . . Temper . . . . . . . . . . . . . . . . Crosssectional area, in.2 . . . . . . . . . . . . . . . . . . .
Extruded Extruded hollow shapes tube
Extruded rod, bar, and solid shapes
0.004 #2.499 2.5005.000 #2.499 2.5005.000 a S S S S Basis . . . . . . . . . . . . . . . . S Mechanical Properties: Ftu, ksi: L ................ ... 130 130 140 140 130 140b 140 LT . . . . . . . . . . . . . . . 140 130b ST . . . . . . . . . . . . . . . ... ... 130 ... 140 Fty, ksi: L ................ ... 85 85 95 95 85 95b 95 LT . . . . . . . . . . . . . . . 95 85b ST . . . . . . . . . . . . . . . ... ... 85 ... 95 Fcy, ksi: L ................ ... 85 85 95 95 LT . . . . . . . . . . . . . . . 95 ... ... ... ... 91 85 85 91 91 Fsu, ksi . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . 210 195 195 210 210 (e/D = 2.0) . . . . . . . . . 266 247 247 266 266 Fbry, ksi: (e/D = 1.5) . . . . . . . . . 142 127 127 142 142 (e/D = 2.0) . . . . . . . . . 171 153 153 171 171 e, percent: L ................ ... 15 15 12 12 15 12b 12 LT . . . . . . . . . . . . . . . 15 15b ST . . . . . . . . . . . . . . . ... ... 15 ... 12 RA, percent: L ................ ... 20 20 15 15 20 15b 15 LT . . . . . . . . . . . . . . . ... 20b ST . . . . . . . . . . . . . . . ... ... 20 ... 15 3 29.1 E, 10 ksi . . . . . . . . . . . 29.1 Ec, 103 ksi . . . . . . . . . . 3 11.1 G, 10 ksi . . . . . . . . . . . µ ................. 0.31 Physical Properties: 0.287 ω, lb/in.3 . . . . . . . . . . . C, K, and α . . . . . . . . . See Figure 6.2.1.0 a Test direction longitudinal for widths less than 9 inches; transverse for widths 9 inches and over. b Applicable to widths $2.500 inches only.
66
MMPDS01 31 January 2003
Figure 6.2.1.1.1. Effect of temperature on the tensile yield strength (Fty) and tensile ultimate strength (Ftu) of A286 alloy (1800EF solution treatment temperature).
67
MMPDS01 31 January 2003
Figure 6.2.1.1.3. Effect of temperature on the bearing ultimate strength (Fbru) and the bearing yield strength (Fbry) for A286 alloy (1800EF solution treatment temperature).
Figure 6.2.1.1.4(a). Effect of temperature on the tensile and compressive moduli (E and Ec) for A286 alloy (1800EF solution treatment temperature).
68
MMPDS01 31 January 2003
Figure 6.2.1.1.4(b). Effect of temperature on the shear modulus (G) of A286 alloy.
Figure 6.2.1.1.4(c). Effect of temperature on Poisson’s ratio (µ) for A286 alloy.
69
MMPDS01 31 January 2003
Figure 6.2.1.1.8(a). Bestfit S/N curves for unnotched A286 bar at 800EF, longitudinal direction.
Correlative Information for Figure 6.2.1.1.8(a) Product Form: Bar, air melted Properties:
TUS, ksi 141.4
TYS, ksi 95.3
Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  800EF Environment  Air
Temp.,EF 800
Specimen Details: Unnotched 0.250 inch diameter Heat Treatment:
No. of Heats/Lots: 1 Equivalent Stress Equation: Log Nf = 45.119.5 log (Seq) Seq = Smax (1R)0.47 Std. Error of Estimate, Log (Life) = 0.418 Standard Deviation, Log (Life) = 0.717 R2 = 65.9%
1650EF for 2 hours, oil quenched and 1300EF for 16 hours, air cooled.
Surface Condition: Not given Reference:
6.2.1.1.8 Sample Size = 17 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
610
MMPDS01 31 January 2003
Figure 6.2.1.1.8(b). Bestfit S/N curves for notched, Kt = 3.4, A286 alloy bar at 800EF, longitudinal direction.
Correlative Information for Figure 6.2.1.1.8(b) Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  800EF Environment  Air
Product Form: Bar, air melted Properties:
TUS, ksi 141.4
TYS, ksi Temp.,EF 95.3 800 Unnotched
Specimen Details: Notched, VGroove, Kt = 3.4 0.375 inch gross diameter 0.250 inch net diameter 0.010 inch root radius, r 60E flank angle, ω Heat Treatment:
No. of Heats/Lots: 1 Equivalent Stress Equation: Log Nf = 11.44.4 log (Seq20) Seq = Smax (1R)0.75 Std. Error of Estimate, Log (Life) = 0.271 Standard Deviation, Log (Life) = 0.387 R2 = 50.9%
1650EF for 2 hours, oil quenched and 1300EF for 16 hours, air cooled.
Sample Size = 13 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Surface Condition: As machined Reference:
6.2.1.1.8
611
MMPDS01 31 January 2003
Figure 6.2.1.1.8(c). Bestfit S/N curves for unnotched A286 bar at 1000EF, longitudinal direction.
Correlative Information for Figure 6.2.1.1.8(c) Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  1000EF Environment  Air
Product Form: Bar, air melted Properties:
TUS, ksi 137.2
TYS, ksi 100.6
Temp.,EF 1000
Specimen Details: Unnotched 0.250 inch diameter Heat Treatment:
No. of Heats/Lots: 1 Equivalent Stress Equation: Log Nf = 44.219.3 log (Seq) Seq = Smax (1R)0.57 Std. Error of Estimate, Log (Life) = 0.566 Standard Deviation, Log (Life) = 0.835 R2 = 54.0%
1650EF for 2 hours, oil quenched and 1300EF for 16 hours, air cooled.
Surface Condition: Not given Reference:
6.2.1.1.8 Sample Size = 18 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
612
MMPDS01 31 January 2003
Figure 6.2.1.1.8(d). Bestfit S/N curves for notched, Kt = 3.4, A286 alloy bar at 1000EF, longitudinal direction.
Correlative Information for Figure 6.2.1.1.8(d) Product Form: Bar, air melted Properties:
TUS, ksi 137.2
TYS, ksi 100.6
Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  1000EF Environment  Air
Temp.,EF 1000 Unnotched
No. of Heats/Lots: 1
Specimen Details: Notched, VGroove, Kt = 3.4 0.375 inch gross diameter 0.250 inch net diameter 0.010 inch root radius, r 60E flank angle, ω Heat Treatment:
Equivalent Stress Equation: Log Nf = 7.862.19 log (Seq35.8) Seq = Smax (1R)0.61 Std. Error of Estimate, Log (Life) = 0.365 Standard Deviation, Log (Life) = 0.510 R2 = 48.7%
1650EF for 2 hours, oil quenched and 1300EF for 16 hours, air cooled.
Sample Size = 17 Surface Condition: As machined Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
6.2.1.1.8
613
MMPDS01 31 January 2003
Figure 6.2.1.1.8(e). Bestfit S/N curves for unnotched A286 bar at 1250EF, longitudinal direction.
Correlative Information for Figure 6.2.1.1.8(e) Product Form: Bar, air melted Properties:
TUS, ksi 109.6
TYS, ksi 96.5
Test Parameters: Loading  Axial Frequency  3600 cpm Temperature  1250EF Environment  Air
Temp.,EF 1250
Specimen Details: Unnotched 0.250 inch diameter Heat Treatment:
No. of Heats/Lots: 1 Equivalent Stress Equation: Log Nf = 30.812.8 log (Seq) Seq = Smax (1R)0.77 Std. Error of Estimate, Log (Life) = 0.513 Standard Deviation, Log (Life) = 0.788 R2 = 57.6%
1650EF for 2 hours, oil quenched and 1300EF for 16 hours, air cooled.
Surface Condition: Not given Reference:
6.2.1.1.8 Sample Size = 13 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
614
MMPDS01 31 January 2003 6.2.2 N155 6.2.2.0 Comments and Properties — N155 alloy, also known as Multimet, is designed for applications involving high stress up to 1500EF. It has good oxidation properties and good ductility and can be fabricated readily by conventional methods. This alloy has been used in many aircraft applications, including afterburner parts, combustion chambers, exhaust assemblies, turbine parts, and bolting. N155 is forged readily between 1650EF and 2200EF. It is easily formed by conventional methods; intermediate anneals may be required to restore its ductility. This alloy is machinable in all conditions; low cutting speeds and ample flow of coolant are required. The weldability of N155 is comparable to that of the austenitic stainless steels. The oxidation resistance of N155 sheet is good up to 1500EF. Some materials specifications for N155 are presented in Table 6.2.2.0(a). Roomtemperature mechanical and physical properties for N155 sheet and tubing in the solutiontreated (annealed) condition are presented in Table 6.2.2.0(b). Bars and forgings are not specified by roomtemperature properties but have specific elevatedtemperature requirements. The effect of temperature on physical properties is shown in Figure 6.2.2.0. Table 6.2.2.0(a). Material Specifications for N155 Alloy
Specification AMS 5532 AMS 5585 AMS 5768 AMS 5769
Form Sheet Tubing (welded) Bar and forging Bar and forging
Condition Solution treated Solution treated Solution treated and aged Solution treated
6.2.2.1 SolutionTreated Condition — Elevatedtemperature curves are presented in Figures 6.2.2.1.1(a) and (b), as well as 6.2.2.1.4(a) and (b). Stressrupture properties are specified at 1500EF for sheet and at 1350EF for bars and forgings; the appropriate specifications should be consulted for detailed requirements.
Figure 6.2.2.0. Effect of temperature on the physical properties of N155 alloy.
615
MMPDS01 31 January 2003 Table 6.2.2.0(b). Design Mechanical and Physical Properties of N155 Alloy
Specification . . . . . . . . . . Form . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . . Thickness, in. . . . . . . . . . . Basis . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ................. LT . . . . . . . . . . . . . . . . Fty, ksi: L ................. LT . . . . . . . . . . . . . . . . Fcy, ksi: L ................. LT . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . e, percent: L ................. LT . . . . . . . . . . . . . . . . E, 103 ksi . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . µ .................. Physical Properties: ω, lb/in.3 . . . . . . . . . . . . C, Btu/(lb)(EF) . . . . . . . K, Btu/[(hr)(ft2)(EF)/ft] α, 106 in./in./EF . . . . . . .
Sheet #0.187 Sa
AMS 5532 Strip and plate Solution treated ... Sa
AMS 5585 Tubing ... S
... 100
... 100
100 ...
... 49b
... ...
49b ...
... ... ...
... ... ...
... ... ...
... ...
... ...
... ...
... ...
... ...
... ...
... 40
... 40 29.2 29.2 11.2 See Figure 6.2.2.1.4(b) 0.300 0.103 (70 to 212EF) See Figure 6.2.2.0 See Figure 6.2.2.0
a Test direction longitudinal for widths less than 9 inches: transverse for widths 9 inches and over. b Typical value reduced to minimum. c Strip = 35. Full section 0.625 thick = 40. Full section >0.625 thick = 30.
616
c
...
MMPDS01 31 January 2003
Figure 6.2.2.1.1(a). Effect of temperature on the tensile ultimate strength (Ftu) of N155 alloy.
Figure 6.2.2.1.1(b). Effect of temperature on the tensile yield strength (Fty) of N155 alloy.
617
MMPDS01 31 January 2003
Figure 6.2.2.1.4(a). Effect of temperature on the tensile and compressive moduli (E and Ec) of N155 alloy.
Figure 6.2.2.1.4(b). Effect of temperature on Poisson’s ratio (µ) for N155 alloy.
618
MMPDS01 31 January 2003
6.3
NICKELBASE ALLOYS
6.3.0 GENERAL COMMENTS — Nickel is the base element for most of the higher temperature heatresistant alloys. While it is more expensive than iron, nickel provides an austenitic structure that has greater toughness and workability than ferritic structures of the same strength level. 6.3.0.1 Metallurgical Considerations Composition — The common alloying elements for nickel are cobalt, iron, chromium, molybdenum, titanium, and aluminum. Cobalt, when substituted for a portion of the nickel in the matrix, improves hightemperature strength; small additions of iron tend to strengthen the nickel matrix and reduce the cost; chromium is added to increase strength and oxidation resistance at very high temperatures; molybdenum contributes to solid solution strengthening. Titanium and aluminum are added to most nickelbase heat resistant alloys to permit agehardening by the formation of Ni3 (Ti, Al) precipitates; aluminum also contributes to oxidation resistance. The nature of the alloying elements in the agehardenable nickelbase alloys makes vacuum melting of these alloys advisable, if not mandatory. However, the additional cost of vacuum melting is more than compensated for by the resulting improvements in elevatedtemperature properties. Heat Treatment — The nickelbase alloys are heat treated with conventional equipment and fixtures such as would be used with austenitic stainless steels. Since nickelbase alloys are more susceptible to sulfur embrittlement than are ironbase alloys, it is essential that sulfurbearing materials such as grease, oil, cutting lubricants, marking paints, etc., be removed before heat treatment. Mechanical cleaning, such as wire brushing, is not adequate and if used should be followed by washing with a suitable solvent or by vapor degreasing. A lowsulfur content furnace atmosphere should be used. Good furnace control with respect to time and temperature is desirable since overheating some of the alloys as little as 35EF impairs strength and corrosion resistance. When it is necessary to anneal the agehardenabletype alloys, a protective atmosphere (such as argon) lessens the possibility of surface contaminations or depletion of the precipitationhardening elements. This precaution is not so critical in heavier sections since the oxidized surface layer is a smaller percentage of the cross section. After solution annealing, the alloys are generally quenched in water. Heavy sections may require air cooling to avoid cracking from thermal stresses. In stressrelief annealing of a structure or assembly composed of an aluminumtitanium hardened alloy, it is vitally important to heat the structure rapidly through the agehardening temperature range, 1200EF to 1400EF (which is also the low ductility range) so that stress relief can be achieved before any aging takes place. Parts which are to be used in the fully heattreated condition would have to be solution treated, air cooled, and subsequently aged. In this case, the stressrelief treatment would be conducted in the solutiontemperature range. Little difficulty has been encountered with distortion under rapid heating conditions, and distortion of weldments of substantial size has been less than that observed with conventional slow heating methods. 6.3.0.2 Manufacturing Considerations Forging — All of the alloys considered, except for the casting compositions, can be forged to some degree. The matrixstrengthened alloys can be forged with proper consideration of cooling rates, atmosphere, etc. Most of the precipitationhardenable grades can be forged, although heavier equipment is required and a smaller range of reductions can be safely attained.
619
MMPDS01 31 January 2003 Cold Forming — Almost all of the wroughtnickelbase alloys in sheet form are cold formable. The lower strength alloys offer few problems, but the higher strength alloys require higher forming pressures and more frequent anneals. Machining — All of the alloys in this section are readily machinable, provided the optimum conditions of heat treatment, type of tool speed, feed, depth of cut, etc., are achieved. Specific recommendations on these points are available from various producers of these alloys. Welding — The matrixstrengtheningtype alloys offer no serious problems in welding. All of the common resistance and fusionwelding processes (except submerged arc) have been successfully employed. For the agehardenable type of alloy, it is necessary to observe some further precautions: (1) Welding should be confined to annealed material where design permits. In full agehardened material, the hazard of cracking in the weld and/or the parent metal is great. (2) If design permits joining some portions only after age hardening, the parts to be joined should be “safe ended” with a matrixstrengthenedtype alloy (with increased cross section) and then age hardened; welding should then be carried out on the “safe ends.” (3) Parts severely worked or deformed should be annealed before welding. (4) After welding, the weldment will often require stress relieving before aging. (5) Material must be heated rapidly to the stressrelieving temperature. (6) In a number of the agehardenable alloys, fusion welds may exhibit only 70 to 80 percent of the rupture strength of the parent metal. The deficiency can often be minimized by design, such as locating welds in areas of lowest temperature and/or stress. The use of special filler wires to improve weldrupture properties is under investigation. Brazing — The solidsolutiontype chromiumcontaining alloys respond well to brazing, using techniques and brazing alloys applicable to the austenitic stainless steels. Generally, it is necessary to braze annealed material and to keep stresses low during brazing, especially when brazing with low melting alloys, to avoid embrittlement. As with the stainless steels, dry hydrogen, argon, or helium atmospheres (80EF dew point or lower) are used successfully, and vacuum brazing is now receiving increasing attention. The aluminumtitanium agehardened nickelbase alloys are difficult to braze, even using extremely dry reducing and inertgas atmospheres, unless some method of fluxing, solid or gaseous, is used. An alternative technique which is commonly used is to preplate the areas to be brazed with ½ to 1 mil of nickel. For some metal combinations, a few fabricators prefer to apply an iron preplate. In either case, the plating prevents the formation of aluminum or titanium oxide films and results in better joints. Most of the hightemperature alloys of the nickelbase type are brazed with NiCrSiB and NiCrSi types of brazing alloy. Silver brazing alloys can be used for lower temperature applications. However, since the nickelbase alloys to be brazed are usually employed for higher temperature applications, the higher melting point, stronger, and more oxidationresistant brazing alloys of the Nicrobraz type are generally used. Some of the goldbase and palladiumbase brazing alloys may be useful under some circumstances in intermediatetemperature applications.
620
MMPDS01 31 January 2003 6.3.1 HASTELLOY X 6.3.1.0 Comments and Properties — Hastelloy X is a nickelbase alloy used for combustorliner parts, turbineexhaust weldments, afterburner parts, and other parts requiring oxidation resistance and moderately high strength above 1450EF. It is not hardenable except by cold working and is used in the solutiontreated (annealed) condition. Hastelloy X is available in all the usual mill forms. Hastelloy X is somewhat difficult to forge; forging should be started at 2150EF to 2200EF and continued as long as the material flows freely. It should be in the annealed condition for optimum cold forming, and severely formed detail parts should be solution treated at 2150EF for 7 to 10 minutes and cooled rapidly after forming. Machinability of Hastelloy X is similar to that of austenitic stainless steel; the alloy is tough and requires low cutting speeds and ample cutting fluids. Hastelloy X can be resistance or fusion welded or brazed; large or complex fusion weldments require stress relief at 1600EF for 1 hour. Hastelloy X has good oxidation resistance up to 2100EF. It age hardens somewhat during long exposure between 1200EF and 1800EF. Some material specifications for Hastelloy X are presented in Table 6.3.1.0(a). Roomtemperature mechanical and physical properties for Hastelloy X sheet are presented in Table 6.3.1.0(b). AMS 5754 does not specify tensile properties for bars and forgings. Figure 6.3.1.0 shows the effect of temperature on physical properties.
Table 6.3.1.0(a). Material Specifications for Hastelloy X
Specification AMS 5536 AMS 5754
Form Sheet and plate Bar and forging
Condition Solution heat treated (annealed) Solution heat treated (annealed)
6.3.1.1 Annealed Condition — The effect of temperature on various mechanical properties is presented in Figures 6.3.1.1.1 and 6.3.1.1.4. In addition, certain stressrupture requirements at 1500EF are specified in AMS 5536 and 5754 for Hastelloy X. Typical tensile stressstrain curves at room and elevated temperatures are presented in Figure 6.3.1.1.6(a). Typical compressive stressstrain and tangentmodulus curves at room and elevated temperatures are presented in Figure 6.3.1.1.6(b).
621
MMPDS01 31 January 2003
Table 6.3.1.0(b). Design Mechanical and Physical Properties of Hastelloy X Sheet and Plate
Specification . . . . . . . . . . Form . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . .
S
0.0100.019 S
... 105
... 105
... 102
... 106
... 105
... 100
... 95
... 45
... 45
... 44
... 47
... 45
... 40
... 40
... ... ...
... ... ...
... ... ...
... ... ...
... ... ...
... ... ...
... ... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... 29
... 35
... 35
... 35
... 35
Thickness, in. . . . . . . . . . . 2.000 S
MMPDS01 31 January 2003
Figure 6.3.1.0. Effect of temperature on the physical properties of Hastelloy X.
623
MMPDS01 31 January 2003
Figure 6.3.1.1.1. Effect of temperature on the tensile ultimate strength (Ftu) and the tensile yield strength (Fty) of Hastelloy X sheet.
Figure 6.3.1.1.4. Effect of temperature on dynamic modulus (E) of Hastelloy X sheet.
624
MMPDS01 31 January 2003
60 .5 hr exposure RT 400 F
50
800 F 1000 F 1200 F 1400 F
Stress, ksi
40
30 1600 F Ramberg  Osgood n (RT) = 10 n (400 F) = 13 n (800 F) = 15 n (1000 F) = 18 n (1200 F) = 19 n (1400 F) = 15 n (1600 F) = 12 n (1800 F) = 7.7 n (2000 F) = 3.8
20 1800 F
10
2000 F
TYPICAL 0 0
2
4
6
8
10
Strain, 0.001 in./in.
Figure 6.3.1.1.6(a). Typical tensile stressstrain curves for Hastelloy X sheet at room and elevated temperatures.
625
12
MMPDS01 31 January 2003
60 RT
RT
.5 hr exposure
700 F 50
700 F 900 F
40
Stress, ksi
900 F
30
20 Ramberg  Osgood n (RT) = 6.9 n (700 F) = 6.7 n (900 F) = 5.6
10
TYPICAL 0 0
2
4
0
5
10
6 Strain, 0.001 in./in. 15
8
20
10
12
25
30
3
Compressive Tangent Modulus, 10 ksi
Figure 6.3.1.1.6(b). Typical compressive stressstrain and compressive tangentmodulus curves for Hastelloy X bar at room and elevated temperatures.
626
MMPDS01 31 January 2003 6.3.2 INCONEL 600 6.3.2.0 Comments and Properties — Inconel 600 is a corrosion and heatresistant nickelbase alloy used for lowstressed parts operating up to 2000EF. It is not hardenable except by cold working and is usually used in the annealed condition. Inconel 600 is available in all the usual mill forms. Inconel 600 is readily forged between 1900EF and 2250EF; “hotcold” working between 1200EF and 1600EF is harmful and should be avoided; cold working below 1200EF results in improved properties. This alloy is readily formed but should be annealed after severe forming operations. The maximum annealing temperature is 1800EF if minimum yieldstrength requirements are to be met consistently. Inconel 600 is susceptible to rapid grain growth at 1800EF or higher, and exposures at these temperatures should be brief if large grain size is objectionable. Inconel 600 is somewhat difficult to machine because of its toughness and capacity for work hardening; highspeed steel or cementedcarbide tools should be used, and tools should be kept sharp. This alloy can be resistance or fusion welded or brazed (using nonsilver containing brazing alloy); large or complex fusion weldments should be stress relieved at 1600EF for 1 hour. Oxidation resistance of Inconel 600 is excellent up to 2000EF in sulfurfree atmospheres. This alloy is subject to attack in sulfurcontaining atmospheres.
Table 6.3.2.0(a). Material Specifications for Inconel 600
Specification AMS 5540 ASTM B166 AMS 5580 ASTM B564
Form Plate, sheet, and strip Bar and rod Tubing, seamless Forging
Condition Annealed Various Annealed Annealed
Some material specifications for Inconel 600 are presented in Table 6.3.2.0(a). Roomtemperature mechanical and physical properties are shown in Tables 6.3.2.0(b), (c), and (d). Figure 6.3.2.0 shows the effect of temperature on the physical properties. 6.3.2.1 Annealed Condition — Elevatedtemperature data for this condition are shown in Figures 6.3.2.1.1 through 6.3.2.1.4.
627
MMPDS01 31 January 2003
Table 6.3.2.0(b). Design Mechanical and Physical Properties of Inconel 600
Specification . . . . . . . . . . Form . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . . Thickness, in. . . . . . . . . . .
AMS 5540 Sheet, strip, and plate Annealed 0.0202.000
Outside Diameter, in. . . . .
...
Basis . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ................. LT . . . . . . . . . . . . . . . . Fty, ksi: L ................. LT . . . . . . . . . . . . . . . . Fcy, ksi: L ................. LT . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . e, percent: L ................. LT . . . . . . . . . . . . . . . . E, 103 ksi . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . µ .................. Physical Properties: ω, lb/in.3 . . . . . . . . . . . . C, K, and α . . . . . . . . . .
S
AMS 5580 Tubing Cold drawn ... 5.001#5.000 6.625 S S
ASTM B564 Forging Annealed ... ... S
... 80
80 ...
80 ...
80 ...
... 35
35 ...
30 ...
35 ...
... 35 51
35 ... 51
30 ... 51
35 ... 51
... 152
... 152
... 152
... 152
... ...
... ...
... ...
... ...
... 30
30 ...
35 ...
30 ...
30.0 30.0 11.0 0.29 0.304 See Figure 6.3.2.0
628
MMPDS01 31 January 2003
Table 6.3.2.0(c). Design Mechanical and Physical Properties of Inconel 600 Bar and Rod
Specification . . . . . . . Form . . . . . . . . . . . . . . Condition . . . . . . . . . . Thickness, in. . . . . . . . Basis . . . . . . . . . . . . . . Mechanical Propertiesa: Ftu, ksi: L .............. LT . . . . . . . . . . . . . Fty, ksi: L .............. LT . . . . . . . . . . . . . Fcy, ksi: L .............. LT . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . Fbry, ksi: (e/D = 1.5) . . . . . . . (e/D = 2.0) . . . . . . . e, percent: L .............. E, 103 ksi . . . . . . . . . Ec, 103 ksi . . . . . . . . G, 103 ksi . . . . . . . . . µ ............... Physical Properties: ω, lb/in.3 . . . . . . . . . C, K, and α . . . . . . .
ASTM B166 Round #0.499 S
0.5001.000 S
120 ...
110 ...
90 ...
Square, hexagon, and rectangle Coldworked 1.0012.500 S
#0.250 S
0.2510.499 S
105 ...
100 ...
95 ...
85 ...
80 ...
80 ...
70 ...
... ... ...
... ... ...
... ... ...
... ... ...
... ... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
... ...
7b
10
12 30.0 30.0 11.0 0.29
5b
7
0.304 See Figure 6.3.2.0
a Mechanical property requirements apply only when specified by purchaser. b Not applicable to thickness 3.000 S S S
Bar and rod
All S
Annealed All S
95 ...
90 ...
85 ...
85 ...
80 ...
45 ...
40 ...
35 ...
35 ...
35 ...
... ... ...
... ... ...
... ... ...
... ... ...
35 ... 51
... ...
... ...
... ...
... ...
... 152
... ...
... ...
... ...
... ...
... ...
20
25
30
...
30b
30.0 30.0 11.0 0.29 0.304 See Figure 6.3.2.0
a Mechanical property requirements apply only when specified by purchaser. b Not applicable to thickness >0.094 inch.
630
MMPDS01 31 January 2003
Figure 6.3.2.0. Effect of temperature on the physical properties of Inconel 600.
631
MMPDS01 31 January 2003
Figure 6.3.2.1.1. Effect of temperature on the tensile ultimate strength (Ftu) and the tensile yield strength (Fty) of Inconel 600.
Figure 6.3.2.1.2. Effect of temperature on the compressive yield strength (Fcy) and the shear ultimate strength (Fsu) of Inconel 600.
632
MMPDS01 31 January 2003
Figure 6.3.2.1.3. Effect of temperature on the bearing ultimate strength (Fbru) of Inconel 600.
Figure 6.3.2.1.4. Effect of temperature on the tensile and compressive moduli (E and Ec) of Inconel 600.
633
MMPDS01 31 January 2003 6.3.3 INCONEL 625 6.3.3.0 Comments and Properties — Inconel 625 is a solidsolution, matrix strengthened nickelbase alloy primarily for applications requiring good corrosion and oxidation resistance at temperatures up to approximately 1800EF and also where such parts may require welding. The strength of the alloy is derived from the strengthening effect of molybdenum and columbium; thus, precipitation hardening is not required and the alloy is used in the annealed condition. The strength is greatly affected by the amount of cold work prior to annealing and by the annealing temperature. The material is usually annealed at 1700 to 1900EF for time commensurate with thickness. The properties in this section are restricted to that annealing range. Because the alloy was developed to retain high strength at elevated temperatures, it resists deformation at hot working temperatures but can be readily fabricated with adequate equipment. The combination of strength, corrosion resistance, and ability to be fabricated, including welding by common industrial practices, are the alloy’s outstanding features. Some material specifications for Inconel 625 are listed in Table 6.3.3.0(a). Roomtemperature mechanical and physical properties for Inconel 625 are listed in Tables 6.3.3.0(b) and (c). Figure 6.3.3.0 shows the effect of temperature on the physical properties. Table 6.3.3.0(a). Material Specifications for Inconel 625
Specification AMS 5599 AMS 5666
Form Sheet, strip, and plate Bar, forging, and ring
Condition Annealed Annealed
6.3.3.1 Annealed Condition — Elevatedtemperature curves for tensile ultimate strength, tensile yield strength, tensile and compressive moduli, and Poisson’s ratio are presented in Figures 6.3.3.1.1(a) and (b), as well as 6.3.3.1.4(a) and (b). Typical stressstrain and tangentmodulus curves are shown in Figures 6.3.3.1.6(a) through (d). Fatigue S/N curves are presented in Figures 6.3.3.1.8(a) through (d).
Figure 6.3.3.0. Effect of temperature on the physical properties of Inconel 625.
634
MMPDS01 31 January 2003
Table 6.3.3.0(b). Design Mechanical and Physical Properties of Inconel 625 Sheet and Plate
Specification . . . . . . . . . . . . Form . . . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . . . .
AMS 5599 Sheet and plate Annealed 0.1410.187 A B
0.1880.250 S
0.2511.000 S
123 124
119 120
... 120
53 54
59 60
59 60
... 60
63 64 83
55 56 79
62 63 82
62 63 79
... ... ...
202 263
212 276
201 261
209 272
202 263
... ...
84 105
94 117
83 103
92 115
92 115
... ...
30
...
30
30
Thickness, in. . . . . . . . . . . . .
#0.062
Basis . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ................... LT . . . . . . . . . . . . . . . . . . Fty, ksi: L ................... LT . . . . . . . . . . . . . . . . . . Fcy, ksi: L ................... LT . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . Fbru, ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . e, percent (Sbasis): LT . . . . . . . . . . . . . . . . . . E, 103 ksi . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . µ .................... Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . C, K, and α . . . . . . . . . . . .
A
B
A
B
A
B
119 120a
127 128
119 120a
126 127
119 120a
125 126
118 119
56 57
62 63
55 56
61 62
54 55
60 61
59 59 79
65 66 84
58 58 79
64 65 84
57 57 79
202 263
216 281
202 263
214 279
88 109
97 121
86 107
95 119
30
...
30
...
0.0630.109 0.1100.140
30 ... 29.8 29.8 11.8 0.28
0.305 See Figure 6.3.3.0
a Sbasis. The rounded T99 values are higher than specification values as follows: Ftu(#0.062) = 123 ksi, Ftu (0.0630.109) = 122 ksi, and Ftu (0.1100.140) = 121 ksi. b Bearing values are “dry pin” values per Section 1.4.7.1.
635
MMPDS01 31 January 2003
Table 6.3.3.0(c). Design Mechanical and Physical Properties of Inconel 625 Bar
Specification . . . . . . . . . . . . . Form . . . . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . . . . . Thickness or diameter, in. . . . Basis . . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L .................... ST . . . . . . . . . . . . . . . . . . . Fty, ksi: L .................... ST . . . . . . . . . . . . . . . . . . . Fcy, ksi: L .................... ST . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . Fbrua, ksi: (e/D = 1.5) . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . Fbrya, ksi: (e/D = 1.5) . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . e, percent (Sbasis): L .................... E, 103 ksi . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . µ ..................... Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . C, K, and α . . . . . . . . . . . . .
0.5000.999 S
AMS 5666 Bar Annealed 1.0001.999 2.0002.999 S S
3.0003.999 S
120 ...
120 ...
120 118
120 118
60 ...
60 ...
60 57
60 57
60 ... 79
59 ... 79
56 60 79
53 60 79
192 234
192 234
192 234
192 234
88 102
88 102
88 102
88 102
30
30
30
30
29.8 29.8 11.8 0.28 0.305 See Figure 6.3.3.0
a Bearing values are “dry pin” values per Section 1.4.7.1.
636
MMPDS01 31 January 2003
Figure 6.3.3.1.1(a). Effect of temperature on the tensile ultimate strength (Ftu) of annealed Inconel 625 sheet and bar.
Figure 6.3.3.1.1(b). Effect of temperature on the tensile yield strength (Fty) of annealed Inconel 625 sheet and bar.
637
MMPDS01 31 January 2003
Figure 6.3.3.1.4(a). Effect of temperature on the tensile and compressive moduli (E and Ec) of annealed Inconel 625.
Figure 6.3.3.1.4(b). Effect of temperature on Poisson’s ratio (µ) for annealed Inconel 625 bar.
638
MMPDS01 31 January 2003 100 Longitudinal and Long Transverse .5 hr exposure
80
RT
Stress, ksi
60 800 F 1200 F 40 Ramberg  Osgood n (RT) = 23 n (800 F) = 24 n (1200 F) = 30 n (1600 F) = 12
1600 F
20
TYPICAL Thickness = 0.050  0.250 in. 0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 6.3.3.1.6(a). Typical tensile stressstrain curves for annealed Inconel 625 sheet at room and elevated temperatures.
100 Longitudinal and Long Transverse 80
Stress, ksi
60
40 Ramberg  Osgood n = 32 TYPICAL
20
Thickness = 0.050  0.250 in.
0 0
2
0
5
4
6 Strain, 0.001 in./in.
8
10 15 20 3 Compressive Tangent Modulus, 10 ksi
10
12
25
30
Figure 6.3.3.1.6(b). Typical compressive stressstrain and compressive tangentmodulus curves for annealed Inconel 625 sheet at room temperature.
639
MMPDS01 31 January 2003 100
80 Longitudinal
Short Transverse
Stress, ksi
60
40
Ramberg  Osgood n (L  tension) = 27 n (ST  tension) = 25 TYPICAL
20 Thickness = 0.500  4.000 in.
0 0
2
4
6
8
10
12
Strain, 0.001 in./in.
Figure 6.3.3.1.6(c). Typical tensile stressstrain curves for annealed Inconel 625 bar at room temperature.
100
80 Short Transverse
Stress, ksi
60 Longitudinal
40 Ramberg  Osgood n (L  comp.) = 26 n (ST  comp.) = 27
20
TYPICAL Thickness = 0.500  1.500 in. 0 0
2
0
5
4
6 Strain, 0.001 in./in.
8
10 15 20 3 Compressive Tangent Modulus, 10 ksi
10
25
12
30
Figure 6.3.3.1.6(d). Typical compressive stressstrain and compressive tangentmodulus curves for annealed Inconel 625 bar at room temperature.
640
MMPDS01 31 January 2003
Figure 6.3.3.1.8(a). Bestfit S/N curves for annealed unnotched Inconel 625 bar, longitudinal direction.
Correlative Information for Figure 6.3.3.1.8(a) Product Form: Bar, 0.75 inch diameter
No. of Heats/Lots: 1
Properties:
Surface Condition: Longitudinally polished
Equivalent Stress Equation: Log Nf = 24.499.62 log (Seq) Seq = Smax (1R)0.42 Std. Error of Estimate, Log (Life) = 22.71 (1/Seq) Standard Deviation, Log (Life) = 0.985 R2 = 90%
Reference:
Sample Size = 27
TUS, ksi 133.2
TYS, ksi 73.8
Temp.,EF RT
Specimen Details: Unnotched 0.250 inch diameter
6.3.3.1.8(a)
Test Parameters: Loading  Axial Frequency  Unspecified Temperature  RT Environment  Air
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
641
MMPDS01 31 January 2003
Figure 6.3.3.1.8(b). Bestfit S/N curves for annealed notched Inconel 625 bar, Kt = 3.0, longitudinal direction. Correlative Information for Figure 6.3.3.1.8(b)
Product Form: Bar, 0.75 inch diameter
No. of Heats/Lots: 1
Properties:
Equivalent Stress Equation: Log Nf = 19.087.70 Log (Seq) Seq = Smax (1R)0.45 Std. Error of Estimate, Log (Life) = 14.31 (1/Seq) Standard Deviation, Log (Life) = 0.959 R2 = 92%
TUS, ksi 133.2
TYS, ksi Temp.,EF 73.8 RT
Specimen Details: VGroove, Kt = 3.0 0.375 inch gross diameter 0.250 inch net diameter 0.013 inch root radius 60E flank angle
Sample Size = 26 Surface Condition: Polished Reference:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
6.3.3.1.8(a)
Test Parameters: Loading  Axial Frequency  Unspecified Temperature  RT Atmosphere  Air
642
MMPDS01 31 January 2003
Figure 6.3.3.1.8(c). Bestfit S/N curves for annealed unnotched Inconel 625 sheet, longtransverse direction.
Correlative Information for Figure 6.3.3.1.8(c) Product Form: Sheet, 0.093 and 0.125 inch thick
No. of Heats/Lots: 2
Properties:
Specimen Details: Unnotched 0.500 inch wide 0.250 inch wide
Equivalent Stress Equation: Log Nf = 26.9110.77 log (Seq) Seq = Smax (1R)0.43 Std. Error of Estimate, Log (Life) = 37.39 (1/Seq) Standard Deviation, Log (Life) = 0.933 R2 = 75%
Surface Condition: As ground
Sample Size = 34
References:
[Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
TUS, ksi 135.4 136.7
TYS, ksi 74.6 69.8
Temp.,EF RT
6.3.3.1.8(a) and (b)
Test Parameters: Loading  Axial Frequency  Unspecified Temperature  RT Environment  Air
643
MMPDS01 31 January 2003
Figure 6.3.3.1.8(d). Bestfit S/N curves for annealed notched Inconel 625 sheet, Kt = 3.0, long transverse direction.
Correlative Information for Figure 6.3.3.1.8(d) Product Form: Sheet, 0.093 and 0.125 inch thick
No. of Heats/Lots: 2
Properties:
Equivalent Stress Equation: Log Nf = 10.353.56 Log (Seq22.89) Seq = Smax (1R)0.64 Std. Error of Estimate, Log (Life) = 10.52 (1/Seq) Standard Deviation, Log (Life) = 0.816 R2 = 96%
TUS, ksi 135.4 136.7
TYS, ksi 74.6 69.8
Temp.,EF RT
Specimen Details: Edge notched, Kt = 3.0 0.625 inch gross width 0.030 inch root radius 0.375 inch net width 60E flank angle
Sample Size = 37 [Caution: The equivalent stress model may provide unrealistic life predictions for stress ratios beyond those represented above.]
Surface Condition: As ground References:
6.3.3.1.8(a) and (b)
Test Parameters: Loading  Axial Frequency  Unspecified Temperature  RT Atmosphere  Air
644
MMPDS01 31 January 2003 6.3.4 INCONEL 706 6.3.4.0 Comments and Properties — Inconel 706 is a vacuummelted precipitationhardened, nickelbase alloy with characteristics similar to Inconel 718 except that Inconel 706 has greatly improved machinability. The alloy has good formability and weldability. Like Inconel 718, Inconel 706 has excellent resistance to postweld strainage cracking. Depending upon choice of heat treatment, this alloy may be used for applications requiring either (1) high resistance to creep and stress rupture up to 1300EF or (2) hightensile strength at cryogenic temperatures or elevated temperatures for short times. The creepresistant heat treatment is characterized by an intermediate stabilizing treatment before precipitation hardening. Inconel 706 also has good resistance to oxidation and corrosion over a broad range of temperatures and environments. Because of close relationship between heat treatment properties and application, the form and applications are listed with specifications in Table 6.3.4.0(a). Roomtemperature mechanical and physical properties are in Table 6.3.4.0(b). The effect of temperature on physical properties is shown in Figure 6.3.4.0. Table 6.3.4.0(a). Material Specifications for Inconel 706
Specification AMS 5605 AMS 5606 AMS 5701 AMS 5702 AMS 5703
Form Sheet, strip, and plate Sheet, strip, and plate Bar, forging, and ring Bar, forging, and ring Bar, forging, and ring
Tensile Creeprupture Tensile Creeprupture Creeprupture
Application 1800EF solution treated 1750EF solution treated 1800EF solution treated 1750EF solution treated 1750EF solution treated, stabilized and precipitation treated
6.3.4.1 SolutionTreated and Aged Condition (Creep Rupture Heat Treatment) — Effect of temperature on mechanical properties is shown in Figures 6.3.4.1.1, 6.3.4.1.4, and 6.3.4.1.5. Typical tensile stressstrain curves are shown in Figure 6.3.4.1.6(a) and typical compressive stressstrain and tangentmodulus curves in Figure 6.3.4.1.6(b). A fullrange tensile stressstrain curve is shown in Figure 6.3.4.1.6(c). Stressrupture properties are specified at 1200EF; the appropriate specification should be consulted for detailed requirements.
645
MMPDS01 31 January 2003
Table 6.3.4.0(b). Design Mechanical and Physical Properties of Inconel 706
Specification . . . . . . . . . . . . . . Form . . . . . . . . . . . . . . . . . . . . . Condition . . . . . . . . . . . . . . . . . Thickness or diameter, in. . . . . Basis . . . . . . . . . . . . . . . . . . . . . Mechanical Properties: Ftu, ksi: L ..................... LT . . . . . . . . . . . . . . . . . . . . Fty, ksi: L ..................... LT . . . . . . . . . . . . . . . . . . . . Fcy, ksi: L ..................... LT . . . . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . . . . Fbrua, ksi: (e/D = 1.5) . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . Fbrya, ksi: (e/D = 1.5) . . . . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . . . . e, percent: L ..................... LT . . . . . . . . . . . . . . . . . . . . RA, percent: L ..................... E, 103 ksi . . . . . . . . . . . . . . . . Ec, 103 ksi . . . . . . . . . . . . . . . G, 103 ksi . . . . . . . . . . . . . . . . µ ...................... Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . . . . C, K, and α . . . . . . . . . . . . . .
AMS AMS 5702 and AMS 5701 5606 AMS 5703 Sheet, strip, and plate Bar and forging Heat treated per indicated specification 0.1882.5002.500#0.187 All 0.015
S
S
S
S
S
180 192 180b 191
180 180
... 180
... 180
185 ...
170 ...
145 147
156 158
148 150
... 150
... 150
150 ...
145 ...
155 158 124
167 170 132
158 161 124
... ... ...
... ... ...
... ... ...
... ... ...
291 380
309 403
291 380
... ...
... ...
... ...
... ...
208 241
223 259
212 246
... ...
... ...
... ...
... ...
... 12
... ...
... 12
... 12
... 12
12 ...
15 ...
E, 103 ksi . . . . . . . . . . Ec, 103 ksi . . . . . . . . . G, 103 ksi . . . . . . . . . µ ................
29.4 30.9 11.4 0.29
Physical Properties: ω, lb/in.3 . . . . . . . . . . C, K, and α . . . . . . . .
0.297 See Figure 6.3.5.0
a Design allowables were based upon data from samples of material, supplied in the solution treated condition, which were aged to demonstrate heat treatment response by suppliers. Properties obtained by the user may be different, if the material has been formed or otherwise cold worked. b Sbasis. The rounded T99 value is 183 ksi. c Bearing values are “dry pin” values per Section 1.4.7.1.
652
MMPDS01 31 January 2003
Table 6.3.5.0(c). Forging
Design Mechanical and Physical Properties of Inconel 718 Bar and
Specification . . . . . . . . . . .
AMS 5662 and AMS 5663
Form . . . . . . . . . . . . . . . . . .
Bar
Condition . . . . . . . . . . . . . .
Forging
0.2501.000
Basis . . . . . . . . . . . . . . . . . .
S
S
S
S
S
185 180 ...
185 180 ...
185 180 ...
185 180 ...
150 150 ...
150 150 ...
150 150 ...
156 ... 111
156 ... 114
309 394
1.001 1.501 2.001 2.501 3.0011.500 2.000 2.500 3.000 4.000
Forging
4.0015.000
#5.000
#10.000
#10.000
S
S
S
S
S
185 180 180
185 180 180
185 180 180
185 180 ...
185 180 ...
180 180 180
150 150 ...
150 150 146
150 150 150
150 150 150
150 150 ...
150 150 ...
150 150 150
156 ... 116
156 156 118
156 156 119
156 156 121
156 156 123
... ... ...
... ... ...
... ... ...
309 394
309 394
309 394
309 394
309 394
309 394
... ...
... ...
... ...
216 257
216 257
216 257
216 257
216 257
216 257
216 257
... ...
... ...
... ...
12 6 ...
12 6 ...
12 6 ...
12 6 ...
12 6 6
12 6 6
12 6 6
12 10 ...
10 10 10
12 12 12
15 8 ...
15 8 ...
15 8 ...
15 8 ...
15 8 8
15 8 8
15 8 8
15 12 ...
12 12 12
15 15 15
E, 103 ksi: Ec, 103 ksi: G, 103 ksi . . . . . . . . . . . . . µ ...................
29.4 30.9 11.4 0.29
Physical Properties: ω, lb/in.3 . . . . . . . . . . . . . C, K, and α . . . . . . . . . . . a b
Bar
Solution treated and aged per indicated specification
Thickness, in. . . . . . . . . . . .
Mechanical Properties: Ftu, ksi: L .................. LTa . . . . . . . . . . . . . . . . . STa . . . . . . . . . . . . . . . . . Fty, ksi: L .................. LTa . . . . . . . . . . . . . . . . . STa . . . . . . . . . . . . . . . . . Fcy, ksi: L .................. ST . . . . . . . . . . . . . . . . . Fsu, ksi . . . . . . . . . . . . . . . Fbrub, ksi: (e/D = 1.5) . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . Fbryb, ksi: (e/D = 1.5) . . . . . . . . . . . (e/D = 2.0) . . . . . . . . . . . e, percent: L .................. LTb . . . . . . . . . . . . . . . . STb . . . . . . . . . . . . . . . . . RA, percent: L .................. LTb . . . . . . . . . . . . . . . . STb . . . . . . . . . . . . . . . . .
AMS 5664
0.297 See Figure 6.3.5.0
Applicable providing LT or ST direction is $2.500 inches. Bearing values are “dry pin” values per Section 1.4.7.1.
653
MMPDS01 31 January 2003
Table 6.3.5.0(d). Design Mechanical and Physical Properties of Inconel 718 Investment Castings
Specification . . . . . . . . . . . . . . . . . . . . . . . . . . .
AMS 5383
Form . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Investment Casting
Condition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
ST
Location within casting . . . . . . . . . . . . . . . . . . .
Any
Thickness, in. . . . . . . . . . . . . . . . . . . . . . . . . . .
#0.500
Basis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
S
Mechanical Properties: Ftu, ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
120
Fty, ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
105
Fcy, ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
105
Fsu, ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
88a
Fbrub, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . . . . . . . .
202
(e/D = 2.0) . . . . . . . . . . . . . . . . . . . . . . . . . . .
248
Fbryb, ksi: (e/D = 1.5) . . . . . . . . . . . . . . . . . . . . . . . . . . .
161
(e/D = 2.0) . . . . . . . . . . . . . . . . . . . . . . . . . . .
188
e, percent . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
3
RA, percent . . . . . . . . . . . . . . . . . . . . . . . . . . .
8
E, 103 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
29.4
3
30.9
3
11.4
Ec, 10 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . G, 10 ksi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . µ ...................................
0.29
Physical Properties:
a b
ω, lb/in.3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
0.297
C, K, and α . . . . . . . . . . . . . . . . . . . . . . . . . . .
See Figure 6.3.5.0
Determined in accordance with ASTM Procedure B769. Bearing values are “dry pin” values per Section 1.4.7.1.
654
MMPDS01 31 January 2003
Figure 6.3.5.1.1. Effect of temperature on the tensile ultimate strength (Ftu) and tensile yield strength (Fty) of solutiontreated and aged Inconel 718.
655
MMPDS01 31 January 2003
Figure 6.3.5.1.4(a). Effect of temperature on dynamic tensile modulus (E) of solutiontreated and aged Inconel 718.
Figure 6.3.5.1.4(b). Effect of temperature on dynamic shear modulus (G) of solutiontreated and aged Inconel 718.
656
MMPDS01 31 January 2003
Figure 6.3.5.1.4(c). Effect of temperature on Poisson’s ratio (µ) for solutiontreated and aged Inconel 718.
657
MMPDS01 31 January 2003 200 L and LT  tension 160 L  compression LT  compression
Stress, ksi
120
Ramberg  Osgood n (L  tension) = 21 n (LT  tension) = 22 n (L  comp.) = 21 n (LT  comp.) = 24
80
40 TYPICAL Thickness = 0.010  0.250 in. 0 0
0
2
5
4
6 8 Strain, 0.001
10
12
14
15 20 25 3 Compressive Tangent Modulus, 10 ksi
30
35
10
Figure 6.3.5.1.6(a). Typical tensile stressstrain, compressive stressstrain, and compressive tangentmodulus curves for solutiontreated and aged Inconel 718 sheet (AMS 5596) at room temperature.
200
L and ST  compression L  tension 160
ST  tension
Stress, ksi
120
80
Ramberg  Osgood n (L  tension) = 18 n (ST  tension) = 14 n (L and ST  comp.) = 13
40
TYPICAL Thickness = 2.000  4.000 in.
0 0
2
4
6
8
10
12
14
Strain, 0.001 in./in. 0
5
10 15 20 25 3 Compressive Tangent Modulus, 10 ksi
30
35
Figure 6.3.5.1.6(b). Typical tensile and compressive stressstrain and compressive tangentmodulus curves for solutiontreated and aged (creeprupture application) Inconel 718 bar (AMS 5662 and AMS 5663) at room temperature.
658
MMPDS01 31 January 2003
.
200
160
Stress, ksi
Compression Tension
120
80
RambergOsgood n (Ltension) = 13 n (Lcomp.) = 8.4
40
TYPICAL Thickness:\ 0.500 in. 0
0
2
4
6
8
10
12
14
25
30
35
Strain, 0.001 in./in. 0
5
10
15
20
3
Compressive Tangent Modulus, 10 ksi Figure 6.3.5.1.6(c). Typical tensile stressstrain, compressive stressstrain, and compressive tangentmodulus curves for solution treated and aged Inconel 718 investment casting (AMS 5383) at room temperature.
659
MMPDS01 31 January 2003
Figure 6.3.5.1.6(d). Typical tensile stressstrain curve (full range) for solution treated and aged Inconel 718 investment casting (AMS 5383) at room temperature.
660
MMPDS01 31 January 2003
Figure 6.3.5.1.7(a). Average isothermal 0.10% creep curves for Inconel 718 forging.
Correlative Information for Figure 6.3.5.1.7(a) Makeup of Data Collection: Heat Treatment: 2 [See Table 6.3.5.1.7(f)] Number of Vendors = Unknown Number of Lots = 2 Number of Test Laboratories = 1 Number of Tests = 32 Specimen Details: Type  Unnotched round bar Gage Length  N.A. Gage Thickness  0.25 inch to 0.375 inch
0.10 Percent Creep Equation: Log t = c + b1 T + b2X + b3X2 + b4X3 T = ER X = log (stress, ksi) c = 185.16 b1 = 0.01778 b2 = 255.25 b3 = 146.28 b4 = 28.65 Analysis Details: Inverse Matrix = [See Table 6.3.5.1.7(f)] Std. Error of Estimate, Log (Hrs) = 0.56 Standard Deviation, Log (Hrs) = 0.99 R2 = 68% [Caution: The creep rupture model may provide unrealistic predictions for temperatures and stresses beyond those represented above.]
661
MMPDS01 31 January 2003
Figure 6.3.5.1.7(b). Average isothermal 0.20% creep curves for Inconel 718 forging.
Correlative Information for Figure 6.3.5.1.7(b) Makeup of Data Collection: Heat Treatment: 2 [See Table 6.3.5.1.7(f)] Number of Vendors = Unknown Number of Lots = 2 Number of Test Laboratories = 1 Number of Tests = 31 Specimen Details: Type  Unnotched round bar Gage Length  N.A. Gage Thickness  0.25. inch  0.375 inch
0.20 Percent Creep Equation: Log t = c + b1 T + b2X + b3X2 + b4X3 T = ER X = log (stress, ksi) c = 185.67 b1 = 0.01778 b2 = 255.25 b3 = 146.28 b4 = 28.65 Analysis Details: Inverse Matrix = [See Table 6.3.5.1.7(f)] Std. Error of Estimate, Log (Hrs) = 0.41 Standard Deviation, Log (Hrs) = 0.98 R2 = 82% [Caution: The creep rupture model may provide unrealistic predictions for temperatures and stresses beyond those represented above.]
662
MMPDS01 31 January 2003
Figure 6.3.5.1.7(c). Average isothermal 0.50% creep curves for Inconel 718 forging.
Correlative Information for Figure 6.3.5.1.7(c) Makeup of Data Collection: Heat Treatment: 2 [See Table 6.3.5.1.7(f)] Number of Vendors = Unknown Number of Lots = 2 Number of Test Laboratories = 1 Number of Tests = 22 Specimen Details: Type  Unnotched round bar Gage Length  N.A. Gage Thickness  0.250 inch  0.375 inch
0.50 Percent Creep Equation: Log t = c + b1 T + b2X + b3X2 + b4X3 T = ER X = log (stress, ksi) c = 185.75 b1 = 0.01778 b2 = 255.25 b3 = 146.28 b4 = 28.65 Analysis Details: Inverse Matrix = [See Table 6.3.5.1.7(f)] Std. Error of Estimate, Log (Hrs) = 0.34 Standard Deviation, Log (Hrs) = 1.10 [Caution: The creep rupture model may provide unrealistic predictions for temperatures and stresses beyond those represented above.]
663
MMPDS01 31 January 2003 . .
180
160
140
Stress, ksi
120
100
80
60
40
20 100
101
102
103
104
105
Time to % Strain, Hrs Figure 6.3.5.1.7(d). Average isothermal 5.00% creep curves for Inconel 718 forging.
Correlative Information for Figure 6.3.5.1.7(d) Makeup of Data Collection: Heat Treatment: 2 [See Table 6.3.5.1.7(f)] Number of Vendors = Unknown Number of Lots = 2 Number of Test Laboratories = 1 Number of Tests = 24 Specimen Details: Type  Unnotched round bar Gage Length  N.A. Gage Thickness  0.250 inch  0.375 inch
5.00 Percent Creep Equation: Log t = c + b1 T + b2X + b3X2 + b4X3 T = ER X = log (stress, ksi) c = 186.16 b1 = 0.01778 b2 = 255.25 b3 = 146.28 b4 = 28.65 Analysis Details: Inverse Matrix = [See Table 6.3.5.1.7(f)] Std. Error of Estimate, Log (Hrs) = 0.37 Standard Deviation, Log (Hrs) = 1.02
[Caution: The creep rupture model may provide unrealistic predictions for temperatures and stresses beyond those represented above.]
664
MMPDS01 31 January 2003 . .
180
160
140
Stress, ksi
120
100
80
60
40
20 100
101
102
103
104
105
Time to Rupture, Hrs Figure 6.3.5.1.7(e). Average isothermal stress rupture curves for Inconel 718 forging.
Correlative Information for Figure 6.3.5.1.7(e) Makeup of Data Collection: Heat Treatment: 2 [See Table 6.3.5.1.7(f)] Number of Vendors = Unknown Number of Lots = 7 Number of Test Laboratories = 2 Number of Tests = 162 Specimen Details: Type  Unnotched round bar Gage Length  N.A. Gage Thickness  0.250 inch  0.375 inch
Stress Rupture Creep Equation: Log t = c + b1 T + b2X + b3X2 + b4X3 T = ER X = log (stress, ksi) c = 186.27 b1 = 0.01778 b2 = 255.25 b3 = 146.28 b4 = 28.65 Analysis Details: Std. Error of Estimate, Log (Hrs) = 0.29 Standard Deviation, Log (Hrs) = 0.63 Within Heat Treatment Variance = 0.071 Ratio of Between to Within Heat Treatment Variance = (at spec pt.) 0.752/ 1 % 0.75/n % 2.25/n 2
*
The standard normal distribution function Fo is that function such that Fo(x) is equal to the area under the standard normal curve to the left of the value x.
982
MMPDS01 31 January 2003 one may conclude (at 5 percent risk of error) that the population from which the sample was drawn is not normally distributed. Otherwise, the hypothesis that the population is normally distributed is not rejected. For further information on this test procedure, see References 9.5.4.1(a) and (b). The same procedure can be used to test the normality of the residuals ei ' y i & a % bxi
i ' 1,...,n
from a regression (see Section 9.5.2.1) assuming uniformity of variance of the residuals over the range of the independent variable. When calculating the test statistic AD, define Z(i) ' e(i)/sy i ' 1,...,n
where e(i), i = 1,...,n are the ordered residuals from smallest to largest and sy is the root mean square error of the regression defined in Section 9.5.5.1 or 9.5.5.2. The justification for this procedure may be found in Reference 9.5.4.1(c). 9.5.4.2 Normal Probability Plot —To graphically illustrate the degree to which a normal distribution fits a set of data, a normal probability plot may be formed by plotting the measured value of each test — point versus X + s Fo1 (P/100) where Fo1 is the inverse standard normal cumulative distribution function.* The line representing the fitted normal distribution is the line passing through the points with equal horizontal and vertical coordinates. If the horizontal axis is labeled with cumulative probabilities (P values) as in Table 9.10.5 rather than Fo1 (P/100) values, the plot will be identical to a plot formed on normal probability paper. Figure 9.5.4.2 illustrates the use of a normal probability plot on Alclad 2524T3 Aluminum Alloy Sheet and Plate data in the 0.0630.128 inch thickness range. There are 309 measured test values with X = 45.24 and s = 1.923. There appears to be a systematic departure from the model (the measured values are higher than expected) in both tails, suggesting that the distribution of the measured values departs from a normal distribution. This model was rejected by the AndersonDarling test for normality. 9.5.4.3 ThreeParameter Weibull Acceptability Test — The threeparameter Weibull acceptability test is designed to determine whether an acceptable proportion of a producer’s population is likely to exceed the specification limit for corresponding material property. Because this test is only used to screen data sets and is not used in the actual calculation of lower tolerance bounds, it is not required that the data be welldescribed by a Weibull distribution to apply this test. To carry out this test, an upper confidence bound (UCB) is calculated for the first percentile of the producer’s population. This UCB value is calculated in the same manner as a T99 value is calculated (in Section 9.5.5.2) with the following modifications:
*
(1)
In solving for the threshold (θ) (Section 9.5.5.2.1), θ should be set equal to 0.10.
(2)
The value of V99 should be taken from Table 9.10.6 rather than Table 9.10.7 when using the formula for T99 (Equation [ 9.5.5.2(a)]) to calculate the UCB value.
The point F01 (P/100) is that value such that the area under the standard normal curve to the left of Fo&1 (P/100) is P/100.
983
MMPDS01 31 January 2003
Figure 9.5.4.2 Probability plot for a normal distribution fitted to a complete TYS data set for Alclad 2524T3 aluminum alloy sheet in the 0.0630.128 inch thickness range rejected.
If UCB is greater than or equal to the specification limit, it is concluded that the producer’s data is acceptable. If UCB is less than the specification limit, it is concluded (with a 5 percent risk of error) that the producer’s data do not meet the specification minimum value. In statistical terms, this method tests (at 5 percent significance level) the hypothesis that at least 99 percent of the producer’s population is greater than the specification limit. If the hypothesis is not rejected (UCB greater than or equal to specification limit), then it is concluded that the producer’s data is acceptable. If the hypothesis is rejected (UCB less than the specification limit), it is concluded that the producer’s data is unacceptable. This technique is applicable only when data have not been censored from the sample. It also assumes that the data are distributed according to a threeparameter Weibull distribution (although normally distributed data and Pearson distributed data are also accommodated by this test). If the data sample is highly skewed, background data should be reviewed to determine whether the skewness is caused by a mixed population. If it is not, the Weibull test procedure can be applied. This test should be applied to both tensile yield and ultimate strengths (in appropriate grain directions), and if a producer’s data is unacceptable for either property, that producer’s data for both properties should be excluded for the purpose of computing T99 and T90 values. 9.5.4.4 AndersonDarling Test for Pearsonality – This section describes a test to determine whether data from a population are satisfactorily described by the Pearson Type III (or gamma) distribution.
984
MMPDS01 31 January 2003 First compute estimates of the population mean, standard deviation, and skewness (denoted by X , S, and q), as described in Section 9.5.5.1. Then calculate the following AndersonDarling statistic:
AD ' & j n
i'1
(2i&1) 3n ln FX,S,q (X(i) ) & 2FX,S,q (X(i) ) & ¯ ¯ n 2
where
Fµ ,σ , q
4 2 x − µ H + σ q q 4 2 x − µ 1− H + σ q q 4 2 x − µ + σ q q 2 Φ 3 1 − + 8 8 ( x) = 9⋅ 2 2 q q 4 2 x − µ + σ q q 2 1− Φ 3 − 1+ 8 8 9⋅ 2 2 q q x− µ Φ σ
q > 0.1265
2 8 9⋅ 2 q
2 8 9⋅ 2 q
q < − 0.1265
0.025 < q ≤ 0.1265
− 0.1265 ≤ q < 0.025 q ≤ 0.025
H(x) is the cumulative distribution function of a chisquare distribution with 8/q2 degrees of freedom. Note that F(x) is the cumulative distribution function of a chisquare distribution with 8/q2 degrees of freedom when q > 0.1265 , and a standard normal distribution when q ≤ 0.025 . Because of numerical computing inconsistencies for large degrees of freedom, a normal approximation to the chisquare distribution is recommended for 0.025 < *q* # 0.1265 . 2 0.3167 + 0.034454 ⋅ ln( n ) ⋅ [ exp(q ) − 1] ,
If the AD is greater than the critical value of
then the data are rejected by the AndersonDarling test for Pearsonality. 9.5.4.5 The Pearson Backoff Option – If the data are rejected by the Pearson AD test, the backoff method may be applied. The following formula should be used to calculate the AD statistic of the backoff method:
ADbackoff (µ) =
Σ(
n n n 1 n 2 2 2 bi+1,i − bi,i i [ln(bi+1,i ) − ln(bi,i )] − 2 i(bi+1,i − bi,i ) + 2 i=1 n i=1 i=1
Σ
Σ
985
)
MMPDS01 31 January 2003
where
j b i,j = min F µ , S , q ( x (i ) ), for j X − 2 ⋅ S / Q − X (n) , then the backoff method cannot be applied. S and Q are defined in Section 9.5.5.1.)
T 99 = X − k 99 (q , n ) ⋅ S − τ backoff
If a backoff is identified, then T99 and T90 should be calculated by the following formulas:
T 90 = X − k 90 (q , n ) ⋅ S − τ backoff where k90(q,n) and k99(q,n) are defined in Section 9.5.5.1. 9.5.4.6 Pearson Probability Plot — To graphically illustrate the degree to which a Pearson Type III (or gamma) distribution fits a set of data, the following procedure for creation of a Pearson probability plot is recommended. This method is appropriate for distributions estimated using uncensored data. The rank of each point selected for plotting is the number of lower test points plus the plotted point plus onehalf the number of other test points equal to the plotted point. Its cumulative probability, P (in percent), is equal to the rank multiplied by 100, divided by one more than the total number of test points: P (in percent) '
(rank)(100) n % 1
The measured value of each test point is plotted versus F1 (P/100) where
986
MMPDS01 31 January 2003 q 2 −1 when q > 01265 . X + s ⋅ ⋅ H ( P / 100) − 4 q q 2 −1 when q < − 01265 . X + s ⋅ 4 ⋅ H 1 − ( P / 100) − q 3 2 2 2 − 1 0.025 < q ≤ 01265 . ⋅ Fo−1 ( P / 100) + 1 − ( P/ 100) = X + s ⋅ ⋅ 8 8 q 9⋅ 2 9⋅ 2 q q 3 2 2 2 X + s ⋅ ⋅ − 1 ⋅ Fo−1 (1 − P / 100) + 1 − − 01265 ≤ q < − 0.025 . 8 8 q 9⋅ 2 9⋅ 2 q q X + s ⋅ F −1 ( P / 100) q ≤ 0.025 o
[
F −1
]
and X , s, and q are population parameter estimates obtained according to the procedures outlined in Section 9.5.5.1. H1 is the cumulative distribution function of a chisquare distribution with 8/q2 degrees of freedom and Fo1 is the inverse standard normal cumulative distribution function. A straight line is then drawn to represent the fitted Pearson distribution. This line may be established by plotting any two points with equal vertical and horizontal coordinates and drawing a line through these two points. The horizontal axis is then labeled with cumulative probabilities (P or P/100) rather than F1 values. If the backoff option is used, the selected distribution can then be described as the bestfit distribution shifted by a small constant, backoff. In this case, the predicted values should also be shifted by the same constant. That is, plot the measured values versus F1(P/100) 
backoff
.
The plotted points should finally be compared with the line to determine whether there appears to be a reasonably good fit. If the backoff option is used, then only deviations where the data fall below the fitted line should be considered as relevant. Figure 9.5.4.6(a) illustrates the use of a Pearson probability plot on Aluminum Alloy Sheet and Plate data in the 0.0630.128 inch thickness range. The estimates of the mean, standard deviation, and skewness parameters are 45.24, 1.92, and 0.12, respectively. There appears to be a systematic departure from the model (the measured values are higher than expected) in both tails, suggesting that the distribution of the measured values is not well approximated by a Pearson distribution. Appropriately, this model was rejected by the AD test for Pearsonality. Figure 9.5.4.6(b) shows a probability plot for the same data, using the distribution estimated with the backoff option of the sequential Pearson procedure, which identified a backoff of 0.2 ksi. The only difference between the two plots is that the predicted values in Figure 9.5.4.6(a) are shifted 0.2 ksi to the left in Figure 9.5.4.6(b). Although the curve of data in Figure 9.5.4.6(b) is further away (on average) from the y=x reference line than the curve of data in Figure 9.5.4.6(a), only negative deviations from the reference line are recognized in the AD goodnessoffit test for a distribution estimated by the backoff method. In
987
MMPDS01 31 January 2003
Figure 9.5.4.6(a). Probability plot for a Pearson distribution fitted to a complete TYS data set for Alcad 2524T3 aluminum alloy sheet in the 0.0630.128 inch thickness range  rejected.
Figure 9.5.4.6(b). Probability plot for a Pearson distribution fitted to complete TYS data for Alcad 2524T3 aluminum alloy plate in the 0.0630.128 inch thickness range using 0.2 ksi backoff  accepted.
988
MMPDS01 31 January 2003 Figure 9.5.4.6(b), only a small proportion of the data are below the predicted values, resulting in an insignificant deviation. The “backoff” model was accepted by the AD test. 9.5.4.7 Modified “AndersonDarling” Test for Weibullness — The “AndersonDarling” test for threeparameter Weibullness is used to determine whether the curve which fits a given set of data can be approximated by a threeparameter Weibull curve. The essence of the test is a numerical comparison of the cumulative distribution function for observed data with that for a fitted Weibull curve over the entire range of property being measured. This test differs from the original version of the AndersonDarling test in that it emphasizes the lower tail. This method can be applied with complete or censored data. The first two steps produce estimates of the parameters of a threeparameter Weibull distribution. Be sure to acknowledge the appropriate degree of censoring in computing the threshold, shape, and scale parameters as described in Sections 9.5.4.7.1 and 9.5.4.7.2. Using the procedure outlined in 9.5.4.7.1, compute the threshold for the goodnessoffit test, 50. Then, using the method described in 9.5.4.7.2, compute the maximum likelihood estimates of the shape and scale parameters for {X(i)  50 : i=1,...,r} where r equals n for the uncensored data and r represents the smallest integer greater than or equal to 4n/5 for 20 percent censoring and n/2 for 50 percent censoring. Denote these estimates by 50 and α50, respectively. Calculate the (censored or uncensored) AD statistic is described in Section 9.5.4.7.3. 9.5.4.7.1 Estimating the Threshold Parameter — This section describes a method for estimating the threshold of a threeparameter Weibull distribution. The same approach is taken for estimating the threshold, whether the purpose is to test goodnessoffit (Section 9.5.4.7), or to directly calculate T99 or T90 values (Section 9.5.5.2). This method applies to uncensored and uppertail censored data; however, different columns of Table 9.10.8 are used. (References 9.5.4.7.1(a) and 9.5.4.7.1(b) provide details of this method for uncensored data.) Let K equal the greatest integer less than or equal to min {4n/15, (1p)n/3}, where p represents the proportion of the upper tail that is censored (p equals 0, 0.2, or 0.5). Define the function R( ) by
R( )' j
3K&2
i'K%1
where
Li( )'
Li( )/ j Li( ) 3K&2 i'1
1 ln X(i%1)& Di
&ln X(i)&
with
1 , n&1
D1 ' n ln 1 % n(n&1) 2
ln 1%
n(n&1)(n&2) 6
ln 1%
D2 '
D3 ' D4 '
n(n&1)(n&2)(n&3) 24
ln 1%
1 n(n&2)
,
2n & 3 (n&1)3 (n&3)
,
6n 4 & 48n 3 % 140n 2 & 176n % 81 n(n&4) (n&2)6 989
,
MMPDS01 31 January 2003 and
Di ' ln &ln 1 &
i % 0.5 n % 0.25
& ln &ln 1 &
i & 0.5 n % 0.25
¯ and S represent the sample mean and sample standard deviation, for i=5,6,...,3K2. Finally, let X respectively. Determine using the appropriate column of Table 9.10.8. The first set of columns in Table 9.10.8 is provided for estimating the threshold, 50, associated with the AndersonDarling goodnessoffit test described here. The second and third sets of columns are provided for estimating 99 and 90, which are needed to determine T99 and T90, as described in Section 9.5.5.2. Each set of columns includes a column for uncensored data, 20 percent uppertail censored data, and 50 percent uppertail censored data. The estimated threshold parameter, , is the solution to the equation R( ) = . The function R( ) is a monotonically decreasing continuous function of . A simple method for finding the solution is as follows. ¯ 100S) and H = 0.999999X(1). If R(L) # , then set = L or if R(H) $ then set = Start with L = min(0, X H. Otherwise reduce the (L,H) interval by calculating M = (L+H)/2 and setting L = M if R(M) $ or by ¯ 106, then set = M and stop. Otherwise, reduce the (L,H) interval setting H = M if R(M) < . If H  L # 2X/ again. 9.5.4.7.2 Estimating the Shape and Scale Parameters — This section describes a method for estimation of the shape and scale parameters of the twoparameter Weibull distribution based on data which may be censored in the upper tail. Estimates of the shape and scale parameters are based on the original data corrected for the estimated threshold, . That is, the calculations in this section are performed based on Z(1), ..., Z(n), where Z(i) = X(i) , with estimated as in Section 9.5.4.7.1. The assumption is made here that if the data are censored, then only the r smallest observations in the sample are observed (1 # r # n), where r is some prespecified number (often based on a percentage); this is called Type II censoring. Thus, the input to this procedure is a total sample size, n, a censored sample size, r, and the sample remaining after censoring Z(1), ..., Z(r). Define r
Σ Z(i) ln Z(i) % (n&r) Z(r) ln Z(r)
g( ) '
i'1
& r
Σ Z(i) % (n&r) Z(r)
1
&
1 r Σ ln Z(i) r i'1
i'1
Note:
When implementing the equation for g( ) in software, it may be necessary to divide each Z term that is raised to the power by a normalizing factor, C, in order to avoid computational difficulties. The factor, C, can be any type of average calculated from the Z values (e.g., geometric mean of the uncensored Z values). Because the Cfactor algebraically cancels out of the equation for g( ), its use does not change the meaning of the equation in any way.
The shape parameter estimate, , is the solution to the equation g( ) = 0. The function g( ) is a monotonically increasing continuous function of . A simple method for finding the solution is as follows. Let Sy denote the standard deviation of Yl, ..., Yr where Yi = ln (Zi) for i=1, ..., r. Calculate I = 1.28/Sy as an initial guess at the solution and calculate g(I). If g(I) > 0, then find the smallest positive integer k such that g(I/2k) < 0 and let L = I/2k and H = I/2k1. If g(I) < 0, then find the smallest positive integer k such that g(2k I) > 0 and let L = 2k1 I, and H = 2k I. Reduce the (L,H) interval by calculating M = (L+H)/2 and setting
990
MMPDS01 31 January 2003 L = M if g(M) # 0 and/or by setting H = M if g(M) $ 0. If HL # 2I/106, then set = M and stop. Otherwise, reduce the (L,H) interval again. Once
has been determined, the scale parameter estimate is defined by 1
α '
1 r
r
Σ Z(i) % (n&r) Z(r)
.
i'1
9.5.4.7.3 Calculating the AndersonDarling Statistic — Once the parameters have been estimated in Sections 9.5.4.7.1 and 9.5.4.7.2, calculate the AndersonDarling statistic by the following steps. For i=1,...,r, let Fi' 1 & exp &
X(i)&
50
50
,
α50
let Fn+1 = 1, and let
C i'
2i&1 . n
Define the AD statistic as
AD ' &j Ci ln Fi&2Fi % r
i'1
r2 n 2 n 2 Fr%1 & F1 . ln Fr%1& 2r Fr%1% 2 2 n
If
AD $
0.3951 % 4.186 x 10&5 n 0.2603 % 4.182 x 10&5 n 0.1761 % 1.842 x 10&5 n
(Uncensored) (20 percent censored) (50 percent censored)
[9.5.4.7.3]
one may conclude (at 5 percent risk of error) that the population from which the sample was drawn is not a threeparameter Weibull population. Otherwise, the hypothesis that the population is a threeparameter Weibull population is not rejected. Equation 9.5.4.7.3 was derived under the assumption that the threshold parameter is estimated, not known. For further information on this test procedure, see Reference 9.5.4.7.3. 9.5.4.8 Identifying Proper Backoff for Weibull Method — Begin with the estimates 50, α50, and 50 obtained according to the procedures outlined in Sections 9.5.4.7.1 and 9.5.4.7.2. Let F (x) represent the cumulative distribution function of the threeparameter Weibull distribution with threshold parameter , and scale and shape parameters, α50 and 50, respectively:
F (x) ' 1 & exp &
991
x& α50
50
.
MMPDS01 31 January 2003 Define the special “backoff” Anderson Darling statistic by
ADB( ) ' n j n
i'1
i n
2
(ln bi & ln ai) &
2i 1 2 2 (bi & ai) % (bi & ai ) , n 2
where ai = min{F (x(i)), i/n}, bi = min{F (x(i+1)), i/n} for i < n, and bn = 1. Let among 0.1, 0.2, 0.3, 0.4, and 0.5 such that ADB(
50

backoff
backoff
) < 0.0359 + 1.2 x 105 n .
be the smallest value
[9.5.4.8]
If none of the five values satisfies Equation 9.5.4.8, the backoff procedure cannot be used to compute T99 and T90. Otherwise, backoff is subtracted from T99 and T90 as calculated from the complete sample. 9.5.4.9 Weibull Probability Plots —To graphically illustrate the degree to which a threeparameter Weibull distribution fits a set of data, the following procedure for creation of a Weibull probability plot is recommended. This method is appropriate for distributions estimated using censored or uncensored data. A method for displaying the fit using a distribution estimated by a backoff option is also described. The rank of each point selected for plotting is the number of lower test points plus the plotted point plus onehalf the number of other test points equal to the plotted point. Its cumulative probability, P (in percent), is equal to the rank multiplied by 100, divided by one more than the total number of test points:
P (in percent) '
(rank)(100) n % 1
The measured value of each test point is plotted versus F1 (P/100) where 1
F
&1
(P/100) '
50
% α50
& ln 1 & (P/100)
50
and 50, α50, and 50 are population parameter estimates obtained according to the procedures outlined in Sections 9.5.4.7.1 and 9.5.4.7.2 . A straight line is then drawn to represent the fitted Weibull distribution. This line may be established by plotting any two points with equal vertical and horizontal coordinates and drawing a line through these two points. The horizontal axis is then labeled with cumulative probabilities rather than F1 values. If the backoff option is used, the selected distribution can then be described as the bestfit distribution shifted by a small constant, backoff. In this case, the predicted values should also be shifted by the same constant. That is, plot the measured values versus F1(P/100) 
backoff
.
The plotted points should finally be compared with the line to determine whether there appears to be a reasonably good fit. With sample sizes on the order of 100 test points, only those points lying between about 10 and 90 percent probability should be considered in making this evaluation. With sample sizes of 1000 test points, these limits can be extended to about 1 and 99 percent. If the distribution was estimated using a method for censored data, then only the uncensored portion of the data used to estimate the distribution should be considered when assessing lack of fit. For instance, if the 20 percent censoring method is selected for use by the sequential Weibull method, then only the lower 80 percent of the data should be
992
MMPDS01 31 January 2003 examined for agreement with the line of best fit. If the backoff option was used, then only deviations where the data fall below the fitted line should be considered as departures. Figure 9.5.4.9(a) illustrates the use of a Weibull probability plot on Alclad 2524T3 Aluminum Alloy Sheet and Plate data in the 0.0630.128 inch thickness range. This is a probability plot based on a Weibull distribution estimated using the 50 percent censoring method. The estimates of the threshold, scale, and shape parameters based on 50 percent censoring are 40.87, 5.26, and 2.09, respectively. Notice that the lower tail does not exhibit serious departures from the model, but significant departures are apparent in the upper tail. But, as mentioned above, only the lower 50 percent of the data should be included in an assessment of this probability plot, because the rest are not used in fitting the model. The model estimated by this method was accepted by the AndersonDarling test for Weibullness.
Figure 9.5.4.9(a). Probability plot for a Weibull distribution fitted with 50 percent censored TYS data for Alcad 2524T3 aluminum alloy sheet in the 0.0630.128 inch thickness range  accepted.
Figures 9.5.4.9(b) and 9.5.4.9(c) illustrate the value of the backoff method and the construction and interpretation of the associated probability plots. Alclad 2524T3 Aluminum Alloy Sheet and Plate tensile yield data in the 0.250 – 0.310 inch thickness range is used for illustration. There are 1202 measured test values. The estimates of the threshold, scale, and shape parameters of the bestfit Weibull distribution, based on the uncensored data, are 40.00, 3.50, and 2.62, respectively. The departures from the reference line in Figure 9.5.4.9(b) suggest that this Weibull distribution does not provide a good fit for the measured values, and it was rejected by AndersonDarling test for Weibullness.
993
MMPDS01 31 January 2003
Figure 9.5.4.9(c) shows a probability plot of the same data, using the distribution estimated with the backoff option of the sequential Weibull procedure, which identified a backoff of 0.2 ksi. The only difference between the two plots is that the predicted values in Figure 9.5.4.9(b) are shifted 0.2 ksi to the left in Figure 9.5.4.9(c). Although the curve of data in Figure 9.5.4.9(c) is further away (on average) from the y=x reference line than the curve of data in Figure 9.5.4.9(b), only negative deviations from the reference line are recognized in the AndersonDarling goodnessoffit test for a distribution estimated by the backoff method. In Figure 9.5.4.9(c), only a small proportion of the data in the very middle of the distribution are below the predicted values, resulting in an insignificant departure from Weibullness.
Figure 9.5.4.9(b). Probability plot for a Weibull distribution fitted to a complete TYS data set for Alcad 2524T3 aluminum alloy plate in the 0.2500.310 inch thickness range  rejected.
9.5.5 DIRECT COMPUTATION WITHOUT REGRESSION —To permit computation of lower tolerance bounds in more of these cases, the Weibull approach was expanded to incorporate two different levels of uppertail censoring and a lastresort conservative “backoff” option. Also, a modified version of the AD test was developed which places more emphasis on the lower tail than the upper tail (Section 9.5.4.7). During the development of the Weibull procedure (Section 9.5.5.2), it became evident how inadequate the traditional normal procedure is for computing tolerance bounds when the data come from a 9.5.5 illustrates the shortcomings of the normal procedure for computing T99 and T90 for distributions* ranging in skewness from minus 1 to plus 1. The second column provides estimates of the probability that skewed
*
Table 9.5.5 is based on data generated from Weibull distributions with varying skewness. All distributions are standardized to a mean of 100 and standard deviation of 5.0.
994
MMPDS01 31 January 2003
Figure 9.5.4.9(c). Probability plot for a Weibull distribution fitted to complete TYS data for Alcad 2524T3 aluminum alloy plate in the 0.2500.310 inch thickness range using 0.2 ksi backoff  accepted.
distribution – even if a goodnessoffit test is applied to screen out nonnormal distributions. Table a sample of size 100 will be “accepted” as normal. Notice that for very skewed Weibull distributions, the proportion accepted by the normal AndersonDarling test is small, but it increases for distributions with skewness near zero. The third column of Table 9.5.5 estimates the coverage, which is the probability (or confidence) that the method will yield a T99 below the true first percentile. This should be 95 percent. If the distribution is negatively skewed then the coverage can be substantially lower than the claimed 95 percent. The fourth column estimates the systematic bias of the procedure. Bias for T99 represents the difference between the 95th percentile of the T99 values produced by the normal procedure minus the true first percentile. (Bias is presented in units of standard deviations. This can be converted to, say, ksi units, if the standard deviation is known.) It can be interpreted as the amount that would have to be subtracted from the T99 values produced by the procedure to get an appropriate answer. The problem is, in practice, one never knows true skewness. Notice that as bias goes up, coverage goes down. The last two columns provide coverage and bias estimates for T90. Although still significant, the errors associated with T90 are much smaller than those for T99. Figure 9.5.5(a) displays the bias of T90 and T99 for skewness between minus1 and plus 1 (again, in units of standard deviations). Normalbased methods can be very good for estimating the mean of a distribution  which is not very sensitive to skewness. However, in MMPDS, much of the emphasis is on estimating the first and tenth percentiles  which are very sensitive to skewness. Table 9.5.5 and Figure 9.5.5(a) are provided to emphasize the notion that applying the normal method can result in very poor tolerance bound estimates due to undetected skewness. It is for this reason that the traditional normal method for computing tolerance bounds is not provided in the Handbook as a recommended procedure. On the other hand, because methods based on the Weibull distribution are computationally intensive and have less intuitive appeal than methods based on the normal distribution, an alternative procedure was
995
MMPDS01 31 January 2003 Table 9.5.5. Performance of Normal Method for Calculating T90 and T99 on Samples of Varying Skewness
T99
T90
Skewness
Percent Accepted
Percent Coverage
Bias (Std. Dev.)
Percent Coverage
Bias (Std. Dev.)
1.00 0.75 0.50 0.25 0.00 0.25 0.50 0.75 1.00
16 40 68 91 98 91 65 21 4
3 11 43 82 98 100 100 100 100
1.0 0.7 0.4 0.2 0.1 0.4 0.6 0.7 0.7
66 78 83 88 93 97 99 100 100
0.22 0.16 0.12 0.08 0.04 0.02 0.06 0.06 0.10
1.2
T99 T90
1.0 0.8
Bias (Std. Devs.)
0.6 0.4 0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.25
1.00
0.75
0.50
0.25
0.00
0.25
0.50
0.75
1.00
1.25
Skewness Figure 9.5.5(a). Estimated Bias of T99 and T90 Using Normal Method on Skewed Data.
996
MMPDS01 31 January 2003 developed based on the Pearson Type III family of distributions. The Pearson family includes the normal distribution as a special case. The Pearson method was incorporated into the Guidelines in 1999. The sequential Weibull procedure (Section 9.5.5.2) and the sequential Pearson procedure (Section 9.5.5.1) were developed based on distributions with skewness between minus 1 and 1. Therefore, the Weibull and Pearson procedures should not be applied if the sample skewness is outside this range. If no systematic effects (e.g., thickness) are identified as significant by regression, then only the nonparametric method (Section 9.5.5.3) should be applied. Current analysis procedures for computing lower tolerance bounds (T90, T99) are described in Figure 9.5.5(b). Three methods are permitted: the sequential Pearson procedure, the sequential Weibull procedure, and the nonparametric procedure. The remainder of this section provides an overview and a roadmap to these procedures. Figure 9.5.5(c) describes the procedure for translating T99 and T90 values to A and B values, and values for publication in the mechanical property tables in this Handbook. In what follows, certain procedures require artificial censoring of the measured data. That is, because the real engineering interest for design lies in lower percentiles of the distribution of a material’s properties, some of the following procedures ignore a portion of the observations in the upper tail. Specifically, we use the notation X(1)#X(2)#...#X(n) to denote the ordered sample, and will frequently refer to the censored sample: X(1)#X(2)#...#X(r). The ratio r/n represents the proportion of the sample which is uncensored. Alternatively, (1r/n) represents the proportion of the sample which is censored. The terms r and n will be used throughout subsequent sections without redefinition. In the case of uncensored data, r=n. If the sequential Pearson analysis procedure is applied, the first step is to perform an AndersonDarling goodnessoffit test for Pearsonality as described in Section 9.5.4.4. If the assumption of normality is not rejected, the lower tolerance bounds may be computed using the methods described in Section 9.5.5.1. If the assumption of Pearsonality is rejected, then the Pearson backoff method (Section 9.5.4.5) should be attempted. This method decreases the estimate of the mean, while holding the standard deviation and skewness estimates constant, until the percentiles of the resulting model are sufficiently less than the sample percentiles. To avoid accepting an extremely inadequate fit, the decrease in the mean is limited to 0.5 ksi. Section 9.5.4.5 describes the method for identifying a proper backoff, denoted by backoff, for the sequential Pearson method. If the appropriate backoff is less than or equal to 0.5 ksi, the lower tolerance bounds should be calculated by first computing bounds based on the complete sample as specified in Section 9.5.5.1, and then subtracting backoff. If an appropriate backoff less than or equal to 0.5 ksi is not identified, then the sequential Weibull procedures described in Section 9.5.5.2 or the nonparametric procedure described in Section 9.5.5.3 should be considered. In most cases it has been found that strength data fit a Pearson distribution better than a Weibull distribution. However, there are times when a Weibull distribution does provide a better fit. Probability plots are helpful in determining which procedure provides the best fit when there is a difference in the T99 and T90 values for the two methods. When the sequential Weibull procedure is applied, a modified AndersonDarling goodnessoffittest is conducted as described in Section 9.5.4.7 for the uncensored sample. If the assumption of Weibullness is not rejected, the lower tolerance bound should be computed using methods described in Section 9.5.5.2 for complete samples. (The risk that one may conclude erroneously that a true Weibull distribution is non
997
MMPDS01 31 January 2003
Acceptable sample (Regression not required) (From Figure 9.5.1)
Pearson
Weibull
Test complete sample f or Pearsonality (Section 9.5.4.4)
Test complete sample f or Weibullness (Section 9.5.4.7) Accept
Accept
Reject
Reject
Test lower 80% f or Pearsonalilty
Test lower 80% f or Weibullness
Accept
Reject
Reject
Test lower 50% f or Pearsonality
Accept
Accept
Compute lower tolerance bounds using appropriately censored model estimates (Section 9.5.5.1)
Test lower 50% f or Weibullness
Reject
Accept
Compute lower toleracnce bounds using appropriately censored model estimates (Section 9.5.5.2)
Reject Accept
Accept
Test Pearson Backof f Option (Section 9.5.4.5)
Test Weibull Backof f Option (Section 9.5.4.8)
Reject
Reject
Try Weibull
Try Pearson
If both methods are acceptable, compare Probability Plots (Sections 9.5.4.6 & 9.5.4.9)
Pearson and Weibull rejected
Use v alues f rom method that prov ides the best f it to lower tail of data
Nonparametric
Is sample size suf f icient f or Nonparametric (n=299 or greater)
Compute lower tolerance bounds using ranked v alues (Section 9.5.5.3)
Figure 9.5.5(b). Procedure for Direct Computation of T99 and T90 When Regression is Not Required.
998
MMPDS01 31 January 2003
C om puted T99 and T90 Values
W ere T99 and T90 c om puted bas ed on at leas t 100 data points ?
No
A and B v alues m ay not be c om puted.
C ollec t m ore data
No Yes
W as a param etric m ethod ac c epted? (W eibull or Pears on)
At leas t 299 data points ?
No
Yes
Yes
A=T 99 rounded B=T 90 rounded
Frac tions greater than 0.75 are us ually rais ed to the nex t larger integer, w hile les s er frac tions are dis regarded.
B v alue is rec orded in m ec hanic al property table.
Is Spec Value (S) 0 and X(1) < T, then let b. If Q < 0 and X(n) > T, then let c. Otherwise, q = Q.
q = 2 • S / ( X − 0.99999 X
). (1) q = 2 • S / ( X − 100001 . X ). (n)
If the data are not rejected by the AndersonDarling test for Pearsonality (described in 9.5.4.4), then T99 and T90 should be calculated by the following formulae: T 99 = X − k 99 (q , n ) ⋅ S T 90 = X − k 90 (q , n ) ⋅ S
where
k 99 (q,n ) = z 99 (q )
[
]
+ exp 2 .556 − 1.229 q + 0.987 q 2 − 0.6542 ⋅ ln (n ) + 0.0897 q ⋅ ln (n ) − 0.1864 q 2 ⋅ ln (n )
k 90 (q,n ) = z 90 (q )
[
]
+ exp 1 .541 − 0 .943 q − 0.6515 q 2 − 0.6004 ⋅ ln (n ) + 0.0684 q ⋅ ln (n ) + 0.0864 q 2 ⋅ ln (n )
3 q2 q 2 z 99 (q ) = − 0.013133 q 2 − 0.003231 q 3 + 0.003139 q 4 + 0.001007 q 5 1− 1− − 2.326348 ⋅ q 36 6
3 q2 q 2 − 1.281552 ⋅ z 90 (q ) = + 0.003814 q 2 − 0.002466 q 3 − 0.000633 q 4 + 0.000122 q 5 1− 1− q 36 6
9101
MMPDS01 31 January 2003 The above formulas for z99(q) and z90(q) should be used for q =/ 0. If q = 0, then z99(q) = 2.326348 and z90(q) = 1.281552. If the data are rejected by the AndersonDarling test for Pearsonality, but accepted under the backoff option of the test (9.5.4.5) with a reduction in the mean of backoff, then the above formulas should be applied to compute then T99 and T90 with the following slight modification:
T99 = X − k99 (q, n ) ⋅ S − τ backoff ,
T90 = X − k90 (q, n ) ⋅ S − τ backoff .
9.5.5.2. Sequential Weibull Procedure — This section describes procedures required for modeling data with the threeparameter Weibull distribution. Section 9.5.4.7.1 describes a method for estimating the threshold parameter, . Section 9.5.4.7.2 describes a method for estimating the shape and scale parameters, and α, respectively. Both methods permit estimation with uppertail censored data. For a good exposition of such procedures, see Reference 9.5.4.1(a). This procedure should be used when a mechanical property value is to be computed directly (not paired with another property for computational purposes) and the population may be interpreted to signify either the property measured (TUS, etc.) or some transformation of the measured value that follows a threeparameter Weibull distribution. This procedure is applicable to Ftu and Fty. It may also be used for Fcy, Fsu, Fbru, and Fbry if a sufficient quantity of data is available. In order to compute the lower tolerance bounds for a threeparameter Weibull population, it is necessary to have (1) an estimate of population threshold, (2) estimates of population shape and scale parameters, and (3) tables of onesided tolerance limit factors for the threeparameter Weibull distribution. The method for estimating the population threshold is presented in Section 9.5.4.7.1, and Section 9.5.4.7.2 contains the method for estimating population shape and scale parameters. Both of these procedures permit estimation with complete or censored data (20 or 50 percent censoring). A tabulation of tolerance limit factors by sample size, censoring level, and population proportion covered by the tolerance interval is presented in Table 9.10.7. For further information on these procedures and tabled values, see References 9.5.5.2.(a) and (b). Let X1,..,Xn denote sample observations in any order and let X(1),...,X(n) denote sample observations ordered from smallest to largest. The first step in calculating T99 and T90 for a threeparameter Weibull population is to obtain an estimate of the population threshold. The population threshold is theoretically the minimum achievable value for the property being measured. However, the real population is being empirically modeled by some Weibull population with a threshold. Since this empirical model is not perfect, there may be a small percentage of observations in the population that fall below the model threshold. Separate threshold estimates, denoted by 99 and 90, will be obtained for T99 and T90 using the methods described in Section 9.5.4.7.1. The second step in calculating mechanical properties for a threeparameter Weibull population is to obtain estimates of population shape and scale parameters for each property. Shape parameter estimates will be denoted by 99 and 90 and scale parameter estimates will be denoted by α99 and α90. Estimation of shape and scale parameters is performed using a maximum likelihood procedure for the twoparameter Weibull distribution, after subtracting off the estimated threshold. (The twoparameter Weibull is equivalent to the threeparameter Weibull with threshold zero.)
9102
MMPDS01 31 January 2003 Using the method outlined in Section 9.5.4.7.2, compute the maximum likelihood estimates of the shape and scale parameters for the censored or uncensored sample {X(i)  99 : i=1,...,r}, where r equals n for uncensored data and r represents the smallest integer greater than or equal to 4n/5 for 20 percent censoring and n/2 for 50 percent censoring. Denote these estimates by 99 and α99, respectively. Using the same procedure, compute estimates 90 and α90 based on the sample {X(i)  90 : i=1,...,r}. With population parameter estimates discussed above at hand, the computation of the lower tolerance bounds is carried out by use of the formulas:
T99 '
99
% Q99 exp
& V99/
99
n
,
[9.5.5.2(a)]
T90 '
90
% Q90 exp
& V90/
90
n
,
[9.5.5.2(b)]
where Q99 Q90 V99 V90
= α99 (0.01005)1/ 99 = α90 (0.10536)1/ 90 = the value in the V99 column of Table 9.10.8 corresponding to a sample of size n and the appropriate degree of censoring, and = the value in the V90 column of Table 9.10.8 corresponding to a sample of size n and the appropriate degree of censoring.
Note that the level of censoring used in estimating the threshold, shape, and scale parameters must be used in determining V99 and V90. Also, because this censoring level is determined by the goodnessoffit test (9.5.4.7), the same censoring level is used for both T99 and T90. If the property that follows a threeparameter Weibull distribution represents a transformation, the lower tolerance bounds (T99, T90) computed by the above formulas must be transformed back to the original units in which the mechanical property is conventionally reported. 9.5.5.3 Nonparametric Procedure — This procedure should be used when a mechanicalproperty value is to be computed directly (not paired with another property for computational purposes) and the form of the distribution of population is unknown (not Pearson Type III or threeparameter Weibull). Distribution should not be considered unknown (1) if tests show it to be Pearson or threeparameter Weibull, (2) if it can be transformed to a Pearson or threeparameter Weibull distribution, or (3) if it can be separated into Pearson or threeparameter Weibull subpopulations. This procedure is applicable to Ftu and Fty. It may also be used for Fcy, Fsu, Fbru, and Fbry if sufficient quantity of data is available. Nonparametric (or distributionfree) data analysis assumes a random selection of test points and uses only the ranks of individual test points and the total number of test points. If test points have been deleted from a sample, the random basis is violated; consequently, this procedure must not be used when there is reason to suspect that the sample may have been censored. As an example, assume that a sample consists of 299 test points selected in a random manner. The test point having the lowest value has rank 1, the test point having the next lowest value has rank 2, etc. Thus, an array of ranked test points might appear as follows:
9103
MMPDS01 31 January 2003
Rank of Test Point
Value of Test Point, ksi
1 2 3 4 5 299
73.3 74.1 75.2 75.3 75.6 85.7
For each rank from a sample of size, n, it is possible to predict, with 0.95 confidence, the least fraction of population that exceeds the value of the test point having rank r. Since only two fractions, or probabilities, are of interest in determination of T99 and T90 values, only the ranks of test points having the probability and confidence of T99 and T90 values are presented in Table 9.10.9. To use this table with a sample size of 299, for example, one would designate the value of the lowest (r=1) test measurement as T99 and the 22nd lowest (r=22) test measurement as T90. For sample sizes between tabulated values, interpolation is permissible. For sample sizes smaller than 299, T99 is smaller than the value of the lowest point and cannot be determined in this manner. 9.5.6 DIRECT COMPUTATION BY REGRESSION ANALYSIS — This section describes the procedure used to determine design allowables by regression analysis if it has been determined that a significant representation relationship exists (see Section 9.5.1.2). Thus a dimensional parameter x (such as x=t, 1/t, etc., where t is thickness) has been determined to be related to the property being considered. 9.5.6.1 PERFORMING THE REGRESSION — The following steps must be performed prior to determining design allowables by regression analysis: (1) Express the property as a simple linear (or quadratic) function of the dimensional parameter and obtain estimates of the coefficient using the least squares regression procedure in Section 9.5.2.1 (or Section 9.5.2.2); for example TUS = a + bx or (SUS/TUS) = a + bx + cx2 where x is thickness or area and a, b, and c are constants from the least squares equation. (2) Determine the root mean square error of regression (sy). See 9.5.2.1(h) and 9.5.2.2(e). The direct computational procedure takes into account errors in the model estimates. If a linear relationship has been determined, compute T99 for Ftu at x = xo, using Equation [9.5.6.1(a)] T99 ' a % bx0 & kN99 sy
[ 9.5.6.1(a)]
where a, b, and sy are computed in the regression of TUS data, k´99 is (1%∆) /n times the 95th percentile of the noncentral t distribution with noncentrality parameter 2.326/ (1%∆) /n and n  2 degrees of freedom, and
9104
MMPDS01 31 January 2003
∆ '
xo & Σ x/n 2
Σ x & Σ x/n 2/n
.
[9.5.6.1(b)]
The equation for computing a T90 is similar with k´90 being used in place of k´99. k´90 is (1%∆) /n times the 95th percentile of the noncentral t distribution with noncentrality parameter 1.282/ (1%∆) /n and n  2 degrees of freedom, where ∆ is defined above. If calculation of the appropriate noncentral t percentile is not possible, the following approximations to k´99 and k´90 may be used: kN99 = 2.326 + exp{0.659  0.514 ln(n) + (0.481  1.42/n)ln(3.71 + ∆) + 6.58/n}
[ 9.5.6.1(c)]
kN90 = 1.282 + exp{0.595  0.508 ln(n) + (0.486  0.986/n)ln(1.82 + ∆) + 4.62/n}.
[ 9.5.6.1(d)]
These approximations are accurate to within 1.0 percent for n > 10 and ∆ < 10. The square root of ∆ is the number of standard deviations between xo and the arithmetic mean of the xvalues. Thus, a ∆ value of 10 would represent an extreme xo value, which is more than three standard deviations from the mean xvalue. If a quadratic relationship has been determined, calculate T99 for Ftu at x = xo using Equation [9.5.6.1(e)] 2
T99 ' a%bxo%cxo & t0.95, n&3,
2.326
Q sy
[ 9.5.6.1(e)]
Q
where a, b, c, sy, and Q are computed by quadratic regression, and the factor
t0.95,n&3, 2.326 Q
is the 95th
percentile of the noncentral t distribution with noncentrality parameter 2.326/ Q and n3 degrees of freedom. To calculate T90 in the presence of a quadratic relationship, use Equation 9.5.6.1(f) 2
T90 ' a%bxo%cxo & t0.95, n&3,
1.282
Q sy
[ 9.5.6.1(f)]
Q
where a, b, c, sy, and Q are computed by quadratic regression, and the factor
t0.95,n&3, 1.282 Q
is the 95th
percentile of the noncentral t distribution with noncentrality parameter 1.282/ Q and n3 degrees of freedom.* The procedures described above permit the determination of design allowables only for specific values of x. When it is desired to present a single allowable covering a range of product thickness (for example, 1.001 to 2.000inch plate), the lowest allowable for the range should be used. Thus, if TUS(LT) decreases continuously with increasing thickness, the TUS(LT) corresponding to x = 2.000 inches would be presented in MMPDS. If the decrease is large, a decrease in product thickness interval can be made: for example, by splitting the 1.001 to 2.000inch interval into two intervals of 1.001 to 1.500 and 1.501 to 2.000 inches.
* Note that critical values for the noncentral t distribution are not tabulated in MMPDS.
9105
MMPDS01 31 January 2003 9.5.7 INDIRECT COMPUTATION WITHOUT REGRESSION (REDUCED RATIOS/DERIVED PROPERTIES) — Ideally, it is desirable to determine Fcy, Fsu, Fbru, Fbry, as well as Ftu and Fty in other than specified test direction by direct computation as described in Sections 9.5.2, and, if sufficient quantity of data is available, direct computation procedures shall be used. Unfortunately, the cost of generating required data for these properties is usually prohibitive. Consequently, this section describes an indirect method of computation to determine the mechanical property values. A derived property is a mechanical property value determined by its relationship to an established tensile property (Ftu or Fty, A, B, or Sbasis). This indirect method of computation is applicable to Ftu and Fty in grain directions other than the specified testing direction, as delineated in the applicable material specification, and for all grain directions for Fcy, Fsu, Fbru, and Fbry. The procedure involves pairing of TUS, SUS, or BUS measurements with TUS measurements for which Ftu has been established or the pairing of TYS, CYS, and BYS measurements with TYS measurements for which Fty has been established. Average values for each lot shall be used when more than one measurement per lot is available. This technique is based on the premise that the mean ratio of paired observations representing related properties provides an estimate of the ratio of corresponding population means. The ratio consists of measurements of the property to be derived as the numerator and measurement of the established tensile property as the denominator. Thus, TUS or TYS in the specified testing direction always appears in the denominator of the ratio of observed values. The grain direction to be used for the denominator is the specified test direction as delineated in the applicable material specification. For most materials, routine quality control (certification) tests are usually conducted only in one grain direction even though the specification may contain mechanical property requirements for two or three grain directions. The typically specified or primary test directions for different product forms of each alloy system are shown in Table 9.2.3.2 and discussed in Section 9.5.7.1. Section 9.5.7.2 discusses the treatment of test specimen location. Section 9.5.7.3 discusses the treatment of clad plates, and Section 9.5.7.4 discusses the computation procedure for minimum design values. 9.5.7.1 Treatment of Grain Direction — Tensile allowables are usually listed according to grain direction in material specifications although some specifications do not indicate a grain direction, which implies isotropy. For MMPDS, it is recommended that tension allowables be shown for each grain direction. When the material is shown to be isotropic, then the same properties should be shown for each direction. Compression allowables are shown by grain direction similar to tension allowables. An example of computing compression allowables for heat treatable plate is shown below. The reduced ratio, R, for longitudinal grain direction, is determined from ratios, r, formed from paired observations for each lot of material, CYS(L)/TYS(LT). Although a longitudinal ratio is being obtained, the divisor is long transverse because this is the specified testing direction (refer to Table 9.2.3.2). The reduced ratio, R, for long transverse grain direction, is determined from ratios, r, formed from paired observations for each lot of material, CYS(LT)/TYS(LT). Similarly the reduced ratios, R, for short transverse grain direction, are determined from ratios, r, formed from paired observations for each lot of material, CYS(ST)/TYS(LT). The ratios, r, determined in the above manner are used in conjunction with Equation 9.5.7.4(b) to obtain a reduced ratio, R, for each grain direction. Equating the reduced ratios, design allowable values are determined from the resulting relationships,
9106
MMPDS01 31 January 2003 R '
or
similarly
and
Fcy(L) Fty(LT)
Fcy(L) ' RFty(LT) Fcy(LT) ' RFty(LT)
Fcy(ST) ' RFty(LT) .
Shear and bearing allowables are usually shown without reference to grain direction. These properties shall be analyzed according to grain direction, and design allowables shall be based on the lowest reduced ratio obtained for longitudinal, long transverse and short transverse (when applicable) directions. An exception is aluminum hand forgings for which shear values shall be presented according to grain direction. In computing the derived properties, paired ratios representing different grain directions shall not be combined in the determination of a reduced ratio. This is based on the premise that, if the ratio for two paired measurements is to provide an estimate of population mean ratio, then paired measurements must represent the same grain direction as that of the corresponding population means. For aluminum die forgings, the longitudinal grain direction is defined as orientations parallel, within ±15E, to the predominate grain flow. The long transverse grain direction is defined as perpendicular, within ±15E, to the longitudinal (predominate) grain direction and parallel, within ±15E, to the parting plane. (Both conditions must be met.) The short transverse grain direction is defined as perpendicular, within ±15E, to the longitudinal (predominate) grain direction and perpendicular, within ±15E, to the parting plane. (Both conditions must be met.) When possible, compression, bearing, and shear tests for three grain directions shall be conducted. 9.5.7.2 Treatment of Test Specimen Location — Testing specifications require a change in test specimen location from t/2 for #1.500 to t/4 for >1.500inch thickness for certain products. Although this change in specimen location may result in t/4 mechanical property ratios which are significantly different from t/2 ratios (different populations), as for aluminum plate, the t/2 and t/4 mechanical property ratios should be treated together for analysis to determine derived properties. 9.5.7.3 Treatment of Clad Aluminum Alloy Plate — For clad aluminum alloy plate, 0.500 inch and greater in thickness, tensile properties are determined using round tensile specimens; consequently, tensile properties represent core material. To present design values which represent the average tensile properties across the thickness of the clad plate, an adjustment must be made in the tensile yield and ultimate strength values (S or A and Bbasis), representing core strength, in the primary test direction(s). These strengths shall be reduced by a factor equal to twice the percentage of the nominal cladding thickness per side. These adjustments in the tensile yield and ultimate strengths shall be made prior to the computation of derived properties, except for short transverse properties. The following footnote, flagged to the appropriate thickness ranges, shall be incorporated into the design allowable table: “These values, except in the ST direction, have been adjusted to represent the average properties across the whole section, including X percent per side nominal cladding thickness.”
9107
MMPDS01 31 January 2003 9.5.7.4 Computational Procedure — Four basic steps are involved in determining design allowable properties by indirect computation: (1) (2) (3) (4)
Determine the ratios of paired observations for each lot of material. Compute the statistics, r and s, for the ratios of paired observations. Determine the lower confidence interval estimate (reduced ratio) for the mean ratio. Use the reduced ratio as the ratio of the derived to the established design allowable.
The ratio of two paired observations is obtained by dividing the measurement of the property to be derived [for example, CYS (LT) for heattreatable aluminum sheet] by the measurement for established tensile property [for example, TYS (LT)] in the specified testing direction. Equations for computing average and standard deviation of the ratios are the same as those in Appendix A. The ratio of the two population means [for CYS (LT) and TYS (LT), respectively] is expected to exceed the lower confidence limit defined as r & t1 & αs/ n
[ 9.5.7.4(a)]
where n r s t1&α
is the number of ratios is the average of n ratios is the standard deviation of the ratios is the 1α fractile of the t distribution for n  1 degrees of freedom. At the risk level of α = 0.05, the appropriate t value is t0.95.
Since the lower confidence interval estimate is used as the ratio between the design allowable properties, the reduced ratio, R, may be defined as R ' r & t0.95 s/ n .
[ 9.5.7.4(b)]
Values of t0.95 for various degrees of freedom, n  1, are tabulated in Table 9.10.4. The reduced ratio may now be used to establish the design allowable for the property to be derived using the example of aluminum sheet, R '
Fcy(LT) Fty(LT)
'
allowable to be derived . established allowable in specified test direction
The derived allowable property is computed by cross multiplying: Fcy (LT) = R Fty (LT) . The basis (A, B, or S), defined in Section 9.1.6, for computed or derived property is assumed to be the same as the basis for Fty or Ftu tensile property in the righthand side of the equation. If only the Sbasis (integer) properties are available to compute the derived properties, these values must be used. However, the unrounded Sbasis Fty or Ftu values computed with the method in Section 9.4 must be used to compute the derived properties if there are 100 or more observations representing 10 heats, casts, or melts; this will ensure the proper statistical confidence in the derived values. The lower of either the Sbasis value computed from Section 9.4 or the T99 value must be used to compute the Abasis derived properties.
9108
MMPDS01 31 January 2003 In a sample of ratios for a given product, effect of thickness on the ratio should be examined. If there is no effect of thickness, ratios for the various thicknesses can be pooled to compute the average and reduced ratio. If there is an effect of thickness, then a regression with thickness should be computed and the average and reduced ratios determined from the regression. See Section 9.5.8 for procedure. 9.5.8 INDIRECT COMPUTATION USING REGRESSION — Regression may also be used to determine reduced ratios when an allowable for a property, such as SUS, is computed indirectly from an already established allowable for TUS. The following assumptions are inherent to the reduced ratio procedure: (1)
The two properties must be distributed according to a bivariate normal distribution.
(2)
The coefficient of variation must be the same for the two properties within particular bounds.
(3)
The average of the ratio of the two properties must be well described by a linear function of the independent variable.
It is also important that paired data be available over the entire range of the dimensional parameter for which there is data for the direct property (TUS). Note that the confidence level associated with allowables computed using the reduced ratio technique may be somewhat below 95 percent. To compute the reduced ratio at x = xo’ in the case of linear regression, use Equation [9.5.8(a)],
Reduced Ratio ' a % bx0 & t0.95,n&2 sy
1%∆ n
[9.5.8(a)]
where ∆ is defined in Equation 9.5.6.1(b), a, b, and sy are computed in the regression of SUS/TUS data (discussed in Section 9.5.6.1), and t.95,n2 is selected from Table 9.10.4 corresponding to n2 degrees of freedom. The allowable for Fsu at xo is then computed as the product of the reduced ratio and the established allowable for Ftu: Fsu = (Reduced Ratio)(Ftu) . To compute the reduced ratio at x = xo’ in the case of quadratic regression, use Equation [ 9.5.8(b)], 2
Reduced Ratio ' a % bxo % cxo & t0.95,n&3 sy Q
[9.5.8(b)]
where a, b, c, sy, and Q are computed in the quadratic regression of SUS/TUS data (discussed in Section 9.5.6.1), and t.95,n3 is selected from Table 9.10.3 corresponding to n3 degrees of freedom. The allowable for Fsu at xo is then computed as the product of the reduced ratio and the established allowable for Ftu: Fsu = (Reduced Ratio)(Ftu) .
9109
MMPDS01 31 January 2003
9.6
ANALYSIS PROCEDURES FOR DYNAMIC AND TIME DEPENDENT PROPERTIES
9.6.1 LOAD AND STRAIN CONTROL FATIGUE DATA — Fatigue has been defined as “the process of progressive localized permanent structural change occurring in a material subjected to conditions that produce fluctuating stresses and strains at some point or points, and which may culminate in cracks or complete fracture after a sufficient number of fluctuations.” For many years, tests have been performed on specimens having simple geometries in attempts to characterize the fatigue properties of particular materials. Fatigue tests have been conducted for many reasons. Basic fatiguelife information may be desired for design purposes, or to evaluate the differences between materials. The effects of heat treatments, mechanical working, or material orientation may also be studied through comparative fatigue testing. Many types of machines and specimen designs have been used to develop fatigue data. Machine types include mechanical, electromechanical, hydraulic, and ultrasonic. Specimens have been designed for testing in cyclic tension and/or compression, bending, and torsion. Cyclic loading conditions have been produced by rotating bending, axial loading and cantilever bending. In and outofphase biaxial and multiaxial fatigue conditions have also been examined using specially designed specimens. Tests have been conducted in a variety of simulated environments including temperatures ranging from cryogenic to near melting point levels. The fatigue data included in MMPDS are limited to constantamplitude axial fatigue data on simple laboratory specimens tested according to ASTM E 606. Data obtained under both strain control and load (stress) control are included. Figure 9.6.1(a) shows examples of trends for stresslife and strainlife fatigue data. Generally, stresslife data for unnotched specimens are limited to stress levels that produce intermediatetolong fatigue lives because of unstable cyclic creep and tensile failure that can occur at high stress ratios in loadcontrol testing. This phenomenon is shown in Figure 9.6.1(b). Strainlife curves are often focused on strain ranges that produce shorttointermediate fatigue lives because of strain rate and frequency limitations which require long testing times to generate longlife fatigue data under strain control. However, there is no inherent limit to the life range that can be evaluated in straincontrol testing. For fatigue to occur, a material must undergo cyclic plasticity, at least on a localized level. The relationship between total strain, plastic strain, and elastic strain is shown in Figure 9.6.1(c). Lowcycle fatigue tests involve relatively high levels of cyclic plasticity. Intermediatelife fatigue tests usually involve plastic strains of the same order as the elastic strains. Longlife fatigue tests normally involve very low levels of cyclic plasticity. These trends are shown in Figure 9.6.1(d). In the MMPDS fatigue analysis guidelines, engineering strain is denoted as e and true or local strain is denoted as ε. These symbols are used interchangeably within MMPDS for small strain values. The limited plasticity involved in intermediate and longlife fatigue tests often results in a similar stressstrain response for both fully reversed straincontrol and fully reversed loadcontrol tests. A fatigue test, under strain control that produces a stable maximum stress of X, should produce (on the average) a fatigue life that is comparable to that obtained for a sample tested under load control at a maximum stress of X. Strictly speaking, the results are likely to be most comparable in terms of crack initiation life and not total life. If the comparison is made in terms of total life, the loadcontrol results will tend to be more conservative than those generated by straincontrol testing. When a specimen cracks in a test under strain control, it will usually display a decrease in maximum tensile load. Under load control, the maximum tensile load will remain constant but stress will increase as the crack grows, resulting in a shorter period of crack growth before the specimen fails.
9110
MMPDS01 31 January 2003
Figure 9.6.1(a). Examples of stresslife and strainlife fatigue trends.
9111
MMPDS01 31 January 2003
Figure 9.6.1(b). Example of cyclic creep phenomenon that can occur in a load control test with a high tensile mean stress [Reference 9.6.1].
Figure 9.6.1(c). A typical hysteresis loop for a material tested in fatigue under strain control illustrating the relationship between stress and strain parameters.
9112
MMPDS01 31 January 2003
Figure 9.6.1(d). An example of a strainlife fatigue curve and the stressstrain response at short, intermediate, and long fatigue lives.
A number of factors can significantly influence fatigue properties for a particular material—whether the data are developed under load or under strain control. The surface condition (such as surface roughness) of the test specimens is an important factor. The methods used for fabricating the specimens are also important—principally because such methods influence the state of surface residual stresses and residual stress profiles. Other factors such as mean stress or strain, specimen geometry (including notch type), heat treatment, environment, frequency and temperature can also be significant variables. In MMPDS, fatigue data are always presented in separate displays for different theoretical stress concentration factors. However, data sets may be presented for various combinations of variables if preliminary analyses indicate that the data sets are compatible. In any case, it is very important to fully document both the input data and their resulting illustrations in MMPDS with regard to variables that can influence fatigue. The selection of the specific procedures and methods that are outlined in this guideline for fatigue data presentation should not be construed as an endorsement of these procedures and methods for life prediction of components. The selection was made for consistency in data presentation only. For the purpose of life prediction, other methods and models are also commonly employed. Depending on the material, component and loading history, other models may be more appropriate for the particular situation. It is beyond the scope of these guidelines to make recommendations with respect to a specific life prediction methodology (e.g., the construction of design allowable fatigue curves). 9.6.1.1 Data Collection and Interpretation — If a set of strain or loadcontrol data for a material of interest meet the minimum requirements, the data should be processed for analysis. Loadcontrol data reports should clearly specify the net section stresses, stress ratios, and associated cycles to failure. Straincontrol data reports should clearly specify the strain levels used, the stable stress response values, and the associated cycles to initiation and/or failure, along with a clear and concise definition of the failure criterion. Acceptable definitions of failure in a straincontrol fatigue test report include: (1)
Total specimen separation
9113
MMPDS01 31 January 2003 (2)
Decrease of 50 percent in the maximum or stabilized tensile load value.
Acceptable definitions of crack initiation in a straincontrol fatigue test report include: (1)
First significant deviation from the stabilized load range or a stabilized rateofchange of the load range. Detection reliability is dependent upon the sensitivity of the monitoring equipment and consequently values as small as 1 to 5 percent are used in some cases, while values as great as 10 to 20 percent are used in other cases.
(2)
Verifiable results from a calibrated nondestructive inspection device, such as an electrical potential drop system.
The definition of crack initiation or failure used in a particular study must be clearly and quantitatively documented. Correlative information that is important for load or straincontrol test data includes detailed specimen dimensions, fabrication procedures (and their sequence), surface finish, product form, environment, frequency, waveform, surface residual stresses, and temperature. Other useful information includes average material tensile properties, product dimensions, and manufacturer. All fatigue data that are not listed as invalid by the author of the test report will be prepared for analysis, except for specimens tested at a maximum stress level greater than the average tensile ultimate strength of the material. The identity of different sources should be retained to determine whether combinations of data are appropriate. If all conditions from the different sources are virtually identical, the data should be analyzed together. Data should be identified as invalid if defects in specimen preparation or testing procedures are discovered. Runouts should be designated differently from failure data, since runouts are given special consideration in the regression analysis used to define mean fatigue curves. Runouts are generally defined as tests that have accumulated some predetermined number of cycles and have been subsequently stopped to reduce test time. Tests which have been stopped due to distinct problems encountered during testing are termed interrupted tests. Typical problems include power failures, temperature deviations, and load spikes. Interrupted tests are generally valid up until time at which the problem occurred. In this context, interrupted tests are treated the same as runouts in determining the mean fatiguelife trends of a data collection. However, if the interruption occurs long before expected failure of the specimen, the information contributed by the interrupted test is minimal, and the data point should be discarded. Data from specimens which exhibit failures outside of the gage section may, in certain circumstances, be included in the analysis and treated as interrupted tests. Failures occurring just outside the gage section are essentially normal failures and should be included for analysis. In straincontrol tests, however, the crack initiation is not sensed by the extensometer. Failures at threads, shoulders, or button heads may be indicative of a problem with the specimen design or test procedure. Straincontrol fatigue data must be accompanied by sufficient information to construct a cyclic stressstrain curve. The cyclic stressstrain curve may be established based on incremental stressstrain results or multiple specimen data for which stable stress amplitudes are defined for the complete range of strain ranges. The method used to define the cyclic stressstrain curve must be recorded so that it can be included in the correlative information along with the strainlife fatigue data displays. 9.6.1.2 Analysis of Data — Once a collection of data is reviewed (see Section 9.6.1.1) and compiled for the material of interest, analysis of that data may begin. An outline of the analysis procedure that is normally followed is given in Figure 9.6.1.2. Each of the elements in the flow chart are discussed in the following sections.
9114
MMPDS01 31 January 2003 The same basic analysis procedure is used for strain and loadcontrol data except these data types are normally analyzed separately even if they represent the same material and product form. The only case where load and straincontrol data can be combined is the situation where some specimens have been switched from strain to loadcontrol testing. In this case, the load and straincontrol data may be analyzed on an equivalent strain basis. In all other cases, loadcontrol data should be analyzed on an equivalent stress basis. Loadcontrol data generated at different stress concentrations should always be analyzed separately. 9.6.1.3 Fatigue Life Models — To clarify the fatigue data trends for a specific stress or strain ratio, a linear regression model can be applied as follows: log(Ni or Nf) = A1 + A2 log(Smax or ∆ε).
[9.6.1.3(a)]
Note that fatigue life is specified as the dependent variable. The alternative approach, using stress or strain as the dependent variable, is sometimes used, but this procedure will not be employed in developing mean fatigue curves in MMPDS. The use of fatigue life or, more specifically, logarithm (base 10) of fatigue life as the dependent variable will be used since stress or strain is the controlled parameter in a fatigue experiment, and the resultant fatigue life is a random variable. If Equation 9.6.1.3(a) does not adequately describe longlife data trends, a nonlinear model (or a more complicated linear model) may be warranted. For example, longlife, loadcontrol data might be modeled by the nonlinear expression log Nj = A1 + A2(Smax  A3)
[9.6.1.3(a)]
or by the more complicated equation [Reference 9.6.1.3] log Nf = A1 + A2 log Smax + A3
logSmax % A4 .
[9.6.1.3(c)]
These more complex forms should only be employed in instances where they are warranted based on a distinct fatigue limit at long lives and when the simpler linear model was inadequate. Standard least squares regression analysis and the procedure for detecting outliers in Section 9.6.1.6 require that the variance be relatively constant at all fatigue life values. Traditionally, the logarithm of fatigue life is approximated by a normal distribution. However, the variability or scatter of fatigue life is generally not constant, but increases with increasing fatigue life. To ensure the reliable use of the outlier detection procedure, a weighting scheme designed to produce a more uniform distribution of residuals is suggested in Section 9.6.1.5.
9115
MMPDS01 31 January 2003 F at igue Lif e Models (Sec tion 9.6.1. 3)
Ev aluation of Mean St res s and Strain Ef f ec t s (Sec tion 9.6.1. 4)
Treat m ent of O utliers (Sec tion 9.6.1. 6)
Yes
R em ov e O utliers
Yes
O utliers D etec ted?
No
As s es s m ent of F atigue Lif e Model (Sec tion 9.6.1. 7)
O ther Models ?
No
I s Model Adequate?
No
Yes
Elim inate D ata f rom C ons iderat ion
D ata Set C om binat ion (Sec tion 9.6.1. 8)
R em ov e D ata Set
No
Is C om binat ion Valid
Yes
Treatm ent of R unouts (Sec tion 9.6.1. 9)
Tim e D ependent Ef f ec ts (Sec tion 9. 6.1.10)
Prepare D ata f or Pres entation (Sec tion 9.9.1)
Figure 9.6.1.2. Flow chart of general fatigue analysis procedure.
9116
MMPDS01 31 January 2003 9.6.1.4 Evaluation of Mean Stress and Strain Effects—Commonly, loadcontrolled fatigue data generated over a range of stress ratios can be represented by the following equivalent stressfatigue life formulation: log Nf = A1 + A2 log (Seq  A4)
[ 9.6.1.4(a)]
where 1&A3
A
Seq ' (∆S) 3(Smax)
A3
Seq ' Smax(1 & R)
The equivalent stress model (and the related equivalent strain model) are derived from Reference 9.6.1.4(a). Equation 9.6.1.4(a) is nonlinear in its general form and must, therefore, normally be optimized through use of a nonlinear regression package. However, the above equation can be solved through a linear analysis, if A3 and A4 are optimized through an iterative solution. The parameter A3 normally lies in the range of 0.30 to 0.70, while A4 represents, in essence, the fatigue limit stress. In cases where the optimum value of A4 is negative or insignificant, it should be omitted. Unnotched data, especially aluminum alloy data, can frequently be represented without using the nonlinear A4 term. Parameter optimization is discussed more thoroughly in Section 9.6.1.5. If A4 is zero or set equal to zero, Equation 9.6.1.4(a) becomes linear in log Smax and log (1R), and it can be written as follows: log Nf = A1 + A2 log Smax + B log (1R)
[ 9.6.1.4(b)]
where B = A2A3. Thus, if A4 is zero, then A3 = B/A2 Straincontrolled fatigue data generated over a range of strain ratios often can be consolidated by the following equivalent strain formulation: log Nf = A1 + A2 log (εeq  A4)
[ 9.6.1.4(c)]
where A
1&A3
εeq ' (∆ε) 3(Smax/E)
.
Note that Equation 9.6.1.4(c) is very similar in form to Equation 9.6.1.4(a). It is important to note, however, that the maximum stress value used in Equation 9.6.1.4(c) is not a controlled quantity. It is a measured quantity and its magnitude depends primarily on the amount of cyclic softening or hardening that occurs in combination with mean stress relaxation. Although Smax can be predicted with reasonable accuracy if the cyclic response of the material is well established, using the stable measured values of Smax, when analyzing straincontrol data for presentation in MMPDS, is preferred. The equivalent stress and strain approaches are very useful for computing mean fatigue life estimates for conditions intermediate to those for which the test data have been generated. Caution should be used, however, in making life predictions for stress/strain conditions beyond the range of those represented in the
9117
MMPDS01 31 January 2003 data base. Also, when only two stress/strain ratios are used in the equivalence formulation, fatigue life estimates at conditions other than those two ratios (either intermediate or beyond) may be unreliable. If the basic formulations just described do not realistically represent the data, alternative equivalent stress or strain formulations should be considered. Two formulations [References 9.6.1.4(b) and (c)], in particular, may apply in these specific instances where equivalent stress is defined as: Seq ' Sa % A3 Sm
[9.6.1.4(d)]
or A
Seq ' Sa % Sm 3
[9.6.1.4(e)]
and equivalent strain is defined as: εeq ' εa % A3 Sm/E
[9.6.1.4(f)]
or A3
εeq ' εa % (Sm/E)
[9.6.1.4(g)]
where Seq Sa εa
= equivalent stress = alternating stress = alternating strain
εeq Sm E
= equivalent strain = mean stress = elastic modulus (from each test result).
Other data consolidation parameters may also be used provided they do not violate other guideline requirements, and they can be proven adequate. Adequacy may be assessed by employing the procedures described in Section 9.6.1.7. To evaluate the adequacy of one equivalent stress or strain formulation compared to another, it is useful to construct a plot of residuals versus stress or strain identifying individual stress or strain ratios. In this way the usefulness of a given formulation for modeling stress or strain ratio effects is visually apparent. 9.6.1.5 Estimation of FatigueLife Model Parameters — The fatiguelife model parameters are estimated to obtain the bestfit S/N or ε/N curve for the data. The procedure used to determine the parameters includes a statistical method for adjusting the fatigue model for the nonconstant variance commonly observed in longlife fatigue data. The motivation for this adjustment is the fact that constant variance is an inherent assumption in least squares regression analysis. To estimate the parameters in Equation 9.6.1.4(a) or Equation 9.6.1.4(c) and adjust the model to incorporate nonuniform variance, the following sixstep procedure is performed.
9118
MMPDS01 31 January 2003 Step 1  Initial Parameter Estimates. If A4 is assumed to be zero, then a linear least squares regression analysis is performed to obtain the initial parameter estimates for A1, A2, and A3. If A4 is to be estimated from the data, a nonlinear least squares regression analysis is performed to obtain the initial parameter estimates for A1, A2, A3, and A4. Runout observations above the minimum equivalent stress (strain) at which a failure occurred should be included in the calculation of the initial parameter estimates and residuals. To facilitate convergence of the nonlinear least squares fit when A4 is to be estimated from the data, the following procedure may be used to obtain starting values. Set A3 equal to 0.5 and calculate equivalent stress (strain) values for each observation. Set A4 equal to onehalf the smallest equivalent stress (strain) not associated with a runout. Using these values of A3 and A4 as constants, obtain least squares estimates of A1 and A2 using a linear regression routine. Step 2  Fitting the Variability Model. The magnitude of the residuals from these fatiguelife models typically increases with decreasing stress or strain as illustrated in Figure 9.6.1.5(a). The residuals plotted are the observed log(life) values minus the predicted log(life) values.
Figure 9.6.1.5(a). Example plot showing increasing magnitude of residuals with decreasing stress/strain levels.
To evaluate the fatiguelife model for nonuniform variance, it is useful to construct a model to estimate the standard deviation of log(life) as a function of equivalent stress (strain). If there is nonuniform variance, such a model can then be used to perform a weighted regression to estimate the fatigue life model parameters where the weight for each observations inversely proportional to its estimated variance.
9119
MMPDS01 31 January 2003 The suggested standard deviation model is *R* 2/π
' σo % σ1
1 ' g Seq Seq
[9.6.1.5(a)]
or *R* 2/π
' σo % σ1
1 ' h εeq εeq
[9.6.1.5(b)]
where R (observed log(life) minus predicted log(life)) represents the residuals from the fatigue life model fitted in Step 1. This model assumes that the standard deviation of log(life) is a linear function of the reciprocal of equivalent stress (strain). The absolute values of the residuals are divided by 2/π so that g(Seq) or h(εeq) is an estimate of the standard deviation of log(life). The intercept, σo, and the slope, σ1, are first estimated by ordinary least squares. If the least squares estimate of σo is negative, σo should be set to zero and σ1 should be estimated by performing a least squares regression through the origin (no intercept term). A 90 percent confidence interval for σ1 should also be obtained. If the lower bound of the confidence interval for σ1 is positive, there is evidence of nonuniform variance and one should proceed to Step 3A. If the confidence interval for σ1 contains zero, there is no evidence of nonuniform variance and one should proceed to Step 3B. If the upper bound of the confidence interval for σ1 is negative, this indicates abnormal behavior requiring further examination of the data set before proceeding with the analysis. Figure 9.6.1.5(b) is a plot of the absolute values of the residuals from Figure 9.6.1.5(a) versus the reciprocal of equivalent stress. The slope and vertical intercept of the least squares line displayed in this plot are the estimated parameters σ1 and σo. Step 3A  Fitting the Weighted Fatigue Model. Adjust the fatigue model for nonconstant variance by dividing each term in the model by g(Seq) or h(εeq), the estimated standard deviation of the dependent regression variable. If the fourparameter fatigue model is being used, the adjusted model becomes log(N) 1 ' A1 g(Seq) g(Seq)
% A2
log(Seq &A4) g(Seq)
[9.6.1.5(c)]
or log(εeq & A4) log(N) 1 ' A1 % A2 g(εeq) g(εeq) g(εeq)
[9.6.1.5(d)]
where Seq and εeq are defined in Equations 9.6.1.4(a) and 9.6.1.4(c). Perform a nonlinear least squares regression analysis (no intercept) using the adjusted model to obtain new estimates of A1, A2, A3, and A4.
9120
MMPDS01 31 January 2003
Figure 9.6.1.5(b). Example plot showing the magnitude of the residuals versus the inverse of equivalent stress/strain levels.
When performing this regression, all runouts above the minimum Seq or εeq at which a failure occurred should be included in the analysis and treated as failures. The inclusion of runouts in this step should be determined based on equivalent stress (strain) values using the value of A3 estimated in Step 1. Assuming that the equivalent stress/strain model is valid, this qualifying stress/strain level allows the use of all runouts above stresses or strains at which failures have been observed. Below this level, there is no statistical evidence that discontinued tests would have failed. Therefore, runouts below the minimum Seq or εeq value at which a failure occurred are not assigned finite life values in estimating the parameters. It should be noted that the regression analysis performed using the adjusted model [Equation 9.6.1.5(c) or (d)] is equivalent to performing a weighted least squares regression analysis using the original fatigue life model [Equation 9.6.1.4(c)] and weights equal to 1/g2(Seq) or 1/g2(εeq). Also, it may be desirable in certain situations to fit alternative standard deviation models to the residuals from Step 1. In this case, simply redefine g(Seq) or g(εeq) to be equal to the desired model and follow Steps 1 through 3 above. Upon completion of Step 3A, proceed to Step 4. Step 3B  Fitting the Unweighted Fatigue Model. Using the initial estimate of A3 obtained in Step 1, calculate equivalent stress (strain) values for all observations including runouts. All runouts above the minimum equivalent stress (strain) at which a failure occurred should be included in the analysis and treated as failures. (See Step 3A for an explanation of this rationale.) Using the same regression techniques employed in Step 1, obtain least squares estimates of the parameters A1, A2, A3, and A4. Step 4  Testing the Significance of Model Parameters. Obtain a 90 percent confidence interval for A4. If the lower bound of the confidence interval is negative, there is no evidence that A4 is different from zero. In this case, assume A4 is equal to zero and repeat Step 3A or 3B, eliminating A4 from the model.
9121
MMPDS01 31 January 2003 Next, obtain a 90 percent confidence interval for A2. If the upper bound of the confidence interval is negative, this indicates that the relationship between log(life) and equivalent stress (strain) is significant. If the upper bound of the confidence interval is positive, there is no evidence of a significant relationship between log(life) and equivalent stress (strain) and the data set should be examined further before proceeding with the analysis. Step 5  Reestimating A1 and A2. If a weighted least squares analysis was performed in Step 3A, A1 and A2 should be reestimated to include the effect of the new value of A3 on the calculation of weights and the inclusion of runouts. First, recompute the weights g(Seq) or g(εeq) using the value of A3 obtained in Step 3A. Then perform a linear regression (no intercept) to obtain updated estimates of A1 and A2 in Equation 9.3.4.10(c) or (d) treating A3 as a constant. The inclusion of runouts in this linear regression should be determined based on equivalent stress (strain) values using the value of A3 obtained in Step 3A. Step 6  Estimating the Standard Deviation and Calculating Standardized Residuals. The method for estimating the “standard deviation of log(life)” (SD) depends on whether there is evidence of nonuniform variance in the fatigue life data. If an unweighted regression was performed in Step 3B to obtain the model parameters, SD should be set equal to the root mean square error (RMSE) associated with the fitted and unweighted fatigue life model. In this case, SD may be calculated as
j Ri /(n&k) n
SD ' RMSE '
2
[ 9.6.1.5(e)]
i ' 1
where k is the number of parameters estimated in Step 3, and Ì Ri ' log N i & log N i
[9.6.1.5(f)]
Ì
where Ri is the residual, log Ni is the logarithm of observed number of cycles, and log Ni is the logarithm of predicted number of cycles associated with the ith observation. If a weighted regression was performed in Step 3A to obtain the model parameters, SD should be reported as linear function of the reciprocal of equivalent stress (strain). This function should be obtained by multiplying the fitted standard deviation model g(Seq) or g(εeq) from Step 2 by the root mean square error (RMSE) associated with the fitted and weighted fatigue life model to obtain an updated standard deviation model. In this case, SD may be calculated as SD ' RMSE( σ0 % σ1/Seq
[9.6.1.5(g)]
SD ' RMSE( σ0 % σ1/εeq
[9.6.1.5(h)]
or
9122
MMPDS01 31 January 2003 where
RMSE ' j WRi /(n & k) , 2
[9.6.1.5(i)]
k is the number of parameters estimated in Step 3, and
WRi '
Ì log N i & log N i
[9.6.1.5(j)]
g Seq,i or εeq,i
with WRi denoting the weighted residual and Seq,i(εeq,i) the equivalent stress (strain) associated with the “ith” observation. As a final step associated with the estimation of fatigue life model parameters, standardized residuals should be calculated for use in the judging the appropriateness of the fitted model. Standardized residuals are calculated as SRi ' Ri/SD
[9.6.1.5(k)]
where the form of the residual Ri is given in Equation 9.6.1.5(f) and the estimated standard deviation SD is given by either Equation 9.6.1.5(e) or 9.6.1.5(h), (j) or (k). Figure 9.6.1.5(c) is a plot of the standardized residuals for the same data plotted in Figure 9.6.1.5(d) but based on a standard deviation model to correct the nonuniform variance. Note that the pattern of nonconstant variance has been eliminated.
Figure 9.6.1.5(c). Example plot showing constant variance of standardized residuals.
Note  When performing any of the regression analyses described above to estimate the parameters A1, A2, A3, and A4, the estimate of A4 should be restricted to be greater than or equal to zero. Some
9123
MMPDS01 31 January 2003 regression programs allow such restrictions as an option. If such an option is not available and if the estimate of A4 is negative, set A4 equal to zero and refit the model treating A4 as a constant. Also note that the parameter estimates obtained from the regression analysis of Step 3A or 3B need not necessarily be reported as the final parameter estimates. If the data set includes runout observations, final estimates of the A1 and A2 parameters may be calculated using the maximum likelihood techniques presented in Section 9.6.1.9, provided that software for performing this procedure is available. 9.6.1.6 Treatment of Outliers — An outlying observation (or outlier) is one that appears to deviate markedly from other observations in the sample in which it occurs. Outliers may essentially be classified into two groups: (1) An extreme value of the random variable inherent in the data (in this case fatigue life). If this is true, the value should be retained in future analyses. (2) An unusual result caused by a gross deviation in material or prescribed experimental procedure or an error in calculating or recording any experimental data. An outlier of the second type is sometimes correctable by a review of the test sample and/or test records, which may provide sufficient evidence for rejection of the observation. An outlying value from a failure that occurred in the fillet of an unnotched fatigue test sample is an example of a potentially rejectable result based on physical evidence alone. The more difficult case is one where an observation is an obvious outlier and no physical reasons can be identified to justify its exclusion. Assuming uniform variance in the standardized residuals over the complete range in equivalent stress or strain, the problem of identifying certain observations as potential outliers should be addressed as follows. Calculate the studentized residuals,
Ti '
SRi 1 & hi
RMSE RMSE(i)
1/2
[9.6.1.6(a)]
for i = 1, ..., n where SRi is the standardized residual from Equation 9.6.1.5(k), RMSE is the root mean square error based on the entire sample as calculated in either Equation 9.6.1.5(e) or Equation 9.6.1.5(i), and RMSE(i) is the root mean square error based on the sample which excludes the ith observation as calculated by either Equation 9.6.1.5(e) or Equation 9.6.1.5(i). The value hi is calculated using the formula X1i ' X2j & 2 X1iX2i ' X1jX2j % X2j ' X1j 2
hi '
2
2
' X1j ' X2j & ' X1jX2j 2
2
2
2
[9.6.1.6(b)]
where X1i is the value of 1/SD for the ith specimen, X2i is the value of log(SeqA4)/SD for the ith specimen and all summations are over j = 1, ..., n. Note that
9124
MMPDS01 31 January 2003 2
RMSE 2(i) '
n & k RMSE 2 & SR1 / l & hi (n & k &1)
[9.6.1.6(c)]
where RMSE is the root mean square error based on the entire sample as calculated in either Equation 9.6.1.5(e) or Equation 9.6.1.5(k) and k is the number of parameters estimated in Step 3 of Section 9.6.1.5. It can be shown that each Ti has a central t distribution with nk1 degrees of freedom. Applying the Bonferroni inequality [Reference 9.6.1.6] to obtain a conservative critical value leads to the following outlier test. Calculate the maximum absolute studentized residual
G ' max Ti
[9.6.1.6(d)]
and declare the data value corresponding to G to be an outlier if
G > t(α/2n, n & k & 1)
[9.6.1.6(e)]
where t(α/2n,nk1) is the upper α/2n percentile point of the central t distribution with nk1 degrees of freedom and α represents the significance level of the outlier test. Under the hypothesis that no outliers are present in the data, the probability is less than α that the data value corresponding to G will be falsely declared an outlier. In applying this test to fatigue life data, a significance level of α = 0.05 is used and the test is first applied to the entire sample. If an outlier is detected, the outlying observation is removed from the sample and the entire analysis is repeated on the smaller sample of n1 observations starting with Step 1 of Section 9.6.1.5. (When a nonlinear least squares fit is performed in Step 1, use the current estimates for A1, A2, A3, and A4 as starting values rather than following the starting value algorithm.) This process of removing outliers and repeating the analysis continues until no outliers are detected in the remaining sample. For straincontrol data, apply the procedure described above replacing Seq with εeq throughout. The data analyst may also wish to carry out the outlier test procedure using a significance level of α = 0.20 in order to identify additional observations that may warrant investigation. To identify even more suspect observations, a larger significance level may be used. Any data values identified by this procedure should be examined but retained in the data set unless physical evidence justifies their exclusion. 9.6.1.7 Assessment of the Fatigue Life Model — The fit of the fatigue model S/N curve to the data may be assessed in two ways—the adequacy of the equivalent stress/strain model and the adequacy of the fatigue life model. The equivalent stress model lack of fit test and the overall lack of fit test described below provide a reasonable assessment of the fatigue life model. When three or more stress (strain) ratios are used, the fit of the equivalent stress (strain) model may be tested by determining the relationship between the standardized residuals from Equation 9.6.1.5(k) and stress (strain) ratio. A difference in the means of the standardized residuals at each stress (strain) ratio indicates that the equivalent stress (strain) model is inadequate. To determine whether or not there is a statistically significant difference in the means of the standardized residuals at each stress (strain) ratio, an
9125
MMPDS01 31 January 2003 analysis of variance should be performed on the standardized residuals using stress (strain) ratio as the treatment variable. A statistical Ftest should be used to determine if the effect of stress ratio is significant at the 5 percent level [Reference 9.6.1.7]. The equivalent stress (strain) model should be considered inadequate when the effect of stress (strain) ratio is significant according to the statistical Ftest. The plot of the standardized residuals versus stress ratio shown in Figure 9.6.1.7(a) illustrates such a relationship between the standardized residuals and stress ratio. Since there would be no such relationship if the equivalent stress model were adequate, the plot indicates that the equivalent stress model must have been misspecified in this case. In addition to the lack of fit shown by differences in standardized residual means, other types of lack of fit could exist. Therefore, it would be prudent to examine stresslife plots in addition to performing the statistical test for lack of fit of the equivalent stress model.
Figure 9.6.1.7(a). Standardized residuals versus stress ratio.
If the equivalent stress (strain) model is inappropriate, then a new equivalent stress (strain) model should be selected. When a suitable stress (strain) model is not available, an alternative strategy is to present the data with best fit regression lines for each stress (strain) ratio. To be acceptable, each curve must meet minimum data requirements and satisfy significance checks as discussed in Section 9.6.1.5. This approach is less desirable than the equivalent stress (strain) modeling approach because it requires the estimation of fatigue trends using a graphical technique for intermediate conditions where no data exist. It should, therefore, be used only in cases where significant fatigue data collections cannot be handled by standard procedures. Once an equivalent stress (strain) model has been found that describes the general fatigue data trends for all stress (strain) ratios, an overall test of the fit of the fatigue model should be performed. The stresslife plot shown in Figure 9.6.1.7(b) is characteristic of an overall lack of fit. To identify such a lack of fit, the DurbinWatson test may be used [Reference 9.6.1.7]. The statistic D should be computed according to the formula
9126
MMPDS01 31 January 2003 j n
Di '
i ' 2
SRi & SRi & 1 2 j n
i ' 1
[9.6.1.7(a)] 2 SRi
where SRi is the ith standardized residual [Equation 9.6.1.5(k)] ordered by increasing values of equivalent stress(strain). If D < 2 & 4.73/n 0.555
[9.6.1.7(b)]
conclude that there is a significant lack of fit at the 5 percent significance level. This equation was derived from the conservative critical value (dL) reported in Table A.6 of Montgomery and Peck [Reference 9.6.1.7]. When an overall lack of fit is determined from this test, the modeling procedure should be repeated with a more appropriate fatigue model.
Figure 9.6.1.7(b). Stresslife plot showing lack of fit.
9.6.1.8 Data Set Combination — In many cases, data from different sources, orientations, etc., may need to be combined for analysis. When data set combinations of this sort are performed, the validity of the combination should be tested with the method described below. The test is similar to that used to determine the adequacy of the equivalent stress (strain) model in the previous section.
9127
MMPDS01 31 January 2003 If there is a relationship between the standardized residuals from Equation 9.6.1.5(k) and the data set from which they were obtained, such as that shown in Figure 9.6.1.8, then the data sets should normally not be combined. To determine whether or not the mean of the standardized residuals is significantly different for any of the data sets, an analysis of variance should be performed on the standardized residuals using data set as the treatment variable. The analysis of variance Ftest should be used to determine if the combined data sets are significantly different at the 5 percent level. When the data sets are found to be significantly different, at least one of the data sets should normally be removed from the data set combination. In this situation, the data analyst may wish to apply a standard multiple comparison procedure to the standardized residual data to determine which standardized residual means are significantly different from the others. For a discussion of standard multiple comparison procedures, see pages 185201 of Winer [Reference 9.6.1.8]. There may be situations where differences between data sets are found to be statistically significant, yet these differences are so small as to be unimportant from an engineering standpoint. If a particular analysis reveals such a case, exceptions may be taken, if clearly noted and explained in the fatigue data proposal.
Figure 9.6.1.8. Standardized residual plot showing different mean trends between data sets.
9.6.1.9 Treatment of Runouts — It is difficult to incorporate information from runouts (or interrupted tests) when using the least squares criterion to fit fatigue life models to data since the failure times for these observations are not known. The runouts must be either ignored or treated as failures and neither of these alternatives adequately incorporates the information contained in the runout observations. Both of these approaches tend to produce smaller predicted lives at a given equivalent stress (strain) value than is appropriate. The treatment of runouts presented below is more appropriate but requires that two of the fatigue
9128
MMPDS01 31 January 2003 life model parameters be estimated by maximum likelihood techniques rather than by least squares procedures. The maximum likelihood procedure is employed to obtain new estimates for the parameters A1 and A2 in Equation 9.6.1.4(a) or 9.6.1.4(c). For the purpose of this analysis, fatigue life (cycles to failure) is assumed to be log normally distributed and the parameters A3 and A4 are considered to be constants which are equal to the values obtained using the procedures of Section 9.6.1.5. The estimated values of A1 and A2 obtained previously are used as initial values. The maximum likelihood procedure then determines the values of A1 and A2 which maximize the loglikelihood function L A1,A2,σ ' j n
1 & di [log f w i /σ % di log S w i
i ' 1
[9.6.1.9(a)]
where f (w) '
1
exp
&
2π
w2 2
[9.6.1.9(b)]
is the standard normal density function, 4
S(w) '
m
f(t) dt
[9.6.1.9(c)]
w
is the survival function for the standard normal distribution, di is equal to 1 if the ith observation is a runout and zero otherwise, σ is a scale parameter to be estimated, and
wi '
log Seq & A4 log(N) 1 & A1 & A2 SD SD SD
[9.6.1.9(d)]
where N is the cycles to failure and SD is the standard deviation for the ith observation as calculated from Equation 9.6.1.5(e) or Equation 9.6.1.5(h). For more information on the maximum likelihood procedure, see Reference 9.6.1.9(a). For use in standard data analysis, the maximum likelihood procedure is conveniently implemented in some statistical software packages such as SAS [see Reference 9.6.1.9(b)]. When runouts are present, the fitted curve produced by maximum likelihood will generally predict longer average cycles to failure at given equivalent stress (strain) values than the fitted curve produced by least squares. Although it would be desirable to update all of the parameters in the fatigue model with
9129
MMPDS01 31 January 2003 maximum likelihood, algorithms to perform maximum likelihood on nonlinear models are not readily available. For this reason, the least squares estimates of the parameters A3 and A4 must be used. 9.6.1.10 Recognition of Time Dependent Effects — All prior discussion has been based on the assumption that time dependent effects in the fatigue data sample of interest are negligible. When dealing with elevated temperature fatigue properties of materials (or room temperature fatigue properties in a corrosive environment, for example), this assumption may not be realistic. Analysis methods that are approved for use in MMPDS do not account for timedependent effects. Therefore, every effort must be made to identify data that embody significant timedependent effects. There are no absolute methods presently available for sensing timedependent effects in fatigue data; however, there are some useful approximation techniques. One of the more useful approaches applied to “suspect” data is to include timedependent terms in the regression model. If the terms are significant, there is reason to believe that the population contains time dependent data. Subdividing the data into subsets that do not show time dependent effect may be possible. If this is not possible, the data set should either be rejected or included with a disclaimer restricting usage of the data to predict performance at other frequencies or temperatures. One other possible indicator of time dependent effects is an abnormal equivalent stress (strain) model. If data for different stress or strain ratios do not fit the customary models (as described in Section 9.6.1.4), or abnormal optimum parameters are defined the problem may be caused by time dependent effects. In the case of the primary equivalent stress (strain) formulation equation the exponent normally is between zero and one. If the A3 exponent approaches or exceeds one, the influence of maximum stress on fatigue life is negligible. This is a very unusual result that usually indicates problems with the data sample. The problem may result from mixed sources, where the data from each source were generated at different stress (strain) ratios. Rejection of such data sets is discussed in Section 9.6.1.8. In the case of the primary equivalent stress model [Equation 9.6.1.4(a)], if the exponent (A3) approaches or is less than zero, it indicates the influence of maximum stress on fatigue life is “too strong”. This result implies that creep is affecting the data. If data are available for a material at a range of different temperatures it may be possible to analyze these sets separately and make comparisons between bestfit mean trend lines for increasing temperatures. If the different mean trend lines are not consistent with the highertemperature curves converging or diverging from the lowertemperature curves, there is probably a significant timedependent effect in the data. The suspect data should either be excluded or included with a disclaimer as previously cited. If data are excluded for timedependent effects, the preliminary analyses of those data should be included in the data proposal and reasons for their exclusion should be given. 9.6.2 FATIGUE CRACK GROWTH DATA — Fatiguecrackpropagation data, recorded in the form of cracklength measurements and cycle counts (ai, Ni) can be presented as crackgrowth curve drawn through the data points as shown in Figure 9.6.2(a). Although data presented in this form indicate general trends, they are not generally useful for design purposes since a variety of stress levels, stress ratios, initial crack conditions, and environmental conditions are encountered. It has been found convenient to model fatiguecrackpropagation damage behavior as rate process and formulate a dependent variable based on the slope of this growth curve, or an approximation to it, namely,
da ∆a • dN ∆N
9130
[ 9.6.2(a)]
MMPDS01 31 January 2003 Results obtained from the theory of linear elastic fracture mechanics have suggested that rate process at the crack tip might be represented as a function of a stressintensity factor, K, which, in general form, may be written as K ' S a g(a,w) ,
[9.6.2(b)]
where g(a,w) is a geometric scaling function dependent on crack and specimen geometry, and S is nominal stress. As a result, the independent variable is usually considered as some function of K. At present, in MMPDS the independent variable is considered to be simply the range of the stress intensity factor, ∆K, and data are considered to be parametric on the stress ratio, R, such that da/dN . ∆a/∆N ' g(∆K,R) ,
[ 9.6.2(c)]
where ∆K = Kmax  Kmin. Values of maximum and minimum stress intensity factors, Kmax and Kmin, respectively, are computed with Equation 9.6.2(b) using respective maximum and minimum cyclic stresses. A crack growth rate curve, as shown in Figure 9.6.2(b), is obtained by plotting the locus of points (da/dN, ∆K) derived from the crackgrowth curve [see Figure 9.6.2(a)] at selected values of crack length, a. Crackgrowthrate curves are generally plotted on loglog coordinates. Within the general curve shape described above, systematic variations in data point locations are observed. When data from tests conducted at several different stress ratios are present, the plot of crackgrowth rate versus stressintensityfactor range will be layered into distinct bands. Layering of data points may also occur as a result of variation in such parameters as test frequency, environment, temperature, and specimen grain direction. 9.6.2.1 Data Collection and Interpretation — Reporting of basic crackgrowth data shall be as complete as possible. In addition to reporting cyclic loading conditions, such as maximum cyclic load and/or stress levels, stress ratio, test frequency, and specimen dimensions, it is particularly important to identify environmental conditions associated with the tests. The number of specimens and number of respective heats should also be identified. Table 9.9.2 serves as an example of the type of information which should be available (or at least is desirable) for each collection of FCP data.
9131
MMPDS01 31 January 2003
Figure 9.6.2(a). Crackgrowth curve.
Figure 9.6.2(b). Crackgrowthrate curve.
9132
MMPDS01 31 January 2003 9.6.3 FRACTURE TOUGHNESS DATA — Fracture toughness of a material is its ability to resist flaw propagation and fracture. This characteristic is a generic quality, somewhat elusive to assess quantitatively. Of several measures of fracture toughness which have evolved for appraising the sensitivity of metals to the presence of small flaws, those based on crack stress or strain analysis appear to be more meaningful for use in design applications. Significant quantification of fracture and flaw propagation behavior of highstrength metals has been achieved through the concept of stress intensity factors. Typical roomtemperature values and effectoftemperature curves for critical stress intensity factors are presented in MMPDS for “information only” where data are available. Basic concepts, testing considerations, and interpretations of fracture toughness are briefly described in the following subsections. A primary factor in fracture behavior of a material is stress state, i.e., planestress or planestrain. In accord with previous definitions, these stress states may be interpreted mechanically as a size or thickness effect within the material. The ideal planestress condition occurs in the twodimensional (σz = 0) case, in which all stresses are restricted to one plane. Typically material loaded in planestress can accommodate extensive plastic deformation adjacent to the flaw prior to fracture, and at fracture exhibit a relatively high K value, as computed by a relationship such as Equation 9.6.2. At the opposite extreme is the ideal planestrain case, in which the third dimension is essentially infinite so that bulk restraint of the material permits no outofplane strains. As a result, plastic deformation is restricted and the material fractures in a nearly elastic manner at a relatively low K value. In real materials, these ideal extremes can be closely approximated by “quasi” conditions of “thin” and “thick” bodies. Variation in stress intensity at fracture over these extremes, and the transition stage between, may be represented as shown previously in Figure 9.2.3.5.3(a). 9.6.3.1 PlaneStrain Fracture Toughness Data — For materials which are inherently brittle, or for structures and flaw configurations which are in triaxial tension due to their thickness or bulk restraint, quasiplanestrainstress conditions can be obtained in a finitesized structural element. Triaxial stress state implicit to plane strain effectively embrittles the material by providing maximum restraint against plastic deformation. In this condition, component behavior is essentially elastic until fracture stress is reached and is readily amenable to analysis in terms of elastic fracture mechanics. This mode of fracture is frequently characteristic of the very high strength metals. 9.6.3.1.1 Data Collection and Interpretation — While a wide variety of fracture specimens are available for specified testing objectives, the notchbend specimen and compact specimen generally offer the greatest convenience and material economics for testing. Details of recommended testing practice are presented in ASTM E399. 9.6.3.2 Plane Stress and Transitional Fracture Toughness — It is convenient to consider critical stressintensity factor values, varying with thickness or stress state, as indices of crackdamage resistance. The stressintensity factor can be used as a consistent measure of crack damage, not only for fracture instability, but also for other levels of crack damage severity, provided the damage is consistently specified and detected. This concept implies that planestress and transitionalfracture toughness of metallic materials, while not necessarily a fixed value for the material, is a characteristic value for a given product form, thickness, grain direction, temperature, and strain rate. 9.6.3.2.1 Data Collection and Interpretation — Because of the complexity of crack behavior in planestress and transitionalstress states, test methods for evaluating material toughness have not been completely standardized; however, several useful methods do exist. Although each configuration generates nearly consistent results when data are properly evaluated, it is recommended that each general flaw configuration be interpreted and applied within its own design context.
9133
MMPDS01 31 January 2003 Middle Tension Panels — Because it simulates typical crack conditions in thinsheet structures, the middle tension panel is a popular testing configuration for evaluating crack behavior. This specimen was illustrated earlier in Figure.9.2.3.5.3(b). The cracktip plasticity and slowstable growth of the crack which commonly occur with planestress or transitional stress state conditions may cause a deviation from abrupt fracture, which is normally associated with crack extension under ideal plane conditions, as illustrated earlier in Figure 9.2.3.5.3(c). Two limiting damage levels are noted in this figure. Point O is the threshold or onset of slow, stable tear where the crack slowly extends after reaching a threshold stress level. Point C is fracture instability. Both levels of crack damage can be associated with a different stress intensity factor, or damage index, for product forms and thicknesses of interest. These damage levels can be identified either directly with the K value as determined from instantaneous stresscrack length coordinate dimensions at these points, or approximately by the coordinates of Point A, which is residual strength, or apparent toughness concept of relating initial crack length to final fracture stress. The stress intensity factor, K, associated with any of these damage levels is determined from Equation 9.6.2(b) where, for this configuration, a = halflength of centerthrough crack g(a,w) = (π sec πa/W)½. The locus of data points can be represented by a parametric stressintensity factor curve, as shown in Figure 9.2.3.5.3(d), where each curve represents a different stressintensity factor formulation. The slow growth curve is superimposed on this figure to illustrate the general relationship between the threshold of stable crack extension, apparent instability, and fracture instability for a typical crack. Because of experimental difficulties associated with precise detection of threshold and instability points, points O and C, apparent toughness, or residual strength concept of crack damage is used in this presentation. This is the locus of data points “A”, noted earlier in Figure 9.2.3.5.3(d), which determine apparent fracture toughness. Kapp ' fc πao secπao/W
1 2
.
[ 9.6.3.2.1]
See Reference 9.2.3.5.3 for additional information. 9.6.3.2.2 Analysis of Data — Since precise definitions of damage mechanisms and their associated instability conditions have not been devised for crack behavior in planestress and transitional stress states, only general constraints can be suggested for screening data. To assure that crack damage or fracture instability occurs under predominantly linear elastic conditions the basic criterion is that net section stress must be less than 80 percent of tensile yield strength, TYS, actually representative of that material. Additional criteria may be imposed by stress and boundary constraints characteristic to specific specimen configurations. Middle Tension Panels — To maintain consistency with the Damage Tolerant Design Handbook [Reference 9.6.3.2.2], a related damage tolerance data document for Air Force contractors, a singular criterion, fc # 0.8 (TYS) (1  2a/W)
9134
[9.6.3.2.2]
MMPDS01 31 January 2003 corresponding to the above net section stress requirement, is imposed on fracture data from middle tension panels. Data which satisfy this criterion are used with Equation 9.6.3.2.1 to define apparent fracture toughness. The validity of elastic fracture in a given set of data may also be substantiated by additional tests conducted to demonstrate that elastic fracture conditions have been achieved and that the associated K value is nearly constant. For example, once a tentative value of Kapp has been determined, it can be confirmed by testing additional panels of larger width (at least 50 percent larger) with the same initial crack length, or by testing the same panel width containing a smaller initial crack length (approximately twothirds of the previous). These additional Kapp values must confirm to the original tentative value. In any case, it is recommended that tests can be conducted at a variety of crack lengths and panel widths whenever practical to obtain a more complete characterization of panel behavior. 9.6.4 CREEP AND CREEPRUPTURE DATA — Creep is defined as timedependent deformation of a material under an applied load. It is usually regarded as an elevated temperature phenomenon, although some materials creep at room temperature. If permitted to continue indefinitely, creep terminates in rupture. (First stage or logarithmic creep exhibited by many materials at lower temperatures is not the subject of this section.) Creep in service usually occurs under varying conditions of temperature and complex (multiaxial) stress, leading to an infinite number of stresstemperaturetime combinations. Creep data for use in general design are usually obtained under conditions of constant uniform temperature and uniaxial stress. This type of data is the subject of this section. 9.6.4.1 Data Collection and Interpretation — After a desired group of creep and/or creeprupture data have been experimentally developed or isolated in preproduction files, it is necessary to carefully collect and interpret these data in accordance with the following guidelines: Stateoftheart for interpreting these types of creep and rupture data requires that a certain amount of judgment be allowed. The general approach will be to optimize one of several empirical equations that best follows the trend of data, using life (or time) as the dependent variable. Independent variables will include stress and temperature for rupture and isostrain creep curves, and will also include strain for isostrain creep curves. Rupture ductility can be an exception to the above because of complex behavior and data scatter. At least a cautionary note should be given in the introductory material on times and temperatures included in rupture data. Some materials exhibit such low elongation in certain timetemperature regions that normal, reasonable values of design creep strain cannot be achieved without risk of fracture. Interpretation of creep and rupture data should also include variables that are reflected in background data reporting requirements (discussed in the next subsection). Depending on the information content of the data, and the type of variable, it may be desirable to develop a series of equations, or to include additional physical variables in the regression analysis. The proposal should demonstrate that these additional variables have been evaluated and appropriately treated in the analysis. The individual interpreting the data should also take note of the following special types of data, and consider the following recommendations on their use: Specification Data—Virtually all alloys used for hightemperature applications are controlled and purchased by a process control variable generally called “spec point”. Therefore, there will often be large quantities of data available from quality control data records at the specification condition. Data will contain many heats, and serve as an excellent measurement source of scatter. Therefore, in regression modeling, specification data are often the major source of scatter measurements. Slope measurements must come from the experimental design matrix.
9135
MMPDS01 31 January 2003 Specification data can also be used to (1) determine, through analysisofvariance techniques, fractions of scatter due to heattoheat variations, etc., (2) determine, through distribution analysis, if data are normal, log normal, etc., and (3) find out, if data are not normal, what transformation is required. Outliers—These can be excluded only if tests are demonstrably invalid, or if the effect on the equation and statistical parameters is unreasonable. Since exclusion of outliers normally involves a certain degree of judgment, it should only be done by a knowledgeable, experienced individual. Discontinued Tests—These can be included if longer lived, or excluded if shorter lived, than average life of the data subset (lot, section thickness, etc.) to which they belong. SteppedTests—If load on the specimen had been increased or decreased after initial loading, this test result shall be excluded. Truncating Data—Certain equations, notably parametrics, often do not properly represent a mix of shorter and longer time data. These equations can severely overpredict creep and rupture lives less than ten to thirty hours. Similarly a preponderance of short time data can cause long lives to be overpredicted. Eliminating such data requires truncating the data (or subset). This is done by removing all data above (or below) a fixed stress level, even though normally acceptable data are excluded. Background Data Reporting—The significance and reliability of creep data generated at elevated temperatures for heatresistant alloys are, to a major extent, a function of detailed factors which relate to the material, its processing, and its testing. Hence, it is necessary to evaluate not only the property data, but also correlative information concerning these factors. It is not possible to specify individual items of correlative information, or the minimum thereof, which must be provided with elevated temperature property data to make those data properly meaningful. Individual alloy systems, product forms, and testing practices can all be quite unique with regard to associated information which should be provided with the data. A certain minimum amount of information is required for all data, including: (1) (2) (3) (4) (5) (6) (7)
Identity of alloy Chemical composition of the specific material tested Form of product (sheet, forging, etc.) Heattreatment condition Producer(s) Specification to which product was produced (AMS specifications are normally considered standard*) Date when part was made.
* Company specification data may be included with federal, military, and industry specification data if it is properly documented and can be shown to compare favorably in creep or stressrupture behavior.
9136
MMPDS01 31 January 2003 Lack of such information is sufficient basis for rejection of a particular data set. In addition, it is vital that the individual submitting data consider those factors which contribute to uniqueness of the alloy, processing, and/or testing, and give thought to information which is pertinent to that uniqueness. Thus, grain size can be a significant variable, not only between cast turbine blades, but within a single blade. Thermomechanical working processes may result in significantly different properties (not only higher, but lower as well); and test specimen design can affect resultant data. It is mandatory that knowledgeable personnel be involved when data are submitted for evaluation and potential use. Any correlative data that can be provided will aid the analyst in identifying valid reasons for rejection of data which may not fit the trends of other data (outliers). Such apparent outliers may be indicated through analysis of betweenheat variance as described in Section 9.6.4.2. These examples illustrate the need for adequate information: (1)
Creeprupture specimens are being machined from cast highstrength, nickelbase alloy turbine blades. At center span location, specimens are 0.070 to 0.090inch diameter, while at the trailing edge, specimens are flat and 0.020inch thick. Flat specimens are typically about one LarsonMiller parameter weaker than round specimens, which is attributable both to thickness effects of the thin specimens and to finer grain size at the trailing edge. In addition, trailing edge specimens exhibit more scatter. Hence, availability of associated information is vital when considering data from specimens machined from cast turbine blades.
(2)
Comparison of creeprupture properties of Waspaloy and Superwaspaloy shows that the latter is much weaker at temperatures approaching the upper bounds of utility of the alloy. The significantly lower properties at higher temperatures are attributed to a finer grain size of Superwaspaloy and also to a recovery process that may well be occurring at these temperatures. This alloy is subjected to extensive thermomechanical working, and some strengthening gained by the associated warm working is lost at higher testing temperatures. This effect clearly indicates that processing history significantly affects levels of mechanical properties and, hence, must be adequately documented when property data are submitted.
9.6.4.2 Analysis of Data — After an acceptable data collection has been obtained and interpreted, it is possible to proceed in analyzing those data and developing mathematical models of creep and creeprupture behavior. The objective of the procedures described in the following paragraphs is to calculate creep and rupture life as a function of test conditions and other significant variables. This calculation is done to provide an average curve and a measure of expected variability about the average. The approach that is discussed involves regression analysis to optimize the fit of an equation to the data set. The following information provides guidelines in the application of regression analysis to creep and rupture data and recommends approaches to specific problems that are frequently encountered. General—It is assumed that life or time is the dependent variable for rupture or isostrain creep equation analysis, respectively, and logarithmic transformation of the dependent variable is normally distributed. The data set will nearly always contain a variety of stresses and temperatures. If the data set is the product of a very wellbalanced test design, good results may be obtained by independently fitting each temperature. Since this type of data set is often not available, and the approach sacrifices the opportunity for interpolation, the discussion will assume that at least temperature and stress are used as independent variables. In order to achieve good results, it may be necessary to consider other variables. Some variables are continuous physical variables that are incorporated into regression variables, e.g., section size. Other variables may occur as discrete subsets that require modifying the regression analysis (this is discussed under
9137
MMPDS01 31 January 2003 Subsets of Data). In such cases, it may be necessary to group data per subset for data reporting if regression analysis cannot easily accommodate the observed subsets. Selection of Equations—For isostrain and rupture time, as a function of stress and temperature, a number of relationships have been proposed. Some useful ones are: (1) log t = c + b1/T + b2X/T + b3X2/T + b4X3/T
[9.6.4.2(a)]
(2) log t = c + b1/T + b2X + b3X2 + b4X3
[9.6.4.2(b)]
(3) log t = c + b1 T + b2X + b3X2 + b4X3
[9.6.4.2(c)]
(4) log t = c + (TTa)(b1 + b2X + b3X2 + b4X3).
[9.6.4.2(d)]
These are the LarsonMiller, Dorn, MansonSuccop, and MansonHaferd, respectively, where c b1 t T X
= = = = =
the regression constant coefficients (b1 through b4) time absolute temperature (Ta is the temperature of convergence of the isostress lines) log S (stress).
While all forms may be used to model a data set with varying degrees of goodness of fit, experience and practice indicate the LarsonMiller relationship adequately models most materials, and is usually the preferred equation form. If data for a given material is available at a variety of creep strain levels as well as the stress rupture point, only one model should be used to describe data trends for each strain level. The decision as to which of the four customary models is chosen should be based on a comparative analysis of data for the most comprehensive data collection, whether that collection be for a specific creep strain level or stress rupture point. In addition, the constant term found in the optimum analysis should be held the same for all creep strain levels. If this is done, it will be possible to construct a composite plot of stress versus parameter for all creep strain levels and the stressrupture level. If none of these standard forms satisfactorily follows data trends, various combinations of stress and temperature may be tried. For example, terms can be selected from a matrix obtained using cross products of T1, To, T1 with S1, So and S1. Methods for generalizing and applying these equations are discussed in Reference 9.6.4.2. The exact form of the functions should reflect data and reasonable boundary conditions. Quadratic, quartic, etc., can be expected to give poor boundary conditions, e.g., zero life at zero stress, and should be avoided. Extrapolation by users of the equation is inevitable (though it is not recommended), so other general equations must be checked for unusual behavior beyond the data—this can be done, in many cases, by differentiating to obtain maxima and minima. In general, short times should give strengths approximately corresponding to tensile yield and ultimate strength; zero stress should predict infinite life.
9138
MMPDS01 31 January 2003 Metallurgical instabilities and transition regions may present difficulties in some analyses. Methods for handling such problems have been discussed in Reference 9.6.4.2. Optimum Fit—Guidelines for an optimum fit are: (1) Minimum number of terms. With two independent variables, σ and T, six regression variables are reasonable, each additional physical variable allowing two additional regression variables. (2) Reasonable curve characteristics for material behavior, including extrapolation. (3) Minimum standard error and maximum correlation coefficient (as long as 1 and 2 are not violated). Standard errors are typically between 0.1 and 0.2. (4) Uniform deviations (see a later paragraph on Weights for a brief discussion of nonuniform deviations and their analytical treatment). Subsets of Data—A nonnormal or multimodal population, or an excessive standard error may indicate the presence of subsets. However, an apparently typical data set may contain subsets that should receive special consideration. One type can be treated by adding physical variables to the regression analysis. For example, different thicknesses of sheet material may give different average lives. Including sheet thickness in the regression should not only improve fit but also avoid the risk of misrepresenting behavior of the material. Section thickness, distance from surface, and grain size are other examples of subsets that can be treated as regression variables. Section thickness and distance from surface refer to location of the specimen in terms of geometry of the original material, e.g., finish work thickness, final heat thickness, etc. A second type is not typically subject to use as a regression variable. Examples of these are orientation (L, LT, and ST), or different heats (chemistry). A decision must be made whether to treat these as unique subsets to be analyzed separately (if properties are different) or as randomly distributed subsets. Orientation will usually be analyzed separately, while heats will usually be randomly distributed subsets. Other methods (e.g., fixed intercept, centered above mean values for each creep level) may be more suited for a given data set and may be tried. The specific procedure used must be indicated in the data package. The theory of treatment of randomly distributed subsets has been developed in Reference 9.2.5.2, while application to lots of material (actually “heats” in chemistry) is considered in Reference 9.6.4.2. Treating subsets as random affects calculation of both average curve and standard error. While effect on standard error may become insignificant as the number of subsets exceeds ten (depending on the relative contribution to total standard error), effect on the trend of the calculated average remains. Lots whose average lives are uniformly displaced (parallel) in logarithm of life, or are not significantly nonparallel, are discussed in Reference 9.6.4.2(a). There is no known published reference for treating nonparallel lots. Data permitting, individual lots can be fitted, withinlot variances pooled, and average and variance of lot averages calculated for selected stresstemperature combinations. After calculating total variance and desired lower level tolerance limit* ( X  ks) at each stress level, curves can be drawn and, if desired, equations be fit to X’s and ( X  ks) ’s. It should be noted that the equation for ( X  ks) is not likely to properly reflect uncertainty in coefficients obtained by normal fitting procedures. Alternately, all data for nonparallel lots can be pooled and variance weighted, providing sufficient lots are represented and average curve is reasonably similar to the first approach.
* Tolerance limits used here are onesided and are normally developed for tolerance levels of 90 or 99 percent at a confidence level of 95 percent.
9139
MMPDS01 31 January 2003
Consistency in Creep and Stress Rupture Trends—When creep data are somewhat limited, an independent analysis of each creep strain level may produce inconsistent trends between different creep strain levels and stress rupture mean curve. There may be cases where very minor extrapolations will produce creep curves that cross over each other or the stress rupture curve. In some instances, this problem can be eliminated, without a significant loss in quality of fit at each creep strain level, by forcing a prescribed relationship to exist between creep curves and stress rupture curve. Parallelism in log(time) is the simplest relationship that can be assumed, but it is also a relationship that is often supported by data trends. A linearly increasing or decreasing separation of creep curves and stress rupture curve in log(time) as a function of stress is also a possibility, but it takes a large quantity of data to verify such trends. If large quantities of data are available, then it is generally preferable to analyze each creep strain level individually. Therefore, about the only practical relationship to assume between individual creep curves and the stress rupture curve is parallelism in log(time). Parallelism in log(time) can be achieved through the addition of a dummy variable to the stress rupture equation for each creep strain level being added to the regression analysis. For example, in the case of the LarsonMiller equation, which (in its third order form) is normally written as log t = c + b1/T + b2X/T + b3 X2/T + b4 X3/T,
[9.6.4.2(a)]
where t = time, hrs T = absolute temperature, ER X = log (stress), ksi, the equation can be modified to include additional terms for each creep level, as follows log t = c + b1/T + b2X/T + b3X2/T + b4X3/T + b5 Y1 + b6 Y2 + ...b4+i Yi
[9.6.4.2(e)]
where the value of Yi new terms are either 0 or 1. If a creep strain level 1 data point is considered, Y1 = 1 and all other Y’s are 0. Similarly, if a creep strain level 2 data point is considered, Y2 = 1 and all other Y’s are 0. If a stress rupture data point is considered, all the Y’s are 0. In this way, the optimized values of additional b’s represent average A in log(time) that each creep curve falls below the stress rupture curve. The usefulness of such an approach must be verified through an examination of quality of fit for each creep strain level compared to raw data trends. Weights—Rupture and isostrain creep curves will not normally require weights to obtain uniform variables. Analysis, including strain as a variable, frequently will. Variables other than strain, temperature, and stress will require evaluation for uniform variance. Reference 9.6.4.2(a) provides further discussion of weighting.
9140
MMPDS01 31 January 2003 Rejection of Analyses—Regression analyses of specific creep or stressrupture data sets should normally be rejected if the R2 statistic for analysis is